1,663 286 8MB
Pages 429 Page size 395 x 600 pts Year 2007
http://72.3.142.35/mghdxreader/jsp/FinalDisplay.jsp;jsessionid=aag1B0...
CIP Data is on file with the Library of Congress Copyright © 2006 by The McGrawHill Companies, Inc. All rights reserved. Printed in the United States of America. Except as permitted under the United States Copyright Act of 1976, no part of this publication may be reproduced or distributed in any form or by any means, or stored in a data base or retrieval system, without the prior written permission of the publisher. 1 2 3 4 5 6 7 8 9 0 DOC/DOC 0 1 2 1 0 9 8 7 6 ISBN 0071457925 The sponsoring editor for this book was Kenneth P. McCombs, the editing supervisors were Caroline Levine and Stephen M. Smith, and the production supervisor was Pamela A. Pelton. It was set in Century Schoolbook by Digital Publishing Solutions. The art director for the cover was Handel Low. Printed and bound by RR Donnelley. McGrawHill books are available at special quantity discounts to use as premiums and sales promotions, or for use in corporate training programs. For more information, please write to the Director of Special Sales, McGrawHill Professional, Two Penn Plaza, New York, NY 101212298. Or contact your local bookstore. This book is printed on acidfree paper. Information contained in this work has been obtained by The McGrawHill Companies, Inc. (“McGrawHill”) from sources believed to be reliable. However, neither McGrawHill nor its authors guarantee the accuracy or completeness of any information published herein, and neither McGrawHill nor its authors shall be responsible for any errors, omissions, or damages arising out of use of this information. This work is published with the understanding that McGrawHill and its authors are supplying information but are not attempting to render engineering or other professional services. If such services are required, the assistance of an appropriate professional should be sought.
Copyright © 2006 by The McGrawHill Companies, Inc., McGrawHill
1 of 1
11/1/2007 12:00 PM
Intersubband Transitions in Quantum Structures, 1st edition 0071457925 Table of Contents Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Terahertz Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Raman Injection and Inversionless Intersubband Lasers Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Intersubband Transitions in Quantum Dots Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures Index
0071457925_CH01_1_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
1 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art
Carlo Sirtori Matériaux et Phénomènes Quantique Université Paris 7, 75251 Paris, France; THALES Research & Technology 91767 Palaiseau cede, France
Roland Teissier CEM2, Université de Montpellier 2 34095 Montpellier, France
1.1 Introduction 1.1.1
Historical introduction
Before the invention of the diode laser, a semiconductor laser based on transitions between Landau levels in a strong magnetic field was proposed by Lax in 1960. This is the first proposal of a semiconductor laser in which the optical transition occurs between low dimensional states of the same band (conduction or valence) rather than by the recombination of electronhole pairs across the semiconductor bandgap. The idea of a unipolar laser was then ignored for many years since only 2 years after the proposal of Lax the first diode laser was demonstrated (Hall et al. 1962). This exploit drew all the attention of the semiconductor community on bandgap lasers and began the race for the first diode laser continuouswave (cw) operation at room temperature. The race ended in 1970 when the first AlGaAs/GaAs heterostructure 1
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_2_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 2
Chapter One
laser in cw operation at room temperature was achieved at nearly the same time by Alferov’s group at the Ioffe Institute in St. Petersburg (Alferov et al. 1970) and by Panish et al. (1970) at Bell Labs (Murray Hill, NJ). The effort to improve the performance of diode lasers and the development of the transistor technology in IIIV compounds had an enormous impact on the epitaxial techniques for the growth of thin semiconductor layers and gave rise to the concept of twodimensional structures such as quantum wells and inversion layers (Cho 1994). In fact, also in 1970, while the diode lasers reached technological maturity, Esaki and Tsu published their seminal paper presenting the concepts of a superlattice (Esaki and Tsu 1970). One year after, Kazarinov and Suris (1971), two scientists also from the Ioffe Institute, suggested that optical gain could be obtained by using transitions between twodimensional states in a superlattice biased by an external electric field. This structure, very innovative with respect to the other semiconductor lasers, introduced the concept of a unipolar device in which the optical transitions could be completely engineered by the judicious choice of the thickness of well and barrier materials, regardless of their energy gap. Years later, after the demonstration of the first quantum cascade (QC) lasers, at a conference Capasso proudly declared, “The QC lasers make us finally free from the bandgap slavery.” It is hard to say if the Kazarinov and Suris structure could really show optical gain, and most likely it is not so for two main reasons. The first is related to the lack of reservoirs of electrons that inject carriers in each active region of the cascade. Without the reservoir it is necessary to bring electrons from the contacts, which makes the structure electrically unstable due to the formation of space charge domains. The second reason, more subtle, comes from the lack of a region where highenergy electrons can be accumulated without backfilling, by thermal effect, the ground state of the laser transition. In other words, the structure proposed by Kazarinov and Suris was lacking the injector, which today is thought to be an essential part of a quantum cascade laser. For more than 15 years after the first proposal no real progress was made toward the realization of a unipolar laser. At the end of the 1980s, and beginning of the 1990s, researchers working on resonant tunneling reawakened the subject (Liu 1988, Henderson 1993). In the span of a few years, several proposals appeared on how to achieve population inversion by using intersubband transitions in superlattices or in coupled quantum wells, but none was implemented into a real laser structure. In 1988, Capasso at Bell Labs was also working on resonant tunneling, and that year he published a review paper in which he proposed a Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_3_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
3
unipolar laser based on a superlattice structure (Capasso et al. 1986). As a matter of fact, he really began to work on light interaction with intersubband transitions only in the 1990s, when Sirtori joined his group to study the linear and nonlinear optical properties of these transitions (Sirtori et al. 2000). The laser project really gained momentum one year later when Faist joined the group of Capasso. A little more than 2 years after his arrival, on January 14, 1994, for the first time Jerome Faist observed laser action from an electrically injected intersubband laser at 4.3ȝm wavelength: The quantum cascade laser was born. The main results were published a couple of months later in Science (Faist et al. 1994). It is interesting to note that in the midinfrared regime (3 m < Ȝ < 15 ȝm) the demonstration of a laser practically anticipated the observation of electroluminescence. This is related to the intrinsic difficulty of observing spontaneous emission from an electron on an excited subband which has a radiative efficiency close to 10í5! In a few years after the first demonstration, the performance of the quantum cascade laser dramatically improved: In 1996, aboveroomtemperature operation in pulsed mode was achieved, and the longwavelength range was extended already to 11 ȝm (Faist et al. 1996, Sirtori et al. 1996). Today quantum cascade lasers in the range of 4 to 10m wavelength operate routinely continuouswave at room temperature with hundreds of milliwatts of optical power (Bewley 2005). At low temperature, the concepts of quantum cascade lasers have been extended into the terahertz region and the whole wavelength range where lasers have demonstrated spans at present from 3.5 to 150 ȝm (Faist et al. 1998). Between the first QC laser demonstration and the present, several contributions were made by many different groups. Before concluding this historical introduction, we mention some of what we believe are the breakthroughs that played a major role in this field. In chronological order, in 1998 a quantum cascade laser in a GaAsbased heterostructure was demonstrated at the Thomson (today Thales) Laboratories (Sirtori et al. 1998); in 2002, terahertz QC lasers were realized at the Scuola Normale Superiore of Pisa, and during the same year the University of Neuchâtel demonstrated the first laser operating in cw at room temperature (Köhler et al. 2002, Beck 2002); and in 2004 roomtemperature highpower devices were developed (Evans et al. 2004a, b). At present there remain several scientific challenges in the field of QC lasers: devices with short wavelength (Ȝ < 3 m), where the development of less conventional heterostructures is needed (GaN or Sbbased materials); the use of onedimensional or zerodimensional structures for the realization of QC lasers based on quantum wires or Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_4_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 4
Chapter One
dots; the improvement of the wall plug efficiency and the comprehension of the gain saturation that limits the peak output power. That said, we are also convinced that the main challenge for this field lies in the development of realworld applications and the establishment of a commercial market. 1.1.2
Quantum engineering
In the last century, the work of engineers dealing with condensed matter, such as for electronics, for optoelectronics, and in general for material science, was in great part related to the manipulation of the material properties directly descendent from the chemistry of the principal constituents. Quantum engineering (Fig. 1.1) does not play with the chemical bonds between atoms as has been done until recently to discover and produce new and advanced materials. Rather, quantum engineering explores the possibility of controlling the material properties by defining the size and the spatial distribution of the constituents at the nanolevel independently of their chemical nature. The final characteristics of this new class of materials come directly from the redefinition of topological properties at the atomic level and can be applied with the same results on different combinations of materials. In this respect nanotechnologies are a direct emanation of the quantum engineering. The quantum cascade laser is an excellent example of how quantum engineering can be used to conceive efficient devices and emitters in the midinfrared (midir). In these devices the princi
Quantum Engineering 1900
1800 Mechanics (Newton Eqs.)
Electricity (Maxwell Eqs.)
Quantum mechanics (Schrödinger Eqs.)
Understanding of the phenomena
2000
Realization of new systems (engineering)
Understanding of the phenomena
Realization of new systems (engineering)
Understanding of the phenomena
Realization of new systems (engineering)
Condensed matter, chemistry, photonics, . . . Figure 1.1 Quantum engineering is a consequence of our time. The rules of quantum mechanics are today sufficiently well known and verified so as to start a new engineering that develops devices based on Schrödinger equation. A similar scheme can be observed, by looking back through the centuries, in mechanics and electronics.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_5_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
5
ples of operation are not based on the physical properties of the constituent materials, but arise from the layer sequence forming the heterostructure. Quantum engineering associated with the recent progress of the epitaxial growth techniques allows one to ascribe within a semiconductor crystal artificial potentials with the desired electronic energy levels and wave functions. This approach is the basis for modifying, in a unique way, the optical and transport properties of semiconductors, opening avenues to artificial materials and the creation of useful devices. A remarkable illustration of this concept is the QC terahertz laser, in which by judiciously introducing less than 2% of Al atoms into a GaAs crystal we transform a piece of bulk semiconductor into a performing farinfrared laser! Another crucial aspect of QC lasers, related to the quantum engineering, is that the fundamental principles of this device are essentially independent of the specific semiconductor system used. As of today, QC lasers have been demonstrated using basically three material systems: GaInAs/AlInAs//InP, which is the original system and the one that still gives the best performance for lasers in the midinfrared range; GaAs/AlGaAs//GaAs, which is the material system for the terahertz laser; and AlSb/InAs//InAs (or //GaSb), which is the most recently exploited and whose very high conduction band discontinuity gives hope for shortwavelength QC lasers. Interestingly, in these three material systems, QC lasers have been fabricated, for instance, at 10 m, confirming that the emission wavelength is totally independent of a particular transition intrinsic to the compounds material. This is unique, and no other laser, semiconductor or not, has this property. 1.1.3
Organization of the chapter
After the introduction in Sec 1.1 of the history of the quantum cascade laser and presentation of the scientific context in which this research is situated, the chapter has three main parts and a brief conclusion. In Sec. 1.2 we recall the fundamentals of quantum cascade lasers. First we describe the main properties of a QC laser and its differences from diode lasers. Then in Sec. 1.2.2 we describe the rules that have to be respected to obtain population inversion between two subbands of the same band, and in Sec. 1.2.3 we give a description of the optical gain based on a simple rate equations model. In Sec. 1.3 we review the stateoftheart of QC lasers and emphasize some of the best results. We then present lasers at short and very long wavelengths of the spectral range and finally give an overview Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_6_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 6
Chapter One
of the material systems in which QC lasers have been fabricated up to now. The physical parameters relevant for the design and control of perfomance, such as conduction band discontinuity and electronic effective mass, are discussed in Sec. 1.4. In Sec. 1.4.5 we also give a basic description of the waveguides used for QC lasers. 1.2 Fundamental Principles of Quantum Cascade Lasers 1.2.1
Unipolarity and cascading
Semiconductor diode lasers, including quantum well lasers, rely on transitions between energy bands in which conduction electrons and valence band holes are injected into the active layer through a forwardbiased pn junction and radiatively recombine across the material bandgap (Yariv 1989). The latter essentially determines the emission wavelength. In addition, because the electron and hole populations are broadly distributed in the conduction and valence bands according to Fermi’s statistics, the resulting gain spectrum is quite broad and its width is on the order of the thermal energy. The unipolar intersubband laser or QC laser differs in many fundamental ways from diode lasers. All the differences are consequences of two main features which are unique to quantum cascade lasers and distinguish them from conventional semiconductor light emitters: unipolarity (electrons only) and a cascading scheme (electron recycling). These two features, shown schematically in Fig. 1.2, are UNIPOLARITY
CASCADING SCHEME
optical transition between subbands
more photons per electon
3 2 1 Schematic representation of two features that characterize a quantum cascade laser. Note that intersubband transitions can be observed also for holes, and therefore QC lasers are also conceivable in the valence band, for instance, using SiGe quantum wells.
Figure 1.2
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_7_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
7
independent and can be used separately, as has been demonstrated experimentally. In 1997 Garcia et al. demonstrated a cascade interband laser at ~830 nm, whereas Gmachl et al. in 1998 demonstrated an intersubband laser without a cascade scheme. The unipolarity in QC lasers is a consequence of the optical transitions that occur between conduction band states (subbands) arising from size quantization in quantum wells. These transitions are commonly denoted as intersubband transitions. Their initial and final states are in the conduction band and therefore have the same curvature in the reciprocal space. If one neglects nonparabolicity, the joint density of states is very sharp, similar to the case of atomic transitions. In contrast to interband transitions, the gain linewidth is now only indirectly dependent on temperature through collision processes and many body effects. Moreover, for these devices the emission wavelength is not dependent on the bandgap of constituent materials, but can be tuned by tailoring the layer thickness. The highest achievable photon energy is ultimately set by the constituent conduction band discontinuity, while on the longwavelength side there are no fundamental limits preventing the fabrication of QC devices emitting in the far infrared. The other fundamental feature of QC lasers is the multistage cascade scheme, whereby electrons are recycled from period to period, contributing each time to the gain and the photon emission. Thus each electron injected above threshold can generate, in principle, Np laser photons, where Np is the number of stages. This leads to a quantum efficiency Șq » 1 and therefore very high optical output power, since both quantities are proportional to Np. 1.2.2 Rules to get intersubband population inversion
In a QC laser, one period of the active zone can be approximated to a threelevel system, as shown in Fig. 1.3. The role of the injector region is to transport electrons from level e1 to level e3 of the next period. Intersubband gain arises from a population inversion between levels e3 and e2. An important parameter for QC laser operation is the injection efficiency Și. It is defined as the ratio of the current injected in level e3 to the total current Și =
J3 J
(1.1)
In the ideal case Și = 1. Deviations from this value can be due either to thermal activation from the injector to continuum or highly excited
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_8_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 8
Chapter One
J τ3
3
Injector
2
τ2
1
Active QW
Figure 1.3
Schematic representation of one active region of a QC laser.
states, or to direct injection of electrons from the injector to the lower states e2 and e1. The first mechanism can be avoided by a proper design of the active zone and by the use of higher energy barriers. The second mechanism can be reduced by the use of a narrow quantum well after the injection barrier that enhances the injector coupling with e3, but lowers the coupling with e2 and e1. If Ĳ3 is the total lifetime of electrons in level e3, the steadystate electron sheet density in this level is given by n3 =
Și J Ĳ e 3
(1.2)
If one assumes that level e2 is populated only through the direct scattering of electrons from level e3, the electron density in e2 is simply given by n2 = n3
Ĳ2 Ĳ32
(1.3)
where Ĳ32 is the mean scattering time from e3 to e2 and Ĳ2 the lifetime of electrons in e2. In this picture, the population inversion reads n3 í n2 =
Și J Ĳ2 Ĳ 1í Ĳ32 e 3
(
)
(1.4)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_9_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
9
In the most unfavorable case in which all the electrons flow sequentially from e3 to e2 (equivalent to saying that Ĳ3 = Ĳ32), n2 has its maximum value n2 =
Ĳ 2Ș i J e
(1.5)
Și J (Ĳ3 í Ĳ2) e
(1.6)
and n3 í n2 =
If the condition Ĳ3 > Ĳ2 is satisfied, population inversion and optical gain are achieved for any current density. A typical way to achieve shorter Ĳ2 is to use the threelevel scheme with the e2 to e1 transition resonant with the LO phonon energy. This is a remarkable feature of QC lasers (QCLs): There is no threshold for population inversion, and gain is present from the first flowing electron. As a result, the laser threshold current density is directly proportional to the optical cavity losses and not related to a transparency condition. Hence, a main issue for achieving a lowthreshold QCL is to reduce optical losses, both by fabricating lowloss waveguides and by using long devices (2 to 4 mm) to reduce the contribution of mirror losses. 1.2.3
Rate equations
The exact determination of the steadystate populations in the two states e2 and e3 involved in the intersubband optical transition is, in general, not straightforward. It results from the quasiequilibrium distribution of the total electron population in the active zone, involving different intersubband scattering mechanisms. These include direct scattering from the previous injector across the injection barrier, or backscattering of hot or lowenergy electrons from the next injector. The contribution of thermalized electrons to the population of e2 is known as the thermal backfilling effect. Backfilling can be avoided by proper design of the injector, giving a large enough energy ǻ (Fig. 1.4) between level e2 and the lower state of the injector. This energy is strongly dependent on the applied electric field, and in that respect, the field necessary to achieve injector alignment to e3 is a critical parameter. Beyond the simple description presented above, the phenomena that govern the population inversion in a more realistic QC laser structure are complex. Different approaches based on the rateequation approximation that include a description of various scattering mechanisms Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_10_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 10
Chapter One
Energy (meV)
600
400
200
Δ 0
200 0
200
400
600
800
Z (Å) Schematic conduction band diagram of a portion of the laser heterostructure at threshold bias. The wavy lines indicate the moduli squared of the calculated wave functions. Indicated also is ǻ, the energy that separates the ground state of the laser transition from the lower state of the injector.
Figure 1.4
between all quantum levels of the active zone have shown fair agreement with experimental characteristics, such as currentvoltage curves (Donovan et al. 2001). However, not all scattering mechanisms are included in these calculations, and typically electronelectron interaction and interface roughness scattering are not taken into account. Another approach is a nonequilibrium Green’s function theory (Lee and Wacker 2002). It allows all the important scattering mechanisms to be included and accesses the currentvoltage characteristics and gain spectra of QCLs. Its advantage over semiclassical rate equation approaches is clear for longwavelength QCLs (terahertz), where the extension of the wave functions is easily beyond the coherence length of a quantum state in a semiconductor. 1.2.4
Gain derivation
To derive the gain of a quantum cascade active region, first we focus on the determination of the intersubband transition probabilities induced by the presence of an incident electromagnetic wave. We consider a linearly polarized electromagnetic plane wave with an electric field E = E0İ cos(Ȧt – q·r) of polarization İ, pulsation Ȧ, and propagation vector q. In a semiconductor material of refractive index n, we have q = nȦ/c. The vector potential A associated with this incident electromagnetic wave is given by the relation E = – A/t and reads
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_11_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
A = í
E0 ( ) ( ) İ (e i Ȧ t í q썉r í e í i Ȧ t í q썉r ) 2Ȧ
11
(1.7)
The action of this incident wave on the electron eigenstates of the heterostructure is given by the timedependent hamiltonian H, written by using the dipolar approximation and the effective mass description (Bastard 1988) as H= í
e A 썉 p = V (e iȦt í e í iȦt ) m*
(1.8)
where e is the electron charge, m* is the effective mass in the quantum well material, and V=
eE0 İ썉p 2m* Ȧ
(1.9)
Under the action of this perturbation hamiltonian, the probability per unit time that an electron makes a transition from the initial state  i of energy Ei to the final state  f of energy Ef is given by the Fermi golden rule: Wif ( ല Ȧ ) =
2ʌ  f  V  i 2 į ( E f í Ei ± ല Ȧ ) ല
(1.10)
Using the momentum matrix element, we have Wif ( ല Ȧ ) =
2 2 2 ʌ e E0  f  İ 썉 p  i 2 į ( Ef í Ei ± ല Ȧ) ല 4m* 2Ȧ2
(1.11)
The – ƫȦ term is associated to the first component of A and corresponds to the absorption of an incident photon ( Ef = Ei + ലȦ), whereas the + ƫȦ term is associated to the second component of A and corresponds to the stimulated emission of a photon ( Ef = Ei ലȦ). In the effective mass approximation, the wave functions of the heterostructure states are in the form ȥi (r) = uȣ i f i (r) f i ( r) =
1 ik 쌩 i 썉r쌩 e Ȥi ( z ) S
(1.12)
where uȣ i is the periodic part of the Bloch function, k쌩i and r쌩 are the twodimensional wave and position vectors in the plane of the layers of area S, and Ȥi(z) is the envelope function, which describes the
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_12_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 12
Chapter One
extension of the electron state in the direction perpendicular to the heterostructure layers. For intersubband transitions, the initial and final states originate from the same band ( uȣi = uȣ f ). In this case, the matrix element of Eq. 1.11 simplifies to the matrix element of the envelope functions f  İ 썉p i
=
f f  İ 썉 p  fi
=
Ȥ f  Ȥi
1 S
d x d y e
í i k 쌩 f 썉r쌩
(İ x p x + İ y p y ) e i k
쌩 i 썉r쌩
+ į ( k 쌩 f í k 쌩 i )İ z Ȥ f  p z  Ȥ i (1.13) Since the envelope functions are orthogonal, the term Ȥ f  Ȥi is null if the final subband is different from the initial one. Consequently, the transition rate from state i to state  f is given by Wif (ലȦ) =
2 2 2ʌ e E0 2 İ  Ȥf  p z  Ȥ i  2 ല 4m 2Ȧ2 z
(1.14)
× į(k 쌩 f í k 쌩i )į( Ef í Ei ± ലȦ)
Alternatively, we can choose to express the matrix element in the r representation, which is a much more common notation. In this case, the transition rate is written using the z dipole moment matrix element and reads Wif (ലȦ) =
2 2 2ʌ e E0 2 İ z  Ȥ f  z  Ȥi 2 4 ല
(1.15)
× į(k쌩f í k쌩i )į( Ef í Ei ± ലȦ) Equations 1.14 and 1.15 contain several important pieces of physical information about intersubband transitions: ■
The optical transitions occur only when the electric field is parallel to the direction of growth z. In fact, only the İz component of the polarization is left in the expressions of the transition rates. This has the immediate consequence that no transitions are possible if the light propagates perpendicular to the sample surface. This is the wellknown intersubband polarization selection rule, which is very well observed experimentally.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_13_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
■
■
13
The optical transitions are vertical in kspace (k쌩f = k쌩i) and, in the parabolic band approximation, the transition energy Eif = Ei í Ef and the transition rate Wif do not depend on the inplane wave vector. The matrix element depends exclusively on the envelope functions and can be tailored by designing the shape of the wave functions in coupled well structures.
In summary, Wif is the general transition rate of an electron from subband i to subband f independent of its twodimensional nature. In reality, the subbands have a finite width that can be accounted for by replacing the delta function for energy conservation by a lorentzian function of half width at half maximum Ȗ: Wif ( ലȦ) =
ʌe 2 E02  zif 2 2ല
Ȗ/ʌ
( Ei f
í ലȦ)2 + Ȗ2
(1.16)
As far as QC lasers are concerned, the relevant quantity is the maximum stimulated emission rate, obtained for ƫȦ = Eif, of Wif max =
e 2 E02 zif 2 2Ȗല
(1.17)
Equation 1.17 is the probability of stimulated emission or absorption of a photon per unit time and per electron present in the initial subband, in the presence of electromagnetic radiation of pulsation Ȧ = Eif / ല and of electric field amplitude E0 in the direction perpendicular to the layers. To derive the propagation gain of a QCL active region, one must consider the geometry of the device (Fig. 1.5). Let us consider an electromagnetic plane wave propagating over a width w in the plane of a heterostructure of thickness Lp containing one QC active period consisting of the three levels of Fig. 1.3. The power density carried by the plane wave of amplitude E0 is given by P=
1 İ ncE02 2 0
(1.18)
and the number of photons of energy ƫȦ crossing the structure per unit time is ĭ=
2 1 İ0ncE0 wL p 2 ലȦ
(1.19)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_14_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 14
Chapter One
z y x
Propagation direction
Lp
w Schematic geometry of the device used to derive the material gain. The growth direction is z, and y is the direction of light propagation.
Figure 1.5
If ƫȦ = E32, the variation of the photon flux over a distance dy is max max d ĭ = W32 n3w dy í W32 n2w dy
(1.20)
where n3w dy (and n2w dy) is the total number of electrons of level e3 (and e2) in the slice of length dy. The first term corresponds to the stimulated emission of photons due to the presence of electrons in e3, while the second corresponds to the absorption of photons due to the presence of electrons in e2. The propagation gain (often also referred to as material gain) is defined as the variation of the photon flux divided by the number of photons (definition equivalent to the absorption coefficient) G=
dĭ / dy ĭ
(1.21)
By using Eqs. 1.19 and 1.20 and the intersubband transition rate (Eq. 1.17), one gets G=
2e 2 z32 2Ȧ (n í n2) İ0nc2ȖL p 3
(1.22)
With the expression of the population inversion in Eq. 1.4 and by using the wavelength Ȝ = 2ʌc / Ȧ (in vacuum) of the propagating light, one finally gets the usual expression of the gain of a QC laser, proportional to the current density,
G = gJ
(1.23)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_15_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
15
where g is the gain coefficient, defined as g=
Ĳ2 4ʌe z32 2 Ș i Ĳ3 1 í Ĳ32 İ0nȜ2ȖL p
(
)
(1.24)
A quantity commonly used in these expressions is the oscillator strength f32 of the intersubband transition f 32 =
2m0Ȧ ല
Z32
2
(1.25)
The gain coefficient can then be written as g = Și
Ĳ2 eല 1 f 32Ĳ3 1 í Ĳ32 İ0cm0 2ȖnL p
(1.26)
In a QC laser, normally the guided optical mode extends in the z direction outside of the active region. The gain is then reduced in the proportion of the spatial overlap ī of the guided mode with the active zone
G = īg J
(1.27)
Up to now, we have considered only one period. If we have an active region composed of Np periods, each having a comparable overlap with the optical mode, we can write ī = īpNp, and therefore
G = ī p Np g J
(1.28)
which makes it evident that the gain is proportional to the number of periods. This consideration is very well observed when ī < 50% and the active region is centered in a flat part of the mode. To conclude, it is interesting to note that the gain coefficient g is not proportional to the number of periods of the active region. The gain multiplication, when using Np periods, is canceled in Eq. 1.24 by the increase of the thickness Lp of the active region with the same factor. As mentioned before, the benefit of a large number of active periods comes from the corresponding increase of the overlap factor ī with the guided optical mode. The gain is quite small compared to that of interband semiconductor lasers. Threshold currents for the QC laser are higher, but much less sensitive to T since the excited state lifetime is by nature intrinsically short.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_16_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 16
Chapter One
1.3 Quantum Cascade Lasers 1.3.1
Summary of present results
Since their invention in 1994, QC lasers have reached maturity. They now are a wellestablished class of optoelectronic devices that can produce coherent radiation in a wide part of the infrared spectrum, although the best performances are obtained in the 5 to 13m wavelength range (Evans et al. 2004a). A remarkable feature of QCLs is their low sensitivity to temperature. Characteristic temperatures T0 of 150 to 200 K are the standard, enabling hightemperature operation of the lasers; in pulsed mode a maximum operating temperature of 450 K (180ƕC) is currently achieved. However, wall plug efficiencies are in the range of 10% to 15% for the best devices, and thermal power management remains an important issue to be solved. Roomtemperature pulsed operation was rapidly obtained (Faist et al. 1996), as well as cw operation (Sirtori et al. 1996). However, the first continuouswave operation of a QC laser at room temperature was reported only 8 years after its first demonstration (Beck et al. 2002). Today, there is no doubt that in the wavelength range of 3.5 to 150 ȝm the QC laser outperforms all other semiconductor laser technologies based on current injection. Room temperature operation in pulsed mode has been achieved on a very wide spectral range, from 4 to 16 ȝm, and peak power on the order of 1 W is routinely obtained (Sirtori et al. 2002, Faist et al. 2002). In the last couple of years, continuouswave operation above room temperature has been demonstrated between 4.8 and 9 ȝm (Beck et al. 2002, Evans et al. 2004b). Record cw optical power of 0.5 W at 6 ȝm (Fig. 1.6) has been recently reported by Evans et al., and the same authors have also reported average power close to 1 W for devices operating at 290 K (Evans et al. 2004a). This is the most important technological result that has been demonstrated for QC lasers, and it opens the route for new important applications, such as wireless communications and highsensitivity optical sensors, based on midinfrared radiation. However, room temperature cw operation is still one of the major challenges for QC lasers, due to the very high threshold power densities that generate strong selfheating of the devices. If we look at the numbers, we see that at 300 K the best lasers reach threshold at current densities on the order of 2 kA/cm2. This would represent a reasonable injected power for laser diodes, where the voltage is typically on the order of the bandgap. However, in QC lasers, due to the cascade Today’s best performance.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_17_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
293 K
CW operation
10
λ = 6 μm
298 K 298 K
8
303 K 308 K
300
6
313 K 200
318 K
4
323 K 328 K
100
Voltage (V)
Optical power (mW)
400
17
2
333 K 0 0
0.2
0.4
0.6
0.8
1.0
1.2
0 1.4
Current (A) Continuouswave light versus current (L – I) curve of an HRcoated, 9ȝmwide and 3mmlong buried heterostructure laser at various heat sink temperatures. The V–I curve at 298 K is also shown. (Reprinted with permission from Evans et al. 2004a. Copyright © 2004, American Institute of Physics.) Figure 1.6
scheme, the voltage is a function of the number of periods, and it can easily reach 10 V, as shown in Fig. 1.6. Highspeed modulation of quantum cascade lasers and mode locking have been the subject of intense investigations by a group of researchers at Bell Labs led by Capasso in recent years (Paiella et al. 2000, 2001). Among all these brilliant experiments, we would like to draw attention to the smallsignal analysis of a laser under highfrequency modulation. The data in Fig. 1.7 are a clear demonstration of the absence of relaxation oscillation resonance for QC lasers. This is direct experimental evidence that the bandwidth of these lasers will be ultimately determined by the photon lifetime in the cavity rather than the resonant coupling between the photon field and the optical gain, as in conventional diode lasers. In parallel, a new type of QCL emerged in 2002 (Köhler et al. 2002)— the terahertz laser emitting in the far infrared at a wavelength of around 100 μm (Ȧ = 3 THz). These devices are discussed in the next section. This rapid progress is the result of intense research, complex quantum engineering, and technological developments in active region and waveguide designs, in the growth of optimized heterostructure materials, and in device processing. We try to summarize hereafter the contributions that we feel are more important in each of the fields just mentioned.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_18_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 18
Chapter One
10
Modulation response
20 K 20
300 mA
30 250 mA 40 200 mA 50 150 mA 60
0
1 Modulation frequency (GHz)
10
Highfrequency modulation response traces of an 8m QC laser at 20 K for different values of the drive current ranging from very near threshold (150 mA), up to one order of magnitude higher photon density (300 mA). These traces were normalized to the experimental frequency response of the receiver and reflect only the modulation response of the QC laser. (After Paiella et al. 2001.)
Figure 1.7
Active region. The active region of the first QCL was based on a simple threequantumwell (QW) scheme, where the laser transition was diagonal between two adjacent QWs. It emitted at a wavelength of 4.3 m at cryogenic temperatures (Faist et al. 1994). Then more vertical transitions were explored, in order to improve the intersubband gain (Sirtori et al. 1998). The most efficient design was commonly considered to be a vertical intersubband transition in two coupled QWs, with a third very thin QW in the injection barrier. The role of the latter QW is to selectively enhance the amplitude of the excited state of the laser in the injection barrier, to increase resonant tunneling injection while preventing direct injection into the lower states. For hightemperature and highpower operation of QC lasers, the efficiency of electron extraction from the lower state of the active quantum wells is an important issue. To overcome the bottleneck in electron extraction from the active region, new designs have been proposed. Superlatticebased active regions (Scamarcio 1997) have produced highefficiency QCLs, thanks to a very rapid carrier extraction in the superlattice miniband. This was, however, to the detriment of electron injection into the upper state e3. The most efficient scheme, called boundtocontinuum (Faist et al. 2001), combines efficient electron injection into a bound state e3 and rapid extraction from a delocalized lower state. Waveguide. Waveguide design is another fundamental issue. As already discussed, QCL performances are directly related to the low Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_19_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
19
optical losses of the laser cavity. The undisputable champion for high performance in the midinfrared range is the InP material used as optical cladding layers. It is a binary compound that provides a large dielectric refractive index contrast with the active region. In addition, InP has high electrical and thermal conductivity, without the need for a high doping level and therefore allows very low freecarrier optical losses. For this reason, QCLs made of materials grown on InP have considerable advantages. Alternative materials can, however, have their interest in specific cases. This material issue for QCL is discussed in greater detail in the following sections. QCLs are very demanding devices in terms of heterostructure growth. Molecular beam epitaxy, with atomic monolayer control, is the technique of choice for their fabrication. The evolution of laser performances was directly related to the progress in growth quality. The question of growth rate stability is very important for the control of the emission wavelength. Shortterm stability (hour scale) impacts the homogeneity of all periods of the active region and consequently the optical gain. The question of interface roughness, due to atomic intermixing or segregation, is of great relevance (Offermans et al. 2003). First, it induces inhomogeneous broadening of the intersubband transition and consequently of the gain curve. In addition, interface fluctuations create a scattering potential in the plane of the epilayers. This is the cause of elastic scattering of electrons in the active region of the QCLs, which affects the electron dynamics and possibly the lifetime of electrons in the excited state (Leulliet et al. 2005). Most important is certainly the decrease of epitaxial defects and subsequent reduction of optical losses. The more advanced realizations are the monolithic growth of complete QCL structures including active region and highpurity cladding layers (Evans et al. 2004a) which reduced optical losses to few cmí1. This appears to be the key for the fabrication of very highperformance devices. Growth.
Processing. Beyond the conventional ridge geometry, solutions have
been proposed to manage the dissipation of the high thermal power generated in the active part of QCLs. The reduction of the total area of QC devices, without the addition of extra waveguide losses, is one of the most important issues presently under investigation. To this end, two processing technologies are under development: (1) the conventional buried heterostructure used by Beck and coworkers (Beck et al. 2002) and (2) the selective current channeling by ion implantation recently demonstrated at the corporate laboratory of THALES (Sirtori et al. 2002). By exploiting this second way of realizing devices Page Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_20_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 20
Chapter One
et al. were able to demonstrate cw operation of GaAsbased quantum cascade lasers up to 150 K (Page et al. 2004). Additional thick electroplated gold on the top contact is another way to spread the heat away from the active region (Evans et al. 2004a, Forget et al. 2005). Monomode emission from distributed feedback (DFB) QCLs has been obtained on InP (Faist et al. 1997) and on GaAs (Schrenk 2000). With such technology, QCLs are a new class of singlemode sources available for applications to chemical sensing or pollution monitoring, of particular interest in the 3 to 5m and 8 to 12m ranges. The implementation of photonic crystals is another field explored toward more compact or surfaceemitting QC devices (Colombelli et al. 2003). QC lasers are a very attractive light source for molecular spectroscopy when they are processed into distributed feedback lasers for wavelength control and stabilization. In Fig. 1.8 the spectra of GaAsbased QC lasers, mounted on a Peltier cooler, are shown. Notice that the emission wavelength varies as function of the temperature, due to the change of the material’s refractive index. This is a very important parameter that allows one to finetune the emission frequency with the molecular resonance. The linewidth of freerunning DFB lasers has been measured in different experiments and gives a value in the 2 to 5 MHz (Kosterev and Tittel 2002, Blaser et al. 2001). When stabilized by means of an electronic feedback loop, for highstability
Intensity (arb. units)
Spectra at maximum optical power
0.1
+35°c +20°c 0°c 20°c 40°c
Device size: 1.5 mm x 30 μm
0.01 0.001 0.0001
1040
1050
1060
1070
Wave number (cm1) Figure 1.8 QC laser spectra of a device processed into DFB. The device operates in pulsed mode (100 ns, 5 kHz) and is mounted on a Peltier element where the temperature is varied between –40 and +35°C. The peak position redshifts with temperature; therefore the far left curve corresponds to +35°C and that on the far right to –40°C. The peak optical power is in excess of 100 mW at all temperatures. Note that in this temperature range the device can be tuned over 5 cmí1. (After Sirtori and Nagle 2003.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_21_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
21
operation, these devices have shown lines with intrinsic width well bellow 1 kHz (Myers et al. 2002). Applications. As they produce compact light sources of coherent radi
ation working cw at room temperature in the midinfrared range, from wavelengths of 4 to 10 m, QCLs become attractive for many applications in this spectral range such as gassensing, freespace optical communications, or optical countermeasures. In the terahertz range, molecular spectroscopy or imaging applications promise the potential for longwavelength QCLs. Gassensing applications include, for example, trace gas detection, pollution or process monitoring, isotope separation, etc. Monomode lasers with narrow spectral width and high side mode suppression ratio are needed for spectroscopic applications. The tunability of the emission wavelength is an important property, obtained through the currentinduced temperature shift of the laser line. HighT operation is also required for most applications. Continuouswave operation is indispensable for highresolution spectroscopic applications. However, cw operation is not absolutely necessary, as demonstrated by the company Cascade Technology. It developed a QCLbased spectroscopic system able to acquire the entire spectrum over one single current pulse (Stevenson 2004). Freespace communications can also benefit from QCL sources emitting in the 3 to 5m and 8 to 12m atmospheric windows. Longer wavelengths are theoretically better because they are less sensitive to Raleigh scattering or bad atmospheric conditions. QCLs are also proposed as candidates for optical countermeasures. However, for such applications consisting of deceiving or blinding adverse infrared sensors, emitted power is still an issue. The versatility of QCL technology and its ability to produce multiwavelength sources could be an advantage in this domain. As far as commercial applications are concerned, new perspectives have appeared with the first MOCVDgrown QCLs (Green et al. 2003). This technique provides a more reliable and industrialfriendly approach for QCL fabrication. Despite its presumed impossibility to produce sharp interfaces, rapidly improving performances of MOCVDgrown QC lasers are reported (Troccoli et al. 2005a). 1.3.2
Frontiers
Beyond the conventional midinfrared QC lasers of increasing maturity, new frontiers are being explored. Thanks to the flexibility of the active region and the cascading scheme, new functionalities or phenomena can be explored inside the laser cavity, such as nonlinear optics Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_22_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 22
Chapter One
or Raman lasing (Troccoli et al. 2005b). However, one of the most attractive research areas is at the frontiers of the emission spectrum, to extend the spectral width of QC laser operation. The longwavelength side is the emerging field of terahertz lasers, which opens new perspectives in terms of imaging or molecular spectroscopy. On the other end of the spectrum, shortwavelength QCLs (Ȝ < 4 m) could be the candidate to fulfill the lack of semiconductor laser sources operating at room temperature in the 3 to 4 m range. New physics. The high intensity of optical field in the cavity of QCLs allows generation of intracavity nonlinear effects. Nonlinearity can originate either from the semiconductor crystal itself or from specifically designed structures inserted in series with the active region. Frequency doubling has been demonstrated (Owschimikow et al. 2003) as well as sideband generation (Dihlon 2005). The coherent light generated in the QCL cavity can also be used to pump intersubband transitions and generate emissions at different wavelengths. This principle gave birth to the intracavity Raman laser (Troccoli 2005b). Terahertz domain. In only a couple of years, since the first demonstration in 2002 (Köhler et al. 2002), the progress on QC terahertz lasers has been astonishing. Not only has the wavelength range been extended by more than a factor of 2 from 67 to 150 m (Worral et al. 2005), but also the operating temperatures have noticeably improved: In continuouswave, terahertz devices operate a few degrees above liquid nitrogen, and in pulsedmode they reach 140 K (Williams et al. 2005). In Fig. 1.9 we report VI and LI characteristics at temperature T = 10 K of a device with an emission wavelength of 103 m (2.9 THz) (Alton et al. 2005). The principles of operation of terahertz QC lasers relie on rather different concepts than do devices in the midinfrared, which take advantage of electronLOphonon scattering processes above the material reststrahlenband to achieve large population inversions. Also for terahertz lasers, efficient depletion of the lower level is essential, while long lifetimes of the upper level are highly desirable. To this end, terahertz active regions are designed to have the optical transition, with a large dipole matrix element, across a minigap 10 to 15 meV wide. The lower laser state is strongly coupled to a wide injector miniband (comprising a high number of subbands), which provides a large phase space where electrons scatter, thus ensuring a fast depletion of the lower state of the laser transition. Moreover, the minibands allow efficient electrical transport, even at high current densities, and suppress thermal backfilling. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_23_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
23
Laser frequency (THz) 1.0
20
4
Voltage (V)
3
0 10.5
11.0
11.5
12.0
12.5
13.0
Photon energy (meV)
2
10
Optical power (mW)
0.5
1
T = 10 K 0
0 0
100
300
200 2
Current density (A/cm ) Electrical and optical characteristics (continuouswave) of a 100mwide ridge terahertz laser at 10 K. The length of the device is 2 mm. In the insert is the highresolution emission spectrum.
Figure 1.9
An additional relevant issue for the terahertz range is the fact that conventional laser waveguides are not suitable, owing to large freecarrier absorption losses and practical limitations on the thickness of epilayer growth. For these longwavelength lasers, the optical confinement is never achieved by using dielectric claddings, but by metallic layers very much as in the case of microwave strips. Even if operating at low temperature, terahertz QC lasers are very promising candidates to become compact sources for imaging systems, or local oscillators for heterodyne detection (Gao et al. 2005). Short wavelength. The first demonstration of a QC laser (Faist et al. 1994) was a device emitting at a wavelength of 4.2 m. The shortest wavelength demonstrated today is 3.5 m, not too far from the first QC laser (Faist et al. 1998). As a matter of fact, the standard wavelength for a QCL is restrained in a wavelength range of around 5 to 13 m. The latter corresponds to photon energies between 100 and 200 meV, easily accessible for intersubband transitions in GaInAs/AlInAs quantum wells. The realization of QC lasers emitting at short wavelength is more difficult, since they are limited by the finite depth of the quantum wells (ǻEc in Fig. 1.14). This parameter sets a limit for the energy level e3, the excited state of the laser transition. In typical QCL designs the energy level e3, measured from the conduction band edge in the QW, has a value of twice the photon energy. Thus, a QCL made of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_24_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 24
Chapter One
GaAs/AlGaAs materials with ǻEc = 0.36 eV will not be able to operate with photons of energy greater than 0.18 eV, that is, below a wavelength of 7 m. This limitation on the short wavelength is fundamental and dependent on the materials. Alternative materials presenting higher conduction band discontinuities are required to achieve QC laser emission below 4 m. This is the main motivation of most of the research on new material systems for QCLs presented below. 1.3.3
Results on different materials
By nature, the concept of a QC laser does not depend on the choice of the well and barrier materials that constitute the heterostructure. However, materialdependent properties will play a significant role in the device characteristics, through their influence on barrier heights, scattering mechanisms, waveguide properties, etc. The different IIIV materials that have been investigated for QC lasers are presented in Fig. 1.10. Among all the possible combinations two material systems have been already amply exploited to produce QC lasers: InGaAs/InAlAs grown lattice matched on indium phosphide (InP) substrate and GaAs/AlGaAs grown on gallium arsenide (GaAs) substrate. 2.5
GaP
Energy gap (eV)
AlAs 2.0
AlAsSb
1.5
AlInAs
AlSb GaAs
InP
1.0 GaSb
GaInAs 0.5 InAs
InSb
0.0 5.4
5.6
5.8
6.0
6.2
6.4
Lattice constant (Å) The different IIIV material systems, as defined by their lattice constants. The heterostructures that have been already used to realize quantum cascade lasers are indicated by the dashed ovals.
Figure 1.10
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_25_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
25
InGaAs/InAlAs on InP. This is the historical material system in which the laser was first demonstrated (Faist et al. 1994). In the midinfrared, InGaAs/AlInAs quantum wells lattice matched on InP substrates are the bestperforming solution for QC lasers. Today, they cover the spectrum from 3.6 to 24 m. CW operation at room temperature is obtained from Ȝ = 4.3 m (Yu et al. 2005) to Ȝ = 9.6 m (Beck et al. 2002). With a ǻEc of 0.52 eV, the standard InP system fails to produce highperformance QCLs below 6 m. However, its spectral range can be extended toward short wavelengths by using strained compensated materials, with increased indium content in the InGaAs wells and increased aluminium content in the InAlAs barriers. This provides a larger band discontinuity of 650 to 750 meV as a function of the In and Al content. As a matter of fact, QCL devices made of these strained materials have shown performances of 300mW continuouswave emission at a wavelength of 4.8 m at room temperature (Evans et al. 2004b) and 160 mW at Ȝ = 4.3 m (Yu et al. 2005). DFB lasers operating cw at room temperature have also been realized with InPbased QCLs, first at a wavelength of 5.4 m (Blaser et al. 2005). GaAs. A few years later, GaAsbased QCLs were demonstrated (Sirtori et al. 1998a). They now range from 8 m to the terahertz domain at wavelengths up to 160 m. In the midinfrared, this material system has less interesting performance that of InPbased materials. The major drawback is the relatively higher threshold at room temperature ( JthGaAs 싀 5JthInP) which makes cw operation almost impossible for these devices above 200 K. On the longwavelength side, GaAs becomes better performing than InP fundamentally for reasons of material purity, which dramatically increase the mobility and the conductivity of the semiconductor at low temperature and guarantee lower waveguide losses. This has allowed the birth and development of the terahertz QC lasers (Köhler et al. 2002). Antimonides at 6.1 Å. Antimonide compound semiconductors are the family of IIIV materials with a crystal lattice constant of about 6.1 Å (Fig. 1.10), which can be grown latticematched on gallium antimonide (GaSb) or indium arsenide (InAs) substrates. This family includes the three binary compounds InAs, GaSb, and AlSb and their alloys. The most interesting property of antimonides for the design of QCL is the remarkably large depth of InAs QW with AlSb barriers ǻEc = 2.1 eV. In principle, it should enable the design of very shortwavelength QCLs down to the nearinfrared range (1.5 m). The available QW depth is, however, limited by the position of the lateral valleys (X or L) of the Brillouin zone. The L valley is 800 meV above the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_26_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art 26
Chapter One
conduction band edge in InAs. Therefore, the emission range for this novel material system is probably restricted to wavelengths greater than 3 m. Other specific issues for the realization of shortwavelength QCLs are presented in Sec. 1.4. A second specificity of antimonides is the very small effective mass in InAs. This leads to significantly stronger intrinsic intersubband optical gain, compared to other material systems (see Fig 1.13 below). Hence, from a material point of view, it is clear that antimonides are a very attractive system for midinfrared QCLs. In spite of the very high conduction band discontinuity, the first QC laser demonstrated in this material system was at 10 m (Ohtani and Ohno 2003). More recently the potential of this heterostructure has been better exploited and lasers emitting at ~4 ȝm have been demonstrated up to room temperature (Teissier et al. 2004). Even though the performances of these devices are very encouraging, they have not yet reached those of the QC laser based on InP. We cannot address any fundamental reasons for this, but just remind that these very recently born devices need more work and optimization. An intermediate solution has been proposed and developed from 2003—to use the antimonide alloy AlAsSb latticematched on InP (Fig. 1.10) as a barrier material with InGaAs as the well material both latticematched on InP. This heterostructure benefits both from the advantages of the InP system and from a high ǻEc provided by the AlAsSb barriers. It is, in our opinion, a very attractive material choice for the short wavelengths, for the most part for technological reasons related to the maturity of the processing and InP waveguide claddings. In principle, however, GaInAs has a higher mass and lower lateral valley energy than InAs, which should give lower gain and reduced effective QW depth. QCLs made of these InGaAs/AlAsSb materials were realized for the first time in 2004 (Revin et al. 2004). The devices emitted at Ȝ = 4.3 m in pulsed mode up to a temperature of 240 K. Recently, very hightemperature operation of similar devices around Ȝ = 4.5 m has been reported (Yang et al. 2005).
InGaAs/AlAsSb on InP.
Si/SiGe. For Si/SiGe the steps toward a unipolar laser are less advanced. Nevertheless, intersubband electroluminescence has been recently observed from QC active regions realized on metamorphic substrate Si0.5Ge0.5 (Diehl et al. 2002). The realization of QC lasers in Si/SiGe would represent a major breakthrough simply because it would represent the first laser based on Si. In this material system, intersubband transitions occur in the valence band, which is a serious complication from the point of view of the theoretical description. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH01_27_03/23/2006 Quantum Cascade Lasers: Overview of Basic Principles of Operation and State of the Art Quantum Cascade Lasers
27
Moreover, the presence of the different hole dispersions (heavy, light, and split off) increases enormously the number of subbands and makes it more difficult to control their energy separation. Even if preliminary, these recent results on electroluminescence represent, in our opinion, the closest yet to the demonstration of a Sibased semiconductor laser. 1.4 Material Issues 1.4.1
Fundamental Parameters m* and ǻEc
In Sec. 1.1 and in particular in the paragraph where we describe our definition of quantum engineering, we insist on the minor dependence that the quantum cascade laser concept has on the material parameters of the heterostructure. Indeed, there are some physical parameters, related to the material system, that have a direct influence on the laser characteristics. At the first order, there are two parameters originating from the heterostructure that have to be taken into account: the conduction band discontinuity ǻEc and the effective mass of the well material m*. 1.4.2
Role of the effective mass m*
The role of m* is complex, but can be easily illustrated by analyzing the formula of the gain (Eq. 1.24). We take the expression of the gain coefficient g and compare its value for two material systems: GaAs and InAs. Moreover, to reduce the influence of the active region design and have a fair comparison of the two materials, we apply this formula to the first two states (E1 and E2) of a quantum well with very high barriers (Fig. 1.11). In the limit of Ĳ2 5 × 1018 cm–3 ), almost metallic, GaAs substrates. High confinement is achieved, but at the expense of high optical losses (ĮW = 50 – 80 cm–1) resulting from penetration into the doped GaAs cladding layer [143]. This solution was then soon discarded; in contrast, as we will see in Sec. 2.4, doublemetal waveguides have now become a mature technology, yielding terahertz QC lasers with excellent performance [94]. Since a major source of optical losses is caused by absorption in the claddings, solutions based on semiinsulating GaAs substrates represented an interesting alternative. To a good approximation, in fact, GaAs semiinsulating substrates can be assumed to be free of
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_66_03/23/2006 Terahertz Quantum Cascade Lasers 66
Chapter Two
Modal intensity (norm.)
0.008
0.006
Γ = 0.07
0.004
0.002
0.000
0
100
200
300
400
500
600
Distance (μm) Figure 2.13 Computed profile of a surfaceplasmon mode of wavelength Ȝ ~ 67 m bound to the interface between undoped GaAs and gold. The very long decay into the semiconductor renders the overlap with any active core of reasonable thickness very small; to highlight this, the 7% overlap with a 10mthick stack has been shaded.
terahertz absorption. The waveguide developed for the first terahertz QC lasers relied on this approach and exploited the presence of a thin, highly doped layer (also used as bottom electrical contact), which was grown directly underneath the lowdoped stack of active SLs [89]. Surface plasmons at the interfaces between the bottom contact layer and the active core on one side and the substrate on the other exist if the dielectric constant ɽ of the contact layer is negative. This can indeed be achieved by adjusting the doping concentration; in the case of GaAs and of the 67m wavelength for the SL active region just described, ɽ turns negative at a doping concentration of ~2.3 × 1017 cm–3. The dielectric constant can then be further tailored to control the decay of the optical mode perpendicular to the interface and to find the appropriate compromise between confinement factor and waveguide losses. In essence, since the thickness of the inserted layer is on the order of the surfaceplasmon skin depth, the two surfaceplasmon modes existing at its interfaces merge into a single mode that is bound to the central layer. The penetration in the surrounding semiconductor is minimized, and a tight confinement with low optical losses is achieved. The actual mode profile of the complete waveguide is shown in Fig. 2.14, where the presence of a highly doped GaAs layer necessary for the top contact and of the final gold layer was included in the calculation. The waveguide employs a doping concentration of 2 × 1018 cm–3 in the central guiding layer, giving a confinement factor ī = 0.47 and losses Įw = 13 cm–1, respectively. Using centrallayerguided (CLG) waveguide concept and a chirped SL active region, the first QC laser at terahertz frequencies was Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_67_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
67
0.06
Mode intensity (norm.)
Bottom contact layer
Gold layer
0.05 0.04 0.03
Γ = 0.47 α = 13 cm1
0.02 0.01 0.00 0
10
20
30
40
Distance (μm) Calculated mode profile along the growth direction of the first terahertz laser structure [89]. The origin of the abscissa is at the top metalsemiconductor interface, and the shaded area indicates the waveguide active core.
Figure 2.14
demonstrated [89]. The sample was grown by MBE on a semiinsulating GaAs substrate, starting with the 800nmthick ndoped (2 × 1018 cm–3) GaAs layer, followed by 104 repetitions of the superlattice (thicknesses are given in the caption of Fig. 2.8) and terminated by a 200nmthick ndoped (5 × 1018 cm–3 ) GaAs layer to facilitate electrical contacting. Ridgegeometry mesas were defined by optical contact lithography and wetchemical etching to a depth exposing the bottom contact layer. Evaporation of GeAu (65 nm) and Au (200 nm) and rapid thermal annealing provided ohmic contacts on top and at the sides of the ridges. FabryPerot cavities were formed by cleaving, and devices were soldered onto a copper block, using an InAg alloy and wirebonded. Figure 2.15 shows the emission of one laser for different drive currents at 8 K heat sink temperature. The characteristic narrowing of the emission spectrum and the nonlinear dependence of the intensity on drive current are clearly observed up to a current of about 880 mA, where the laser threshold is reached. Lasing takes place at ~4.4 THz, on the highenergy side of the luminescence line, probably owing to the reduced waveguide losses at shorter wavelengths. Singlemode emission is obtained, most likely a consequence of the relatively narrow gain spectrum and the wide FabryPerot mode spacing. The spontaneous emission at low drive currents (300 mA) displays a full width at halfmaximum of 2 meV, similar to the value obtained from luminescence structures with only 40 periods (see Fig. 2.11). These latter spectra are best fitted with a lorentzian line shape which, together with the absence of any broadening when increasing the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_68_03/23/2006 Terahertz Quantum Cascade Lasers 68
Chapter Two
Energy (meV) 15
16
17
18
19
20
21
22
Intensity (arb. units)
1.24 A 0.85 A 0.75 A 0.70 A 0.60 A 0.45 A 0.30 A
x2 x4
120
130
140
150
160
170
180
1
Wave number (cm ) Figure 2.15 Emission spectra from a terahertz laser device for different drive currents,
recorded at 8 K by applying 200nslong pulses at intervals of 2 s [89]. The lowest curves have been multiplied by factors of 4 and 2, respectively, for clarity. The 1240mA laser spectrum was scaled down by several orders of magnitude. The full width at half maximum decreases from 2 meV at 450mA drive current to 0.5 meV at 850 mA, as the threshold current of 880 mA is approached. Subthreshold spectra were collected with a resolution of 2 cm–1 (60 GHz), while the 1240mA spectrum was obtained with the maximum 0.125cm–1 (3.75GHz) resolution of the apparatus.
number of SL periods, indicates the high quality and uniformity of the growth throughout the whole 10mthick activematerial stack. Figure 2.16 shows the LI and VI characteristics of the device. At a heat sink temperature of 8 K, the output peak power was estimated to be more than 2 mW, with a threshold current density of 290 A/cm2 [89]. The latter was already a very small value for QC lasers, and it allowed operation of these first devices at duty cycles up to 10%. The threshold current increases with temperature up to the maximum operating temperature of 50 K. Currentvoltage characteristics are similar to those observed in the luminescence structure. The electric field at threshold is 7.5 kV/cm. This is larger than the design value of 3.5 kV/cm, probably as a result of the nonnegligible spreading resistance in the bottom contact layer.
2.4 Progress in Performance 2.4.1 Optimized fabrication and continuouswave operation
Soon after the first demonstration [89], another terahertz QC laser was developed with analogous characteristics but a different choice of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_69_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
69
Current density (A/cm2)
2.0 Voltage (V)
1.5 1.0 0.5
Peak output power (mW)
2.5
0.0 Current (A) Figure 2.16 Lightcurrent characteristics of a 180mwide and 3.1mmlong laser ridge
[89]. Data were recorded in pulse mode, applying 100nslong pulses at a repetition rate of 333 Hz. The peak power values represent what is collected from a single facet onto the detector. At the lowest temperature the device emits more than 2 mW. By increasing the duty cycle to 0.5%, the peak power reduces to 1 mW due to the stronger heating, as is shown by the dashed curve labeled with an asterisk. At the maximum operating temperature of 50 K we observe still 120 W of peak output power. The VI curve at a temperature of 8 K is also displayed.
the waveguide parameters, optimized for the lowest losses rather than for the confinement factor [144]. Even lower thresholds were obtained (< 200 A/cm2), but high reflection coatings had to be provided to the laser back facet owing to the smaller gain. These are, in general, easy to realize through deposition of thin insulation and Au metallization; however, they require care as they tend to peel off after thermal cycling. In any case, despite the excellent current densities, also these devices could be operated only in pulsed mode. To reduce the detrimental joule heating of the laser and allow for continuouswave operation, several main avenues were immediately pursued in improving the fabrication processes. First, a most relevant aspect is the distance of the lateral side contacts from the laser ridge [145]. As the bottom highly doped layer is relatively thin, it is also quite resistive, and it is therefore important to have the lateral contacts as close as possible to the active region, so as to minimize the applied voltage. On the other hand, the distance should still be sufficient to prevent a coupling of the optical mode to the contact metal, which would increase the waveguide losses. The best compromise for 4.4THz lasers was found in a few tens of micrometers. Second, the top metallization on the laser ridge was modified so that the annealed ohmic contact was restricted only to two narrow stripes (10 – 15 m wide) at the edges of the ridge [146]. This reduces the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_70_03/23/2006 Terahertz Quantum Cascade Lasers 70
Chapter Two
absorption losses, which are believed to be higher in the annealed material; the interface quality is in fact quite relevant as the optical mode peaks precisely there. Another evaporation step of Cr/Au or Ti/ Au was then used to cover the remaining portion of the laser and complete the waveguide. A schematic view of a processed laser is shown in Fig. 2.17. This type of device fabrication is presently the standard one commonly employed for terahertz QC lasers with CLG waveguides. These changes in fabrication enabled continuouswave operation of terahertz QC lasers, initially with relatively low emitted powers of a few hundred microwatts up to almost 40 K [146]. In parallel, cw operation was also obtained by mainly reducing the device size through narrowing of the ridges, which could then be contacted using extended metallic regions and polymide insulation to avoid shorting [145]. Soon afterward optimized devices were fabricated yielding similar cw and pulsed performance and output powers of various milliwatts [91]. The measured powers of a typical uncoated laser device and of a laser with a backfacet coating are reported in Fig. 2.18 as a function of cw drive current. For the uncoated device, almost 2.5 mW was obtained at low temperatures, with still more than 500 W at 40 K. Lasing ceased at around a 45 K heat sink temperature. These values translate to 7.5 and 1.5 mW, respectively, of total emitted power per facet, using the mimimum 0.33 collection efficiency estimated for the setup. At 10 K, a low threshold current density of 210 A/cm2 was recorded. In the linear regime from threshold to 1 A, the slope efficiency, again corrected with the factor of 0.33, is 17 mW/A. This can be compared with the expected value ĮM P hȞ 1 Ĳ = Np I Į M + ĮW q0 2
(2.3)
where P is the optical power; I the injection current; ĮM and ĮW the outcoupling and waveguide loss, respectively; hȞ the photon energy; Np = 104 the number of periods; and q0 the electronic charge. The factor of 1/2 stems from the fact that only one facet is considered. The
Cr/Au GeAu/Au n+ GaAs SI GaAs Figure 2.17
Schematic view of a processed and cleaved laser bar from the front facet.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_71_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
71
Current (A)
Output power (mW)
Without coated back facet With coated back facet
Current density (A/cm2) Figure 2.18 Lightcurrent characteristics of a 1.96mmlong and 150mwide chirped SL
laser, recorded in cw operation at different heat sink temperatures, are plotted with solid lines [91]. The power values represent what was collected from one facet onto a calibrated pyroelectric detector after correction for the transmittance of the polyethylene window (0.63). The collection efficiency was estimated to be 0.33. The device stopped operating in cw mode at a heat sink temperature of 45 K. Dashed lines represent data collected from a 2.23mmlong device with a coated back facet. Output powers are in this case more than 4 mW at 10 K and still 1.6 mW at 40 K. The maximum operating temperature increased only slightly to about 48 K. Due to the slightly different device size, the scale of the current refers only to the dashed lines.
dimensionless constant Ĳ takes into account the fact that in QC lasers the lowerstate population differs significantly from zero and that the injection efficiency Și of carriers into the upper laser state can deviate from unity. In a rate equation framework, Ĳ can be derived as [147–149] Ĳ = 1í
Ĳ1 1 Ĳ1 Ĳ2 í1 í Ĳ2 Și Ĳ21 Ĳ + Ĳ (1 í Ĳ / Ĳ ) 1 2 1 21
(
)
(2.4)
where Ĳ2 and Ĳ1 are the total lifetimes of the upper and lower laser levels, respectively, and Ĳ21 denotes the scattering time of electrons from level 2 to level 1. The presence of a considerable population in the lower laser level at threshold [137], indicated by the ratio of lifetimes Ĳ1/Ĳ21, is the main reason for the reduction of the slope efficiency from its ideal value. Inserting lifetimes calculated by using Monte Carlo simulations [137, 150], a slope efficiency of 55 mW/A can be computed, assuming unity injection efficiency. The difference with the experimental value of 17 mW/A may be due to heating effects, uncertainties in the measurements, other scattering mechanisms not included in the simulations, and a nonunity injection efficiency. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_72_03/23/2006 Terahertz Quantum Cascade Lasers 72
Chapter Two
Substantial improvements in threshold current density, output powers, and slope efficiency were obtained from a laser with its back facet covered with the highreflection coating. Data recorded from this device are represented by the dashed lines in Fig. 2.18. A reduction of the threshold current density by about 10% (to 185 A/cm2) is achieved, and simultaneously the estimated maximum output power increases to more than 4 mW [91]. In pulsed mode, the best devices showed threshold current densities as low as 130 A/cm2 at 10 K and a highest operating temperature of 75 K [151]. Figure 2.19 shows the voltage and the differential resistance across the device as a function of the cw injected current. The VI characteristics follow the wellknown behavior of high resistance at low currents, and a turnon toward lower differential resistance when minibands align. The measured threshold voltage differs from the design value of 3.8 V by 0.3 V, which is attributed to residual series resistance in the bottom contact layer and electrical contacts. The differential resistance is displayed as well, showing the characteristic drop at threshold when the onset of stimulated emission reduces the lifetime Ĳ2. Its clear visibility is in general a good indication of a high injection efficiency [147]. 2.4.2
New designs and waveguides
The desire to improve the thermal behavior of terahertz QC lasers and the need of extending the operating frequency range toward even lower
Voltage (V)
Differential resistance (Ω)
Current (A)
2 Current density (A/cm )
Figure 2.19 Voltagecurrent characteristics of the laser of Fig. 2.18, recorded in cw operation at a heat sink temperature of 7 K [91]. The derivative is also shown. The sharp drop in differential resistance at threshold is caused by the reduction of the upperstate lifetime by stimulated emission.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_73_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
73
Energy (eV)
frequencies immediately fostered innovative ideas in the quantum design of the active region. Following a development path similar to that of the midinfrared case, the improvement on the original chirped superlattice was the implementation of boundtocontinuum (BTC) transitions [152]. The band diagram of an exemplary structure is displayed in Fig. 2.20. In essence, the SL concept is reinterpreted by making use of a spatially diagonal transition to reduce the nonradiative loss of carriers from the upper laser level and improve the injection efficiency. The name stems from the fact that, contrary to the minibandlike lower state, the upper laser level is mostly localized in a “defect” well of the SL periodic potential. As such, one can speak of donorlike and acceptorlike states, according to their being closer in energy to the upper or lower miniband. For a given transition frequency, the former type provides larger oscillator strengths, owing to the wave function symmetry; on the other hand, the latter simplifies the design of the injection, since the upper miniband can be well separated in energy. The first implementation of the boundtocontinuum scheme in the terahertz range already yielded devices operating above liquid nitrogen temperature [92]; yet, as we will see, the concept enjoyed the greatest success in the realization of lasers with high output power and low emission frequencies. The above approach tries to address the issue of the upperstate lifetime, but obviously reducing the lifetime of the lower lasing level is also very important to establish and maintain a significant population
Active region
Injector
Distance (nm) Figure 2.20 Selfconsistent calculation of a portion of the conduction band structure of a
2.8THz boundtocontinuum laser under an applied bias of 2.9 kV/cm [153]. The layer sequence, starting from the injection barrier to the left of the active region, is (in nanometers) 3.9/9.6/0.9/12.4/0.9/13.4/1.1/11.7/1.8/11.2/2.3/10.7/2.6/10.9/3.0/9.3, where Al0.15 Ga0.85 As barriers are in boldface and the first 9 nm of the 10.9nmwide GaAs well is silicon doped at 5 × 1016 cm–3.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_74_03/23/2006 Terahertz Quantum Cascade Lasers 74
Chapter Two
inversion. In the BTC design as well as in the previously described chirped SL laser, extraction of carriers from the lower level mainly occurs through electronelectronactivated scattering into states of the injector miniband. Efficient depletion of the lower state in these terahertz QC lasers is hindered by the insufficient cooling of the electron distribution, and its effective lifetime, defined as in the inverse of the net scattering rate out, is strongly influenced by the electronic temperature due to the small dispersion of the injector miniband. In midinfrared QC lasers, on the contrary, population inversion up to room temperature and above is maintained by exploiting resonant fast electronphonon scattering as the extraction process. The idea, however, cannot be transferred in a straightforward manner to the terahertz range. In fact the small transition energy means that any process that is energetically resonant for electrons in the lower lasing subband is “almost” resonant also for those in the upper subband. Therefore, using emission of optical phonons as the depletion mechanism would seriously compromise the transition lifetime. To circumvent this difficulty, one possibility is to spatially separate the region where LO phonon emission takes place from the optical transition. This concept was already examined in Ref. 137, and the simulation predicted that a much larger population inversion than that attainable in superlattices was feasible. The first working structure was realized only a couple of years later using a simpler design targeting 3THz emission frequency [154]. The band diagram is reported in Fig. 2.21. A single large well contains two subbands (labeled 2 and 3) roughly divided by the energy of the LO phonon (36 meV in GaAs); the terahertz transition, on the other hand, is realized using tunnelsplit states in two coupled wells, so as to raise the energy of the lowest subband 4 enough to couple it with the upper subband 3 of the phonon stage. Just another well is then used to optimize injection. The first lasers based on this design already showed promising characteristics, with a low dependence on temperature of the threshold current [154]. A poor injection efficiency, however, compromised the overall performance. This issue was well addressed in subsequent designs—so much so that this approach holds the present records in terms of highest operating temperatures [94], as will be discussed in the following. Also in this case Monte Carlo simulations were employed to model the transport and gain characteristics, showing the importance of impurity scattering in accounting for large electronic temperatures [155, 156]. An alternative design based on optical phonon emission relies on interlacing photon and phonon emitting stages bridged by appropriate minibands [157]. Figure 2.22 shows a portion of the conduction band structure of an 80m wavelength device under an applied bias of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_75_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
75
E
= 13.9 meV 54 z = 6.4 nm 54
2′
5 4 3 2
1′ 39.3 meV
1 Conduction band profile of the structure based on phonon depopulation of Ref. 154 calculated by using a selfconsistent Schrödinger and Poisson solver at 64 mV/ module, which corresponds to a field of 12.2 kV/cm. The fourwell module is outlined. Beginning with the left injection barrier, the layer thicknesses in angstroms are 54/78/24/64/38/148/24/94. The 148Å well is doped at n = 1.9 × 1016 cm3, yielding a sheet density of 2.8 × 1010 cm2. (Reprinted with permission from [154]. Copyright © 2003, American Institute of Physics.)
Figure 2.21
5.4 kV/cm. While the minibands, labeled A and B in Fig. 2.22, ensure good control of the transport characteristics and allow for a wide range of currents and voltages, the LO phonon stage efficiently shortens the Current density (A/cm)
A B
5
1
LO phonon
Wave number (cm )
Injection barrier
3
(a)
4
5
Peak power (mW)
10
0
(b)
Figure 2.22 (a) Portion of the conduction band structure of the interlaced cascade design
under an average electric field of 5.4 kV/cm. The optical transition is between the two states drawn in boldface and has a dipole moment of 7.2 nm. The layer thicknesses can be found in Ref. 157. The phonon emission is indicated by the dashed arrow. Minibands A and B are connecting the phonon to the photon and the photon to the phonon stage, respectively. (b) Lightcurrent characteristics of a 4.72mmlong and 150mwide device, recorded in pulsed operation at a duty cycle of 3.5 %. The maximum output power of 10 mW is reached at 30 K, and still 4 mW is obtained at 80 K. The device stops operating at 95 K. Note the very weak temperature dependence of the slope efficiency.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_76_03/23/2006 Terahertz Quantum Cascade Lasers 76
Chapter Two
effective lifetime Ĳ1 of the lower lasing state. Extraction of carriers from this level still occurs through ee scattering into the states comprising miniband B; but the lower states of the miniband are strongly coupled to the phonon stage, and therefore rapid extraction from these states is provided by electronphonon scattering. The expectation of a short lifetime Ĳ1 and negligible thermal backfilling is indeed confirmed in this structure, as is best seen from the LI characteristics in Fig. 2.22. The slope efficiency, i.e., the derivative of the output power versus injection current, is virtually independent of temperature, which indicates a constant Ĳ1. In fact, lasing at temperatures higher than the currently achieved 95 K appears to be limited solely by the maximum current density that can be passed through the device. The residual threshold dependence on temperature seems, then, to be mainly determined by the nonradiative relaxation of upperstate electrons. Comparisons of this interlaced approach with the previous direct phonon extraction scheme, in samples with similar waveguide and growth conditions, showed analogous temperature dependence but possibly better absolute thresholds. Beyond these first preliminary results, however, no further implementations have yet been reported. On the waveguide front, recent developments have seen the emergence of doublemetal waveguides [93]. As can be seen in Fig. 2.23, they offer the clear advantage of providing unity confinement Ƚ. A price is paid on the absorption losses, of which, however, only a fraction of about onethird is due to the metallic claddings. In the end, the ratio ī/Įw is very similar to that of CLG waveguides; however, the high confinement factor and hence modal gain is beneficial as the total losses to be compensated also include the mirror outcoupling Įm. Furthermore, the optical mode is strongly squeezed in a core definitely smaller than the wavelength; no cutoff frequency in fact exists for TM modes in this type of configuration. This translates into a large “impedance mismatch” with vacuum at the ridge facets, considerably increasing their reflectance. While this property is clearly useful in minimizing Įm even without highreflection coatings, it also poses problems in extracting high output powers. Finally, as the mode is deeply linked to the two metallic interfaces, the ridge width can be considerably shrunk, yielding very small devices with low drive currents and excellent cw performance. All these characteristics are naturally even more helpful with longer emission wavelengths, and, in fact, QC lasers at 2.1 THz have been realized thanks to this approach [97]. The fabrication of the first doublemetal lasers used an InAu wafer bonding technique [93]. An Al0.5Ga0.5 As layer grown before the waveguide core was employed as etch stop in the substrate removal. An important aspect was the use of a thin, lowtemperaturegrown GaAs cap layer to avoid annealing of the ohmic contacts, which have to be deposited after the bonding Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_77_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
13
9
Active region
Semi−insulating GaAs substrate 8 13
(b) Mode Intensity (arb. units)
11 10
n+ contact layer Au
12 Re {ε}
Al0.5Ga0.5As layer
αw = 2.7 cm1 Γ = 0.127
12 αw = 17.8 cm
11
1
Γ = 0.98 Au
Active region 0
10
Re {ε}
Mode Intensity (arb. units)
(a)
77
10 9
Au 20 30 Distance (μm)
40
50
60
Figure 2.23 Mode intensity (solid lines) and real part of the dielectric constant (dashed lines) for (a) the SI surfaceplasmon waveguide and (b) the doublesided metal waveguide of Ref. 93. The dotted lines represent the square of the modal effective index. (Reprinted with permission from [93]. Copyright © 2003, American Institute of Physics.)
procedure. Since then, the technique has been successively refined, in particular concerning the structural quality of the bonding interface which is relevant for the device thermal resistance. At the same time, the standard CLG waveguide has undergone some interesting makeover. The highly doped layer buried under the core can be substituted by more layers with various doping densities [158]. This solution allows the possibility of controlling separately the boundary conditions of the surface plasmons on the two sides, thereby resulting in a better compromise between optical losses and confinement factor. In the case of a 2.5THz laser, a confinement factor of about 48% is reached, with 10cm–1 absorption losses. These values easily permit the use of such waveguides even at long wavelengths, providing very low threshold currents and high output powers [98]. 2.4.3 Hightemperature and longwavelength operation
The first terahertz QC laser to operate above liquid nitrogen, at temperatures up to 95 K, was the BTC device demonstrated by Scalari et Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_78_03/23/2006 Terahertz Quantum Cascade Lasers 78
Chapter Two
al. [92]. The luminescence intensity recorded from that structure indicated that the temperature dependence of the threshold current could be ascribed to the nonradiative relaxation of electrons in the upper level. Basically, through collisions, electrons can gain sufficient inplane kinetic energy to be able to relax via emission of LO phonons to the lower subbands. This process is indeed very difficult to suppress by quantum design. The only solution is to make the optical transition more and more diagonal in space, to reduce the overlap of the states. This can be accomplished only at the expense of losing dipole matrix element for the optical transition, and up to now, very diagonal structures have not shown lasing in the terahertz range. Research has then focused on optimizing the injection by carefully tailoring the thickness of tunnel barriers and the doping concentration. It was in fact shown that the injection process also plays a fundamental role in degrading performance with increasing temperature [150]. This allowed reduction of parasitic conduction paths and improved the dynamic current range, but brought only marginal improvements in the maximum temperature, which was raised to about 100 K in pulsed and 70 K in cw operation [159]. On the other hand, as can be seen in Fig. 2.24, the output powers achieved are indeed quite spectacular, with slope efficiencies of 170 mW/A (once corrected for collection) and threshold currents as low as 100 A/cm2. Very recently cw operation at liquid nitrogen temperature has been demonstrated at 2.9 THz using a buried waveguide for better heat dissipation [160]. Designs based on optical phonon emission for the depopulation of the lowest lasing subband have immediately shown good potential for hightemperature operation. Not only do they provide faster extraction of carriers from the active region, but also they possess a large energy separation of the optical transition from the ground state of each cascade period [154]. The latter is an important characteristic as it suppresses thermal backfilling from electrons in the injectors downstream. As previously explained for the interlaced design [157], the insensitivity of the output slope efficiency to temperature observed in these devices demonstrates that the lifetime of the lower lasing state is relatively unaffected by the increasing temperature. Furthermore, once fit with the usual empirical formula J th = J1 + J0 exp
T T0
(2.5)
the threshold current densities showed a characteristic temperature T0 > 30 K, larger than superlattice or BTC structures, in both the interlaced and the coupledwell devices [94, 157]. Despite these useful characteristics, the maximum operating temperature was still hovering Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_79_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
79
Current density (A/cm2) 0
100
200
300
400
500
600
250
700
70
(a)
60 210
40 K
190
64 K
50 40 30
170
3
4
5 6 1/L (cm1)
74 K
7
20
4
10 K
3 2
0.02
10 K
10
98 K
0 50
30 K 40 K
0.01
40 30
1 0 0
84 K
(b)
0.03
5
S dR (Ω⋅cm2)
Applied bias (V)
λ = 87 μm
53 K
0 100 200 300 400 500 600
20
J (A/cm2) 60 K
λ = 87 μm
10
68 K
0
0.5
1.0
Peak power (mW)
10 K
10 K
1.5
2.0
Optical power (mW)
J (A/cm2)
230
0 2.5
Current (A) Figure 2.24 (a) Peak optical output power versus injected current in pulsed mode at a
duty cycle of 2% at various temperatures, as measured from the 3.4THz laser of Ref. 159. The sample was processed into a 1.6mmlong and 210mwide waveguide with back facet coating. The inset shows pulsed threshold current as a function of inverse laser length with back facet coating measured at 10 K. (b) CW optical power from a single facet of the same device as a function of drive current for various heat sink temperatures. Inset: Bias voltage as a function of injection current and differential resistance deduced from the VI curve for two samples with different injection barriers. (Reprinted with permission from [159]. Copyright © 2004, American Institute of Physics.)
around 90 K, owing to the poor lowtemperature thresholds [161]. Current injection was then improved by thickening the injection barrier and changing the spatial profile of the wave functions; doublemetal waveguides were also implemented to exploit the larger confinement factor. As can be seen in Fig. 2.25, these advancements allowed the threshold current densities to be reduced to about 600 A/cm2, resulting in maximum pulsed operating temperatures of about 140 K [94]. The
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_80_03/23/2006 Terahertz Quantum Cascade Lasers 80
Chapter Two
introduction of further refinements in the injector design and a better control of the waferbonding technology of metallic waveguides enabled phononcoupled terahertz QC lasers to reach a high performance level also in cw. Figure 2.26 displays cw LI traces from Ref. 96. The lasers operated up to 93 K, with output powers in the milliwatt range. The ultimate goal is represented by the possibility of reaching laser operation at room temperature, or at least on thermoelectrically cooled stages. It should be said that highvalue applications, such as security scanners in airports or medical imaging systems in hospitals, could live with cryogenic temperatures, provided the practical system is reliable and sufficiently turnkey. In any case it can be expected that further advances in quantum design and waveguide technology will lead to optimized structures capable of lasing at higher temperatures. To really tackle room temperature, however, some breakthrough is needed. This could come from new materials (nitrides, for instance, are being Current (A) 1 1.5
0.5
60 60 K
12 10 8
40 K
40
81 K 5K
6 4
102 K 113 K
100 K
2 0
Jth=J0+J1eT/T0
T0 = 33 K
50 100 T (K)
250
0 2
1300 1000 700
0
20
123 K 131 K
140 K
Jth (A/cm2)
Bias (V)
14
0
2
500 150
500 750 1000 1250 Current density (A/cm2)
121 K 127 K 137 K
1500
1
Peak optical power (arb. units)
18 16
0
0
Figure 2.25 Emitted light and bias versus current at various temperatures for the metalmetal 3.8THz devices of Ref. 94. They were measured using 200ns pulses repeated at 1 kHz. The LI characteristics in the upper panel are measured from a 60mwide, 2.48mmlong ridge. The VI characteristics are measured using a smaller structure 100 m wide, and 1.45 mm long. The lower panel displays LI characteristics from a 150mwide, 2.74mmlong ridge, along with its threshold current density versus temperature in the inset. Note that the current axis is only applicable to the 60mwide device. (Reprinted with permission from [94]. Copyright © 2003, American Institute of Physics.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_81_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
81
Current density (A/cm2)
91.5 K
300
400
500
600
700
Heatsink temperature
1.8 10 K 1.6 1.4 41 K 1.2 56 K 1 0.8 70 K 0.6 77 K 0.4 87 K 0.2 93 K 0
3.19 THz (94.0 μm)
102 103 104 2.9 3 3.1 3.2 3.3 3.4 3.5 Frequency (THz)
12 5K
40
Bias (V)
9 78 K
30
6 20
78 K 3
5K
10
0
Optical power (mW)
101
200
Differential resistance (Ω)
100
Intensity (arb. unts)
0
0 0
0.05
0.1
0.15
0.2
0.25
0.3
0.35
0.4
Current (A) Continuouswave characteristics measured from a 40mwide, 1.35mmlong ridge laser of Ref. 96. The upper panel shows the LI characteristics for various heat sink temperatures. The inset shows the cw spectrum at a heat sink temperature of 91.5 K. The linewidth is limited by the spectrometer resolution of 0.125 cm–1. The lower panel shows the cw VI and dV/dI–I characteristics at heat sink temperatures of 5 and 78 K. (Reprinted with permission from [96]. Copyright © 2004, American Institute of Physics.) Figure 2.26
proposed) with larger LO phonon energies, or from nanostructured devices (such as quantum dots) where the electronic motion is confined in all directions and the subband dispersion is broken into individual levels. In all instances these approaches aim at reducing the main source of nonradiative relaxation from the upper lasing state linked to LO phonon emission. They are, however, quite challenging from the point of view of present technical knowledge. Several applications, particularly in astronomy and chemical recognition, involve detection at frequencies in the range of 1.5 to 2.5 THz. A chirped superlattice design similar to the one described in Sec. 2.3 led to lasing at 3.5 THz with comparable performance [162]. Moving toward longer wavelengths, however, the BTC concept appeared to be more favorable and formed the basis of lasers emitting at 3.5 THz [92] and then 2.8 THz [153]. Optimized designs were then developed for 2.9 THz [95] and 2.4 THz [159] with impressive output powers of tens of milliwatts and low threshold currents also in cw; see Fig. 2.27 for Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_82_03/23/2006 Terahertz Quantum Cascade Lasers 82
Chapter Two
exemplary LI curves. More recently, BTC lasers have begun to be realized at the desired emission frequencies required for specific sensing applications. In particular we show in Fig. 2.28 the spectra of two lasers emitting around 4.8 and 2.55 THz, important for the detection of atomic oxygen and of the OH radical, respectively [98]. The latter shows a record low threshold current density of about 75 A/cm2 with a high cw output power of 6 mW per facet (33% collection efficiency) and a maximum cw operating temperature of 56 K. All these devices were based on the CLG waveguide concept that was employed in the first 4.4THz laser. It is clear, though, that as the wavelength increases (2 THz corresponds to 150 m), it becomes progressively more difficult to maintain a large confinement factor without resorting to impractically thick active regions. As already explained, an improvement certainly comes from using multiple highly doped layers, as was done in the case of the 2.5THz structure. In this direction, however, doublemetal waveguides seem to have the advantage, as they can display ī close to unity independently of wavelength and thickness. Indeed, they have recently allowed the lowest emission frequency of 2.1 THz to be reached by phononcoupled devices [97]. Current (A) 0.0
0.6
1.2
Frequency (THz) 2.8 2.9 3.0
Intensity (arb. units)
Power (mW)
10 K
1 210 A/cm2 not purged
15
10
5
1.8
30 K
15
40 K 0 1 210 A/cm2 purged
50 K 10
0 1 100 A/cm2 purged
60 K 5
0
65 K
92 94 96 98 100 102 Frequency (cm1)
70 K 69 K x 20 0
0 0
100
200
300
Current density (A/cm2) Figure 2.27 Emitted power as a function of current density for the 2.9THz device of Ref. 95 operated cw. The ripples are due to atmospheric water absorption. Inset: Spectra at different current densities. To highlight the effect of water absorption, the top panel was measured with the optical path unpurged. (Reprinted with permission from [95]. Copyright © 2004, American Institute of Physics.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_83_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
2.55
80
85
Frequency (THz) 2.70 4.50 4.80
5.10
Intensity
2.40
83
90 150 160 Wave number (cm1)
170
Figure 2.28 FabryPerot emission spectra of BTC quantum cascade lasers operating near 2.55 and 4.8 THz.
As discussed in Sec. 2.5, lasing at 1.9 THz has also been reported in high magnetic fields using singlewell structures [163]. Beyond waveguiding, the major issue related to further extending the operation wavelength concerns the injection efficiency. When the transition energy is only a few millielectronvolts, tunnel injection has to be very selective, posing stringent conditions on the injector miniband width and coupling. The net result is usually a poorer conductance or small useful voltage range. This decreases the maximum current densities available to pump the active region. More and more diagonal transitions could possibly alleviate this problem, but how far down in frequency QC lasers will be able to go is still an open question.
2.5 New Research Directions and Outlook 2.5.1
Singlemode devices
The lasers described in the previous sections employed a multimode FabryPerot cavity; therefore, singlemode operation is observed only occasionally with very short resonators and over a limited range of injection currents [91, 162]. Stable singlemode emission at a precisely designed frequency is, however, highly desirable for most applications. For this purpose, the concept of distributed feedback (DFB) has been successfully implemented also in terahertz QC devices [164]. The peculiar surfaceplasmon structure of the waveguide required the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_84_03/23/2006 Terahertz Quantum Cascade Lasers 84
Chapter Two
realization of rather unconventional DFB gratings for the diffraction of light propagating along the laser ridge. In the first devices a periodic corrugation was etched into the thin, highly doped semiconductor contact layer underneath the top metallization. This causes a modulation of the real part of the modal refractive index; lasers featuring such grating still displayed a regularly spaced FabryPerot spectrum, but with two modes strongly suppressed, as can be seen by the dashed curves in Fig. 2.29. This is a typical feature of indexcoupled DFB lasers with only moderate coupling strength but strong reflectivity at the FabryPerot facets. To enhance the coupling constant and increase mode discrimination, an additional loss modulation was introduced by depositing and annealing GeAu/Au contacts [91] selectively on the crests of the etched grating. By comparing devices with an annealed contact across the entire ridge [89] and devices where only two narrow ridges have been contacted [91], this further processing step is estimated to introduce a difference in waveguide losses of ~8 cm–1. Thus, complexcoupled DFB resonators, which are much more effective in achieving singlemode operation than bare indexcoupled devices, are obtained with an estimated coupling constant of 4 cm–1. Devices were accordingly fabricated with grating periods ȁ of 9.2 and 9.4 m on a sample nominally identical to that of Ref. 91. No other changes were introduced in the fabrication process. Figure 2.29 shows the spectra (solid lines) of two such devices (length = 3.2 mm and ȁ = 9.2 m in one device and length = 4.4 mm with ȁ = 9.4 m in the other). Lasing takes place within the previously observed stopband, as expected for a complexcoupled DFB laser. The shift of the emission wavelength corresponds precisely to the change of grating period, and an effective refractive index of 3.68 can be extracted, in good agreement with the calculated value of 3.73. The coupling is now sufficiently strong to achieve singlemode operation under all injection currents and operating temperatures. The tuning of the emission wavelength with temperature and current is below the resolution of the experimental apparatus. However, a tuning coefficient of 4 MHz/mA and an instantaneous linewidth of 30 kHz were recently measured for 4.66 and 3.69THz FabryPerot lasers [165]. While we can expect a similar tuning coefficient for our device, the emission linewidth of a DFB laser is typically well below that of a FabryPerot structure. The technique just described produces gratings with rather limited coupling coefficients, thereby making long laser cavities necessary for the achievement of singlemode operation. This affects the device performance, increasing the driving currents and hindering lasing in continuouswave mode. The issue becomes more and more relevant with increasing emission wavelengths as the DFB grating period has to be proportionally enlarged. An elegant way of realizing a Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_85_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
85
Intensity (norm.)
Frequency (THz)
Wave number (cm1) Figure 2.29 Spectra of five different DFB lasers with grating periods of 9.4, 9.2, and
8.6 m, respectively, collected at an injection current close to the maximum output power [164]. In the upper two panels, the dashed lines correspond to spectra recorded from devices in which the distributed feedback was implemented only by removing 150 nm of the top contact layer. The appearance of a stopband in the original FabryPerot spectrum indicates a predominant indexmodulation. The solid lines are spectra recorded from devices in which an additional lossmodulation was introduced by an annealedcontact grating (see text). In this case, the stronger modulation leads to stable singlemode emission. In the bottom panel, the spectrum of a 150 nm etched device with no annealedcontact grating and ȁ = 8.6 m is shown.
onedimensional photonic crystal for surfaceplasmon modes has been recently demonstrated [166]. A slit opened in the metallic layer acts as a barrier for the wave propagation as no surface plasmon is supported there. Part of the light is reflected back, part is transmitted by tunneling across the slit, and part is scattered out of the interface mode. A periodic series of slits then acts as a photonic crystal structure, and if the slits are sufficiently thin (much narrower than the wavelength), this can be accomplished with minimal scattering losses. This idea was applied to the fabrication of DFB QC lasers emitting near 2.5 THz. Devices were processed from a sample featuring a BTC active region and the modified version of the CLG waveguide described in Sec.2.4. The procedure follows the one of Ref. 91 until the deposition of the last metallic layer. This is patterned by electronbeam lithography with a series of slits at the Ȝ/2 DFB period (see inset of Fig. 2.31). Electronbeam lithography, while not necessary for resolution reasons, is very useful to easily vary the grating period and test different slit widths. For the latter, the best compromise between grating strength and diffraction losses was found at approximately 2m width (close to 10% Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_86_03/23/2006 Terahertz Quantum Cascade Lasers 86
Chapter Two
Intensity (arb. units)
of the period length). Singlemode operation was obtained in pulsed and continuouswave, with a sidemode suppression ratio of at least 20 dB, as can be seen in the spectrum of Fig. 2.30. The position of the emission peak shifts with the grating period, in reasonable agreement with the computed modal refractive index of 3.65. It is interesting to notice that, contrary to the one depicted in Fig. 2.31, the first devices based on this concept featured a top metallization extending to the very edge of the ridge, in order to leave a larger area for bonding. However, they frequently showed emission from more than one transverse mode, as exemplified in the right inset of Fig. 2.30; a narrower metallization has been adopted to solve this issue. The procedure can be further simplified by avoiding the liftoff step. In this case the resist used in the electronbeam lithography fills the slits, with the final gold layer covering everything. While the operating principle is analogous, this approach simplifies the bonding and in general yields better performance, probably owing to decreased scattering losses. The output power of one such DFB laser, approximately 2 mm long, is plotted as a function of drive current in Fig. 2.31. The emission is single mode in the whole current and temperature ranges of operation, with about 8 mW measured at 10 K and a low threshold current density of about
1 Wave number (cm ) 1
Wave number (cm )
Wave number (cm1) Singlemode emission spectrum in logarithmic scale of a 2.5THz DFB laser with a 16.5m slit periodicity and narrow top metallization. It was collected in pulsed mode at 1% duty cycle and 0.92A drive current, close to the maximum output power. In the left inset we plot the spectra of three lasers with different DFB periods and wide metallization. The upper two were collected close to threshold, while the lowest one is at a higher current in order to better show the DFB mode, here somewhat detuned from the maximum gain (hence the presence also of FabryPerot modes). The right inset shows a spectrum at higher current of the 16.4m laser of the left inset. The appearance of a second transverse mode is evident. Figure 2.30
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_87_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
87
Power (mW)
Current density (A/cm2)
Current (A) Lightcurrent characteristics of a 2.5THz DFB QC laser. Solid lines refer to pulsed operation with 5% duty cycle and were collected from one facet with f/1 parabolic optics on a calibrated pyroelelectric detector; dashed lines were obtained by mounting a Winston cone in front of the laser and using a pyroelectric power meter (33% estimated collection efficiency). The inset shows a scanning electron microscope picture of a surfaceplasmon DFB grating.
Figure 2.31
100 A/cm2. The performance decreases in continuouswave mode with a slight increase in threshold and reduced maximum operating temperature (from 70 to 55 K). Note, however, that the difference in measured power might be ascribed in part to the different collection efficiencies of the two setups. 2.5.2 Terahertz lasers in high magnetic fields
When an intense magnetic field is applied perpendicular to the plane of a twodimensional electron gas in a semiconductor heterostructure, the electronic energy spectrum is completely modified. The free inplane motion of the electrons is now constricted into Landau orbits, breaking up the subband dispersion into discrete energy levels. The relevance of this effect to the operation of QC lasers stems from the possibility it offers to suppress LOphonon emission, known to be the dominant nonradiative relaxation mechanism. Owing to energy conservation and thanks to the small phonon dispersion, the lifetime of a midinfrared intersubband transition can be dramatically increased when the magnetic field intensity is such that no two states exist that are separated by the LOphonon energy or, vice versa, resonantly lowered when the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_88_03/23/2006 Terahertz Quantum Cascade Lasers 88
Chapter Two
latter condition is verified. The light output intensity of midinfrared QC lasers is then strongly modulated with varying magnetic field [167], reproducing the behavior expected from a zerodimensional intersubband quantum box laser [168]. The situation at terahertz frequencies, i.e., transition energies below the optical phonon resonance, is more complicated, because many scattering mechanisms, such as carriercarrier, impurities, and interface roughness, play a relevant role. Thus, the response to the application of a magnetic field may differ from structure to structure, depending on the design concept. It is true that, as in the midinfrared case, a general characteristic is the modulation of the transition upperstate lifetime. In terahertz QC lasers, however, nonradiative relaxation is enhanced when ǻE =
ല eB N m*
(2.6)
where ǻE is the unperturbed transition energy and N is an integer, i.e., when an excited Landau level of the lower subband comes into coincidence with the ground level of the upper subband. In this case resonant tunneling between Landau levels (mainly taking place through shortrange disorder) opens up an additional relaxation channel, reducing the population inversion. On the contrary, when the Landau level ladders are off resonance, scattering rates are minimized. This behavior was actually first demonstrated by measuring the intensity of spontaneous emission in electroluminescence experiments [84, 169], but later it was confirmed in the operation of terahertz lasers [170, 171]. Data from a chirped superlattice structure identical to that of Sec. 2.3 are plotted in Fig. 2.32. As expected, oscillations deriving from the above mechanism are seen in both the threshold current and the output power [170]. A reduction of the threshold current density by about a factor of 2 is observed at 4.3 T with respect to the zerofield value. Together with the corresponding decrease of current seen at constant bias voltage, this result is a strong indication of reduced scattering rate out of the upper lasing state. Note, however, that the maximum output power is always smaller than without the magnetic field, and actually displays a decreasing trend with increasing field. This originates from the positive magnetoresistance of the injector miniband where relaxation is progressively quenched due to the inplane quantization. In general, a similar lifetime modulation should hold also for the lowest lasing subband, when in or out of resonance with the Landau ladders of the injector states. In this case, though, the result on the lasing properties is opposite, since a lifetime reduction corresponds to Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_89_03/23/2006 Terahertz Quantum Cascade Lasers
Energy (meV)
Terahertz Quantum Cascade Lasers
7 6
(a)
20
5
4
3
89
2
10
1
IN (arb.units)
PMAX (arb.units)
Jth (A/cm2)
0 (b)
300
3.045 V < Vbias < 3.075 V
250 200
(c)
1.0
0.5 Vbias ~ 3.85 V 0.0 1.0
(d)
0.5 Vbias = 3.7 V 0.0 0
1
2
3 4 5 Magnetic field (T)
6
7
Figure 2.32 (a) Energy of the most relevant Landau levels for the laser of Ref. 170 plotted
as a function of magnetic field with respect to the lowest subband ground state. Dashed lines show the typical Landau level broadening. (b) Threshold current density as a function of magnetic field. (c) Maximum output power as a function of magnetic field. (d) Normalized current at the constant bias voltage of 3.7 V. This curve was obtained from the experimental data by subtracting the decaying background current.
a more efficient extraction and therefore to improved population inversion. This effect appears to be less important in superlattices, where depletion of the lowest subband is already efficient [170]. In contrast, it was clearly observable in a structure lasing between the third and second subbands of a singlequantumwell active region [172]. This design concept proved invaluable in studying the high field regime, in which the cyclotron energy is larger than the photon energy. For this purpose a device was engineered for a low emission frequency of 1.9 THz, corresponding to a magnetic field of only 4.7 T [163]. The structure exhibited lasing only in a magnetic field of at least 2.5 T, and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_90_03/23/2006 Terahertz Quantum Cascade Lasers 90
Chapter Two
various peculiar features were observed at higher fields. First, a strong reduction of waveguide losses was observed above 6 T, which is attributed to the reduction of free carrier absorption when the cyclotron energy becomes comparable to level broadening. Second, a strong reduction of output power was found at 9.3 T, where no more interLandaulevel resonances should be observed. At this field the photon energy is onehalf the cyclotron energy, and the feature is a clear signature of carriercarrier scattering events in which energy and momentum are conserved with one electron that scatters out of the upper lasing level to a lower Landau level of the second subband and a second electron that scatters up to a higher Landau level. This configuration in fact presents a maximum for the carriercarrier scattering probability [173]. Most importantly a progressive reduction of threshold current density was seen at even higher magnetic fields, with a strong temperature dependence from 4.2 to 20 K (see Fig. 2.33). Under these conditions, as is known to happen in the quantum Hall effect, electrons localize in the potential fluctuations due to the residual sample disorder. Extremely long intersubband lifetimes are then observed, since all scattering mechanisms are efficiently suppressed. A threshold current density as low as 1 A/cm2 was achieved, with a temperature activation compatible with a 1meV localization energy [163].
20 15
5
(A/cm2)
0
2
rrent density
10
Threshold cu
40 30
2 6
ag
M
4 8
tic
ne
12
10 ) (T ld
fie
0
10
40 30 ) e (K 20 r ratu e p Tem
50
60
70
Dependence of threshold current density on temperature and magnetic field for a 3.5mm, 320mwide device of Ref. 163. The change in lasing regime is evident above 6 T and below 20 K. (Reprinted with permission from [163]. Copyright © 2004 by the American Physical Society.)
Figure 2.33
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_91_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
2.5.3
91
Open challenges and future research
Since their initial demonstration terahertz QC lasers have made rapid and substantial progress. They have reached a level of performance such that the first terahertz applications employing QC laser sources are appearing in imaging [174, 175] and spectroscopy [176]. They already display output power levels ideal for most conceivable uses, except maybe longrange remote sensing, and their narrow linewidth and frequency stability make them an ideal candidate for local oscillators in heterodyne systems. As already mentioned in Sec. 2.5.2, however, room temperature operation and frequencies below 2 THz remain as the main challenges left before widespread device exploitation can take place. While the latter objective is within reach of current technology, hightemperature operation would require some breakthrough development. The latest magnetic field results clearly encourage the investigation of zerodimensional structures. A final aspect is the tunability of singlemode emission. Temperature (or current) tuning is presently limited to 3 to 4 GHz. This would be sufficient for highsensitivity spectroscopy, but poses very stringent requirements on the fabrication of devices targeting a specific frequency. Solutions allowing broadband tunability, such as external cavities, are being explored [98]. On the other hand, terahertz QC lasers, with their peculiar waveguides and long emission wavelengths, also represent an ideal playground in which to experiment with new ideas for surfaceplasmonbased photonics, such as electrically controllable optical circuits or disordered systems. In the end, the commercial future of terahertz QC lasers is still hard to predict and will most likely be determined by the general success of terahertzbased technologies. Nowadays the possibility of performing molecular detection in biological environments (for instance, for DNA or protein sensing) or detection of hidden substances (explosives, drugs, biochemical agents) in security controls is attracting a huge interest in terahertz radiation, and the same can be said for imaging of biological tissues in medical applications (tooth cavities, superficial tumors, etc.). Nevertheless the commercial fortune will be decided mainly by market rules: Will terahertz photonics be able to provide unique highvalue capabilities to justify a strong economic effort in its realworld implementation? Or will it be able to tackle the relevant applications at a lower cost than other competing technologies? The answers to these questions will be decided in the near future.
2.6 Acknowledgments We would like to express our gratitude to all the people who have been working with us on the development of terahertz quantum cascade Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_92_03/23/2006 Terahertz Quantum Cascade Lasers 92
Chapter Two
lasers; in particular, Harvey Beere and David Ritchie of the Cavendish Laboratory, University of Cambridge; Edmund Linfield and Giles Davies at the University of Leeds; Rita Iotti and Fausto Rossi at the Politecnico di Torino; Sukhdeep Dhillon and Carlo Sirtori at Thales Research and Technology; Stefano Barbieri, Jesse Alton, and John Fowler at Teraview; Lukas Mahler, Jihua Xu, Tonia Losco, Richard Green, Cosimo Mauro, and Fabio Beltram of the NEST CNRINFM Center at the Scuola Normale Superiore. Further we would like to thank Jerome Faist and his group at the University of Neuchâtel and Qing Hu and his coworkers at the Massachusetts Institute of Technology for kindly allowing the use of their figures in this chapter and for contributing so much to the success of terahertz QC lasers. Finally, we would like to acknowledge the financial support by the European Commission through the IST projects WANTED and TERANOVA, through the Marie Curie RTN POISE, and through the PASR project TERASEC; by the Fondazione Cassa di Risparmio di Pisa through the project Teralight; and by Physical Sciences Inc. of Andover.
References 1.
L. Esaki, “New phenomenon in narrow germanium pn junction,” Phys. Rev. 109, p. 603, 1958.
2.
W. T. Read, “A proposed highfrequency negative resistance diode,” Bell Sys. Tech. J. 37, p. 401, 1958.
3.
R. N. Hall, “Tunnel diodes,” IRE Trans. Electron Devices 7, p. 1, 1960.
4.
J. B. Gunn, “Microwave oscillation of current in IIIV semiconductors,” Solid State Commun. 1, p. 88, 1963.
5.
J. B. Gunn, “Instabilities of current in IIIV semiconductors,” IBM J. Dev. Res. 8, p. 141, 1964.
6.
C. A. Lee, R. L. Batdorf, W. Wiegman, and G. Kaminsky, “The read diode and avalanche, transittime, negativeresistance oscillators,” Appl. Phys. Lett. 6, p. 89, 1965.
7.
R. L. Johnston, B. C. DeLoach, and B. G. Cohen, “A silicon diode oscillator,” Bell Sys. Tech. J. 44, p. 369, 1965.
8.
R. N. Hall, G. E. Fenner, J. D. Kingsley, T. J. Soltys, and R. O. Carlson, “Coherent light emission from GaAs junctions,” Phys. Rev. Lett. 9, p. 366, 1962.
9.
B. Senitzky and A. A. Oliner, “Submillimeter waves—a transition region,” in Proceedings of the Symposium on Submillimeter Waves, J. Fox, ed., vol. 20, Press of the Polytechnic Institue of Brooklyn, New York, 1970.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_93_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
93
10.
K. H. Yang, P. L. Richards, and Y. R. Shen, “Generation of farinfrared radiation by picosecond light pulses in LiNbO3,” Appl. Phys. Lett. 19, p. 320, 1971.
11.
G. Mourou, C. V. Stancampiano, and D. Blumenthal, “Picosecond microwave pulse generation,” Appl. Phys. Lett. 38, p. 470, 1981.
12.
D. H. Auston, “Subpicosecond electrooptic shock waves,” Appl. Phys. Lett. 73, p. 713, 1983.
13.
D. H. Auston, K. P. Cheung, and P. R. Smith, “Picosecond photoconducting hertzian dipoles,” Appl. Phys. Lett. 45, p. 284, 1984.
14.
C. Fattinger and D. Grischkowsky, “Point source terahertz optics,” Appl. Phys. Lett. 53, p. 1480, 1988.
15.
M. Bass, P. A. Franken, J. F. Ward, and G. Weireich, “Optical rectification,” Phys. Rev. Lett. 9, p. 446, 1962.
16.
G. A. A’skaryan, “Cherenkov radiation and transition radiation from electromagnetic waves,” Sov. Phys. JETP 15, p. 943, 1962.
17.
B. B. Hu, X.C. Zhang, D. H. Auston, and P. R. Smith, “Freespace radiation from electrooptic crystals,” Appl. Phys. Lett. 56, p. 506, 1990.
18.
L. Xu, X.C. Zhang, and D. H. Auston, “Terahertz beam generation by femtosecond optical pulses in electrooptic materials,” Appl. Phys. Lett. 61, p. 1784, 1992.
19.
E. R. Brown, F. W. Smith, and K. A. McIntosh, “Coherent millimeter wave generation by heterodyne conversion in in lowtemperaturegrown GaAs photoconductors,” J. Appl. Phys. 73, p. 1480, 1993.
20.
E. R. Brown, K. A. McIntosh, K. B. Nichols, and C. L. Dennis, “Photomixing up to 3.8 THz in lowtemperaturegrown GaAs,” Appl. Phys. Lett. 66, p. 285, 1995.
21.
J. A. Valdmanis, G. A. Mourouand, and C. W. Gabel, “Subpicosecond electrical sampling,” IEEE J. Quantum Electronics 19, p. 664, 1983.
22.
Q. Wu and X.C. Zhang, “Freespace electrooptic sampling of terahertz beams,” Appl. Phys. Lett. 67, p. 3523, 1995.
23.
A. Nahata, A. S. Weling, and T. F. Heinz, “A wideband coherent terahertz spectroscopy system using optical rectification and electrooptic sampling,” Appl. Phys. Lett. 69, p. 2321, 1996.
24.
Q. Wu and X.C. Zhang, “Ultrafast electrooptical field sensors,” Appl. Phys. Lett. 68, p. 1604, 1996.
25.
A. Nahata, D. H. Auston, T. F. Heinz, and Q. Wu, “Coherent detection of freely propagating terahertz radiation by electrooptic sampling,” Appl. Phys. Lett. 68, p. 150, 1996.
26.
D. H. Auston and K. P. Cheung, “Coherent timedomain farinfrared spectroscopy,” J. Opt. Soc. Am. B 2, p. 606, 1985.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_94_03/23/2006 Terahertz Quantum Cascade Lasers 94
Chapter Two
27.
K. P. Cheung and D. H. Auston, “Excitation of coherent phonon polaritons with femtosecond optical pulses,” Phys. Rev. Lett. 55, p. 2152, 1985.
28.
K. P. Cheung and D. H. Auston, “A novel technique for measuring farinfrared absorption and dispersion,” Infrared Phys. 26, p. 23, 1986.
29.
B. B. Hu and M. C. Nuss, “Imaging with terahertz waves,” Opt. Lett. 20, p. 807, 1995.
30.
D. Mittleman, “Terahertz imaging,” in Sensing with Terahertz Radiation, Optical Sciences, D. Mittleman, ed., vol. 95, p. 117, Springer, Berlin, 2002.
31.
D. M. Mittleman, R. H. Jacobsen, and M. C. Nuss, “Tray imaging,” IEEE J. of Selected Topics in Quantum Electronics 2, p. 679, 1996.
32.
K. J. Siebert, H. Quast, R. Leonhardt, T. Löffler, M. Thomson, T. Bauer, and H. G. Roskos, “Continuouswave alloptoelectronic terahertz imaging,” Appl. Phys. Lett. 80, p. 3003, 2002.
33.
S. Wang and X.C. Zhang, “Tomographic imaging with a terahertz binary lens,” Appl. Phys. Lett. 82, p. 1821, 2003.
34.
D. M. Mittleman, S. Hunsche, L. Boivin, and M. C. Nuss, “Tray tomography,” Opt. Lett. 22, p. 904, 1997.
35.
J. L. Johnson, T. D. Dorney, and D. M. Mittleman, “Enhanced depth resolution in terahertz imaging using phaseshift interferometry,” Appl. Phys. Lett. 78, p. 835, 2001.
36.
M. Koch, “Biomedical applications of THz imaging,” in Sensing with Terahertz Radiation, Optical Sciences, D. Mittleman, ed., vol. 95, p. 295, Springer, Berlin, 2002.
37.
J. M. Chamberlain, N. N. Zinonev, A. J. Fitzgerald, E. Berry, G. C. Walker, J. W. Handley, M. A. Smith, and R. E. Miles, “What constitutes a useful and meaningful terahertz image?” in 2002 IEEE Tenth International Conference on Terahertz Electronics Proceedings, J. M. Chamberlain, P. Harrison, R. E. Miles, A. G. Davies, E. H. Linfield, and S. Withington, eds., vol.10, p. 81, IEEE, Piscataway, 2002.
38.
D. Mittleman, ed., Sensing with Terahertz Radiation, Springer, Berlin, 2002.
39.
B. Ferguson and X.C. Zhang, “Materials for terahertz science and technology,” Nature Materials 1, p. 26, 2002.
40.
M. Nagel, F. Richter, P. HaringBolivar, H. Kurz, A. Bosserhoff, and R. Büttner, “Integrated THz biomolecular sensors for DNA,” in 2002 IEEE Tenth International Conference on Terahertz Electronics Proceedings, J. M. Chamberlain, P. Harrison, R. E. Miles, A. G. Davies, E. H. Linfield, and S. Withington, eds., vol. 10, p. 70, IEEE, Piscataway, 2002.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_95_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
95
41.
M. Nagel, P. HaringBolivar, M. Brucherseifer, H. Kurz, A. Bosserhoff, and R. Büttner, “Integrated THz technology for labelfree genetic diagnostics,” Appl. Phys. Lett. 80, p. 154, 2002.
42.
R. Huber, F. Tauser, A. Brodschelm, M. Bichler, G. Abstreiter, and A. Leitenstorfer, “How manyparticle interactions develop after ultrafast excitation of an electronhole plasma,” Nature 414, p. 286, 2001.
43.
A. A. Andronov, I. V. Zverev, V. A. Kozlov, Y. N. Nozdrin, S. A. Pavlov, and V. N. Shastin, “Stimulated emission in the longwavelength IR region from hot holes in Ge in crossed electric and magnetic fields,” JETP Lett. 40, p. 804, 1984.
44.
A. A. Andronov, A. M. Belyantsev, V. I. Gavrilenko, E. P. Dodin, Z. F. Krasil’nik, V. V. Nikoronov, and S. A. Pavlov, “Induced hothole milli(cyclotronresonance meter emission in germanium in fields negativeeffectivemass amplifier and generator),” JETP Lett. 40, p. 989, 1984.
45.
Y. B. Vasil’ev and Y. L. Ivanov, “Frequency of stimulated emission during transitions through lighthole Landau levels in germanium,” Sov. Tech. Phys. Lett. 10, p. 398, 1984.
46.
A. A. Andronov, “Hot electrons in semiconductors and submillimeter waves,” Sov. Phys. Semicond. 21, p. 701, 1987.
47.
Y. P. Gousev, I. V. Altukhov, K. A. Korolev, V. P. Sinis, M. S. Kagan, E. E. Haller, M. A. Odnoblyudov, I. N. Yassievich, and K.A. Chao, “Widely tunable continuouswave THz laser,” Appl. Phys. Lett. 75, p. 757, 1999.
48.
P. Pfeffer, W. Zawadzki, K. Unterrainer, C. Kremser, C. Wurzer, E. Gornik, B. Murdin, and C. R. Pidgeon, “ptype Ge cyclotronresonance laser: Theory and experiment,” Phys. Rev. B 47, p. 4522, 1993.
49.
H. Eisele, “Conventional and novel approaches to RF power generation with twoterminal devices at terahertz frequencies,” in 2002 IEEE Tenth International Conference on Terahertz Electronics Proceedings, J. M. Chamberlain, P. Harrison, R. E. Miles, A. G. Davies, E. H. Linfield, and S. Withington, eds., vol. 10, p. 13, IEEE, Piscataway, 2002.
50.
E. R. Brown, J. R. Söderström, C. D. Parker, L. J. Mahoney, K. M. Molvar, and T. C. McGill, “Oscillations up to 712 GHz in InAs/AlAs resonanttunneling diodes,” Appl. Phys. Lett. 58, p. 2291, 1991.
51.
A. Maestrini, J. Ward, J. Gill, H. Javadi, E. Schlecht, G. Chattopadhyay, F. Maiwald, N. R. Erickson, and I. Mehdi, “A 1.7 – 1.9 THz local oscillator source,” IEEE Microwave Wireless Comp. Lett. 14, pp. 253–255, 2004.
52.
S. J. Allen, J. S. Scott, M. C. Wanke, K. Maranowski, A. C. Gossard, M. J. W. Rodwell, and D. H. Chow, “Terahertz dynamics in quantum structures: Towards a fundamental terahertz oscillator,” in Terahertz Sources and Systems, NATO Science Series, R. Miles, P. Harrison, and D. Lippens, eds., vol. 27, p. 3, Kluwer Academic, Dordrecht, 2001.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_96_03/23/2006 Terahertz Quantum Cascade Lasers 96
Chapter Two
53.
R. P. Joshi, S. Viswanadha, P. Shah, and R. D. del Rosario, “Monte Carlo analysis of GaNbased Gunn oscillators for microwave power generation,” J. Appl. Phys. 93, p. 4863, 2003.
54.
E. Starikov, P. Shiktorov, V. Gruzinskis, L. Reggiani, L. Varani, J. C. Vaissière, and J. H. Zhao, “Monte Carlo simulation of the generation of terahertz radiation in GaN,” J. Appl. Phys. 89, p. 1161, 2001.
55.
L. N. Kurbatov, A. D. Britov, S. M. Karavaev, S. D. Sivachenko, S. N. Maksimovskii, I. I. Ovchinnikov, M. M. Rzaev, and P. M. Starik, “FarIR heterojunction lasers tunable to 46.2 m,” JETP Lett. 37, p. 499, 1983.
56.
A. P. Shotov, O. I. Davarashvili, and A. V. Babushkin, “Laser heterostructures using Pb1–xSnxSe1–yTey solid solutions,” Sov. Tech. Phys. Lett. 5, p. 629, 1979.
57.
B. G. Girich, D. M. Gureev, I. I. Zasavitskii, T. I. Koropotkina, E. P. Kulygina, B. N. Matsonashvili, M. I. Nikolaev, O. V. Pelevin, G. V. Flusov, and A. P. Shotov, “Laser Pb1–xSnx Te heterostructures,” Sov. Physics Semic. 12, p. 70, 1978.
58.
J. N. Walpole, A. R. Calawa, S. R. Chinn, S. H. Groves, and T. C. Harman, “CW, operation of distributed feedback Pb1–xSnx Te lasers,” Appl. Phys. Lett. 30, p. 524, 1977.
59.
R. F. Kazarinov and R. A. Suris, “Possibility of the amplification of electromagnetic waves in a semiconductor with a superlattice,” Sov. Physics Semic. 5, p. 707, 1971.
60.
R. F. Kazarinov and R. A. Suris, “Electric and electromagnetic properties of semiconductors with a superlattice,” Sov. Physics Semic. 6, p. 120, 1972.
61.
K. L. Wang and P.F. Yuh, “Theory and applications of bandaligned superlattices,” IEEE J. Quantum Electronics 25, p. 12, 1988.
62.
F. Capasso, K. Mohammed, and A. Y. Cho, “Resonant tunneling through double barriers, perpendicular quantum transport phenomena in superlattices, and their device applications,” IEEE J. Quantum Electronics 22, pp. 1853–1869, 1986.
63.
M. Helm, P. England, E. Colas, F. D. Rosa, and S. J. Allen, “Intersubband Emission from Semiconductor Superlattices Excited by Sequential Tunneling,” Phys. Rev. Lett. 63, p. 74, 1989.
64.
M. Helm, E. Colas, P. England, F. DeRosa, and S. J. Allen, “Observation of gratinginduced intersubband emission from GaAs/AlGaAs superlattices,” Appl. Phys. Lett. 53, p. 1714, 1988.
65.
R. Ferreira and G. Bastard, “Evaluation of some scattering times for electrons in unbiased and biased single and multiplequantumwell structures,” Phys. Rev. B 40, p. 1074, 1989.
66.
A. Seilmeier, H.J. Hübner, G. Abstreiter, G. Weimann, and W. Schlapp, “Intersubband relaxation in GaAsAlGaAs quantum well structures observed directly by an infrared bleaching technique,” Phys. Rev. Lett. 59, p. 1345, 1987.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_97_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
97
67.
J. Faist, F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho, “Quantum cascade laser,” Science 264, pp. 553–556, 1994.
68.
A. Evans, J. S. Yu, J. David, L. Doris, K. Mi, S. Slivken, and M. Razeghi, “Hightemperature highpower continuouswave operation of buried heterostructure quantumcascade lasers,” Appl. Phys. Lett. 84, pp. 314– 316, 2004.
69.
J. Faist, C. Gmachl, F. Capasso, C. Sirtori, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, “Distributed feedback quantum cascade lasers,” Appl. Phys. Lett. 70, p. 2670, 1997.
70.
C. Gmachl, F. Capasso, J. Faist, A. L. Hutchinson, A. Tredicucci, D. L. Sivco, J. N. Baillargeon, S. N. G. Chu, and A. Y. Cho, “Distributed feedback quantum cascade lasers,” Appl. Phys. Lett. 72, p. 1430, 1998.
71.
R. Köhler, C. Gmachl, A. Tredicucci, F. Capasso, D. L. Sivco, S. N. G. Chu, and A. Y. Cho, “Singlemode tunable, pulsed, and continuous wave quantumcascade distributed feedback lasers Ȝ ~ 4.6 – 4.7 m,” Appl. Phys. Lett. 76, p. 1092, 2000.
72.
D. Hofstetter, M. Beck, T. Aellen, and J. Faist, “Hightemperature operation of distributed feedback quantumcascade lasers at 5.3 m,” Appl. Phys. Lett. 78, p. 396, 2001.
73.
A. Tredicucci, C. Gmachl, F. Capasso, A. L. Hutchinson, D. L. Sivco, and A. Y. Cho, “Singlemode surfaceplasmon laser,” Appl. Phys. Lett. 76, p. 2164, 2000.
74.
D. Hofstetter, J. Faist, M. Beck, A. Müller, and U. Oesterle, “Demonstration of highperformance 10.16 m quantum cascade distributed feedback lasers fabricated without epitaxial regrowth,” Appl. Phys. Lett. 75, p. 665, 1999.
75.
J. Faist, F. Capasso, D. L. Sivco, A. L. Hutchinson, S. N. G. Chu, and A. Y. Cho, “Short wavelength (Ȝ ~ 3.4 m) quantum cascade laser based on strained compensated InGaAs/AlInAs,” Appl. Phys. Lett. 72, p. 680, 1998.
76.
R. Colombelli, F. Capasso, C. Gmachl, A. L. Hutchinson, D. L. Sivco, A. Tredicucci, M. C. Wanke, A. M. Sergent, and A. Y. Cho, “Farinfrared surfaceplasmon quantumcascade lasers at 21.5 m and 24 m wavelengths,” Appl. Phys. Lett. 78, pp. 2620–2622, 2001.
77.
C. Sirtori, P. Kuck, S. Barbieri, P. C. J. Nagle, M. Beck, J. Faist, and U. Oesterle, “GaAs/Alx Ga1–x As quantum cascade lasers,” Appl. Phys. Lett. 73, p. 3486, 1998.
78.
K. Ohtani and H. Ohno, “An InAsbased intersubband quantum cascade laser,” Jap. J. Appl. Phys. 2 41, p. L1279, 2002.
79.
K. Ohtani and H. Ohno, “InAs/AlSb quantum cascade lasers operating at 10 m,” Appl. Phys. Lett. 82, p. 1003, 2003.
80.
M. Rochat, J. Faist, M. Beck, U. Oesterle, and M. Ilegems, “Farinfrared (Ȝ ~ 88 m) electroluminescence in a quantum cascade structure,” Appl. Phys. Lett. 73, pp. 3724–3726, 1998.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_98_03/23/2006 Terahertz Quantum Cascade Lasers 98
Chapter Two
81.
B. S. Williams, B. Xu, Q. Hu, and M. R. Melloch, “Narrowlinewidth terahertz intersubband emission from threelevel systems,” Appl. Phys. Lett. 75, pp. 2927–2929, 1999.
82.
J. Ulrich, R. Zobl, N. Finger, K. Unterrainer, G. Strasser, and E. Gornik, “Terahertzelectroluminescence in a quantum cascade structure,” Physica B 272, p. 216, 1999.
83.
J. Ulrich, R. Zobl, W. Schrenk, G. Strasser, K. Unterrainer, and E. Gornik, “Terahertz quantum cascade structures: intra versus interwell transition,” Appl. Phys. Lett. 77, pp. 1928–1930, 2000.
84.
J. Ulrich, R. Zobl, K. Unterrainer, G. Strasser, and E. Gornik, “Magneticfieldenhanced quantumcascade emission,” Appl. Phys. Lett. 76, p. 19, 2000.
85.
B. S. Williams and Q. Hu, “Optimized energy separation for phonon scattering in threelevel terahertz intersubband lasers,” J. Appl. Phys. 90, p. 5504, 2001.
86.
B. S. Williams, H. Callebaut, Q. Hu, and J. L. Reno, “Magnetotunneling spectroscopy of resonant anticrossing in terahertz intersubband emitters,” Appl. Phys. Lett. 79, p. 4444, 2001.
87.
R. Colombelli, A. Straub, F. Capasso, C. Gmachl, M. I. Blakey, A. M. Sergent, S. N. G. Chu, K. W. West, and L. N. Pfeiffer, “Terahertz electroluminescence from superlattice quantum cascade structures,” J. Appl. Phys. 91, p. 3526, 2002.
88.
S. A. Lynch, R. Bates, D. J. Paul, D. J. Norris, A. G. Cullis, Z. Ikonic, R. W. Kelsall, P. Harrison, D. D. Arnone, and C. R. Pidgeon, “Intersubband electroluminescence from Si/SiGe cascade emitters at terahertz frequencies,” Appl. Phys. Lett. 81, p. 1543, 2002.
89.
R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, D. A. Ritchie, R. C. Iotti, and F. Rossi, “Terahertz semiconductorheterostructure laser,” Nature 417, pp. 156–159, 2002.
90.
A. Tredicucci, F. Capasso, C. Gmachl, D. L. Sivco, A. L. Hutchinson, and A. Y. Cho, “High performance interminiband quantum cascade lasers with graded superlattices,” Appl. Phys. Lett. 73, pp. 2101–2103, 1998.
91.
R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, D. A. Ritchie, S. Dhillon, and C. Sirtori, “Highperformance continuouswave operation of superlattice terahertz quantumcascade lasers,” Appl. Phys. Lett. 82, pp. 1518–1520, 2003.
92.
G. Scalari, L. Ajili, J. Faist, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Farinfrared Ȝ ~ 85 m boundtocontinuum quantumcascade lasers operating up to 90 K,” Appl. Phys. Lett. 82, pp. 3165–3167, 2003.
93.
B. S. Williams, S. Kumar, H. Callebaut, Q. Hu, and J. L. Reno, “Terahertz quantumcascade laser at Ȝ ~ 100 m using metal waveguide for mode confinement,” Appl. Phys. Lett. 83, pp. 2124–2126, 2003.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_99_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
99
94.
B. S. Williams, S. Kumar, H. Callebaut, Q. Hu, and J. L. Reno, “Terahertz quantumcascade laser operating up to 137 K,” Appl. Phys. Lett. 83, pp. 5142–5144, 2003.
95.
S. Barbieri, J. Alton, H. E. Beere, J. Fowler, E. H. Linfield, and D. A. Ritchie, “2.9 THz quantum cascade lasers operating up to 70 K in continuous wave,” Appl. Phys. Lett. 85, pp. 1674–1676, 2004.
96.
S. Kumar, B. S. Williams, S. Kohen, Q. Hu, and J. L. Reno, “Continuouswave operation of terahertz quantum cascade lasers above liquidnitrogen,” Appl. Phys. Lett. 84, pp. 2494–2496, 2004.
97.
B. S. Williams, S. Kumar, Q. Hu, and J. L. Reno, “Resonant phonon terahertz quantum cascade laser operating at 2.1 THz (Ȝ 싇 141 m),” Electron. Lett. 40, pp. 431– 433, 2004.
98.
A. Tredicucci, L. Mahler, T. Losco, J. Xu, C. Mauro, R. Köhler, H. E. Beere, D. A. Ritchie, and E. H. Linfield, “Advances in THz quantum cascade lasers: fulfilling the application potential,” in Proc. SPIE, Novel Inplane Semiconductor Lasers IV, C. Marmelstein and D. P. Bour, eds., vol. 5738, SPIE, in press.
99.
H. Eisele, “Active twoterminal devices for terahertz power generation by multiplication,” in Terahertz Sources and Systems, NATO Science Series, R. Miles, P. Harrison, and D. Lippens, eds., vol. 27, p. 69, Kluwer Academic, Dordrecht, 2001.
100.
S. M. Duffy, S. Verghese, and K. A. McIntosh, “Photomixers for continuouswave terahertz radiation,” in Sensing with Terahertz Radiation, Optical Sciences, D. Mittleman, ed., vol. 95, p. 193, Springer, Berlin, 2002.
101.
E. A. Michael, B. Vowinkel, R. Schieder, M. Mikulics, M. Marso, and P. Kordoš, “Largearea travelingwave photonic mixers for increased continuous terahertz power,” Appl. Phys. Lett. 86, 111120, 2005.
102.
J. Darmo, T. Müller, G. Strasser, K. Unterrainer, T. Le, G. Tempea, and A. Stingl, “Intra and extracavity THz generation from optically and electrically confined photoconducting layers,” in 2002 IEEE Tenth International Conference on Terahertz Electronics Proceedings, J. M. Chamberlain, P. Harrison, R. E. Miles, A. G. Davies, E. H. Linfield, and S. Withington, eds., vol. 10, p. 67, IEEE, Piscataway, 2002.
103.
E. Peytavit, S. Arscott, D. Lippens, G. Mouret, S. Matton, P. Masselin, R. Bocquet, J. F. Lampin, L. Desplanque, and F. Mollot, “Terahertz frequency difference from vertically integrated lowtemperaturegrown GaAs photodetector,” Appl. Phys. Lett. 81, p. 1174, 2002.
104.
R. Kersting, K. Unterrainer, G. Strasser, H. F. Kauffmann, and E. Gornik, “FewCycle THz Emission from Cold Plasma Oscillations,” Phys. Rev. Lett. 79, p. 3038, 1997.
105.
X.C. Zhang, B. B. Hu, J. T. Darrow, and D. H. Auston, “Generation of femtosecond electromagnetic pulses from semiconductor surfaces,” Appl. Phys. Lett. 56, p. 1011, 1990.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_100_03/23/2006 Terahertz Quantum Cascade Lasers 100
Chapter Two
106.
X.C. Zhang, Y. Jin, L. E. Kingsley, and M. Weiner, “Influence of electric and magnetic fields on THz radiation,” Appl. Phys. Lett. 62, p. 2477, 1993.
107.
M. B. Johnston, D. M. Whittaker, A. Corchia, A. G. Davies, and E. H. Linfield, “Simulation of terahertz generation at semiconductor surfaces,” Phys. Rev. B 65, 165301, 2002.
108.
A. Rice, Y. Jin, X. F. Ma, X.C. Zhang, D. Bliss, J. Larkin, and M. Alexander, “Terahertz optical rectification from [110] zincblende crystals,” Appl. Phys. Lett. 64, p. 1324, 1994.
109.
J. J. Carey, R. T. Bailey, D. Pugh, J. N. Sherwood, F. R. Cruickshank, and K. Wynne, “Terahertz pulse generation in an organic crystal by optical rectification and resonant excitation of molecular charge transfer,” Appl. Phys. Lett. 81, p. 4335, 2002.
110.
Y. S. Lee, T. Meade, T. B. Norris, and A. Galvanauskas, “Tunable narrowband terahertz generation from periodically poled lithium niobate,” Appl. Phys. Lett. 78, p. 3583, 2001.
111.
E. Bründermann, D. R. Chamberlin, and E. E. Haller, “High duty cycle and continuous terahertz emission from germanium,” Appl. Phys. Lett. 76, p. 2991, 2000.
112.
E. Bründermann, A. M. Linhart, H. P. Röser, O. D. Dubon, W. L. Hansen, and E. E. Haller, “Miniaturization of pGe lasers: progress toward continuous wave operation,” Appl. Phys. Lett. 68, p. 1359, 1996.
113.
A. V. Muravjov, S. H. Withers, H. Weidner, R. C. Strijbos, S. G. Pavlov, V. N. Shastin, and R. E. Peale, “Single axialmode selection in a farinfrared pGe laser,” Appl. Phys. Lett. 76, pp. 1996–1998, 2000.
114.
A. V. Muravjov, S. H. Withers, R. C. Strijbos, S. G. Pavlov, V. N. Shastin, and R. E. Peale, “Actively modelocked pGe laser in Faraday configuration,” Appl. Phys. Lett. 75, pp. 2882–2884, 1999.
115.
M. A. Odnoblyudov, I. N. Yassievich, M. S. Kagan, Y. M. Galperin, and K. A. Chao, “Population inversion induced by resonant states in semiconductors,” Phys. Rev. Lett. 83, p. 644, 1999.
116.
A. Yariv, Optical Electronics in Modern Communications, 5th ed., Oxford University Press, Oxford, 1997.
117.
K. Kawase, J. Shikata, K. Imai, and H. Ito, “Transformlimited, narrowlinewidth, terahertzwave parametric generator,” Appl. Phys. Lett. 78, p. 2819, 2001.
118.
K. Imai, K. Kawase, H. Minamide, and H. Ito, “Achromatically injectionseeded terahertzwave parametric generator,” in 2002 IEEE Tenth International Conference on Terahertz Electronics Proceedings, J. M. Chamberlain, P. Harrison, R. E. Miles, A. G. Davies, E. H. Linfield, and S. Withington, eds., vol. 10, p. 56, IEEE, Piscataway, 2002.
119.
K. Imai, K. Kawase, H. Minamide, and H. Ito, “Achromatically injectionseeded terahertzwave parametric generator,” Opt. Lett. 27, p. 2173, 2002.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_101_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
101
120.
T. Tanabe, K. Suto, J. Nishizawa, K. Saito, and T. Kimura, “Tunable terahertz wave generation in the 3 to 7THz region from GaP,” Appl. Phys. Lett. 83, p. 237, 2003.
121.
T. Tanabe, K. Suto, J. Nishizawa, T. Kimura, and K. Saito, “Frequencytunable highpower terahertz wave generation from GaP,” J. Appl. Phys. 93, p. 4610, 2003.
122.
S. G. Pavlov, R. K. Zhukavin, E. E. Orlova, V. N. Shastin, A. Kirsanov, H.W. Hübers, K. Auen, and H. Riemann, “Stimulated emission from donor transitions in silicon,” Phys. Rev. Lett. 84, p. 5220, 2000.
123.
S. G. Pavlov, H.W. Hübers, M. H. Rümmeli, R. K. Zhukavin, E. E. Orlova, V. N. Shastin, and H. Riemann, “Farinfrared stimulated emission from optically excited bismuth donors in silicon,” Appl. Phys. Lett. 80, p. 4717, 2002.
124.
V. N. Shastin, R. K. Zhukavin, E. E. Orlova, S. G. Pavlov, H.W. Hübers, M. H. Rümmeli, J. N. Hovenier, T. O. Klaassen, H. Riemann, I. V. Bradley, and A. F. G. van der Meer, “Stimulated terahertz emission from groupV donors in silicon under intracenter photoexcitation,” Appl. Phys. Lett. 80, p. 3512, 2002.
125.
P. G. O’Shea and H. P. Freund, “Freeelectron lasers: status and applications,” Science 292, p. 1853, 2001.
126.
G. L. Carr, M. C. Martin, W. R. McKinney, K. Jordan, G. R. Neil, and G. P. Williams, “Highpower terahertz radiation from relativistic electrons,” Nature 420, p. 153, 2002.
127.
M. AboBakr, J. Feikes, K. Holldack, G. Wstefeld, and H.W. Hübers, “Steadystate farinfrared coherent synchrotron radiation detected at BESSY II,” Phys. Rev. Lett. 88, 254801, 2002.
128.
M. AboBakr, J. Feikes, K. Holldack, P. Kuske, W. B. Peatman, U. Schade, G. Wstefeld, and H.W. Hübers, “Brilliant, coherent farinfrared (THz) synchrotron radiation,” Phys. Rev. Lett. 90, 094801, 2003.
129.
P. Helminger, J. K. Messer, and F. C. de Lucia, “Continuously tunable coherent spectroscopy for the 0.1 to 1.0 THz region,” Appl. Phys. Lett. 42, p. 309, 1983.
130.
S. Komiyama, O. Astafiev, V. Antonov, T. Kutsuwa, and H. Hirai, “A singlephoton detector in the farinfrared range,” Nature 403, p. 405, 2000.
131.
J. J. A. Baselmans, M. Hajenius, J. R. Gao, T. M. Klapwijk, P. A. J. de Korte, B. Voronov, and G. Gol’tsman, “Doubling of sensitivity and bandwidth in phonon cooled hot electron bolometer mixers,” Appl. Phys. Lett. 84, pp. 1958–1960, 2004.
132.
W. Knap, Y. Deng, S. Rumyantsev, and M. S. Shur, “Resonant detection of subterahertz and terahertz radiation by plasma waves in submicron fieldeffect transistors,” Appl. Phys. Lett. 81, p. 4637, 2002.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_102_03/23/2006 Terahertz Quantum Cascade Lasers 102
Chapter Two
133.
S. Kono, M. Tani, P. Gu, and K. Sakai, “Detection of up to 20 THz with a lowtemperaturegrown GaAs photoconductive antenna gated with 15 fs light pulses,” Appl. Phys. Lett. 77, p. 4104, 2001.
134.
B. Xu, Q. Hu, and M. R. Melloch, “Electrically pumped tunable terahertz emitter based on intersubband transitions,” Appl. Phys. Lett. 71, p. 440, 1997.
135.
R. C. Iotti and F. Rossi, “Carrier thermalization versus phononassisted relaxation in quantumcascade lasers: a Monte Carlo approach,” Appl. Phys. Lett. 78, p. 2902, 2001.
136.
R. C. Iotti and F. Rossi, “Nature of Charge Transport in QuantumCascade Lasers,” Phys. Rev. Lett. 87, 146603, 2001.
137.
R. Köhler, R. C. Iotti, A. Tredicucci, and F. Rossi, “Design and simulation of terahertz quantum cascade lasers,” Appl. Phys. Lett. 79, pp. 3920– 3922, 2001.
138.
B. Xu and Q. Hu, “Grating coupling for intersubband emission,” Appl. Phys. Lett. 70, p. 2511, 1997.
139.
R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, and D. A. Ritchie, “Highintensity interminiband terahertz emission from chirped superlattices,” Appl. Phys. Lett. 80, pp. 1867– 1869, 2002.
140.
C. Sirtori, C. Gmachl, F. Capasso, J. Faist, D. L. Sivco, A. L. Hutchinson, and A. Y. Cho, “Longwavelength (Ȝ ~ 8 – 11.5 m) semiconductor lasers with waveguides based on surface plasmons,” Opt. Lett. 23, pp. 1366– 1368, 1998.
141.
A. Tredicucci, C. Gmachl, M. C. Wanke, F. Capasso, A. L. Hutchinson, D. L. Sivco, S. N. G. Chu, and A. Y. Cho, “Surface plasmon quantum cascade lasers at Ȝ ~ 19 m,” Appl. Phys. Lett. 77, p. 2286, 2000.
142.
K. Unterrainer, R. Colombelli, C. Gmachl, F. Capasso, H. Y. Hwang, A. M. Sergent, D. L. Sivco, and A. Y. Cho, “Quantum cascade lasers with double metalsemiconductor waveguide resonators,” Appl. Phys. Lett. 80, pp. 3060–3062, 2002.
143.
M. Rochat, M. Beck, J. Faist, and U. Oesterle, “Measurement of farinfrared waveguide loss using a multisection singlepass technique,” Appl. Phys. Lett. 78, p. 1967, 2001.
144.
M. Rochat, L. Ajili, H. Willenberg, J. Faist, H. E. Beere, A. G. Davies, E. H. Linfield, and D. A. Ritchie, “Lowthreshold terahertz quantum cascade lasers,” Appl. Phys. Lett. 81, p. 1381, 2002.
145.
S. Barbieri, J. Alton, S. S. Dhillon, H. E. Beere, M. Evans, E. H. Linfield, A. G. Davies, D. A. Ritchie, R. Köhler, A. Tredicucci, and F. Beltram, “Continuouswave operation of terahertz quantumcascade lasers,” IEEE J. Quantum Electronics 39, p. 586, 2003.
146.
L. Ajili, G. Scalari, D. Hofstetter, M. Beck, J. Faist, H. Beere, G. Davies, E. Linfield, and D. Ritchie, “Continuouswave operation of farinfrared quantum cascade lasers,” Electron. Lett. 38, pp. 1675–1676, 2002.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_103_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
103
147.
C. Sirtori, F. Capasso, J. Faist, A. L. Hutchinson, D. L. Sivco, and A. Y. Cho, “Resonant tunneling in quantum cascade lasers,” IEEE J. Quantum Electronics 34, p. 1722, 1998.
148.
V. B. Gorfinkel, S. Luryi, and B. Gelmont, “Theory of gain spectra for quantum cascade lasers and temperature dependence of their characteristics at low and moderate carrier concentration,” IEEE J. Quantum Electronics 32, p. 1995, 1996.
149.
J. Faist, F. Capasso, C. Sirtori, D. L. Sivco, A. L. Hutchinson, and A. Y. Cho, “Vertical transition quantum cascade laser with Braggconfined excited state,” Appl. Phys. Lett. 66, p. 538, 1995.
150.
D. Indjin, P. Harrison, R. W. Kelsall, and Z. Ikonic, “Mechanisms of temperature performance degradation in terahertz quantumcascade lasers,” Appl. Phys. Lett. 82, pp. 1347–1349, 2003.
151.
A. Tredicucci, R. Köhler, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, and D. A. Ritchie, “Terahertz quantum cascade lasers,” Physica E 21, pp. 846–851, 2004.
152.
J. Faist, M. Beck, T. Aellen, and E. Gini, “Quantumcascade lasers based on a boundtocontinuum transition,” Appl. Phys. Lett. 78, pp. 147–149, 2001.
153.
R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Quantum cascade lasers emitting at (Ȝ > 100 m),” Electron. Lett. 39, pp. 1254–1255, 2003.
154.
B. S. Williams, H. Callebaut, S. Kumar, Q. Hu, and J. L. Reno, “3.4THz quantum cascade laser based on LOphonon scattering for depopulation,” Appl. Phys. Lett. 82, pp. 1015–1017, 2003.
155.
H. Callebaut, S. Kumar, B. S. Williams, Q. Hu, and J. L. Reno, “Analysis of transport properties of tetrahertz quantum cascade lasers,” Appl. Phys. Lett. 83, p. 207, 2003.
156.
H. Callebaut, S. Kumar, B. S. Williams, Q. Hu, and J. L. Reno, “Importance of electronimpurity scattering for electron transport in terahertz quantumcascade lasers,” Appl. Phys. Lett. 84, p. 645, 2004.
157.
R. Köhler, A. Tredicucci, C. Mauro, F. Beltram, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Terahertz quantumcascade lasers based on an interlaced photonphonon cascade,” Appl. Phys. Lett. 84, pp. 1266–1268, 2004.
158.
D. Indjin, Z. Ikoniü, P. Harrison, and R. W. Kelsall, “Surface plasmon waveguides with gradually doped or NiAl intermetallic compound buried contact for terahertz quantum cascade lasers,” J. Appl. Phys. 94, pp. 3249–3252, 2003.
159.
L. Ajili, G. Scalari, J. Faist, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “High power quantum cascade lasers operating at Ȝ 싇 87 and 130 m,” Appl. Phys. Lett. 85, pp. 3986–3988, 2004.
160.
J. Alton, S. S. Dhillon, C. Sirtori, A. de Rossi, M. Calligaro, S. Barbieri, H. E. Beere, E. H. Linfield, and D. A. Ritchie, “Buried waveguides in
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_104_03/23/2006 Terahertz Quantum Cascade Lasers 104
Chapter Two
terahertz quantum cascade lasers based on twodimensional surface plasmon modes,” Appl. Phys. Lett. 86, 071109, 2005. 161.
B. S. Williams, S. Kumar, H. Callebaut, Q. Hu, and J. L. Reno, “3.4 THz terahertz quantumcascade laser operating above liquid nitrogen temperature,” Electron. Lett. 39, p. 915, 2003.
162.
R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, and D. A. Ritchie, “Lowthreshold quantumcascade lasers at 3.5 THz (Ȝ ~ 85 m),” Opt. Lett. 28, pp. 810–812, 2003.
163.
G. Scalari, S. Blaser, J. Faist, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Terahertz emission from quantum cascade lasers in the quantum hall regime: evidence for many body resonances and localization effects,” Phys. Rev. Lett. 93, 237403, 2004.
164.
L. Mahler, R. Köhler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Singlemode operation of terahertz quantum cascade lasers with distributed feedback resonators,” Appl. Phys. Lett. 84, pp. 5446–5448, 2004.
165.
A. Barkan, F. K. Tittel, D. M. Mittleman, R. Dengler, P. Siegel, G. Scalari, L. Ajili, J. Faist, H. E. Beere, E. H. Linfield, A. G. Davies, and D. A. Ritchie, “Linewidth and tuning characteristics of THz quantum cascade lasers,” Opt. Lett. 29, p. 575, 2004.
166.
J. C. Weeber, Y. Lacroute, A. Dereux, E. Devaux, T. Ebbesen, C. Girard, M. U. González, and A. L. Baudrion, “Nearfield characterization of Bragg mirrors engraved in surface plasmon waveguides,” Phys. Rev. B 70, 235406, 2004.
167.
D. Smirnov, C. Becker, O. Drachenko, V. V. Rylkov, H. Page, J. Leotin, and C. Sirtori, “Control of electronopticalphonon scattering rates in quantum box cascade lasers,” Phys. Rev. B 66, 121305, 2002.
168.
C. Becker, C. Sirtori, O. Drachenko, V. V. Rylkov, D. Smirnov, and J. Leotin, “GaAs quantum box cascade lasers,” Appl. Phys. Lett. 81, pp. 2941–2943, 2002.
169.
S. Blaser, M. Rochat, M. Beck, D. Hofstetter, and J. Faist, “Terahertz intersubband emission in strong magnetic fields,” Appl. Phys. Lett. 81, pp. 67–69, 2002.
170.
J. Alton, S. Barbieri, J. Fowler, H. E. Beere, J. Muscat, E. H. Linfield, D. A. Ritchie, A. G. Davies, R. Köhler, and A. Tredicucci, “Magnetic field inplane quantization of population inversion in a THz superlattice quantum cascade laser,” Phys. Rev. B 68, 081303, 2003.
171.
V. Tamosiunas, R. Zobl, J. Ulrich, K. Unterrainer, R. Colombelli, C. Gmachl, K. West, L. Pfeiffer, and F. Capasso, “Terahertz quantum cascade lasers in a magnetic field,” Appl. Phys. Lett. 83, p. 3873, 2003.
172.
G. Scalari, S. Blaser, L. Ajili, J. Faist, H. E. Beere, E. H. Linfield, D. A. Ritchie, and A. G. Davies, “Population inversion by resonant magnetic confinement in terahertz quantumcascade lasers,” Appl. Phys. Lett. 83, pp. 3453–3455, 2003.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_105_03/23/2006 Terahertz Quantum Cascade Lasers Terahertz Quantum Cascade Lasers
105
173.
K. Kempa, P. Bakshi, A. Scorupsky, C. G. Du, G. Feng, R. Zobl, G. Strasser, C. Rauch, C. Pacher, K. Unterrainer, and E. Gornik, “Intersubband transport in quantum wells in strong magnetic fields mediated by single and twoelectron scattering,” Phys. Rev. Lett. 88, 226803, 2002.
174.
J. Darmo, V. Tamosiunas, G. Fasching, J. Kröll, K. Unterrainer, M. Beck, M. Giovannini, J. Faist, C. Kremser, and P. Debbage, “Imaging with a terahertz quantum cascade laser,” Opt. Express 12, pp. 1879–1884, 2004.
175.
D. R. Chamberlin, P. R. Robrish, W. R. Trutna, G. Scalari, M. Giovannini, L. Ajili, and J. Faist, “Imaging at 3.4 THz with a quantumcascade laser,” Appl. Opt. 44, pp. 121–125, 2005.
176.
D. C. Larrabee, G. A. Khodaparast, F. K. Tittel, J. Kono, G. Scalari, L. Ajili, J. Faist, H. E. Beere, A. G. Davies, E. H. Linfield, D. A. Ritchie, Y. Nakajima, M. Nakai, S. Sasa, M. Inoue, S. Chung, and M. B. Santos, “Application of terahertz quantumcascade lasers to semiconductor cyclotron resonance,” Opt. Lett. 29, pp. 122–124, 2004.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH02_106_03/23/2006 Terahertz Quantum Cascade Lasers
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_107_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
3 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers
Roberto Paiella Department of Electrical and Computer Engineering and Photonics Center Boston University Boston, Massachusetts
Rainer Martini Department of Physics and Engineering Physics Stevens Institute of Technology Hoboken, New Jersey
Alexander Soibel Jet Propulsion Laboratory California Institute of Technology Pasadena, California
H. C. Liu Institute for Microstructural Sciences National Research Council Ottawa, Ontario, Canada
Federico Capasso Division of Engineering and Applied Sciences Harvard University Cambridge, Massachusetts
107
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_108_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 108
Chapter Three
3.1 Introduction The investigation of the highspeed dynamics of semiconductor lasers has long been one of the main thrusts of research in the development of these devices, due to favorable properties and important applications [1–7]. With their electric injection pumping mechanism, semiconductor lasers can be used to directly convert highspeed signals from the electrical to the optical domain—a function of central importance in the field of optical communications. Their small size and relatively low power consumption allow for the efficient delivery to the active region of electric signals at speeds of several tens of gigahertz, when properly designed device structures and packaging are used. Furthermore, their short cavity lengths compared to other types of lasers allow for passive modelocked operation at uniquely high repetition rates [8–10], which can be extended into the terahertz region [11]. A key parameter in determining the dynamic properties of a laser is the relaxation lifetime Ĳ of the laser population inversion. In conventional semiconductor lasers based on interband recombination, the population inversion (i.e., the density of conduction band electrons and valence band holes) primarily decays through spontaneous radiative recombination and bandtoband carriercarrier scattering (Auger recombination). The resulting carrier lifetime is on the order of a few nanoseconds [7]. While this is faster than in most other types of lasers, it effectively limits the directcurrent (dc) modulation bandwidth to ~10 to 20 GHz [12]. In addition, the practical use of directly modulated interband lasers as highspeed optical transmitters is severely limited by their large wavelength chirp [13, 14]. In quantum cascade (QC) lasers, the population inversion results from a nonequilibrium electronic distribution in the conduction subbands of properly designed coupled quantum wells or superlattices [15, 16]. Nonradiative electronic decay from a higherenergy subband to a lowerenergy one is primarily mediated by the emission of longitudinal optical (LO) phonons, as illustrated schematically in Fig. 3.1. This relaxation mechanism can be extremely fast; the corresponding carrier lifetime Ĳ ranges from a few picoseconds to a few hundred femtoseconds [17], depending on the mutual wave function overlap and energy separation between the initial and final electronic states. Thus, in QC lasers the dynamics of the population inversion are significantly faster compared to all other laser systems, by 3 orders of magnitude or more. Incidentally, this also means that intersubband active materials have intrinsically low radiative efficiencies; highperformance lasing is nonetheless obtained with these materials, through the design of active stages with particularly shortlived lower laser levels and through the use of the cascading scheme. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_109_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
109
E
F
E3 hν E2 E1
k
Figure 3.1 Inplane energy dispersion of the bottom three subbands of a typical QC laser active stage. The optical transitions are denoted by the dotted arrows. The solid arrows illustrate nonradiative decay processes mediated by the emission of LO phonons. The time scale of these processes ranges from a few picoseconds to a few hundred femtoseconds. The energy separation of the bottom two subbands is by design approximately equal to the LO phonon energy, which makes the intersubband relaxation rate between these two subbands particularly fast.
From the point of view of highspeed laser dynamics, the ultrafast carrier lifetime of QC lasers is an attractive feature with important implications. As described below, it leads to an ultrawide modulation response with no relaxation oscillation resonance—unlike all other laser systems—and with an intrinsic cutoff frequency that can exceed 100 GHz [18–21]. Combined with the negligibly small chirp parameter of intersubband transitions at their line center [15, 22–24], these properties make QC lasers ideally suited for use as highspeed optical data sources. Some work to explore this application has already been reported, in particular in the area of optical wireless communications [25–27] where the use of midinfrared (midir) light has potential advantages [28]. In addition, these properties provide a major motivation to the development of QC lasers operating at nearir wavelengths, for use in ultrabroadband fiberoptic communications. Another unique feature of intersubband devices—with important implications to their dynamic properties—is the giant ultrafast optical nonlinearities associated with real electronic transitions between subbands. These are among the strongest optical nonlinearities ever observed, due to their resonant nature and to the large oscillator strengths of intersubband transitions [29–33]. At the same time, unlike most other resonant nonlinearities, they exhibit ultrafast response times, given by the picosecond intersubband relaxation lifetimes. This combination of ultrafast response and giant nonlinear optical coefficients is unique and has significant device applications. For example, it plays an important role in the operation of modelocked QC lasers [34, 35], where a large selfphase modulation due to a refractive index nonlinearity of the active material itself is observed. Furthermore, this combination is extremely attractive for alloptical switching and information processing applications. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_110_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 110
Chapter Three
This chapter describes the dynamic properties of QC lasers and their applications. In particular, Sec. 3.2 is devoted to the response of these devices to highspeed current modulation and to the use of directly modulated QC lasers for freespace optical communications. Section 3.3 presents various techniques that have been demonstrated to generate picosecond pulses with midir QC lasers, namely, gain switching, active mode locking, and passive mode locking. Finally, in Sec. 3.4 a brief outlook for future directions of research in this area is presented. 3.2 HighSpeed Modulation Properties of Quantum Cascade Lasers 3.2.1 Absence of relaxation oscillations and ultrawide bandwidth
The dynamic properties of a laser manifest themselves most directly in its modulation response, i.e., the laser modulation efficiency as a function of modulation frequency. This is obtained by adding a smallsignal timeharmonic component of frequency ȍ to the pumping level above threshold and measuring the corresponding harmonic component of the output power as a function of ȍ. The modulation response of a typical highspeed interband diode laser is plotted in Fig. 3.2 (dashed line); its main feature is a pronounced resonance peak associated with relaxation oscillations. These are coupled damped oscillations of the population inversion and the laser field toward their steadystate values, which follow any dynamic change in the laser pumping level [36]. The coupling and damping mechanisms are provided by stimulated emission and gain saturation. As shown in Fig. 3.2, these transient oscillations produce a resonance enhancement of the laser modulation response at their characteristic frequency fR, typically a few gigahertz in interband lasers. Furthermore, the modulation response becomes increasingly weaker as the drive frequency is increased above this resonance, so that fR provides a measure of the laser intrinsic modulation bandwidth. In QC lasers the situation is radically different, as illustrated by the continuous line in Fig. 3.2. Due to the ultrafast carrier relaxation dynamics in these devices, transient oscillations of the population inversion and hence of the photon density are overdamped, and no resonance appears in the frequency response. The modulation dynamics of QC lasers are then, to a large extent, simply limited by their picosecond carrier lifetime, so that intrinsic bandwidths in excess of 100 GHz can be obtained. We emphasize that this is the only laser system demonstrated so far that does not exhibit relaxation oscillations.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_111_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
111
Modulation response (dB)
10
5 0 5 Interband QC laser
10
15 1
10 Modulation frequency (GHz)
100
Figure 3.2 Schematic modulation response of a typical interband diode laser (dashed line) and QC laser (solid line). The latter is characterized by the absence of the relaxation oscillation resonance and by a cutoff frequency that can exceed 100 GHz.
This property of QC lasers has been extensively investigated in the past few years, both theoretically [18–21] and experimentally [20]. Early work [18] even predicted the possibility of terahertz cutoff frequencies, although this conclusion has been subsequently disputed [21]. To put this discussion in a quantitative framework, here we use a simple argument based on the “textbook” expression for the laser modulation response [36]. This is characterized by two poles at the following complex frequencies
Ȧ± =
cg N P i 1 + ± n 2 Ĳ
(
)
cgN P 1 cg N P 1 1 + í Ĳp n n 4 Ĳ
(
)
2
(3.1)
where Ĳ is the lifetime of the upper laser state, Ĳp is the photon lifetime, c is the speed of light in vacuum, gN is the differential gain, n is the modal refractive index, and P is the intracavity photon density [the quantity n/(cgNP) is often referred to as the stimulated emission lifetime Ĳst]. This expression is very general provided that the lower laser state has negligible population, an assumption that is quite valid in QC lasers. In interband devices, the second term in the square root is negligible, so that the two poles of Eq. 3.1 have a nonzero real part. Correspondingly, a resonance is introduced in the modulation response at the frequency fR = Re(Ȧ±)/(2ʌ) (the relaxation oscillation frequency). On the other hand, in QC lasers, due to their ultrashort carrier lifetime Ĳ, the second term in the square root of Eq. 3.1 typically dominates, so that the two poles are pure imaginary and no such Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_112_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 112
Chapter Three
resonance exists. The intrinsic cutoff frequency is then given by f3 dB = Im(Ȧí)/(2ʌ) and is maximized by decreasing the lifetimes Ĳ, Ĳp, and Ĳst. The latter is inversely proportional to the output power and therefore can be minimized by operating the laser well above threshold. An important limit is obtained in the case Ĳp § Ĳ > Ĳst, where f3 dB is simply equal to 1/(2ʌĲ). Using a typical calculated value Ĳ = 1.5 ps gives f3 dB § 106 GHz. Even larger bandwidths can be achieved by decreasing the photon lifetime, e.g., shortening the cavity length, and by decreasing the carrier lifetime, e.g., increasing the wave function overlap between the upper and lower laser states as in superlattice active regions. The predicted absence of relaxation oscillations in QC lasers was experimentally verified in Ref. 20 through direct measurements of the modulation response of several devices. To minimize parasitic effects, a cryogenic highspeed laser package based on a semirigid coaxial cable and a 50ȍ microstrip line was developed. Furthermore, the devices were processed with relatively thick insulating layers underneath the top metal contacts, to reduce the chip bypass capacitance. A chalcogenide glass (Ge0.25Se0.75), deposited over the QC laser ridge by pulsed laser ablation, was used for this purpose [37]. A cross section of the resulting laser waveguide is shown in the inset of Fig. 3.3. Figure 3.4 shows exemplary modulation response traces of two QC lasers for different values of the dc drive current, measured using a highspeed quantum well infrared photodetector (QWIP) [38]. Both lasers emit near 8 m and are based on the “vertical” transition design in a threecoupledquantumwell GaInAs/AlInAs active region [39]. These devices can be operated in continuouswave (cw) mode up to about 120 K; therefore, all the data presented are for cryogenic temperatures. The dc lightcurrentvoltage characteristics of one of the lasers are plotted in Fig. 3.3. As illustrated by the data of Fig. 3.4, no relaxation oscillation resonance peak appears in the modulation response of these devices. Some features are observed in these traces that resemble weak resonance peaks (e.g., near 6 and 8 GHz), but they remain at exactly the same frequencies as the laser optical power is varied by over one order of magnitude, whereas fR strongly varies with optical power according to Eq. 3.1. Thus these features are attributed to parasitic effects. It is also important to mention that no sign of relaxation oscillations is found even for values of dc bias approaching the cw threshold for which P ĺ 0. In this limit, no matter how fast the laser intrinsic response, the relaxation oscillation frequency is expected from Eq. 3.1 to eventually enter the relatively lowfrequency range tested. Therefore these results provide conclusive evidence of the absence of relaxation oscillations in the QC lasers tested.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_113_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
113
2
0
1
Current density (kA/cm ) 2 3 4 5
6
7
8
50
30 4 20 2 10 Metal contact Active layer Insulator
0 0.0
0.1
0.2
0.3
Output power (mW)
40
6 Bias (V)
8
0
0.4
Current (A) Figure 3.3 CW lightcurrentvoltage characteristics of one of the QC lasers used to
demonstrate the absence of relaxation oscillations in these devices, measured at a temperature of 20 K. Inset: schematic cross section of the laser waveguide. The shaded areas represent, in order of increasingly dark shading, the chalcogenide dielectric blocking layer, the active material, the metal contact, and the cladding regions. The capacitance and resistance symbols indicate the main chip parasitics limiting the laser highfrequency response.
Regarding the laser modulation bandwidth, all traces in Fig. 3.4 exhibit a lowfrequency shoulder up to about 2 GHz and a cutoff frequency near 7 GHz. Both of these features are attributed to parasitic effects; in particular, from the estimated capacitance of the dielectric blocking layers C § 10 pF and the measured differential resistance above threshold R § 2 ȍ, it is concluded that the cutoff frequency is to a large extent RClimited. The experimental observation of the predicted ultrawide modulation bandwidth of QC lasers will require more extensive microwave engineering of the device package and chip layout, or alternative parasiticfree measurement techniques such as alloptical modulation by activelayer photomixing [40]. 3.2.2 Negligible linewidth enhancement factor
A characteristic feature of interband semiconductor lasers is a relatively large variation of the refractive index of the lasing mode(s) with injection current [4, 7, 36]. This property is commonly described by a parameter variously referred to as the linewidth enhancement Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_114_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 114
Chapter Three
T = 20 K
50 60
(a)
400 mA
50 60
300 mA
Modulation response (dB)
50 60
200 mA
50 60
150 mA
0.1
1
T = 80 K
50 60
10
(b)
325 mA 300 mA 250 mA
70 0.1
1
10
Frequency (GHz) Figure 3.4 (a) Exemplary highfrequency modulation response traces of the QC laser of Fig. 3.3 at 20 K, for different values of the drive current ranging from very near threshold (150 mA) up to over one order of magnitude higher photon density (400 mA). These traces were normalized with the experimental frequency response of the receiver and reflect only the modulation response of the QC laser. (b) Highfrequency modulation response of a different laser, for different values of the laser bias at 80 K.
factor, the chirp parameter, or Henry’s Į parameter after the seminal paper by C. H. Henry describing its impact on the laser linewidth [41]; it is defined as
Į = í
4ʌ dįn / d N Ȝ0 d g / d N

Ȝ = Ȝ0
(3.2)
where Ȝ0 is the freespace emission wavelength, įn is the carrier contribution to the refractive index, g is the gain coefficient, and N is the carrier density in the active region. The relatively large value of Į in interband lasers, most typically in the range of 4 to 6, has several important—and mostly undesirable— effects [4, 7, 36]. Most notably, it leads to a broadening of the laser linewidth by the factor of 1 + Į2 [41], since it causes a strong coupling
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_115_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
115
of carrier density fluctuations to variations in the index and hence in the emission frequency. This linewidth enhancement is undesirable in applications requiring a high degree of temporal coherence, such as highresolution sensing. Similarly, a large value of Į causes a significant wavelength chirping upon direct modulation [13, 14]. Combined with the large dispersion of standard optical fibers, this latter effect severely limits the use of directly modulated diode lasers as data sources in fiberoptic communications. Physically, the nonzero Į parameter of interband lasers can be traced back to the asymmetric gain spectra associated with optical transitions between two bands of opposite curvature (the conduction and valence bands) [36]. This argument is illustrated in Fig. 3.5. The carrierinduced refractive index spectrum įn(Ȝ) is related to the gain spectrum g(Ȝ) through the KramersKronig relations; by the nature of these relations, if g(Ȝ) is symmetric about the wavelength Ȝ0 of the lasing mode, then įn(Ȝ0) is zero independent of the carrier density; and vice versa, if g(Ȝ) is asymmetric about Ȝ0, then įn(Ȝ0) is nonzero and varies with N. In QC lasers the gain spectrum is symmetric to a high degree of approximation due to the very similar inplane dispersion of the lasing subbands. Thus, unlike the case of interband semiconductor lasers, įn(Ȝ0) Ł 0 and the chirp parameter is nearly zero in these devices. Incidentally, it should also be mentioned that at wavelengths sufficiently detuned from Ȝ0, the index dependence on carrier density dįn/dN is actually very large in intersubband transitions, leading to giant index nonlinearities associated with these transitions [30]. The negligible chirp parameter of intersubband lasers was predicted in the original report of QC laser action [15], and since then it has been verified in a few experiments [22–24]. In Ref. 22, the gain spectrum of a GaInAs/AlInAs 4.6ȝm device was first measured as a function of bias g
ν0
g
ν δn
ν0 Interband
ν
ν0
ν δn
ν0
ν
Intersubband
Schematic gain coefficient g and carrierinduced refractive index įn versus optical frequency Ȟ for the case of interband (left) and intersubband transitions (right). The dotted and solid lines correspond to two different values of the injected carrier density N. In the case of intersubband transitions, at the frequency Ȟ0 of maximum gain įn is zero independent of N.
Figure 3.5
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_116_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 116
Chapter Three
current with the HakkiPaoli technique [42]; the KramersKronig relations were then used to calculate the corresponding refractive index spectra. From these data, a very small value of 0.1 was obtained for the Į parameter. It should be mentioned that the numerical accuracy of this technique is limited due to the limited frequency range of the gain spectrum used in the KramersKronig integrals. In any case, this measurement provided the first experimental indication of the very small chirp parameter associated with intersubband laser transitions. A more accurate procedure has been used recently [23, 24] in which the refractive index change with bias current was determined from the measured wavelength shifts of the FabryPerot modes. In these measurements, a slightly larger—and negative—value of Į § –0.5 was obtained for a GaInAs/AlInAs 8.2ȝm device, which was attributed mainly to carrier heating effects. Finally, an indirect but very significant confirmation of the small Į parameter of QC lasers is provided by measurements of their emission linewidth: in particular, a value of 12 kHz was inferred for an 8.5ȝm QCDFB (distributed feedback) laser in a frequency stabilization feedback loop [43], which is extremely small for a semiconductor device. 3.2.3 Applications of highspeed quantum cascade lasers
As discussed in the previous sections, QC lasers can be directly modulated at speeds of several tens of gigahertz, with no spectral distortion caused by the relaxation oscillation resonance and with negligible chirp. Thus they are ideally suited to be used as data sources in broadband optical communications. The electron cascading scheme is also favorable in this respect, as it allows for slope efficiencies that are larger than the conventional limit of one emitted photon per injected electron. This is advantageous for applications in microwavephotonics communication links, whose radiofrequency (RF) gain and signaltonoise ratio are proportional to the square of the transmitter slope efficiency [44]. These considerations strongly motivate the development of QC lasers emitting at nearir wavelengths—in the lowloss transmission window of optical fibers—for use as ultrahighspeed data sources in fiberoptic communications. In the more traditional QClaser heterostructure materials, i.e., GaInAs/AlInAs lattice matched to InP and GaAs/ AlGaAs, the conduction band offset ǻEc is too small ( 0.5 eV) to accommodate nearir intersubband transitions. Therefore, novel quantumwell systems with larger ǻEc are currently being explored toward this goal, including antimonybased compounds [45] and groupIII nitrides [46–50]. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_117_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
117
In recent years, highspeed data transmission using midir QC lasers has also been investigated [51], in light of its potential application in the field of freespace optical communications [25–27]. Optical wireless is a promising approach for the development of rapidly deployable, costeffective, and secure communication links, e.g., for special events, in the battlefield, or in disaster recovery sites. Due to its favorable atmospheric transmission properties, midir light at 3 to 5 or 8 to 13 ȝm is, in principle, better suited to this application compared to nearir radiation. In particular, both light scattering and scintillation effects, which provide the dominant sources of propagation losses in optical wireless systems [52], exhibit a strong dependence on the laser frequency that favors longer wavelengths, especially under conditions of low visibility [28]. The potential of QC lasers as highspeed digital data sources was first investigated in the bit error rate (BER) measurements reported in Ref. 51. Midir devices similar to the ones discussed in Sec. 3.2.1 were directly modulated with a nonreturntozero pseudorandom bit stream at 2.5 Gb/s, and their output was measured with a highspeed QWIP. Errorfree data transmission (BER < 10–12) was obtained for a wide range of operating temperatures and bias currents. The corresponding eye diagrams are clear and open, as illustrated in Fig. 3.6a and b for an 8.1ȝm device at 20 and 85 K, respectively, although some fluctuations in the average “1” and “0” levels are observed. These are likely due to heating of the laser during long “on” times, and therefore they can be 300 200
(a)
10
3
10
5
10
7
10
9
(c)
100 0
200 300 0.0 300 200
0.2
0.4
0.6
0.8
1.0
(b)
Bit error rate
Signal (mV)
100
100 0 100
10
11
10
13
200 300 0.0
0.2
0.4
0.6
Time (ns)
0.8
1.0
6
4 2 Attenuation (dB)
0
Figure 3.6 Measured eye diagram of an 8.1ȝm QC laser at a heat sink temperature of
(a) 20 K and (b) 85 K. The bit rate is 2.5 Gb/s. (c) Corresponding bit error rate versus received power at 85 K. An attenuation of 0 dB (i.e., full transmission) corresponds to a received power of about 1 mW in this measurement.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_118_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 118
Chapter Three
expected to vanish if a returntozero modulation format is used, which is especially suitable for higher data rates. The minimum received power (where BER = 10–9 by convention) of this allintersubband transmission system is about 0.5 mW, or 50% of the total detected power, as shown in Fig. 3.6c. This is quite large compared to typical fiberoptic systems, mainly due to the lower quantum efficiency and higher noise equivalent power of the QWIP detector used and to the abovementioned variations in the detected digital levels. A similar highspeed QC laser was also used to demonstrate freespace optical transmission of complex digital data (multimedia satellite channels) over a distance of about 200 m [27]. The device was modulated with a relatively highfrequency signal (750 MHz to 1.45 GHz) received from a satellite dish, containing about 800 television channels and 100 radio channels. The modulated beam was transmitted across an outdoor 100m path to a retroreflector, mounted on a neighboring building in the Murray Hill, N.J., campus of Bell Laboratories, Lucent Technologies. The reflected beam was then collected with an f/8 telescope and detected with a highresponsivity mercury cadmium telluride detector. A total transmission loss of about 10 dB was measured, which was attributed to beam divergence and losses in the optical elements. A typical RF spectrum of the transmitted data is plotted in Fig. 3.7a (continuous line), together with the original signal from the satellite dish (dashed line). The transmission loss is found to increase with increasing frequency due to the limited bandwidth of the detector (~1 GHz); as a result, the number of actually decoded channels was reduced to around 650. A screenshot of one such channel (an
Signal level (dBm)
70 75 80 85
Transmitted signal Received signal
90
1.0
1.2 Frequency (GHz)
1.4 (b)
(a) Figure 3.7 (a) RF spectrum of a digital signal consisting of a few hundred television and radio channels as received from a satellite dish with a lownoise block downconverter (dashed line) and after transmission over a 200m freespace optical link (solid line). The link consists of an 8.1ȝm QC laser directly modulated with the signal from the down converter, bulk optics, and a HgCdTe detector. (b) Screenshot of one television channel after transmission over the same link.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_119_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
119
advertising page from the digital satellite provider) obtained with a standard satellite settop box is shown in Fig. 3.7b. Excellent video and audio quality was observed with no degradation after several hours of nonstop operation. Finally, to investigate the benefits of using midir light for optical wireless, a second beam was included in the optical path, originating from a 0.85m diode laser and detected with a standard Si detector. Similar performance was obtained from the two links under typical weather conditions. However, in the presence of dense fog, the midir link still displayed adequate transmission even as the nearir signal was below its detection limit (Fig. 3.8), as expected from the reduced atmospheric propagation losses at longer wavelengths. A more systematic comparison of the performance of nearir and QCbased midir optical wireless communication links has been carried out recently, using wellcontrolled atmospheric conditions in the Pacific Northwest National Laboratory’s Aerosol Wind Tunnel Research Facility [53]. Again the QClaser link consistently showed a higher level of performance, especially in the presence of large densities of atmospheric scatterers. 3.3 Ultrafast Pulse Generation QC lasers are also excellent candidates for the generation of ultrashort pulses of midir light due to their wellestablished strengths, such as
Signal strength (arb. units)
1 MidIR link
In (IQC / Iopt)
NearIR link
0.1
5
4
3
Time
03:21
03:50
04:19
04:48
Time Figure 3.8 Comparison of the received intensities of the midir (Ȝ = 8.1m) freespace
optical link of Fig. 3.7 and a nearir (Ȝ = 0.85m) link employing the same optics, as a function of time during a foggy night. Fog came up at around 2 a.m. and progressively dissipated during the measurement. The inset is a logarithmic plot of the ratio of the two curves in the main graph and represents the time evolution of the difference in optical losses at the two wavelengths as the structure of the fog changed.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_120_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 120
Chapter Three
compactness, low power consumption, and wavelength tunability by design, as well as their favorable dynamic properties. The development of such midir ultrafast laser sources is motivated by several applications, including timeresolved spectroscopy and coherent control of the many chemical and biological species exhibiting resonant absorption in the midir. In the following, we will review various techniques that have been employed to generate picosecond light pulses with GaInAs/AlInAs QC lasers—again based on the “vertical” transition design in threecoupledquantumwell active regions. These experiments were the first demonstrations of semiconductorbased ultrafast optical sources emitting in the midir. 3.3.1
Gain switching
Gain switching is a technique for the generation of picosecond light pulses from injection lasers, which relies on the large buildup and subsequent rapid depletion of the population inversion following a shortlived electrical excitation [5, 6]. Its main advantage lies in its inherent simplicity, since, for instance, it does not require specially fabricated devices or external cavity configurations. In Refs. 54 and 55, several QC lasers mounted in a relatively highspeed cryogenic setup were gainswitched with an integrated step recovery diode (HP 33002A comb generator), as shown in Fig. 3.9a. This device, when driven with a sinusoidal voltage waveform of the appropriate frequency and power, generates a train of electrical pulses having full width at half maximum (FWHM) as short as 90 ps, at a repetition rate of about 100 MHz. The laser emission was detected with a highspeed QWIP and measured with a sampling oscilloscope. A typical pulse obtained from a gainswitched 7.7ȝm QC laser is shown in Fig. 3.9b. The measured pulse FWHM in this figure is 89 ps, corresponding to an estimated actual FWHM ǻĲ of about 45 ps if the response time of the detection electronics (~ 61 ps) is accounted for. This is shorter than the width of the electrical pulses used to drive the laser by roughly a factor of 2 or more, since the electrical pulses are likely broadened by the laser parasitics. The reason is the finite time required for stimulated emission to build up following the initial creation of a large nonequilibrium population inversion, which effectively shortens the rise time of the optical pulses compared to the electrical ones. This is similar to what happens in gainswitched interband diode lasers. In the latter devices, each pulse essentially corresponds to the first spike of relaxation oscillations, and as a result the optical fall time can also be significantly shortened [5, 6]. In QC lasers, relaxation oscillations are overdamped, as described in Sec. 3.2.1, so that the optical pulse shape is expected to follow more closely the electrical one, except for the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_121_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
121
100 MHz
Comb generator
QC laser
(a)
Optical power (mW)
40 DC bias
20
89 ps
0 0
200
400
Time (ps)
(b) (a) Circuit diagram of the experimental setup used to demonstrate gain switching of QC lasers. (b) Oscilloscope trace of a pulse generated by a gainswitched 7.7ȝm QC laser at 10 K, measured with a highspeed QWIP. The oscillations observed after the main peak are attributed to microwave reflections between the comb generator and the laser. Figure 3.9
initial delay in photon emission. Thus, somewhat counterintuitively, the faster carrier dynamics of intersubband devices can actually lead to longer pulses in this case. 3.3.2
Active mode locking
Active mode locking of semiconductor lasers is achieved by modulating the laser current at the cavity roundtrip frequency frt (i.e., the frequency separation between neighboring longitudinal modes) so that a large number of modes are driven above threshold by the modulation sidebands of their neighbors [5, 6, 36]. This forces all the lasing modes to oscillate with their phases locked to one another; as a result, their amplitudes add coherently to produce a train of short optical pulses with repetition rate frt. Typical interband lasers are sufficiently short that the corresponding roundtrip frequencies are prohibitively large (> 100 GHz), so that external cavity configurations or multisection devices are commonly used to reduce the modulation frequency. On the other hand, optimum performance of QC lasers is achieved with relatively long devices (typically 1.5 to 3 mm) [16], so that a simple monolithic approach becomes suitable. In the first demonstration of actively modelocked QC lasers [35], 3.75mmlong devices were used, with corresponding roundtrip frequencies close to 12 GHz. These devices were processed and packaged for highspeed operation as described in Sec. 3.2.1; in the experiment, they were biased with a direct current slightly above Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_122_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 122
Chapter Three
Optical power (arb. units)
threshold and modulated with the output of a lowphasenoise synthesized RF signal generator. The initial evidence of mode locking is presented in Fig. 3.10a, where several optical spectra of the laser output are shown, corresponding to different values of the modulation frequency fm. When the detuning between frt (11.653 GHz in this case) and fm is sufficiently large (~70 MHz), as in the top and bottom traces, the spectrum consists of a single lasing mode with its modulation sidebands. As the detuning is decreased, more and more modes appear in the spectrum as they are brought above threshold by their neighbors’ sidebands, indicating effective mode locking. The dependence of the spectral response on the RF power in actively modelocked QC lasers was studied in Ref. 56. Figure 3.11 shows optical spectra of a QC laser operating at a constant dc bias I = 1.6 A and modulated at a frequency near frt, for different values of the RF power PRF. When PRF 14 dBm, the active modulation results only in the excitation of two weak neighboring modes or RF sidebands. A small increase in the RF modulation above 14 dBm triggers a considerable change in the emitted spectrum and results in the transition from cw to pulsed emission. In the pulsed emission regime, the spectral width ǻȞ (and pulse duration) depends weakly on the RF power, as shown in the inset of Fig. 3.11. A fit to the data at high RF powers gives the 0.18, following spectral width dependence on the RF power: ǻȞ 싀 I RF where I RF 싌 P RF / 50 ȍ is the RF current before the 50ȍimpedance bias tee. This result is in good agreement with theoretical predictions for actively modelocked lasers, giving ǻȞ 싀 I 0.25 [36]. RF
fM = 11.570 GHz
1.0 A
11.610 GHz 1.1 A 11.630 GHz 11.653 GHz
1.3 A
11.680 GHz 1.5 A 11.700 GHz 1.7 A
11.720 GHz
39.5 39.7 39.9 Optical frequency (THz) (a) 10 K
40.1
38.0
38.5 39.0 39.5 Optical frequency (THz) (b) 80 K
Figure 3.10 (a) Optical spectra of a 7.6ȝm QC laser under largesignal RF modulation causing active mode locking, for different values of the modulation frequency fM close to the laser roundtrip frequency (11.653 GHz). The heat sink temperature is 10 K, and the dc bias is 900 mA (approximately 11% above the laser threshold). (b) Optical spectra of the same actively modelocked device at 80 K, for different values of the dc bias. The RF drive frequency was varied at each bias to maximize the spectral width; the optimum frequencies were found to lie in the small range of 11.611 to 11.614 GHz.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_123_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
123
Power (dBm) 30 26 15 Δν (GHz)
1000
14
100
10
2 7.62
7.64
7.66
7.68
1E3
7.70
0.01
0.1
Irf (A)
7.72
Wavelength (μm) Figure 3.11 Optical spectra of a modulated QC laser at constant dc bias I = 1.6 A and temperature T = 20 K for different values of the RF modulation power. The RF frequency is f = 11.46 GHz, close to the cavity roundtrip frequency. Inset: spectral width of the QC laser emission plotted versus RF modulation current. The dc laser bias is I = 1.3 A, the temperature T = 20 K, and the modulation frequency f = 11.486 GHz. The straight line is a quadratic leastsquares fit to the data at high RF powers (data points above PRF = 2 dBm or IRF = 5.6 mA are included in this fit).
The resulting timevarying optical waveforms are too fast to be properly resolved via direct detection. An accurate characterization of their temporal features, such as pulse width and modulation depth, requires secondorder autocorrelation measurements [6]. Unfortunately, at the time of the work described in this chapter, no suitable secondorder autocorrelation setup was available for operation in the midir at the relatively low peak power levels of these devices, on the order of a few hundred milliwatts. Incidentally, work is ongoing in the labs of one of the coauthors (Capasso) to develop such a setup based on twophoton absorption in a properly designed QWIP [57]. In any case, in Ref. 35 evidence of QC laser pulsed emission and an estimate of the pulse duration were obtained from a detailed analysis of the optical spectra at resonance (i.e., for fm = frt). As shown in Fig. 3.10b, a large dip develops at the center of these spectra as the bias current is increased. This feature cannot be explained in terms of unlocked multimode cw emission, given the primarily homogeneously broadened narrow gain curves of the QC lasers used, as evidenced by subthreshold electroluminescence measurements. On the other hand, the spectral shapes of Fig. 3.10b are a classic signature of short laser pulses undergoing strong selfphase modulation (SPM) [58]. Namely, in the presence of a quadratic (Kerr) nonlinearity in the refractive index, the optical field acquires a timevarying phase proportional to the pulse intensity profile. The observation of SPM in this context is not surprising, given the very large nonlinear index n2 of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_124_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 124
Chapter Three
intersubband transitions [30], estimated at ~10í9 cm2/W in the present devices at optical frequencies slightly detuned (~100 GHz) from the line center. These considerations form the basis for a technique to estimate the duration of ultrafast laser pulses first outlined in Ref. 59. As is well known, e.g., from nonlinear optical studies in fiber optics [58], in the presence of SPM the spectrum of a train of optical pulses develops an oscillatory envelope and broadens to
ǻȦrms =
2 log 2 4 2 ɮ 1+ ǻĲ 3 3 max
(3.3)
where ǻȦrms is the rootmeansquare spectral width, ǻĲ is the pulse FWHM, and a gaussian pulse shape is assumed. Finally, ɮmax is the maximum nonlinear phase shift which in the present context is given by ɮmax =
4ʌL īn2 Imax Ȝ
(3.4)
where L is the laser cavity length, ī is the confinement factor, and Imax is the pulse peak intensity. Numerical studies [58] indicate that a first pronounced dip appears in the optical spectrum when ɮmax reaches the value 1.5ʌ; and additional dips are predicted to occur at higher values of ɮmax. Referring to the spectra in Fig. 3.10b, a dip is observed starting approximately at the bias of 1.1 A, for which ǻȦrms = 148 GHz; by using this value in Eq. 3.3 with ɮmax = 1.5ʌ, an estimate for the pulse duration of about 5 ps is obtained. Incidentally, values of ɮmax of order ʌ in these modelocked QC lasers are consistent with the pulse peak intensities—estimated from the measured average powers—and with the calculated nonlinear index n2 of the lasing transition. Numerical simulations of the amplification of picosecond pulses in QC active media also predict spectral shapes similar to the data of Fig. 3.10b [60]. In general, the minimum pulse duration of a modelocked laser is limited by the width of the gain spectrum ǻf, which is relatively narrow in QC lasers. Under ideal active modelocking conditions, the pulse FWHM ǻĲ is given by [36] ǻĲ =
2 log 2 1 1 4 ʌ M / f mǻ f
(3.5)
where M is the gain modulation depth, estimated to be near 5% for the experimental conditions of Ref. 35. Using ǻf § 3 THz for a typical 8ȝm QC laser and fm = 12 GHz, Eq. 3.5 gives ǻĲ = 4 ps, which is close Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_125_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
125
to the estimate above. To generate shorter—and hence more energetic—pulses, intersubband active media can be designed with larger gain bandwidths. In particular, ultrabroadband QC lasers have been demonstrated based on a cascade of threewell active stages of different emission wavelengths, capable of simultaneous multimode emission from 6 to 8 ȝm (ǻf § 12 THz) [61]. An investigation of active mode locking in similar devices optimized for cw operation [62] has also been reported [56]. Very broad (> 2 THz) emission spectra indicative of selfphase modulation were observed; however, these consisted of two separate groups of modes, which suggested the possibility of two independent trains of pulses simultaneously excited in the laser cavity. 3.3.3
Passive mode locking
In the case of passive or selfmode locking, a laser emits a train of ultrafast pulses with repetition rate equal to the roundtrip frequency even without any external modulation. This requires a sufficiently fast saturable loss mechanism (i.e., a source of optical loss that decreases with increasing intensity) within the laser cavity. In the presence of such a mechanism, it becomes favorable for the laser to emit ultrashort pulses because of their higher instantaneous intensity, and hence lower losses, relative to cw emission [5, 6, 36]. Typical passively modelocked interband diode lasers employ saturable absorbers, e.g., introduced by proton bombardment or ion implantation, or consisting of properly designed multiplequantumwell structures [5, 6]. In Ref. 34, passive mode locking was observed in several QC lasers based on relatively standard activematerial designs and without any intentionally introduced saturable absorbers. The experimental evidence of selfmodelocked operation in these devices is summarized in Figs. 3.12 and 3.13. Several QC lasers emitting near 5 or 8 μm were used, whose main distinctive feature is a particularly long cavity length ( 3.5 ȝm). When biased with a direct current over a wide range, these devices emit an extremely broad multimode spectrum (up to onehalf of the gain spectrum) characterized by a smooth multipeaked envelope; examples are shown in Fig. 3.12. As discussed in Sec. 3.3.2, this spectral shape is indicative of pulsed emission in the presence of strong SPM, and cannot otherwise be explained if a cw laser output is assumed. To confirm that the devices were correspondingly selfpulsating at their cavity roundtrip frequency frt, their output was detected with a fast QWIP and measured with an electrical spectrum analyzer. As shown in Fig. 3.13a, a sharp feature centered at frt (~ 13 GHz in this case) is observed, whose peak power corresponds to a modulation amplitude on the laser beam on the order of the measured average optical power. This feature results from Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_126_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 126
Chapter Three
Optical power
0.4 A 0.6 A 0.7 A 1.0 A 1.5 A 2.2 A
36
37 38 Optical frequency (THz)
0.6 A 50 60 70
Oscilloscope signal (arb. units)
QWIP photocurrent (dBm)
Figure 3.12 Optical spectra of a 3.5mmlong 8ȝm QC laser under conditions of selfmode locking for different values of the dc bias current. The laser heat sink temperature is 80 K.
1.0 A
0.7 A
0.6 A
80 12.970 12.972 Frequency (GHz) (a)
4
6 8 Time (ns) (b)
10
Figure 3.13 (a) RF spectrum of the photocurrent generated by the selfmodelocked QC laser of Fig. 3.12 in a highspeed QWIP. The laser is held at a temperature of 80 K and driven with a dc injection current of 0.6 A. (b) Oscilloscope traces of the emission of a 3.75mmlong 8ȝm QC laser under conditions of selfmode locking for different values of the bias current at 15 K. These traces were obtained by detecting the laser output with the QWIP and mixing the resulting photocurrent with a 12.008GHz reference signal in a doublebalanced RF mixer. The result is an oscillatory trace with frequency of 1 GHz, corresponding to the fundamental harmonic component of the laser output at 13.008 GHz (the roundtrip frequency of this device).
the mutual beating of adjacent modes in the optical spectrum. Its large magnitude, strong stability, and narrow width (typically less than 100 kHz) indicate the presence of at least partial phase locking among the lasing modes. Incidentally, we note that to infer complete phase locking, a stable and narrow microwave beat note at higher harmonics of the roundtrip frequency and a nonlinear autocorrelation trace with a peak value of 8:1 with respect to the background are required. In a subsequent report [63], the QWIP photocurrent from a selfmodelocked Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_127_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
127
QC laser was also analyzed directly in an oscilloscope using an RF downconversion technique with a 12GHz reference signal. Exemplary results are shown in Fig. 3.13b: periodic oscillations with relatively constant amplitude are observed, which is indicative of stable QC laser pulsations. The exact mechanism responsible for the observed selfmode locking is still the subject of experimental and theoretical investigations. In Ref. 34 it was attributed to Kerr lensing, which is well known to cause selfmode locking in Ti:sapphire and other solidstate lasers [64]. This phenomenon arises from a refractive index nonlinearity inside the laser cavity with positive nonlinear index n2, which leads to a narrowing of the laser beam diameter with increasing optical power. If the laser optical losses increase with increasing beam diameter (e.g., due to coupling of the optical mode with the top metal contacts in QC lasers), the net result is a saturable loss mechanism. Kerr lensing in selfmodelocked QC lasers is consistent with the observation of strong SPM in these devices (which is indicative of a large intracavity n2) and with their long cavity lengths (for which the abovementioned saturable loss contribution is large relative to the non saturable mirror losses). Furthermore, this interpretation was substantiated by farfield beam profile measurements, in which evidence of mode narrowing during pulsed emission was observed [34]. On the other hand, a complete theoretical description of selfmodelocked QC lasers is complicated by their very fast gain relaxation dynamics, and will likely require the inclusion of more complex and less conventional phenomena than the simple Kerrlensing mechanism just described. What is particularly unusual is the fact that the gain recovery time in these devices is shorter than their cavity roundtrip times; in existing theories of passive mode locking, the opposite is true [65]. Capasso has recently established collaboration with Franz Kaertner’s group at M.I.T. to further investigate the physics of these devices. Similarly, the temporal features of these selfmodelocked optical waveforms, i.e., their pulse duration and modulation depth, have not yet been fully characterized. As previously mentioned, the accurate measurement of these quantities requires secondorder autocorrelation techniques that are not presently available in the midir for the power levels of these devices. In the initial report of Ref. 34, the indirect technique described in Sec. 3.3.2 (based on the shape of the optical spectra) was used to estimate the pulse width; an approximate value of 3 ps was obtained for the device of Fig. 3.12. Subsequently, a different approach has been employed based on QC lasers specially designed for intracavity second harmonic generation (SHG) [63]. A portion of the conduction band diagram of these devices is given in Fig. 3.14a together with the wave functions squared of the relevant Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_128_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 128
Chapter Three
4 3 2 1
Active region
Injector
1.2 0.4
SHG power (nW)
55 kV/cm
Second harmonic power (nW)
Current (A) 1.5
1.8
1 0.1 0.01
0.01
0.05
0.09
Optical power (W)
0.2
0.0 10
20
30
40
50
60
70
80
Laser power (mW) (a)
(b)
Figure 3.14 (a) Conduction band diagram of one active stage sandwiched between
two injectors of a QC laser designed for intracavity SHG. The wave functions squared of the relevant bound states, referenced to their respective energy levels, are also shown. The laser transition is between levels 3 and 2, as indicated by the wavy arrow. A resonant nonlinearity for SHG results from the cascaded intersubband transitions 432 and 543. (b) Timeaverage power of the SHG signal versus timeaverage power of the fundamental signal, for a 4.5mmlong QC laser based on the design of (a). The solid line is a quadratic leastsquares fit to the data at low laser powers (up to 40 mW), where the laser emission is singlemode and cw. At larger power levels, the device exhibits selfmode locking. The same data on a logarithmic scale are shown in the inset.
bound states [66, 33]. The laser transitions occur between the states labeled 3 and 2 in the active stages; at the same time, two triplets of equally spaced levels (345 and 234) allow for resonant SHG. As a result, the emission of these devices contains a fundamental signal near 7.2 ȝm and its second harmonic near 3.6 m. QC lasers based on this design—and with sufficiently long cavities—were also found to selfmodelock, and an estimate of their pulse width was obtained from the dependence of the timeaverage SHG power on the power of the fundamental signal. This is plotted in Fig. 3.14b for a 4.4mmlong device. At fundamental powers below ~40 mW, the emission is singlemode and cw, and the SHG power is well described by the squarelaw fit shown by the solid line. At larger fundamental power levels 65 mW, the laser reaches a regime of pulsed emission, and a substantial increase in SHG power relative to the solid line is observed, by a factor k of about 5.6. This increase is due to the larger instantaneous fundamental power—and hence larger SHG efficiency—during pulsed emission and can be written as
k=
2 ln 2 T ʌ ǻĲ
(3.6)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_129_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
129
where T is the cavity roundtrip time, ǻĲ is the pulse FWHM, and a gaussian pulse shape is assumed [63]. From the measured value of k § 5.6 and T § 104 ps, a pulse duration of about 12 ps was inferred for this device. This result is in fair agreement with the value (9 ps) estimated for the same device by using Eq. 3.3. 3.4 Conclusions and Outlook In conclusion, we have described the highspeed modulation properties of QC lasers and the use of these devices to generate ultrashort pulses of midir radiation. Intersubband laser transitions are unique in their very fast relaxation lifetimes of order 1 ps—much faster than even the typical cavity roundtrip times. In addition they are characterized by a negligible linewidth enhancement factor and simultaneously by a very large nonlinear index at optical frequencies sufficiently detuned (~ 100 GHz) from their line center. These features lead to interesting and favorable dynamic properties, including the absence of relaxation oscillations, ultrawide modulation bandwidths, and the lack of wavelength chirping upon direct modulation, all of which have been reviewed in this chapter. Furthermore we have described the experimental demonstration of gainswitched, actively modelocked, and selfmodelocked QC lasers, which represent the first semiconductorbased ultrafast lasers in the midir. An important implication of these unique dynamic features is the prediction that directly modulated QC lasers can, in principle, provide superior highspeed performance compared to all existing optical data sources, both direct and externally modulated (the latter having the disadvantage of added optical losses, higher RF power consumption, and larger footprint). In addition, the combination of large optical nonlinearities and ultrafast response is very attractive for alloptical information processing, a key enabling ingredient of future ultrabroadband communication networks which is not adequately covered by existing device technologies. As a result, significant interest currently exists in the development of intersubband devices at nearir wavelengths, for operation in fiberbased optical communications. Toward this goal, novel quantum well systems with sufficiently large conduction band offsets are being explored [45–50]. A second important direction of future work in this area is the further investigation of modelocked emission from QC lasers. So far the temporal characteristics of their output waveforms—most notably their pulse widths—have only been estimated by using indirect methods. The development of highperformance ultrafast QC lasers would certainly benefit from the availability of a sensitive secondorder autocorrelation measurement system at midir wavelengths. The use of QWIPs based Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_130_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 130
Chapter Three
on twophoton absorption is particularly promising in this respect [57]. In addition, a complete theoretical description of the observed selfmodelocked operation has yet to be reported. Its development will be extremely valuable to clarify the physics of these devices and perhaps to provide guidelines for the design of QC lasers particularly well suited for ultrafast pulsed emission. 3.5 Acknowledgments Several past and present collaborators have made significant contributions to the research described in this chapter, and their work is gratefully acknowledged. We would especially like to thank the following researchers: J. N. Baillargeon, C. G. Bethea, A. Y. Cho, S. N. G. Chu, L. Diehl, C. Gmachl, A. L. Hutchinson, H. Y. Hwang, F. X. Kartner, M. L. Peabody, A. M. Sergent, D. L. Sivco, and E. A. Whittaker. References 1.
K. Y. Lau and A. Yariv, IEEE J. Quantum Electron. 21, 121 (1985).
2.
R. S. Tucker, J. Lightwave Technol. 3, 1180 (1985).
3.
J. E. Bowers, Solid State Electron. 30, 1 (1987).
4.
M. Osinski and J. Buus, IEEE J. Quantum Electron. 23, 9 (1987).
5.
K. Y. Lau, J. Lightwave Technol. 7, 400 (1989).
6.
P. Vasil’ev, Ultrafast Diode Lasers: Fundamentals and Applications (Artech House, Norwood, MA, 1995).
7.
L. A. Coldren and S. W. Corzine, Diode Lasers and Photonic Integrated Circuits (Wiley, New York, 1995), chap. 5.
8.
P. Vasil’ev and A. B. Sergeev, Electron. Lett. 25, 1049 (1989).
9.
S. Sanders, L. Eng, J. Paslaski, and A. Yariv, Appl. Phys. Lett. 56, 310 (1990).
10.
Y. K. Chen, M. C. Wu, T. TanbunEk, R. A. Logan, and M. A. Chin, Appl. Phys. Lett. 58, 1253 (1991).
11.
S. Arahira, Y. Matsui, and Y. Ogawa, IEEE J. Quantum Electron. 32, 1211 (1996).
12.
J. E. Bowers, B. R. Hemenway, A. H. Gnauck, and D. P. Wilt, IEEE J. Quantum Electron. 22, 833 (1986).
13.
C. Harder, K. J. Vahala, and A. Yariv, Appl. Phys. Lett. 42, 328 (1983).
14.
T. L. Koch and J. E. Bowers, Electron. Lett. 20, 1038 (1984).
15.
J. Faist, F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho, Science 264, 553 (1994).
16.
C. Sirtori and R. Teissier, Chap. 1 of this book.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_131_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
131
17.
T. Elsaesser, Chap. 4 of this book.
18.
N. Mustafa, L. Pesquera, C. Y. L. Cheung, and K. A. Shore, IEEE Photon. Technol. Lett. 11, 527 (1999).
19.
J. Faist, F. Capasso, C. Sirtori, D. L. Sivco, and A. Y. Cho, Quantum Cascade Lasers in Intersubband Transition in Quantum Wells: Physics and Device Application II, (Academic Press, London, 2000), chap. 8.
20.
R. Paiella, R. Martini, F. Capasso, C. Gmachl, H. Y. Hwang, D. L. Sivco, J. N. Baillargeon, A. Y. Cho, E. A. Whittaker, and H. C. Liu, Appl. Phys. Lett. 79, 2526 (2001).
21.
F. Rana and R. J. Ram, Phys. Rev. B65, 125313 (2002).
22.
J. Faist, F. Capasso, C. Sirtori, D. L. Sivco, A. L. Hutchinson, and A.Y. Cho, Appl. Phys. Lett. 67, 3057 (1995).
23.
M. Lerttamrab, S. L. Chuang, C. Gmachl, D. L. Sivco, F. Capasso, and A. Y. Cho, J. Appl. Phys. 94, 5426 (2003).
24.
J. Kim, M. Lerttamrab, S. L. Chuang, C. Gmachl, D. L. Sivco, F. Capasso, and A. Y. Cho, IEEE J. Quantum Electron. 40, 1663 (2004).
25.
R. Martini, C. Gmachl, J. Falciglia, F. G. Curti, C. G. Bethea, F. Capasso, E. A. Whittaker, R. Paiella, A. Tredicucci, A. L. Hutchinson, D. L. Sivco, and A. Y. Cho, Electron. Lett. 37, 191 (2001).
26.
S. Blaser, D. Hofstetter, M. Beck, and J. Faist, Electron. Lett. 37, 778 (2001).
27.
R. Martini, C. Bethea, F. Capasso, C. Gmachl, R. Paiella, E. A. Whittaker, H. Y. Hwang, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, Electron. Lett. 38, 181 (2002).
28.
V. E. Zuev, in Laser Monitoring of the Atmosphere, E. D. Hinklet ed. (Springer, Heidelberg, 1976).
29.
M. M. Fejer, S. J. B. Yoo, R. L. Byer, A. Harwit, and J. S. Harris, Jr., Phys. Rev. Lett. 62, 1041 (1989).
30.
M. Segev, I. Grave, and A. Yariv, Appl. Phys. Lett. 61, 2403 (1992).
31.
F. Capasso, C. Sirtori, and A. Y. Cho, IEEE J. Quantum Electron. 30, 1313 (1994).
32.
E. Rosencher, A. Fiore, B. Vinter, V. Berger, Ph. Bois, and J. Nagle, Science 271, 168 (1996).
33.
C. Gmachl, O. Malis, and A. A. Belyanin, Chap. 5 of this book; A. A. Belyanin, M. Troccoli, and F. Capasso, Chap. 6 of this book.
34.
R. Paiella, F. Capasso, C. Gmachl, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, Science 290, 1739 (2000).
35.
R. Paiella, F. Capasso, C. Gmachl, H. Y. Hwang, D. L. Sivco, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, Appl. Phys. Lett. 77, 169 (2000).
36.
A. Yariv, Quantum Electronics, 3d ed. (Wiley, New York, 1989).
37.
C. Gmachl, H. Y. Hwang, R. Paiella, D. L. Sivco, J. N. Baillargeon, F. Capasso, and A. Y. Cho, IEEE Photon. Technol. Lett. 13, 182 (2001).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_132_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers 132
Chapter Three
38.
H. C. Liu, J. Li, M. Buchanan, and Z. R. Wasilewski, IEEE J. Quantum Electron. 32, 1024 (1996).
39.
C. Gmachl, A. Tredicucci, F. Capasso, A. L. Hutchinson, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, Appl. Phys. Lett. 72, 3130 (1998).
40.
M. A. Newkirk and K. J. Vahala, Appl. Phys. Lett. 52, 770 (1988).
41.
C. H. Henry, IEEE J. Quantum Electron. 18, 259 (1982).
42.
B. W. Hakki and T. L. Paoli, J. Appl. Phys. 46, 1299 (1975).
43.
R. M. Williams, J. F. Kelly, J. S. Hartman, S. W. Sharpe, M. S. Taubman, J. L. Hall, F. Capasso, C. Gmachl, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, Optics Lett. 24, 1844 (1999).
44.
C. H. Cox, H. V. Roussell, R. J. Ram, and R. J. Helkey, Technical Digest for International Topical Meeting on Microwave Photonics 1998, 157 (1998).
45.
A. Neogi, Chap. 10 of this book.
46.
C. Gmachl, H. M. Ng, S.N. G. Chu, and A. Y. Cho, Appl. Phys. Lett. 77, 3722 (2000).
47.
K. Kishino, A. Kikuchi, H. Kanazawa, and T. Tachibana, Appl. Phys. Lett. 81, 1234 (2002).
48.
D. Hofstetter, S.S. Schad, H. Wu, W. J. Schaff, and L. F. Eastman, Appl. Phys. Lett. 83, 572 (2003).
49.
N. Iizuka, K. Kaneko, and N. Suzuki, Electron. Lett. 40, 962 (2004).
50.
I. Friel, K. Driscoll, E. Kulenica, M. Dutta, R. Paiella, and T. D. Moustakas, J. Crystal Growth 278, 387 (2005).
51.
R. Martini, R. Paiella, C. Gmachl, F. Capasso, E. A. Whittaker, H. C. Liu, H. Y. Hwang, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, Electron. Lett. 37, 1290 (2001).
52.
P. F. Szajowski, G. Nykolak, J. J. Auburn, H. M. Presby, G. E. Tourgee, E. J. Korevaar, J. Schuster, and I. I. Kim, Proc. SPIE, Optical Wireless Communications, E. J. Korevaar, ed., vol. 3552, 29 (1998).
53.
R. Martini, C. Glazowski, E. A. Whittaker, W. W. Harper, Y. F. Su, J. F. Shultz, C. Gmachl, F. Capasso, D. L. Sivco, and A. Y. Cho, Proc. SPIE, Quantum Sensing and Nanophotonic Devices, M. Razeghi and G. J. Brown, eds., vol. 5359, 196 (2004).
54.
R. Paiella, F. Capasso, C. Gmachl, C. G. Bethea, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, and A. Y. Cho, Appl. Phys. Lett. 75, 2536 (1999).
55.
R. Paiella, F. Capasso, C. Gmachl, C. G. Bethea, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, IEEE Photon. Technol. Lett. 12, 780 (2000).
56.
A. Soibel, F. Capasso, C. Gmachl, M. L. Peabody, A. M. Sergent, R. Paiella, H. Y. Hwang, D. L. Sivco, A. Y. Cho, H. C. Liu, C. Jirauschek, and F. X. Kartner, IEEE J. Quantum Electron. 40, 844 (2004).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_133_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers HighSpeed Operation and Ultrafast Pulse Generation
133
57.
H. C. Liu and H. Schneider, Chap. 7 of this book.
58.
G. P. Agrawal, Nonlinear Fiber Optics (Academic Press, San Diego, 1995), chap. 4.
59.
C. H. Lin and T. K. Gustafson, IEEE J. Quantum Electron. 8, 429 (1972).
60.
J. M. Tang, P. S. Spencer, and K. A. Shore, Appl. Phys. Lett. 77, 2449 (2000).
61.
C. Gmachl, D. L. Sivco, R. Colombelli, F. Capasso, and A. Y. Cho, Nature 415, 883 (2002).
62.
A. Soibel, F. Capasso, C. Gmachl, D. L. Sivco, M. L. Peabody, A. M. Sergent, and A. Y. Cho, Appl. Phys. Lett. 83, 24 (2003).
63.
A. Soibel, F. Capasso, C. Gmachl, M. L. Peabody, A. M. Sergent, R. Paiella, D. L. Sivco, A. Y. Cho, and H. C. Liu, IEEE J. Quantum Electron. 40, 197 (2004).
64.
D. E. Spence, P. N. Kean, and W. Sibbett, Optics. Lett. 16, 42 (1991).
65.
H. Haus, IEEE J. Quantum Electron. 12, 169 (1976).
66.
N. Owschimikow, C. Gmachl, A. A. Belyanin, V. Kocharovsky, D. L. Sivco, R. Colombelli, F. Capasso, and A. Y. Cho, Phys. Rev. Lett. 90, 043902 (2003).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH03_134_03/23/2006 HighSpeed Operation and Ultrafast Pulse Generation with Quantum Cascade Lasers
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_135_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
4 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures
Thomas Elsaesser MaxBornInstitut für Nichtlineare Optik und Kurzzeitspektroskopie MaxBornStr. 2 A D12489 Berlin, Germany
4.1
Introduction
Intersubband (IS) excitations in lowdimensional semiconductors have been a topic of research for more than 30 years [1–4]. Starting from early work on heterostructures [5], linear IS absorption spectra have been studied for a large variety of quasitwodimensional semiconductors made from IIIV and IIVI material systems. Such experimental work has been complemented by detailed theoretical calculations, addressing electronic subband structure, transition energies, dipole strength, and selection rules as well as Coulomb mediated manybody effects among carriers, the latter mostly for electrons. The dynamics of intersubband excitations and related carrier relaxation can be inferred only indirectly from experiments under steadystate conditions. Such dynamics occur in the ultrashort time domain and are relevant for understanding both the basic physical properties of IS excitations and the highspeed, highfrequency response of optoelectronic devices making use of IS transitions [6]. Femtosecond nonlinear spectroscopy in the midto farinfrared spectral range represents a powerful method for studying such phenomena [7]. 135
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_136_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 136
Chapter Four
It allows for a realtime observation of the fundamental nonequilibrium dynamics, in this way separating different types of processes. There are three different regimes of ultrafast IS response: 1. Resonant excitation of an IS transition by a coherent electric field transient generates a quantumcoherent superposition of electron wave functions in the optically coupled subbands, resulting in a coherent macroscopic IS polarization. As long as such polarization exists, it has a welldefined phase relationship with the external electric field, allowing for its nonlinear control by ultrashort pulses. The IS polarization is subject to phasedestroying scattering processes of carriers, leading to a dephasing on a (sub)picosecond time scale. In the linear IS absorption spectra, this dephasing gives rise to a homogeneous broadening of the spectral envelope. 2. Coherent optical excitation can also induce coherent electron motion in IS devices under bias. Electron wave packets consisting of a nonstationary superposition of subband wave functions are relevant for coherent tunneling in quantum cascade strucures and other devices based on vertical transport. 3. After the decay of quantum coherence by dephasing, the ultrafast IS dynamics are entirely determined by transient carrier distributions in the different subbands and their relaxation. Coulomb interactions within the carrier plasma as well as different types of carrierphonon interactions lead to carrier thermalization, i.e., the formation of a quasiequilibrium distribution, and subsequent cooling by phonon emission. Femtosecond studies of IS excitations have provided detailed insight into the phenomena outlined above and, in particular, have allowed for dissecting the different nonequilibrium processes in the timeresolved response. In addition, first experiments on coherent nonlinear control of IS excitations and coherent carrier transport in quantum cascade structures have been reported. Such work is reviewed in this chapter with the main emphasis on ultrafast IS dynamics of singlecomponent carrier plasmas, i.e., electrons or holes, in quantum wells and quantum cascade structures. The chapter is organized as follows. In Sec. 4.2, the basic properties of IS excitations in semiconductor quantum wells are introduced, followed by a description of experimental techniques applied in ultrafast spectroscopy (Sec. 4.3). Coherent optical IS excitations and phase relaxation are discussed in Sec. 4.4. Section 4.5 gives an overview of carrier relaxation following IS excitation, including inter and intrasubband carrier relaxation and cooling. In Sec. 4.6, recent optical studies of electron transport in quantum cascade
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_137_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
137
structures are presented, providing evidence for the quantumcoherent character of electron transport into the optically active region of such device structures. Conclusions are given in Sec. 4.7. 4.2 Optical Intersubband Excitations in Semiconductor Quantum Wells Optical intersubband transitions of electrons have been investigated in a variety of quasitwodimensional semiconductors, i.e., heterostructures, quantum wells (QWs), and superlattices, mainly by measuring the linear IS absorption bands and, to a lesser extent, IS emission spectra. As most ultrafast timeresolved studies of IS excitations have concentrated on QWs, the following discussion is restricted to such systems [8–12]. For a more extended discussion of IS transitions, see Ref. 4. Quantum confinement of electrons and holes results in the formation of conduction and valence subbands which are characterized by a quantization of the carrier k vector and energy in the direction perpendicular to the QW plane and quasifree carrier motion in the QW plane with a continuous energy dispersion as a function of the inplane k vector kฌ = (kx, ky ) (Fig. 4.1). Doping the QW or modulationdoping the barriers introduces a quasistationary electron or hole plasma populating the lowest subband. IS absorption of light induces a transition between different subbands, i.e., changes the quantized kz value, whereas the inplane wave vector remains unaffected (apart from the very small photon momentum). Consequently, the IS dipole points into the direction perpendicular to the QW layer. In a singleparticle picture, the dipole moment
ฒ
M IS ∝ e
crystal
ฒ
ȗ ( z ) Ș 썉 z ȗಾ( z ) d z
cell
u(r)u* (r) d 3 r
(4.1)
is taken between the envelope functions ȗ(z) and ȗƍ(z) of the optically coupled subbands (in the first integral, e is elementary charge and Ș is polarization vector of light) weighted by the (second) integral over the cellperiodic Bloch functions [13]. The second integral yields unity when normalized Bloch functions are used. For an infinitely deep QW of thickness L, the dipole moment of the n = 1 ĺ 2 transition is given by MIS = (16 / 9ʌ2 )eL. The large spatial extension of the envelope functions on a nanometer length scale L results in large IS dipole moments and absorption cross sections of up to 10í13 cm2. The polarization selection rules for symmetric QWs allow IS transitions between subbands of different parity, that is, n = 1 ĺ 2, n = 2 ĺ 3, n = 1 ĺ 4, but not n = 1 ĺ 3. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_138_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 138
Chapter Four
E
GaAs 2
Absorption
AI0.35Ga0.65As
3
1 kll
z
90 100 110 Photon energy (meV)
(a)
k
(110)
k
(100) 0.3
HH B LHSO 2
12
1.2 x 10
cm
0.2
HH 2
ptype δdoping 2
LH HH
0.1
LHSO 1
Hole energy (eV)
0.4
Si
SO
0.0
HH 1
1.0 d = 4.4 nm
0.5 1.0
0.5
0.0 9
0.5
0.0 1.0
2 2 MlS (nm )
Ge0.5Si0.5
Si
150
200
Photon energy (meV)
1
kll (10 m ) (b) Figure 4.1 (a) Schematic of the conduction subband structure of a quantum well with
quantized electron energies for motion in the direction perpendicular to the QW plane and a quasifree continuum of states for inplane motion. The panel on the righthand side shows the IS absorption line of an ntype modulationdoped GaAs/Al0.3Ga0.7 As multipleQW structure containing 51 QWs of 10nm width (electron concentration 5 × 1010 cmí2, sample temperature 10 K). (b) Schematic of the valence subband structure of a 4.4nmwide Si0.5Ge0.5/Si quantum well. The inplane dispersion of the strongly mixed heavyhole (HH), lighthole (LH), and splitoff (SO) bands and the IS dipole moment 2 M IS was calculated with the k·p method. The HH1 ĺ HH2 absorption line measured with a sample containing 10 QWs is shown on the righthand side (hole concentration 1.2 × 1012 cmí2, sample temperature 15 K).
In general, the line shape of IS transitions is determined by the inplane subband dispersion, manybody effects in the carrier plasma, and scattering processes resulting in a broadening of the transition. In a singleparticle picture, IS transitions originating from different kฌ states are uncoupled, and the overall IS absorption spectrum represents a superposition of transitions from all populated initial states. For a nearly parallel dispersion of conduction subbands (Fig. 4.1a), the transition energy is independent of kฌ, resulting in a deltalike joint density of states and a narrow IS absorption line centered at EIS = Ej í Ei, where Ej,i are the band minima of the optically Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_139_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
139
coupled subbands. For nonparallel inplane dispersions of the optically coupled bands, the transition energies cover a certain range resulting in an inhomogeneous broadening of the IS absorption. In a similar way, sample imperfections, e.g., fluctuations of the QW thickness, alloy fluctuations, and carrier localization in disordered QWs lead to a distribution of transition energies and inhomogeneous broadening. For valence subbands with their strong mixing of heavy and light hole states, the distribution of transition energies is highly complex and the IS dipole moment becomes kdependent (Fig. 4.1b). Manybody effects in the carrier plasma modify this singleparticle picture substantially [1, 14–20]. Coulomb interactions result in a coupling of IS transitions from different kฌ states, affecting the energy position, shape, and width of the absorption line. A coherent excitation of coupled IS transitions leads to collective charge oscillations in the z direction. The corresponding charge separation during such oscillations generates additional restoring forces, i.e., makes the plasma more rigid, and thus blueshifts the absorption line [1]. This depolarization shift is accompanied by a substantial spectral narrowing of the IS absorption [17]. In addition to the depolarization shift, exchange interactions occur between an electron excited to a higher subband and the quasihole left behind in the original carrier distribution. This interaction partly compensates the depolarization blue shift. There are theoretical predictions of excitonic IS features due to the attractive Coulomb interaction between the excited electron and the quasihole which have, so far, not been identified in experiments [21, 22]. Manybody effects are particularly pronounced at high carrier concentrations in wide QWs. For narrow GaAs/AlGaAs QWs of sub10nm width and low carrier concentrations N 싨 5 × 1010cm2, they are less relevant, and one observes a behavior closer to that of the singleparticle picture. Scattering processes that destroy the quantum mechanical phase between the optically coupled subbands lead to a dephasing of the macrosopic coherent IS polarization and a corresponding broadening of the IS absorption line [7, 23]. Carriercarrier and carrierphonon scattering and scattering from the QW disorder potential are processes relevant for dephasing. In the absence of memory effects, i.e., in the Markov limit, dephasing results in a homogeneous broadening ǻ Ȧ = 2 / T2 characterized by the dephasing time T2, the decay time of the macroscopic polarization. Dephasing is discussed in greater detail in Sec 4.4. So far, IS transitions in individual QWs have been considered. In multipleQW systems containing a highdensity carrier plasma, radiative coupling effects of IS excitations in different QWs may occur [24, 25]. Under such conditions, the local electric field acting on a particular QW consists of a superposition of the external light field and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_140_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 140
Chapter Four
the internal optical field generated by excitation of the other QWs. Such coupling leads to strong changes of both the linear and nonlinear IS response. The IS absorption spectrum in Fig. 4.1a was recorded with an ntype modulationdoped GaAs/Al0.3Ga0.7As multipleQW sample of high structural quality and low electron concentration (51 QWs of L = 10 nm width, electron density N = 5 × 1010cm2 ) [26]. The sample was processed into a prism to achieve interaction of the IS dipole and the z component of the incident electric field. The absorption line displays a small width of approximately 4 meV, pointing to a negligible inhomogencous broadening. In Fig. 4.1b, the IS absorption band of holes in Si0.5Ge0.5/Si QWs is shown ( N = 1.2 × 1012cm2 ). Calculations suggest a kdependent dipole moment and a substantial inhomogencous broadening of this line [27]. Steadystate linear spectroscopy does not allow for a separation of the different broadening mechanisms and the underlying couplings between different elementary excitations, resulting in complex carrier dynamics. The basic nonequilibrium dynamics of carriers occur in the ultrafast time domain below 1 ps, and thus nonlinear infrared spectroscopy with femtosecond time resolution has developed into an important tool to unravel such phenomena. This has provided detailed insight into both coherent IS polarizations and carrier dynamics following IS excitation, as will be discussed in the following. 4.3 Experimental Techniques Femtosecond studies of IS dynamics are based on nonlinear spectroscopy using ultrashort pulses in the mid to farinfrared spectral range. In this section, the state of the art in infrared pulse generation is briefly reviewed, followed by an introduction to the spectroscopic methods for monitoring ultrafast coherent and incoherent carrier dynamics. 4.3.1
Femtosecond midinfrared pulses
Femtosecond midinfrared generation relies mainly on nonlinear frequency conversion of laser pulses at shorter wavelength in the nearinfrared. Freeelectron lasers represent another type of infrared source that is presently undergoing a rapid development [28] but has found limited application in IS spectroscopy so far [29]. The secondorder nonlinearity Ȥ(2) of transparent bulk crystals is exploited to generate femtosecond midinfrared pulses by parametric amplification, differencefrequency mixing, and/or optical rectification [30, 31]. Pulses at center frequencies Ȧp, Ȧs, and Ȧi with Ȧp = Ȧs + Ȧi and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_141_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
141
Ȧi < Ȧs < Ȧp ( p: pump, s: signal, i: idler) interact with one another in the nonlinear medium [30] under nonresonant conditions; i.e., absorption in the nonlinear material is negligible at all three frequencies. In parametric generation and amplification, pulses at Ȧs and Ȧi are generated and amplified by transferring energy from an intense pump pulse at Ȧp. In differencefrequency mixing, pulses at Ȧi = Ȧp – Ȧs are derived from two input pulses at Ȧp and Ȧs. Optical rectification represents a special case of differencefrequency mixing where Ȧ p 싇 Ȧs and Ȧi 싇 ǻ Ȧ, the spectral bandwidth of the input pulses. The phase relationship between the electric fields of the three interacting pulses is set by the phasematching condition k p = k s +k ki , where kp,s,i= np,s,i(Ȧp,s,i/c) are the respective wave vectors. This phasematching condition can be fulfilled by adjusting the refractive indices np,s,i in birefringent nonlinear media (c: vacuum velocity of light) [30]. Changing the phasematching angle through rotation or variation of the temperature of the nonlinear crystal allows for frequency tuning of the generated pulses. Even for phasematched parametric frequency conversion, the mismatch of the group velocities of the three interacting pulses limits the effective interaction length in the nonlinear medium and determines the minimum pulse duration achieved [32]. For idler wavelengths Ȝ i = 2 ʌ c / Ȧi of up to 5 ȝm, bulk and periodically poled LiNbO3, LiIO3, KNbO3, betabarium borate (BBO), and KTiOPO4 (KTP) have been used as nonlinear materials. AgGaS2 represents a standard material for Ȝi up to 12 ȝm [33], and AgGaSe2 and GaSe allow parametric mixing at even longer wavelengths up to Ȝ i 싇 20ȝm . Data on nonlinear materials and their application for frequency conversion have been collected in Ref. 31. In most sources of femtosecond infrared pulses, the peak intensities of the input pulses are between 1 GW/cm2 and 1 TW/cm2, resulting in an energy conversion efficiency into the midinfrared between several 10í5 and several percent. There are (1) parametric generation schemes for femtosecond midinfrared pulses at megahertz repetition rates and comparably low peak intensities and energies per pulse, and (2) sources for intense pulses working at much lower kilohertz repetition rates. For generating pulses of 30 to 300fs duration at high repetition rate, optical rectification of the broadband output of modelocked Ti:sapphire oscillators [34–38], optical parametric oscillators synchronously pumped by femtosecond pulse trains [39–41] and a combination of both techniques [42–44] have been applied. Such sources have found widespread applications in nonlinear spectroscopy of solids. Intense nearinfrared pulses generated in regenerative Ti:sapphire and, in some cases, Cr:forsterite amplifiers at kilohertz repetition rates have been used for pumping a variety of parametric conversion schemes. For a recent overview, see Refs. 45 and 46. In the wavelength range from Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_142_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 142
Chapter Four
2.5 to approximately 10 ȝm, such sources provide pulses of 50 to 150fs duration and energies up to 50 ȝJ [47–49]. Very recently, tunable infrared pulses with an electric field amplitude of up to megavolts per centimeter have been generated between 10 and 20 ȝm by differencefrequency mixing of spectral components of an amplified 25fs pulse in a thin GaSe crystal [50]. This technique allows for the generation of welldefined fewcycle pulses of very high peak intensity. A complete characterization of femtosecond pulses requires a measurement of their timedependent electric field in amplitude and absolute carrier phase. In contrast to the visible and nearinfrared, such measurements are possible for midinfrared electric field transients by electrooptic sampling, a technique that was originally developed for the farinfrared around 300 ȝm [51]. The infrared pulse induces a change of the refractive index in a birefringent electrooptic crystal, e.g., ZnTe, which is proportional to its momentary electric field and monitored through the polarization rotation of an ultrashort probe pulse (Fig. 4.2a). By changing the delay between infrared and probe pulse, the timedependent electric field of the infrared pulse is determined. For a quantitative measurement, the probe pulse has to be short compared to the period of the infrared field, and the group velocity dispersion in the electrooptic crystal has to be limited. Using 10fs pulses at 800 nm and ZnTe crystals typically of 10ȝm thickness, infrared pulses down to a wavelength of approximately 7 ȝm have been characterized [51]. This technique has been extended to characterize intense midinfrared pulses generated at a 1kHz repetition rate [50]. In such recent experiments, 13fs pulses from the 75MHz repetition rate oscillator of an amplified Ti:sapphire laser system sample the electric field of the midinfrared pulses at a 1kHz repetition rate. An electronic gating technique is applied to measure the polarization rotation of the probe pulse overlapping in time with the midinfrared pulse. The timedependent electric field of an intense pulse generated in a 30ȝmthick GaSe crystal is plotted in Fig. 4.2b, together with its intensity spectrum centered at 15 ȝm (Fig. 4.2c). The electric field transient gives a width of the temporal intensity envelope [full width at half maximum (FWHM), pulse duration] of approximately 50 fs. In addition to electrooptic sampling, other standard techniques for characterizing ultrashort pulses have been applied in the midinfrared. Measurements of interferometric autocorrelations and frequencyresolved optical gating (FROG) have allowed for an analysis of the optical phase of the pulses relative to a reference pulse, information sufficient to determine the frequency chirp of the pulses [52–54].
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_143_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
143
FIR beam
Wollaston Photodiodes polarizer ZnTe 13 fs 780 nm
/4 (a)
Electric field (MV/cm)
1
0
1 0.2
0.1
30
20
0.0
0.2 0.1 Time (ps) (b) Wavelength (μm) 10
0.3
Power (nirm.)
1
0 10
20
30
40
Frequency (THz) (c) Figure 4.2 (a) Experimental scheme for measuring transient electric fields by electrooptic sampling. (b) Timedependent electric field of a femtosecond midinfrared pulse generated by optical rectification in a 30mthick GaSe crystal. The signal measured in the setup of (a) is plotted as a function of the delay time between the midinfrared pulse and the 13fs nearinfrared probe pulse. The midinfrared center frequency of 20 THz corresponds to a wavelength of 15 m. The absolute field amplitude reaches very high values around 1 MV/cm. (c) Intensity spectrum of the pulse in (b).
4.3.2
Spectroscopic techniques
In the following, techniques for monitoring coherent IS excitations and carrier relaxation are outlined briefly. A coherent IS polarization induced by femtosecond excitation gives rise to a coherent emission with a carrier frequency determined by the IS transition energy (Fig. 4.3a). Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_144_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 144
Chapter Four
The temporal envelope of the emitted electric field is determined by both the driving pulse envelope and the dynamics of the IS polarization. Coherent IS emission has been studied with different phaseresolving detection schemes, e.g., based on electrooptic sampling [55, 56] or (linear) interferometry with a reference pulse [57]. In the first scheme, the emission is sampled by nearinfrared pulses which are synchronized with the infrared pulse generating the transient IS polarization. To record interferograms, a synchronized reference pulse in the midinfrared is brought to interference with the coherent emission from the sample, and the resulting signal is measured by a timeintegrating detector as a function of delay between the excitation and the reference pulse. Nonlinear spectroscopic techniques are required for a separation of the IS broadening mechanisms and the underlying microscopic interactions in the time domain. For this purpose, fourwavemixing methods exploiting the thirdorder nonlinearity of the semiconductor are a powerful tool which has been developed to high sophistication [7]. The most elementary degenerate fourwavemixing scheme is depicted schematically in Fig. 4.3b. Femtosecond pulses of identical photon energy propagating into the directions k1 and k2 generate a transient grating in the sample from which a small fraction of the respective pulse is (self)diffracted into the directions 2k2 í k1 and 2k1 í k2. These coherent thirdorder signals depend on the time delay ǻ t12, the socalled coherence time, between the first and the second pulses and thus reflect the time evolution of the coherent polarization in the sample. There are two main methods to analyze the diffracted signal: 1. In the simplest case, the diffracted intensity is recorded with a timeintegrating detector as a function of the delay time ǻ t12 (TIFWM). The signals diffracted into the directions 2k2 í k1 and 2k1 í k2 are symmetric in time with respect to zero delay between the incident pulses, the temporal separation of their maxima, the socalled peak shift, reflecting the degree of spectral inhomogeneity in the ensemble of optically driven transitions. Most experiments in the literature are based on this technique, which gives information on the buildup and decay, i.e., dephasing, of the macroscopic nonlinear polarization in the sample. For an optically thin sample, small diffraction efficiency, and perfect phasematching, the slowly varying amplitude approximation gives the following expression for the homodyne detected intensity IHOM of the diffracted signal [58]: IHOM =
ʌ Ȧ2 2 l 2n (Ȧ) c
í
( )
dt P 3 (t, ǻt12)2
(4.2)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_145_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
145
Sample
(a)
Phaseresolved detection
2
(b)
1
Sample k1
∆t12
k2
∆t13
TIFWM
3 2k2  k1
TRFWM
(c) Epr
Sample
τ
P (3) Epr
Epu
(d) Epr
Spectrograph and detector
Sample
τ
Detector
P (3) Epu
Epr
Figure 4.3 Experimental techniques of nonlinear spectroscopy. (a) Scheme of a propagation measurement. A coherent infrared pulse interacts with the sample, and the transmitted light is detected in a phaseresolved way, e.g., by electrooptic sampling, (b) Degenerate fourwavemixing scheme. Pulses 1 and 2 of mutual delay ǻt12 generate a transient grating in the sample from which a fourwavemixing signal is (self)diffracted into the direction 2k2 í k1. This signal is either detected by a timeintegrating detector (TIFWM) or timeresolved by convolution with a third reference pulse in a nonlinear crystal (TRFWM, time delay ǻt13). (c) Pumpprobe configuration with spectrally integrated detection of the probe pulse. (d) Spectrally resolved pumpprobe experiment.
for the transition frequency Ȧ, the refractive index n(Ȧ), the sample thickness l, and the thirdorder polarization P(3)(t, ǻ t12). In the simplest theoretical approximation, the nonlinear polarization has been analyzed with the optical Bloch equations for an ensemble of independent twolevel systems [7]. This approach gives a single exponential decay exp (í ǻ t12 / t decay ) of IHOM. The decay time tdecay
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_146_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 146
Chapter Four
has values of T2/2 and T2/4 for a homogeneously and an inhomogeneously broadened set of twolevel systems, respectively (T2 is the dephasing time). For semiconductors, this frequently applied model does not represent an adequate description, as it neglects the Coulomb interactions among the carriers and thus does not account for manybody effects strongly influencing the nonlinear response of a semiconductor. Here, more sophisticated models, e.g., based on the semiconductor Bloch equations, have to be used [7, 59]. 2. Information on the inherent time evolution of the diffracted signal can be obtained in timeresolved detection schemes [7, 26]. For instance, gating of the diffracted signal by sumfrequency mixing with a third pulse gives the time envelope of the diffracted intensity convoluted with the third pulse (TRFWM, Fig. 4.3b). Such measurements have provided insight into manybody and/or local field effects influencing the nonlinear response, as discussed in detail elsewhere [7]. Threepulse photon echo measurements and interferometric techniques of signal detection in which the diffracted electric field is heterodyned with a reference pulse represent other methods to analyze the temporal structure of nonlinear polarizations [60]. The incoherent redistribution of carriers following IS excitation has mainly been studied by pumpprobe methods. Such methods are based on a twopulse interaction scheme (Fig. 4.3c) in which a first pump pulse generates a population change in the optically coupled subband states. The resulting change of transmission/absorption is probed by a weak second pulse at the same or a different spectral position and is measured as a function of the delay time between pump and probe. The transmitted probe intensity is detected in a timeintegrating way, either by detecting the full probe spectrum or by dispersing the probe light to measure transient spectra. In the perturbative limit, pumpprobe studies of nonlinear absorption are thirdorder in the electric field. A thirdorder polarization is generated in the sample by two interactions with the pump and one interaction with the probe field. This polarization is detected through the field that it radiates into the propagation direction of the probe, and the two electric fields interfere on the timeintegrating detector. The measured signal reflects transient polarizations and population changes; i.e., both real and imaginary parts of the nonlinear susceptibility contribute. For a pulse envelope varying slowly in time compared to the period of the optical field, the spectrally integrated absorption change ǻĮ(Ȧpr) measured by a probe pulse of frequency Ȧpr is given by [58]
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_147_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
ǻĮ(Ȧpr) = í log
=
147
T (Ȧpr) T0(Ȧpr)
4 ʌ Ȧpr cn (Ȧpr)
Im
í
* (t ) P dt Epr
(3 )
(t, Ĳ )
/
í
dt
 Epr(t )2 (4.3)
Here, T(Ȧpr) and T0(Ȧpr) represent the transmission of the sample with and without excitation, c is the velocity of light, n(Ȧpr) is the refractive index of the sample, and Epr(t) and P(3)(t, Ĳ) are the timedependent electric field of the probe pulse and the thirdorder polarization, the latter containing the nonlinear response of the sample and depending on the pumpprobe delay Ĳ [58]. For a spectrally resolved detection of the probe pulse (Fig. 4.3d), the measured signal is given by ǻĮ(Ȧ) =
4 ʌ Ȧpr cn (Ȧ)
Epr(Ȧ)2
0
( )
* (Ȧ) Im P 3 (Ȧ) / Epr
dȦ Epr(Ȧ)2
(4.4)
dt exp(iȦt ) Epr(t ) is the Fourier transform of the Here Epr(Ȧ) = í timedependent probe field, and P(3)(Ȧ) is the nonlinear polarization component at the frequency Ȧ. Pumpprobe schemes for investigating IS excitations are displayed in Fig. 4.4. In Fig. 4.4a, the pump pulse promotes carriers from the n = 1 to the n = 2 subband by resonant absorption on the IS transition. The resulting nonlinear change of IS absorption is probed by a second pulse, either at the same spectral position as the pump or tunable in the range of the IS absorption line [61]. The nonlinear absorption changes observed in such experiments give information on the transient populations of optically coupled states in the lower and the upper subbands. In the simplest case of parallel inplane dispersions and negligible manybody effects, the absorption change is proportional to the difference of the total populations in the two subbands, and the IS relaxation time can be extracted. In general, however, intrasubband redistribution and manybody coupling of carriers contribute to the absorption change, requiring an indepth analysis of the measured signal. Changes of the carrier distribution by IS excitation also lead to changes of the nearinfrared interband absorption (Fig. 4.4b). In particular, one expects an absorption decrease by statefilling on interband transitions whose final k states are populated after the IS excitation. Similarly, initially blocked interband transitions whose final states are depopulated by IS excitation exhibit an increase of absorption (Fig. 4.4c). This fact and the selection rules for interband
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_148_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 148
Chapter Four
CB
E n e rg y
n=1 Distribution function f(E)
n=2 n=1
0
k 
1
n = 1 interband absorption α(ω) n=1 n=2 VB (a)
(b)
(c)
3
3
Pump
Injector
Probe 2
2
1
1
Injector
Active region
Active region
(d) Pumpprobe schemes for measuring carrier dynamics after IS excitation. (a) The probe pulse (dashed line) measures nonlinear changes of IS absorption induced by the pump pulse (solid line). (b) Probing of the transient (n = 2) interband absorption after resonant IS excitation. (c) Schematic of the inplane dispersion for scheme (b) with a probe pulse on the n = 1 interband transition and the n = 1 electron distribution. (d) Scheme for studying carrier transport in quantum cascade devices. The pump pulse induces a depletion of the IS population inversion on the 3 ĺ 2 transition. The motion of electrons through the injector barrier is monitored via probing transmission changes (gain recovery) on the same transition.
Figure 4.4
transitions enable one to selectively monitor the n = 1 and n = 2 carrier distributions with probe pulses in the nearinfrared [62]. In addition to absorption changes caused by population effects, the measured signal might be influenced by manybody effects. In particular, transient absorption features related to the Coulomb enhancement of the interband absorption and the Fermi edge singularity of the plasma could play a role. A recent experimental study [63] demonstrates, however, that such signals are limited to a narrow spectral range of a few millielectronvolts and show a small amplitude for moderate carrier densities at low temperatures. For 100fs probe pulses, the spectral bandwidth of the probe is much larger than this narrow energy interval, and thus population effects dominate the signals. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_149_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
149
A pumpprobe technique has also been applied to study electron transport in quantum cascade structures [64]. In such experiments, the structure was electrically biased with a quasistationary carrier distribution in the injectors and the active regions. Under conditions of population inversion between subbands 3 and 2 in each active region, a femtosecond pump pulse resonant to the IS transition 3 ĺ 2 depletes the population of subband 3 (Fig. 4.4d), leading to a decrease of the quasistationary optical gain. A probe pulse on the same transition measures the recovery of the gain as a function of pumpprobe delay, in this way monitoring electron transport from the injector into subband 3. All pumpprobe schemes of Fig. 4.4 involve a single carrier species, i.e., electrons or holes. Moreover, the total carrier concentration is constant in the schemes of Fig. 4.4a to c, and IS excitation results exclusively in a redistribution of carriers. This makes the analysis of the data much simpler than in the case of interband excitation, where both electrons and holes contribute to the optical signal. Selective observation of electron IS dynamics is also possible with interband Raman excitation, as demonstrated in Refs. 65 and 66. In such experiments, population of the n = 2 conduction subband is created by a Raman process and probed via the antiStokes Raman signal generated with a probe pulse at a different photon energy. The strength of the antiStokes signal shifted by the intersubband transition energy relative to the center of the probe pulse is measured as a function of time delay to the pump and reflects the population dynamics of the upper subband. 4.4 Coherent Intersubband Dynamics Ultrafast coherent spectroscopy has concentrated on measuring the dynamics of macroscopic IS polarizations to unravel the time scale and mechanisms of dephasing [23, 26]. More recently, the coherent infrared emission originating from IS polarizations in QWs has been analyzed in phase and amplituderesolved experiments in both the linear [55, 57] and nonlinear [55, 56] regimes. The latter work has led to the demonstration of IS Rabi flopping and, in a more general sense, coherent control of IS polarizations. 4.4.1
Intersubband dephasing
Fourwavemixing techniques have been applied to study IS dephasing. Initially, experiments were performed on the n = 1 ඎ 2 IS transition of electrons in ntype modulationdoped GaInAs/AlInAs multiple QWs of 6nm width [23]. In a degenerate fourwavemixing experiment, two Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_150_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 150
Chapter Four
infrared pulses of 130fs duration excited the IS transition resonantly, and the (self)diffracted intensity was measured as a function of the coherence time (TIFWM; see Fig. 4.3b). This signal rises within the time resolution of the experiment and displays a subsequent decay with a time constant depending on the electron concentration in the sample. For N = 1.5 × 1011 cmí2, a decay time of 80 fs was measured, whereas a sub50fs decay occurs for N = 1.5 × 1012 cmí2 . A theoretical model based on the timedependent HartreeFock equations accounting for manybody effects was used to analyze the experimental results. A dephasing time of T2 싇 300 fs and T2 200 fs was derived for an electron concentration of N = 1.5 × 1011 cmí2 and N = 1.5 × 1012 cmí 2, respectively. Such dephasing times are substantially shorter than the lifetime of electrons in the n = 2 subband of approximately 1 ps. The homogeneous line widths corresponding to the measured dephasing times are smaller than the overall width of the IS absorption lines in the different samples, pointing to a pronounced inhomogeneous broadening of the IS transitions. Such inhomogeneity originates mainly from structural imperfections of the QWs. In a second series of experiments, an ntype modulationdoped GaAs/ Al0.3Ga0.7As multipleQW sample (51 QWs) of high structural quality and L = 10 nm width was studied at a low electron density of 10 N = 5 × 10 cmí2 [26]. The IS absorption spectrum of this sample is shown in Fig. 4.1a. Degenerate fourwavemixing experiments were performed with 130fs pulses resonant to this absorption line. In addition to timeintegrated detection of the signal diffracted into the direction 2k2 í k1, its time structure was analyzed by mixing it with a 100fs reference pulse in a nonlinear crystal and measuring the resulting sumfrequency signal as a function of the delay between the reference pulse and the signal (TRFWM). In Fig. 4.5b, the fourwavemixing signal recorded with timeintegrated detection is plotted as a function of the time delay ǻt12 between the two pulses generating the transient grating. Data are presented for excitation 10 percent of the n = 1 electrons to the n = 2 subband (solid circles) and for excitation of 30 percent of the electrons (open circles). The signal rises within the time resolution of the experiment, shows a maximum at § 100 fs, and decays afterward on a time scale of 1 ps, reflecting the decay of the macroscopic IS polarization. One derives a decay time Ĳ = 160 ± 15 fs, independent of the excitation density. The lifetime T1 of electrons in the n = 2 subband was determined independently by pumpprobe measurements in which the nonlinear change of IS absorption induced by the pump pulses was monitored by weak delayed probe pulses. In Fig. 4.5a, the spectrally integrated absorption change ǻA is plotted versus the delay time between pump Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_151_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
151
Pumpprobe delay (fs) 0
∆A (norm)
10
500
1000
(a)
1
E (meV)
TIFWM signal (norm)
T = 550 fs 1 1
(b)
0.1
0.01 0
500
1000
Coherence time (fs) (a) Bleaching of the IS absorption in an ntype modulationdoped GaAs/ AlGaAs multipleQW sample measured with resonant excitation (sample temperature of 15 K). Inset: pulse spectrum (open circles) and IS absorption line (solid line). The spectrally integrated absorption change íǻA = ln(T/T0) is plotted versus the delay time between pump and probe (T and T0 are sample transmission with and without excitation respectively). The absorption change displays a single exponential decay with a time constant of T1 = 550 fs. (b) Timeintegrated fourwavemixing signal diffracted into the direction 2k2 í k1 for excitation of 10% (solid circles) and 30% (open circles) of the n = 1 electrons as a function of the time delay ǻt12 between the incident pulses (logarithmic ordinate scale). The signal decays with a time constant of 160 fs. Figure 4.5
and probe. The strong IS bleaching decays with a time constant T1 = 550 fs, i.e., markedly slower than the polarization decay in Fig. 4.5b, by relaxation of the n = 2 electrons back to the n = 1 subband. Thus, population relaxation makes a minor contribution to the dephasing of the IS polarization. Fourwavemixing experiments with timeintegrated detection give no direct information on the predominant type of spectral broadening of the IS transition, i.e., homogeneous versus inhomogeneous broadening. In the homogeneous case, one expects a free induction decay whereas a photon echolike signal occurs for an inhomogeneously broadened transition [7]. To distinguish between these two cases, we performed an experiment with timeresolved detection of the fourwavemixing signal [26]. In Fig. 4.6a, the timeresolved fourwavemixing signals are shown for different fixed values of the delay ǻt12 between the pulses generating the transient grating. With increasing ǻt12, the maximum of the signal shifts to later times. A plot of the position of the respective maximum Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_152_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Chapter Four
∆t12
∆t13
(a)
(b) m=1 Delay time ∆t12 (fs)
600 400 200 0
Peak position ∆t13 (fs)
152
87 fs 20 fs 113 fs 380 fs 513 fs 780 fs 500
0
500
1000 1500
Real time ∆t (fs) 13 Figure 4.6 (a) Timeresolved fourwavemixing signals for different fixed time delays ǻt12 of the two pulses generating the transient grating in the sample. The intensity of the upconverted signal is plotted versus the realtime delay ǻt13 between pulse 1 and the gating pulse 3. (b) Peak positions of the transient signals for different ǻt12 (symbols) compared to a linear dependence ǻt13 = ǻt12 + 13 0 fs with a slope of 1 (solid line). Inset: schematic of the pulse sequence, the polarization induced by pulse 1 (dashed line), and the FWM signal (thick solid line).
max as a function of ǻt12 displays a linear dependence ǻt13 = ǻt12 + 130 fs with a slope of 1 (Fig. 4.6b). This demonstrates that the fourwavemixing signal reaches a maximum at a fixed time (of 130 fs) after the second pulse for all values of t12. Such behavior is indicative of a freeinduction decay of the IS polarization, i.e., homogeneous broadening of the IS transition, for which the signal is emitted immediately after the second pulse [7]. In contrast, emission of a photon echo from an inhomogeneously broadened transition requires a rephasing of the polarization components at different frequencies within the line width and leads to a signal emission at ǻt12 after the second pulse. In the plot of Fig. 4.6b, this would lead to a slope of 2, which can be clearly ruled out on the basis of the experiment. The timeintegrated fourwavemixing signal originating from a homogeneously broadened system decays with a time constant of T2/2 [7]. The data in Fig. 4.5b thus give an IS dephasing time T2 = 2Ĳ = 320 fs corresponding to a homogeneous line width of 4 meV. This number is in excellent agreement with the measured line width of 3.7 meV (see Fig. 4.1a) and confirms the predominant homogeneous broadening of the IS transition in this highquality sample. Intrasubband electronelectron scattering represents the main mechanism by which the quantum mechanical phase between the n = 1 and n = 2 wave functions is destroyed. For the small electron
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_153_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
153
concentration in the sample studied, the scattering rate and thus T2 are independent of the excitation density as the phase space available for scattering remains essentially unchanged. For a similar sample with 11 í2 an electron concentration of N = 6 × 10 cm , a pronounced increase of the dephasing rate with excitation density has been found, which is related to the unblocking of phase space upon excitation of carriers to the n = 2 subband. Such behavior is discussed in greater detail in Ref. 26. 4.4.2 Coherent dynamics of intersubband polarizations
Coherent IS polarizations give rise to coherent light emission on the IS transition. Measuring such electric field transients with an amplitudeand phaseresolved detection scheme, e.g., by electrooptic sampling, provides direct access to the polarization dynamics and the underlying couplings in the carrier plasma. Coherent IS emission was first studied in the linear regime where the generated IS polarization depends linearly on the field of an ultrashort driving pulse. In Ref. 57, femtosecond excitation from the valence to the n = 1 and n = 2 conduction subbands of undoped asymmetric QWs has been applied to generate a coherent IS polarization. The IS emission was detected interferometrically, as discussed in Sec. 4.3.2. The emission displays a carrier frequency determined by the IS transition energy and an envelope decaying on a time scale of several hundreds of femtoseconds. The origin of this decay has not been clarified in such linear measurements, and both dephasing and inhomogeneous broadening may contribute. In the following, studies with resonant IS excitation of electrons by femtosecond midinfrared pulses are presented, covering both the linear and the nonlinear regimes of material response. Coherent IS polarizations were generated with the femtosecond infrared source described in Sec. 4.3.1 [50], and the transmitted light was detected by electrooptic sampling, allowing for a measurement of absolute optical phases rather than just relative phases with respect to a reference field. The transmitted light consists of the transmitted part of the excitation pulse plus the coherent emission from the IS polarization. To isolate the IS emission, the transmitted pulse was subtracted from the total signal. In Figs. 4.7 and 4.8, results for a GaAs/AlGaAs multipleQW sample with an electron concentration of N = 5 × 1011 cmí2 (IS absorption spectrum in Fig. 4.1a) are shown [56]. For amplitudes of the driving field 5 kV/cm (Fig. 4.7), the sample response is in the linear regime, and the emission reflects the gradual buildup of the macroscopic IS polarization followed by the free induction decay with the dephasing Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_154_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 154
Chapter Four
Electric fiald (kV/vm)
(a)
Reemitted
(b) (a) Experimental geometry for studying coherent IS emission. A midinfrared pulse excites the sample of prism shape, and the transmitted light is analyzed by electrooptic sampling in a ZnTe crystal. (b) Incident (thin line) and reemitted (thick line) electric field as a function of time. The sample response is in the linear regime. The reemitted field displays a free induction decay with a 180 degree phase shift with respect to the driving field. Figure 4.7
time of 320 fs. In the resonant excitation scheme applied here, the IS polarization is 90 degrees out of phase with the driving field. The field reemitted from the layered sample is proportional to P / t [67, 68], adding another phase shift of 90 degrees. As a result, the emitted field is 180 degrees out of phase with the driving field, corresponding to an overall absorptive response of the sample. The characteristics of the emitted field change drastically on increasing the driving field. In Fig. 4.8a and b, the envelope of the emitted field displays a strong modulation and zeros in amplitude during the driving pulse. The number of emission periods during the pulse increases from two in Fig. 4.8a to three in Fig. 4.8b for an increase of the maximum amplitude of the driving field by a factor of 2. The maximum emission amplitude shows a sublinear increase, i.e., pronounced saturation, with the amplitude of the driving field. In addition, there is a change of the phase of the emitted field with respect to the driving field in successive emission periods. In Fig. 4.8a, emission in the first period is out of phase with the driving fields, similar to the linear case, whereas emitted and driving fields are in phase in the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_155_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
20
155
(a)
(b)
(c)
Figure 4.8 Coherent IS emission in the nonlinear regime. (a, b) Driving field and reemitted field for different amplitudes of the excitation pulse. The reemitted field displays a time evolution characteristic of Rabi flopping with several emission periods and phase jumps of 180 degrees between such periods, (c) Pulse area derived from the time evolution of the excitation pulse (dashed line) and from the reemitted field in (b) (symbols, solid line).
second period. In Fig. 4.8b, one observes a sequence of outofphase, inphase, and outofphase emission. The results summarized in Fig. 4.8 are a clear manifestation of IS Rabi oscillations induced by the strong driving field resonant to the IS transition. Both the amplitude of the macroscopic polarization and the population inversion between the optically coupled subbands undergo oscillations at the Rabi frequency ȍ = MISE/ ല where MIS is the IS dipole moment (Eq. 4.1) and E is the driving field. The optical Bloch equations for noninteracting twolevel systems represent the most elementary description of this phenomenon [7, 69]. In this density matrix approach, the macroscopic polarization P(t), which is connected to the offdiagonal element ȡ12(t) of the density matrix, is described by a differential equation containing a nonlinear term proportional to the population inversion between the two optically coupled subbands. This term leads to a saturation of the polarization amplitude and determines its phase. In Fig. 4.8a, there is a first period in which a complete population inversion builds up ȡ22(t ) /t > 0 , followed by a second period in which this inversion decreases by stimulated emission ȡ22(t ) / t < 0 . Correspondingly, the emitted field Eem(t ) ∝ P(t ) / t and the driving field are out of phase in the first period and in phase in the second Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_156_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 156
Chapter Four
period. The amplitude of the emitted field is zero for maximum inversion, i.e., at t = 0.65 ps in Fig. 4.8a. Increasing the driving field even further (Fig. 4.8b) results in an increase of the Rabi frequency and an additional emission period. The basic features of the results of Fig. 4.8 are reproduced by the optical Bloch equations. Closer inspection, however, reveals discrepancies between this elementary picture and the experiment. In Fig. 4.8c, the pulse area Ĭ = ʌ/2 (ȍt)dt is plotted as a function of time. The dashed line gives Ĭ as derived from the time evolution of the driving field. On the other hand, the pulse area can be derived from the measured progress of the Rabi oscillations. For a pulse area of ʌ/2, the amplitude of the coherent emission reaches a maximum, followed by a zero at ʌ where the population inversion is maximum. At 3ʌ/2, the (stimulated) emission is maximum and then disappears at 2ʌ where all electrons are back in the original subband (zero inversion). Based on such predictions of the optical Bloch equations, the symbols in Fig. 4.8c were derived from the emission transient in Fig. 4.8b. There is a substantial discrepancy between the pulse areas from this analysis and from the time evolution of the driving field. In other words, the measured Rabi frequency is essentially constant throughout the driving pulse, although the amplitude of the driving field changes strongly. This behavior clearly points to a failure of the simple Bloch picture. There are essentially two different mechanisms that can modify the Bloch picture. First, local field effects may occur; i.e., the local field acting on a particular QW may consist of the external driving field plus the field generated by the polarizations in the other QWs of the sample. For the low electron concentration of the present sample, such effects are, however, of minor importance. Second, Coulomb mediated manybody effects enhance the IS dipole moment by introducing a coupling between IS transitions originating from different kฌ states. For small driving fields, this coupling prevails, and the collective response leads to a stronger transition dipole and higher Rabi frequencies during the leading and trailing wings of the driving pulse. At, high driving fields around the pulse maximum, the manybody interaction is weaker than the coupling to the external field, and thus the behavior is closer to that of the singleparticle picture with a smaller transition dipole and lower Rabi frequency. The interplay of manybody couplings and the interaction with the driving field make the instantaneous Rabi frequency less sensitive to the external field, in qualitative agreement with the behavior found in Fig. 4.8b. Radiative coupling effects are present in samples with higher electron concentrations. In the linear regime, radiative coupling in multipleQW structures leads to a strong modification of the IS absorption strength of the sample. More specifically, the total Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_157_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
157
absorption cross section is no longer proportional to the electron concentration. For a particular QW, the field reemitted by the other QWs compensates the external field, resulting in a smaller local field and, as a consequence, a strongly reduced IS absorption. In the nonlinear regime, the time structure of the field transmitted through the sample and the overall nonlinear transmission are strongly affected by radiative coupling, as is evident from a very recent study [70]. In conclusion, the results discussed here demonstrate how the nonlinear IS response can be controlled by external optical fields, allowing for a change of IS polarizations and populations over a wide range. Such schemes are highly attractive for optical switching and display all the features required for implementing quantum bits. Femtosecond excitation allows for tailoring the phasecoherent response and, in particular, for subpicosecond switching times. 4.5
Intersubband Relaxation Processes
IS relaxation processes of carriers have been studied under a variety of conditions including both interband excitation of electronhole plasmas [71, 72] and direct IS excitation of a singlecomponent electron or hole plasma in doped QW systems and heterostructures. In the latter case, the total carrier concentration is constant; i.e., IS excitation and the subsequent relaxation are equivalent to redistributing a single type of carrier on a femtosecond to picosecond time scale. This fact facilitates the analysis of the relaxation scenario substantially and enables one to extract much more specific information on microscopic processes than in the case of photogenerated electronhole plasmas. Resonant IS excitation generates an initial nonequilibrium distribution of electrons or holes populating states in the optically coupled subbands. As time evolves, different relaxation processes transform such nonequilibrium populations into a quasiequilibrium distribution, eventually reestablishing the initial situation. The relevant relaxation processes are 1. IS scattering of carriers from higher subbands back to the initially populated subband 2. Carrier thermalization, i.e., the formation of quasiequilibrium carrier distributions 3. Carrier cooling, i.e., the transfer of excess energy from the carrier plasma to the lattice by phonon emission The time scales of such processes depend on the energy spacing of the subbands, the carrier density, the excitation density, and microscopic
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_158_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 158
Chapter Four
coupling parameters. IS scattering, thermalization, and cooling are not strictly sequential but occur in overlapping time windows determined by the underlying carriercarrier and carrierphonon scatterings. In Fig. 4.9, the relaxation of electrons after resonant IS excitation at an energy EIS > ലȦLO (ലȦLO is the optical phonon energy) is illustrated schematically. The femtosecond excitation pulse promotes electrons from the n = 1 to the n = 2 subband (Fig. 4.9a). This creates an excess population of n = 2 electrons and a nonequilibrium distribution of n = 1 electrons. Due to the nearly parallel inplane dispersion of the two subbands, the excitation depletes n = 1 states in a broad range of energies from the bottom of the n = 1 subband up to the quasiFermi level of the initial distribution. The n = 2 carriers undergo IS scattering by interaction with optical phonons into highlying states of the n = 1 subband (Fig. 4.9b). Such energetic electrons scatter with the cold sea of unexcited n = 1 electrons and with phonons, in this way relaxing toward the bottom of the subband. This relaxation and simultaneous scattering of the initially unexcited electrons result in a thermalization of the overall electron distribution toward a hot quasiequilibrium distribution (Fig. 4.9c) which subsequently cools down to lattice temperature. In general, the observation of such a relaxation scenario requires a measurement of transient electron distributions in the femtosecond time domain. IS scattering, i.e., the depopulation of the n = 2 subband,
(a) CB
(c)
(d)
Hot fermilike n = 1 distribution
Nonthermal n = 1 distribution
Energy
n=2
(b)
n=1
kll
0
1 f (E)
0
f (E)
1
∆T/T0 0
Schematic of relaxation processes occurring after IS excitation of electrons. (a) Inplane dispersion of the two optically coupled conduction subbands (CB) indicating the optical transition (vertical arrow) and the backscattering by phonons (diagonal arrow). (b) Schematic electron distribution f(E) in the n = 1 subband after IS scattering. The distribution consists of the backscattered electrons at high energy and the cold sea of unexcited electrons at the bottom of the subband. Dashed line: initial Fermi distribution of electrons. (c) Hot electron distribution after thermalization of the n = 1 electrons displaying a pronounced highenergy tail. (d) Schematic change of transmission on the n = 1 interband transition due to the changes of the electron distribution in (c). Figure 4.9
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_159_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
159
has been studied in pumpprobe experiments monitoring the nonlinear changes of IS absorption (see Fig. 4.4a). In this scheme, the probe pulse averages over a broad range of kฌ states and IS scattering and intrasubband thermalization in the n = 1 subband are difficult to separate. For nearly parallel subband dispersions, however, all backscattered electrons contribute to IS absorption independent of their inplane wave vector, making the measured absorption change quite insensitive to intrasubband redistribution. In this limit, the absorption change is proportional to the difference of the total n = 1 and n = 2 electron populations. Based on this assumption, such measurements have been interpreted in terms of a dominant contribution from IS relaxation with IS scattering times between 100 fs and several picoseconds for QWs made from GaAs/AlGaAs (see Fig. 4.5a), GaInAs/ InP, GaN/AlGaN, and other IIIV and IIVI material systems. Much more detailed insight into carrier relaxation is possible with the pumpprobe scheme of Fig. 4.4b and c in which changes of the electron distribution are monitored via changes of the interband absorption [62]. Transient population and depopulation of kฌ states by electrons result in a decrease and an increase of interband absorption into those states, respectively (Fig. 4.9d). In Figs. 4.10 and 4.11, results of such measurements are shown for ntype modulationdoped GaInAs/ AlInAs multiple QWs (L = 8 nm, 50 QWs) with an electron concentration 11 í2 of N = 5 × 10 cm . In Fig. 4.10, the timedependent nonlinear transmission change is shown for probe photon energies at the onset of the n = 2 interband absorption between 1.130 and 1.150 eV. One finds a transient increase of transmission, i.e., a bleaching, which rises within the time resolution of the experiment and decays with a time constant ĲIS = 1 ps. The bleaching is caused by the transient electron population of the n = 2 conduction subband, leading to a blocking of the corresponding interband transitions. The decay of the signal is due to the depopulation of the n = 2 subband by IS scattering back to the n = 1 subband. The transient behavior of the n = 1 electrons is evident from absorption spectra recorded in the range of the n = 1 absorption edge around 900 meV. Here, one probes states at the bottom of the n = 1 subband which are initially populated by the electron plasma. In Fig. 4.11, spectra are displayed for various delay times after the IS excitation (solid circles). At 0.2 ps (Fig. 4.11a), a decrease of transmission in the range of the initially populated electron states is found which is due to the depletion by the excitation pulse. At later times (Fig. 4.11b to e), the amplitude of this signal rises, and in addition a delayed decrease of absorption occurs at higher photon energies. For delay times between 0.4 and 1.1 ps, the maximum amplitude of this bleaching signal is substantially smaller than that of the absorption Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_160_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Chapter Four
Change of transmission ∆T/T0 (x103)
160
Delay time (ps) Figure 4.10 IS relaxation of electrons in ntype modulationdoped GaInAs/AlInAs
quantum wells (sample temperature of 8 K). The change of transmission ǻ T / T0 = (T í T0) / T0 on the n = 2 interband transition is plotted as a function of pumpprobe delay (T and T0 are sample transmission with and without excitation, respectively, on the IS transition at 200 meV). The solid line represents the result of an EMC simulation of electron dynamics, giving an IS relaxation time of 1 ps. Dashed line: crosscorrelation of pump and probe pulses.
increase occurring below the initial Fermi level, whereas similar amplitudes are approached after 2 ps. These changes of interband absorption occur on a time scale which is substantially slower than the dephasing of IS polarizations discussed in Sec. 4.4.1. Furthermore, manybody effects have a minor influence on the transient spectra because of the moderate electron concentration. The spectra are determined by the difference of the transient and the initial equilibrium electron distribution, and thus their time evolution reflects IS scattering and electron redistribution. Under such conditions, Ensemble Monte Carlo (EMC) techniques to solve the Boltzmann equation for the electron distribution functions are an appropriate tool to analyze the relaxation scenario. The experiments were simulated by an EMC approach described in Refs. 73 and 74. IS and intrasubband electronelectron and electronphonon scattering, the Pauli exclusion principle, and nonequilibrium phonons were taken into account. IS excitation was simulated by promoting about 15% of the electrons from the n = 1 to the n = 2 subband with a 130fs pulse that was resonant to the IS transition between the n = 1 and n = 2 conduction subbands of parallel inplane dispersion. For comparison with the measured absorption changes, the difference between the transient and the initial electron distribution in each subband was multiplied by the steplike absorption coefficient of the respective valence to conduction Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_161_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
EFi
161
(a)
(c)
(d)
n = 1 Electon distribution f (E)
Change of transmission ∆T / T0
(b)
(e)
Photon energy (meV) Electron energy (meV) Transient spectra on the n = 1 interband transition measured after IS i excitation of electrons in GaInAs/AlInAs quantum wells ( EF is initial Fermi level of the electrons). Left column: The change of transmission is plotted versus the center photon energy of the probe pulses of 13meV bandwidth. Data are shown for delay times of (a) 0.2 ps, (b) 0.4 ps, (c) 0.8 ps, (d) 1.1 ps, and (e) 2.0 ps. Solid lines: calculated spectra from EMC simulations. Right column: calculated electron distributions showing the formation of a quasiequilibrium distribution within 2 ps (solid lines). Dashed lines: initial electron distribution. Figure 4.11
band transition and convoluted with the temporal and spectral envelope of the 100fs probe pulses (spectral bandwidth 13 meV). IS relaxation of the n = 2 electrons occurs with a characteristic time constant of 1 ps, as is evident from the decay of the signal in Fig. 4.10. This decay is very well reproduced by the EMC simulation (solid line), indicating that emission of confined and interface optical phonons via the polar interaction represents the main scattering mechanism. IS scattering requires emission of optical phonons with large q vectors. Due to the q dependence of the coupling matrix element, IS scattering rates are substantially smaller than the intraband scattering rates connected with optical phonon emission at much smaller q vectors. IS scattering transfers nonequilibrium electrons into highlying n = 1 states. No bleaching due to accumulation of backscattered carriers in those highlying states was detected, demonstrating that spreading Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_162_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 162
Chapter Four
of the backscattered electrons over a broad energy range occurs much faster than the supply of nonequilibrium carriers with the IS scattering time of 1 ps. The redistribution of nonequilibrium electrons of high energy is part of the thermalization process within the n = 1 subband. Thermalization requires a transfer of such electrons toward the bottom of the subband. This relaxation involves both emission of optical phonons, transferring excess energy to the lattice, and Coulomb scattering between high and lowenergy carriers, the latter process heating the cold electron plasma. The transient interband absorption spectra of Fig. 4.11 reveal the nonthermal character of the n = 1 electron distribution for a surprisingly long time interval of 2 ps. Just after the IS excitation (delay time 0.2 ps, Fig. 4.11a), one observes a transmission decrease from the onset of the n = 1 interband absorption up to the Fermi edge EFi of the initially cold distribution. The EMC simulation for 0.2 ps (solid lines) gives a constant depletion of the initial Fermi distribution (dashed line) by 15% of the carriers consistent with the excitation conditions. The EMC simulation shows that the rate of electronelectron scattering into states below the initial Fermi level is reduced by (1) the small fraction of unoccupied states to which electrons can be transferred, i.e., Pauli blocking, and (2) screening of the Coulomb interaction. As a result, the carrier depletion between the bandgap and the initial Fermi level persists for hundreds of femtoseconds, as is directly evident from the data in Fig. 4.11b. The inelastic Coulomb scattering between cold and backscattered electrons results in a transfer of cold electrons to states above the initial Fermi level EFi , thus forming an enhanced highenergy tail of the distribution. In Fig. 4.11, this is evident from the enhancement of the induced absorption below EFi and the bleaching, i.e., population, above EFi . Between 0.2 and 1 ps, the very broad highenergy tail results in an amplitude of the bleaching much smaller than that of the induced absorption. After a time delay of about 2 ps, this distinctly nonthermal distribution has evolved into a hot Fermi distribution with similar amplitudes for the enhanced absorption and bleaching. The main energy transfer to the cold plasma occurs at times between 500 fs and 2 ps, due to the delayed supply of energetic carriers from the n = 2 subband. The quantitative analysis shows that about 50% of the excess energy of the backscattered electrons goes into the cold electron plasma whereas the other 50% is transferred to the lattice via LO phonon emission. The IS scattering and thermalization processes evident from the results in Figs. 4.10 and 4.11 are followed by electron cooling via phonon emission. Monitoring the transient interband spectra up to delay times of 50 ps gives detailed information on the cooling kinetics and allows one to derive the instantaneous carrier temperature, as discussed in detail in Ref. 75. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_163_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
163
(a) n=2 n=1
(b)
Change of transmission ∆T / T0
Absorption = In(T)
The IIIV material systems discussed so far display a limited polarity of the crystal lattice and thus a moderate coupling of electrons and optical phonons via the polaroptical interaction. In contrast, group III nitrides are characterized by a very high polarity and strong electronphonon coupling, properties which should lead to polaronic signatures in the line shape of IS absorption [76] and to different nonequilibrium dynamics of electrons. Very recently, evidence for such phenomena has been found in a femtosecond pumpprobe study of IS dynamics of electrons in a GaN/Al0.8Ga0.2N heterostructure [77]. The linear n = 1 ĺ 2 IS absorption of this sample displays a structureless envelope extending over more than 200 meV (Fig. 4.12a). Transient IS absorption spectra were measured in twocolor pumpprobe experiments where a 100fs pump pulse centered at 355 meV excites the sample and the resulting change of transmission is measured by independently tunable probe pulses of 50fs duration. In Fig. 4.12b and c, transient spectra are shown for time delays of 0 and 100 fs. The spectrum for zero delay exhibits a transmission increase over a spectral range much wider than that of the pump spectrum,
(c)
Photon energy (meV) (a) Measured (symbols) and calculated (solid lines) linear n = 1 ĺ 2 IS absorption of a GaN/Al0.8Ga0.2N heterostructure (sample temperature of 10 K). Inset: schematic potential energy diagram of the heterostructure and probability densities of electrons in the n = 1 and n = 2 subbands. (b, c) Measured (symbols) and calculated (solid lines) transient IS spectra for two different time delays after excitation by pump pulses centered at 355 meV. Clear signatures of optical phonon sidebands of IS absorption are observed. Dashdotted line: spectrum of the pump pulse. Figure 4.12
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_164_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 164
Chapter Four
pointing to a substantial homogeneous broadening of the band. There are two pronounced transmission maxima at 260 and 340 meV, both redshifted with respect to the maximum of the pump spectrum. After 100 fs, this substructure has essentially disappeared, pointing to a very rapid spectral diffusion within the absorption band. Timeresolved measurements at fixed spectral positions have been presented in Ref. 77. At the maximum of the linear IS absorption, one observes a decay of the transmission increase with a time constant of 380 fs. Around 340 meV, the transmission kinetics display a first 80fs decay followed by a slower 380fs decay. The amplitude ratio of the 380fs components is close to the ratio of linear IS absorption at the two spectral positions. The separation of the two transmission maxima in Fig. 4.12b is close to the LO phonon energy of GaN of 92 meV. This finding points to a vibronic substructure of the spectrum which originates from the strong coupling of electrons and LO phonons in GaN. This behavior can be described within the independent boson model by considering the energy states and the dynamics of the IS polaron, a quasiparticle of mixed electronLOphonon character [58, 78]. An analysis based on such a model is presented in Ref. 77 and accounts for the linear and nonlinear spectra shown in Fig. 4.12 (solid lines). The pump pulse overlaps with the  n = 1, Ȟ = 0 to  n = 2, Ȟ = 1 transition (ǻȞ = 1, Ȟ is vibrational quantum number) around 340 meV. The slight red shift of the transmission maximum with respect to the maximum of the pump spectrum is due to the initial motion of the vibronic wave packet in the n = 2 state. In addition, the pump induces a transmission increase on the ǻȞ = 0 transition through depletion of the  n = 1, Ȟ = 0 state and optical gain from the  n = 2, Ȟ = 1 state. Such pronounced spectral features are washed out by spectral diffusion, i.e., a modulation of the transition energies due to coupling of the polaron to other fluctuating excitations in the system. This process gives rise to the fast 80fs decay of the transmission change observed at 340 meV. All transmission changes decay by population relaxation from the n = 2 states with a time constant of 380 fs. So far, energy separations of the optically coupled subbands larger than the optical phonon energies have been considered. Work on IS scattering for subband energy spacings smaller than the optical phonon energy has led to controversial results, and IS scattering times between 500 fs and 750 ps have been claimed [65, 79–82] . For small subband spacings, both carrier density and temperature have a strong influence on IS relaxation. For degenerate carrier distributions, i.e., a quasiFermi level within the subband, Pauli blocking substantially reduces the free phase space available for scattering, in this way affecting both carriercarrier and carrierphonon scattering rates. For high carrier Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_165_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
165
temperatures, optical phonon emission by the most energetic carriers can result in an acceleration of IS scattering, an effect suggested by EMC simulations of the early experiments of Ref. 65. Thus, the measurement of IS scattering times for EIS < ലȦLO,TO requires a careful characterization of the initial and transient carrier distributions [82]. In contrast to electron relaxation, IS scattering of holes has remained nearly unexplored [27, 83]. The inplane dispersion of valence subbands is quite complex with pronounced nonparabolicities and mixing between heavyhole (HH), lighthole (LH), and splitoff (SO) bands (cf. Fig. 4.1b). For SiGe/Si QWs, the inplane dispersion of the HH1 and HH2 subbands is different with an IS energy spacing depending on the inplane wave vector. This results in a distribution of IS transition energies and a broadening of the IS absorption line, making the transient IS absorption sensitive to carrier redistribution in the HH1 subband. IS relaxation of holes has been studied in femtosecond pumpprobe experiments with a ptype modulationdoped SiGe/Si QW sample consisting of 10 Si0.5Ge0.5 QWs of 4.4nm width separated by 18nmthick Si barriers [27]. The holes introduced by doping populate the HH1 subband with a density of N = 1.2 × 1012cmí 2 . The femtosecond pump pulse is resonant with the HH1 ĺ HH2 transition and excites approximately 30% of the holes to the HH2 band. Transient spectra measured with a probe pulse on the same transition are shown in Fig. 4.13. At early time delays, a strong increase of transmission occurs around the center of the IS absorption line. As time evolves, this bleaching decreases and an additional absorption increase is observed at small photon energies, i.e., on the lowenergy tail of the stationary IS absorption line. The kinetics of bleaching and enhanced absorption at early times are different: The bleaching shows a rise within the time resolution and a pronounced decay within the first 2 ps (Fig. 4.14a, dashed line), whereas a delayed rise and a much slower decay are found for the enhanced absorption (Fig. 4.14a, solid line). Both signal components decay completely on a time scale of 50 ps (not shown). The transient spectra in Fig. 4.13 reflect both IS scattering of excited holes from the HH2 back to the HH1 subband and intraHH1 subband redistribution of carriers. The strong bleaching at early delay times is mainly due to a depletion of the optically coupled HH1 states and stimulated emission from the HH2 subband. The stimulated emission component decays through the depopulation of the HH2 subband by IS scattering of holes into highlying states of the HH1 subband. The depletion of HH1 states around kฌ = 0 and the interaction of the backscattered holes at high energy with the unexcited holes in the HH1 subband initiate an intraband thermalization process by which a hot quasiequilibrium distribution is formed. To establish the highenergy Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_166_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Chapter Four
Change of transmission ∆T/T0 (%)
166
Photon energy (meV) Transient IS spectra of holes in ptype modulationdoped SiGe/Si quantum wells (sample temperature of 10 K). The change of transmission induced by a pump pulse centered at 170 meV (bandwidth of 20 meV) is plotted versus photon energy within the spectrum of the probe pulse (symbols). Data are shown for different pumpprobe delays. Solid lines: calculated difference spectra for thermalized hole distributions of a given hole temperature.
Figure 4.13
tail of this distribution, holes are scattered from states around kฌ = 0 into states at larger k vectors. This process leads to an additional delayed bleaching at the center of the steadystate IS line and a delayed enhanced absorption on the red wing as the HH1HH2 energy separation decreases with increasing kฌ vector. Eventually, the hot quasiequilibrium distribution cools down to the lattice temperature by phonon emission. A quantitative analysis of the data on the basis of this picture allows one to extract the pure IS scattering dynamics [27]. The solid lines in Fig. 4.13 represent spectra calculated for a hot quasiequilibrium distribution in the HH1 subband. At a 2ps delay, this modeling is in good agreement with the data, giving a transient hole temperature of 270 K. At earlier delays, the measured bleaching signal is stronger than predicted by this model, reflecting the contribution due to IS scattering. To determine the latter component, the calculated thermal spectra with an amplitude fitting the enhanced absorption at lower photon energies were subtracted from the overall signal. The time evolution of the resulting IS scattering signal is shown in Fig. 4.14b and gives an IS scattering time of 250 fs.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_167_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures
6
Integral difference ∆T/T (arb. units) 0
Transmission change ∆T/T0 (%)
Ultrafast Dynamics of Intersubband Excitations
167
(a)
(b)
Time delay (ps)
(a) Change of IS transmission at 168 meV (dashed line) and 140 meV (solid line) as a function of pumpprobe delay. (b) Fast bleaching signal derived by the subtraction procedure explained in the text (symbols). At delays longer than 70 fs, the kinetics reflect IS scattering of holes with a time constant of 250 fs (solid line). Figure 4.14
IS scattering of holes in SiGe/Si QWs is dominated by emission of optical phonons via the deformation potential interaction. There are two relaxation channels: a direct backscattering from the HH2 to the HH1 subband and a sequential process in which a hole scatters into the LHSO1 subband and from there into the HH1 subband. Calculations give an overall scattering time of 225 fs with a dominant contribution from the cascaded process [27]. Such a number is in very good agreement with the experimental results. In conclusion, IS excitation of carriers induces a complex relaxation scenario by which the original equilibrium distribution of electrons or holes is reestablished. For IS transition energies higher than the optical phonon energy, IS scattering times range from 100 fs up to about 1 ps, depending on the strength of the carrierphonon interactions and the details of the inplane subband dispersion. The dominant relaxation mechanism consists in the emission of optical phonons via the polaroptical interaction or the optical deformation potential. For subband energy spacings below the optical phonon energy, carriercarrier Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_168_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 168
Chapter Four
scattering and, in hot carrier distributions, phonon emission result in somewhat longer IS scattering times. IS scattering is followed by carrier thermalization in the lower subband on a femtosecond to picosecond time scale, leading to a hot quasiequilibrium distribution. Eventually, carrier cooling by phonon emission transfers the excess energy to the lattice on a time scale of 1 to 50 ps. 4.6 Quantum Transport in Quantum Cascade Structures Since the first demonstration in 1994 [84], impressive progress has been made in extending the spectral range and optimizing the performance parameters of quantum cascade lasers. This fact is documented in other chapters of this book. From the viewpoint of basic physics, quantum cascade structures are interesting model systems to study unipolar carrier transport in different regimes, in particular for a wide range of carrier concentrations. In the quantumcoherent regime, electronic wave packets representing a nonstationary superposition of envelope wave functions can move through such structure by a sequence of coherent tunneling processes [85–94]. Coherent transport is highly relevant for the operation of quantum cascade lightemitting devices and is connected with ultrafast propagation and relaxation dynamics. In the following, recent experiments on coherent electron transport in GaAs/ AlGaAs quantum cascade structures are discussed [64, 95]. The electronic structure of a quantum cascade laser under forward bias is shown in Fig. 4.15a [84, 96–98]. The bias is chosen in such a way that at least one of the injector subbands (state g) is in resonance with the upper laser subband 3 of the active region downstream. Electrons are transferred from the injector region, which represents a reservoir of electrons, through a barrier into the active region, which consists of three coupled quantum wells. Under steadystate conditions, a quasistationary population exists in subband 3 and gives rise to IS emission on the 3 ĺ 2 optical IS transition with an energy larger than the energy of the optical phonons. Electrons in subband 3 have an intrinsic lifetime of approximately 1 ps. In contrast, the lifetime of subband 2 is much shorter (썑 100 fs) due to efficient electron relaxation to subband 1 via resonant LO phonon emission and electron transfer from both subbands 2 and 1 into the next injector region. As a result, a population inversion builds up between subbands 3 and 2, resulting in optical gain and laser action on the 3 ĺ 2 IS transition. The nature of the electronic transport from the injector into subband 3, a process crucial for the performance of the device, has led to some controversy in the literature. On the one hand, this transport has been described on the basis of resonant tunneling pictures, invoking Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_169_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
Injector
600
Active region Energy (meV)
169
g
400
3
F = 60 kV / cm Injector Active region
2
200
g
1
3
0 0
∆Eab = hνosc
2>
τ2
20 40 60 80 Propagation coordinate z (nm) (a) a>
g g> =
a> + b> 21/2
b>
a> 3> = b> 1/2 2
τ3
(b)
(a) Conduction band diagram of a GaAs/Al0.3Ga0.7 As quantum cascade structure with an active region consisting of three coupled quantum wells under forward bias. The probability densities of electrons in the injector subband g and 3 subbands of the active region are also shown. The laser transitions occur between subbands 3 and 2. Such probability densities are based on envelope wave functions calculated without the tunnel coupling between subbands g and 3. (b) Scheme of coherent electron transport from the injector ground subband g into the upper laser subband 3 in the picture of resonant tunneling. The levels b and a are bonding and antibonding eigenstates of the electronic hamiltonian including the tunnel coupling between g and 3 . The latter represent coherent superpositions of b and a . Figure 4.15
a quantumcoherent superposition of states in subbands g and 3 [97–99]. Yet recent Monte Carlo simulations of incoherent electron dynamics, which neglect coherent transport phenomena, give rather high electronelectron scattering rates, resulting in quasithermal carrier distributions in each subband under steadystate operation conditions [89, 100, 101]. The high scattering rates suggest a minor role of quantum coherence for electron transport. In Sec. 4.3 (Fig. 4.4d), a pumpprobe scheme for studying such electron transport via the depletion and recovery of IS gain has been described. In these experiments, the quasistationary gain in GaAs/ AlGaAs quantum cascade structures with 10 periods of injector and active region [96, 102] was depleted by a 150fs pump pulse resonant to the 3 ĺ 2 lasing transition at a wavelength of 10 m (photon energy 124 meV). The subsequent time evolution of the optical gain was Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_170_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 170
Chapter Four
Power (arb. units)
Currentinduced transmission change ∆T / T0 (%)
monitored by weak probe pulses which were spectrally dispersed after interaction with the sample. Such measurements were performed for several samples in a wide range of injection currents, sample temperatures, and pump intensities [64, 95]. In Figs. 4.16 through 4.18, results for a sample with 33% Al in the barriers and an injection barrier of 6.2nm width are presented [96]. The timeresolved transmission changes in Fig. 4.16a to d represent the difference between a pumpprobe curve with an injection current density j = 7 kA/cm2 applied and a pumpprobe curve without current as a function of the time delay between pump and probe pulses. The quasistationary transmission increase before zero delay is due to the currentinduced gain present in absence of the femtosecond pulses. Upon femtosecond excitation, the gain is depleted both on the shortwavelength wing (Fig. 4.16a) and at the maximum (Fig. 4.16b) of the gain spectrum (Fig. 4.16f). The gain recovers completely within several hundreds of femtoseconds. During this period, the transmission changes consist of a decay transient superimposed by pronounced
(a)
(b)
(e)
(f )
(c)
(d)
Delay time (ps) (a–d) Timeresolved transmission changes of a GaAs/AlGaAs quantum cascade structure under forward bias (injection current density j = 7 kA/cm2, nominal sample temperature of 10 K). The change of transmission ¨T/T0 = [T(j, t) – T(j = 0, t)]/T (j = 0, t) is plotted as a function of pumpprobe delay t for different wavelength positions in the probe spectrum (symbols); T(j, t) is the transmission through the sample for a current density j. The energy of pump and probe pulse resonant to the 3 ĺ 2 transition was 7500 and 75 pJ, respectively. Solid lines: exponentially decaying cosine function (a) or decaying exponential functions (c, d) convoluted with the crosscorrelation between pump and probe. (e) Fourier transforms of the transients (a, b). (f) Electroluminescence spectrum of the sample for j = 7 kA/cm2 (solid line) and spectrum of the pump and probe pulses (dashed line). The arrows indicate the wavelength positions at which the transients (a–d) were recorded. Figure 4.16
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_171_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
(b)
Currentinduced transmission change ∆T / T0 (%)
(a)
171
Delay time (ps) (a) Transmission changes of a quantum cascade structure measured for different energies of the pump pulse at a probe wavelength of Ȝ = 10 m (symbols, current density of 7 kA/cm2, sample temperature of 10 K). Solid lines: slowly varying signal component. (b) Oscillatory component of the signal, i.e., total signal minus slowly varying component (symbols), and exponentially decaying cosine fit curves convoluted with the crosscorrelation of pump and probe pulses (solid lines). Figure 4.17
oscillations which are particularly strong at the gain maximum. The Fourier transforms of the oscillatory components (Fig. 4.16e) show a maximum at 2 THz corresponding to an oscillation period of 500 fs. Transients taken outside the emission spectrum (Fig. 4.16e and d) display a different time evolution: There is a transmission increase at early time delays followed by a decay depending on the particular probe wavelength. The modulation in Fig. 4.16c, which starts at negative delay times, is caused by nonlinear optical effects such as the perturbed free induction decay and coherent pumpprobe coupling. Oscillatory features are absent at positive time delays. Such transients reflect carrier dynamics in the injector and are not discussed further [95]. Similarly, oscillations are absent for reverse bias. In Fig. 4.17, timeresolved transmission changes measured at Ȝ = 10 m, the gain maximum, are presented for different energies of the pump pulse, i.e., different levels of gain saturation (current density Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_172_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 172
Chapter Four
j = 7 kA/cm2, lattice temperature is 10 K). For weak saturation (Fig. 4.17a), one finds several oscillations of small amplitude and a long dephasing time of approximately 700 fs. With increasing pump energy, the oscillation amplitude grows linearly up to a pulse energy of 2.5 nJ and then starts to saturate. Concomitantly, dephasing becomes faster whereas the oscillation frequency of 2 THz remains unchanged. Data taken for different injection currents and a pump energy of 7.5 nJ are summarized in Fig. 4.18. Transmission oscillations occur in a wide range of injection currents, starting from j = 70 A/cm2 well below the regime of quasistationary gain up to j = 8 kA/cm2. Between j = 0.3 and 8 kA/cm2, the oscillation amplitude remains essentially unchanged whereas dephasing becomes faster with increasing current. Gain saturation by the intense midinfrared pump pulses leads to a strong reduction of the electron population of subband 3, which is subsequently compensated for by the transfer of electrons from the injector region through the injection barrier into subband 3. The electrons dumped by the excitation pulse into subband 2 leave the active region very quickly by LO phonon scattering to subband 1 and
(b)
Currentinduced transmission change ∆T / T0 (%)
(a)
Delay time (ps) Transmission changes of a quantum cascade structure at a probe wavelength of Ȝ = 10 m for different injection current densities. (a) Measured transmission change (symbols) and slowly varying component of the signal with frequencies 1 THz (solid lines). (b) Oscillatory signal component as in Fig. 4.17b.
Figure 4.18
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_173_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
173
transfer into the next injector. Thus, they do not contribute to the pumpprobe signal for delay times longer than 100 fs. As a result, the gain saturation and recovery dynamics are dominated by the population dynamics in the upper laser subband 3. The results demonstrate the oscillatory character of electron motion after gain saturation. This behavior gives evidence of coherent resonant tunneling of electrons through the injection barrier, as depicted schematically in Fig. 4.15b. Under bias, the subbands g and 3 are in resonance, and the tunnel coupling forms bonding b and antibonding a energy eigenstates. These are energetically split by an energy ǻEab which is determined by the width and height of the injection barrier and by the voltage applied. Coherent superpositions of states a and b represent the basis for wave packet propagation from the injector ground state g into the upper laser state 3 . In the experiment, the femtosecond pump pulse depletes the subband 3 = (1 / 21 / 2) (b í a ), i.e., both eigenstates a and b , and initiates a coherent wave packet motion by which electrons tunnel from the injector through the injection barrier into the active region. The tunneling carriers arrive after onehalf the oscillation period T osc = h / ǻEab in state 3 of the active region. As the electron lifetime in state 3 (Ĳ3 Ѥ 1 ps ) is longer than the oscillation period Tosc, most of the electrons will move back into the injector, resulting in a gain depletion at delay times tD § Tosc. This picture of coherent transport is strongly supported by comparing the results for samples with different injection barriers. Such studies reveal a change of the measured oscillation frequencies proportional to ǻEab [64]. In principle, this picture implies a doublet structure of the electroluminescence spectrum. However, the strong broadening of the electroluminescence spectra (Fig. 4.16f ) smears out such a line structure. The oscillatory electron motion is damped on a time scale of several hundreds of femtoseconds; i.e., the dephasing time is comparable to the period of the oscillations. Two mechanisms contribute to such damping: (1) the inhomogeneous broadening of the tunnel couplings due to injection barrier width and height fluctuations and (2) the homogeneous dephasing of the quantum coherence between the states a and b . Mechanism 1 leads to a destructive interference of oscillations of different frequencies. Homogeneous dephasing is mainly caused by electronelectron scattering in the injector which destroys the quantum mechanical phase between the states making up the wave packet. For electron densities of several 1011 cm–2 in the injector, Monte Carlo simulations suggest sub100fs scattering times, substantially shorter than the observed dephasing times of the electron wave packets. Thus, only a fraction of the scattering events result in dephasing. Moreover, electronelectron scattering allows one to generate transport Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_174_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 174
Chapter Four
coherences [103–105]: Among the injector states between which electrons can be scattered are the coherent superpositions g of the electronic eigenstates a and b . If a scattering event populates g on a time scale short compared to the oscillation period TOSC, a coherent superposition of such eigenstates is generated which is in phase with the electron oscillation between the injector and the active region. In this way, the oscillation is enhanced, a mechanism which is also behind the pronounced gain overshoot after depletion by the pump pulse (cf. Figs. 4.16 to 4.18). A more detailed discussion of such a mechanism is given in Ref. 95. The amplitude of the oscillatory electron transport depends linearly on the pump energy up to the value of 2.5 nJ, where the optical gain is fully saturated. With increasing pump level, the dephasing of the oscillations becomes faster, reflecting enhanced scattering rates in the injector. This enhanced scattering has been attributed to a heating of the electron distribution in the injector region by the carriers transferred from the preceding active region [95]. It is interesting to note that the oscillation frequency of the electron wave packet remains essentially unchanged upon increasing the injection current (Fig. 4.18). First, the bias on the device changes only weakly with injection current, as is evident from its currentvoltage characteristics. For a change of injection current of over two orders of magnitude (Fig. 4.18), the electric field on the structure varies between 30 and 65 kV/cm. Calculations of the electronic band structure in this bias range predict three anticrossings between injector subbands and the upper laser subband with nearly identical tunnel splittings of 7 meV, corresponding to an oscillation frequency of 1.7 THz. This is close to the measured oscillation frequency of 2 ± 0.5 THz. The results presented here demonstrate that quantum coherences between coupled subbands play a central role in the electron transport through quantum cascade structures; i.e., a description in terms of incoherent drift diffusion processes is incomplete. After femtosecond gain depletion, quantum coherence manifests itself in pronounced gain oscillations due to coherent wave packet motion between the injector and the upper laser state. Such results explain the empirical finding that the design of the injection barrier is crucial to the performance of a quantum cascade laser. A full theoretical understanding of this complex scenario is still missing and requires a model combining quantum transport and decoherence processes by electronelectron scattering. 4.7 Conclusions The dynamics of IS excitations occur in the ultrafast time domain, covering a range from several tens of femtoseconds up to picoseconds. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_175_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
175
Optical IS excitation induces coherent IS polarizations and/or transport coherences. Such quantum coherences decay by a variety of dephasing processes which, in most cases, are governed by carriercarrier and, to a lesser extent, carrierphonon scattering. Optical IS polarizations can be generated and manipulated in a wide parameter range by nonlinear interaction with ultrashort infrared pulses. Such schemes may lead to novel methods for processing information, e.g., by exploiting the properties of coupled IS transitions. Transport coherences play a central role in quantum cascade devices, in particular for the injection of carriers into the optically active regions. Although the first studies of quantum transport in these devices have been reported, much more experimental and theoretical work is required to understand the transport behavior in detail, e.g., the role of different scattering processes for decoherence. Incoherent carrier relaxation following IS excitation has been studied extensively for electrons, and the processes of IS scattering, carrier thermalization, and cooling are understood in quite some detail. Open questions in this area involve carrier dynamics in closely spaced subbands, e.g., in terahertz quantum cascade lasers, and IS scattering of holes in a wider range of systems. The combination of sophisticated growth methods for quantum wells and quantum cascade devices of high structural quality and ultrafast nonlinear optics to unravel their properties will remain a powerful approach for clarifying the microscopic physics of intersubband excitations. I would like to acknowledge the important contributions of my present and former coworkers Michael Woerner, Klaus Reimann, Robert A. Kaindl, Felix Eickemeyer, and Stephan Lutgen. It is my pleasure to thank Paolo Lugli, Munich, Tilmann Kuhn, Münster, and Andreas Knorr and their coworkers for a theoretical analysis of experimental results and many discussions. I am indebted to Klaus Ploog, and Richard Hey, Paul Drude Institute, Berlin; Harald Künzel, Heinrich Hertz Institute, Berlin; Karl Brunner and Gerhard Abstreiter, Walter Schottky Institute, Munich; Daniel Hofstetter, Neuchatel; Lester Eastman and his coworkers, Cornell; Carlo Sirtori at Thales, Orsay; as well as Karl Unterrainer and Gregor Strasser, TU Vienna; for the highquality samples studied in the experiments. I also thank the Deutsche Forschungsgemeinschaft for financial support. References 1.
T. Ando, A. B. Fowler, and F. Stern, Rev. Mod. Phys. 54, 437 (1982).
2.
E. Rosencher et al. (eds.), Intersubband Transitions in Quantum Wells, Plenum Press, New York, 1992.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_176_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 176
Chapter Four
3.
S. S. Li, and Y. K. Su (eds.), Intersubband Transitions in Quantum Wells: Physics and Devices, Kluwer Academic Publishers, Boston, 1998.
4.
M. Helm, in Intersubband Transitions in Quantum Wells: Physics and Device Applications I, F. Capasso and H. C. Liu (eds.), Semiconductors and Semimetals, vol. 62, 2000, p. 1.
5.
A. Kamgar, P. Kneschaurek, G. Dorda, and J. F. Koch, Phys. Rev. Lett. 32, 1251 (1974).
6.
M. Woerner and T. Elsaesser, in Ultrafast Phenomena Semiconductors, K. T. Tsen (ed.), Springer, Berlin, 2001, p. 93.
7.
J. Shah, Ultrafast Spectroscopy of Semiconductors and Semiconductor Nanostructures, 2d ed., Springer, Berlin, 1999.
8.
L. C. West and S. J. Eglash, Appl. Phys. Lett. 46, 1156 (1985).
9.
M. Zachau, P. Hegelsen, F. Koch, D. Grützmacher, R. Mayer, and P. Balk, Semicond. Sci. Technol. 3, 1029 (1988).
10.
H. Lobentanzer, W. König, W. Stolz, K. Ploog, T. Elsaesser, and R. J. Bäuerle, Appl. Phys. Lett. 53, 571 (1988).
11.
T. Fromherz, E. Koppensteiner, M. Helm, G. Bauer, J. F. Nützel, and G. Abstreiter, Phys. Rev. B50, 15073 (1994).
12.
S. J. Allen, G. Brozak, E. Colas, F. DeRosa, P. England, J. Harbison, M. Helm, L. Florez, and M. Leadbeator, Semicond. Sci. Technol. 7, B1 (1992).
13.
C. Weisbuch and B. Vinter, Quantum Semiconductor Structures: Fundamentals and Applications, Academic Press, Boston, 1991.
14.
A. Pinczuk, S. SchmittRink, G. Danan, J. P. Valladares, L. N. Pfeiffer, and K. W. West, Phys. Rev. Lett. 63, 1633 (1989).
15.
S. L. Chuang, M. S. C. Luo, S. SchmittRink, and A. Pinczuk, Phys. Rev. B46, 1897 (1992).
16.
M. S. C. Luo, S. L. Chuang, S. SchmittRink, and A. Pinczuk, Phys. Rev. B48, 11086 (1993).
17.
M. Zaluzny, Phys. Rev. B43, 4511 (1991).
18.
M. Zaluzny, Phys. Rev. B49, 2923 (1994).
19.
P. von Allmen, Phys. Rev. B46, 13351 (1992).
20.
R. J. Warburton, K. Weilhammer, J. P. Kotthaus, M. Thomas, and H. Kroemer, Phys. Rev. Lett. 80, 2185 (1998).
21.
B. Vinter, Phys. Rev. Lett. 35, 598 (1975).
22.
D. E. Nikonov, A. Imamoglu, L. V. Butov, and H. Schmidt, Phys. Rev. Lett. 79, 4633 (1997).
23.
R. A. Kaindl, S. Lutgen, M. Woerner, T. Elsaesser, B. Nottelmann, V. M. Axt, T. Kuhn, A. Hase, and H. Künzel, Phys. Rev. Lett. 80, 3575 (1998).
24.
S. Nojima, Phys. Rev. B41, 10214 (1990).
25.
A. Liu, Phys. Rev. B55, 7796 (1997).
in
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_177_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
177
26.
R. A. Kaindl, K. Reimann, M. Woerner, T. Elsaesser, R. Hey, and K. H. Ploog, Phys. Rev. B63, 161308(R) (2001).
27.
R. A. Kaindl, M. Wurm, K. Reimann, M. Woerner, T. Elsaesser, C. Miesner, K. Brunner, and G. Abstreiter, Phys. Rev. Lett. 86, 1122 (2001).
28.
G. M. H. Knippels, R. F. X. A. M. Mols, A. F. G. van der Meer, D. Oepts, and P. W. van Amersfoort, Phys. Rev. Lett. 75, 1755 (1995).
29.
B. N. Murdin, W. Heiss, C. J. G. M. Langerak, S. C. Lee, I. Galbraith, G. Strasser, E. Gornik, M. Helm, and C. R. Pidgeon, Phys. Rev. B55, 5171 (1997).
30.
Y. R. Shen, The Principles of Nonlinear Optics, chap. 5, Wiley, New York, 1984.
31.
V. G. Dmitriev, G. G. Gurzadyan, and D. N. Nikogosyan, Handbook of Nonlinear Optical Crystals, SpringerVerlag, Berlin, 1991.
32.
A. M. Weiner, IEEE J. Quantum Electron. 19, 1276 (1983).
33.
T. Elsaesser, A. Seilmeier, W. Kaiser, P. Koidl, and G. Brandt, Appl. Phys. Lett. 44, 383 (1984).
34.
M. Joffre, A. Bonvalet, A. Migus, and J. L. Martin, Opt. Lett. 21, 964 (1996).
35.
A. Bonvalet, M. Joffre, J. L. Martin, and A. Migus, Appl. Phys. Lett. 67, 2907 (1995).
36.
R. A. Kaindl, D. C. Smith, M. Joschko, M. P. Hasselbeck, M. Woerner, and T. Elsaesser, Opt. Lett. 23, 861 (1998).
37.
R. A. Kaindl, F. Eickemeyer, M. Woerner, and T. Elsaesser, Appl. Phys. Lett. 75, 1060 (1999).
38.
R. Huber, A. Brodschelm, F. Tauser, and A. Leitenstorfer, Appl. Phys. Lett. 76, 3191 (2000)
39.
E. S. Wachman, D. C. Edelstein, and C. L. Tang, Opt. Lett. 15, 136 (1990).
40.
Q. Fu, G. Mak, and H. M. van Driel, Opt. Lett. 17, 1006 (1992).
41.
K. C. Burr, C. L. Tang, M. A. Arbore, and M. M. Fejer, Opt. Lett. 22, 1458 (1997).
42.
A. Lohner, P. Kruck, and W. W. Rühle, Appl. Phys. B59, 211 (1994).
43.
J. M. Fraser, D. Wang, A. Hache, G. R. Allan, and H. M. vanDriel, Appl. Opt. 36, 5044 (1997).
44.
S. Ehret, and H. Schneider, Appl. Phys. B66, 27 (1998).
45.
For an overview, see W. R. Bosenberg, and R. C. Eckardt (eds.), Special issue on parametric devices, J. Opt. Soc. Am. B12, 2084 (1995).
46.
V. Petrov, F. Rotermund, and F. Noack, J. Opt. A: Pure Appl. Opt. 3, R1 (2001).
47.
F. Seifert, V. Petrov, and M. Woerner, Opt. Lett. 19, 2009 (1994).
48.
R. A. Kaindl, M. Wurm, K. Reimann, P. Hamm, A. M. Weiner, and M. Woerner, J. Opt. Soc. Am. B17, 2086 (2000).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_178_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 178
Chapter Four
49.
P. Hamm, R. A. Kaindl, and J. Stenger, Opt. Lett. 25, 1798 (2000).
50.
K. Reimann, R. P. Smith, A. M. Weiner, T. Elsaesser, and M. Woerner, Opt. Lett. 28, 471 (2003).
51.
Q. Wu, and X. C. Zhang, Appl. Phys. Lett. 71, 1285 (1997).
52.
J. A. Gruetzmacher and N. P. Scherer, Rev. Sci. Instrum. 73, 2227 (2002).
53.
B. A. Richman, K. W. DeLong, and R. Trebino, Nucl. Instrum. Meth. A358, 268 (1995).
54.
D. T. Reid, P. LozaAlvarez, C. T. A. Brown, T. Beddard, and W. Sibbett, Opt. Lett. 25, 1478 (2000).
55.
F. Eickemeyer, M. Woerner, A. M. Weiner, T. Elsaesser, R. Hey, and K. H. Ploog, Appl. Phys. Lett. 79, 165 (2001).
56.
C. W. Luo, K. Reimann, M. Woerner, T. Elsaesser, R. Hey, and K. H. Ploog, Phys. Rev. Lett. 92, 047402 (2004).
57.
A. Bonvalet, J. Nagle, V. Berger, A. Migus, J. L. Martin, and M. Joffre, Phys. Rev. Lett. 76, 4392 (1996).
58.
S. Mukamel, Principles of Nonlinear Optical Spectroscopy, Oxford, 1995.
59.
H. Haug, and S. W. Koch, Quantum Theory of the Optical and Electronic Properties of Semiconductors, World Scientific, Singapore 1993.
60.
D. M. Jonas, Annu. Rev. Phys. Chem. 54, 425 (2003).
61.
A. Seilmeier, H. J. Hübner, G. Abstreiter, G. Weimann, and W. Schlapp, Phys. Rev. Lett. 59, 1345 (1987).
62.
S. Lutgen, R. A. Kaindl, M. Woerner, T. Elsaesser, A. Hase, H. Künzel, M. Gulia, D. Meglio, and P. Lugli, Phys. Rev. Lett. 77, 3657 (1996).
63.
H. Wang, J. Shah, T. C. Damen, S. W. Pierson, T. L. Reinecke, L. N. Pfeiffer, and K. West, Phys. Rev. B52, R17013 (1995).
64.
F. Eickemeyer, K. Reimann, M. Woerner, T. Elsaesser, S. Barbieri, C. Sirtori, G. Strasser, T. Müller, K. Bratschitsch, and K. Unterrainer, Phys. Rev. Lett. 89, 047402 (2002).
65.
D. Y. Oberli, D. R. Wake, M. V. Klein, J. Klem, T. Henderson, and H. Morkoc, Phys. Rev. Lett. 59, 696 (1987)
66.
M. C. Tatham, J. F. Ryan, and C. T. Foxon, Phys. Rev. Lett. 63, 1637 (1989).
67.
T. Stroucken, A. Knorr, P. Thomas, and S. W. Koch, Phys. Rev. B53, 2026 (1996).
68.
J. E. Sipe, J. Opt. Soc. Am. B4, 481 (1987).
69.
F. Bloch, Phys. Rev. 70, 460 (1946).
70.
T. Shih, C. W. Luo, K. Reimann, M. Woerner, T. Elsaesser, I. Waldmüller, A. Knorr, R. Hey, and K. H. Ploog, Phys. Rev. B72, 195338 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_179_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures Ultrafast Dynamics of Intersubband Excitations
179
71.
J. A. Levenson, G. Dolique, J. L. Oudar, and I. Abram, Phys. Rev. B41, 3688 (1990).
72.
S. Hunsche, K. Leo, H. Kurz, and K. Köhler, Phys. Rev. B50, 5791 (1994).
73.
S. M. Goodnick and P. Lugli, Phys. Rev. B37, 2587 (1988).
74.
A. Tomita, J. Shah, J. E. Cunningham, S. M. Goodnick, P. Lugli, and S. L. Chuang, Phys. Rev. B48, 5708 (1993).
75.
S. Lutgen, R. A. Kaindl, M. Woerner, A. Hase, and H. Künzel, Solid State Commun. 106, 425 (1998).
76.
S. Butscher, J. Förstner, I. Waldmüller, and A. Knorr, Phys. Status Solidi B241, R49 (2004).
77.
Z. Wang, K. Reimann, M. Woerner, T. Elsaesser, D. Hofstetter, J. Hwang, W. J. Schaff, and L. F. Eastman, Phys. Rev. Lett. 94, 037403 (2005).
78.
S. SchmittRink, D. A. B. Miller, and D. S. Chemla, Phys. Rev. B35, 8113 (1987).
79.
B. N. Murdin, G. M. H. Knippels, A. F. G. van der Meer, C. R. Pidgeon, C. J. G. M. Langerak, M. Helm, W. Heiss, K. Unterrainer, E. Gornik, K. K. Geerinck, N. J. Hovenier, and W. T. Wenckebach, Semicond. Sci. Technol. 9, 1554 (1994).
80.
J. N. Heyman, K. Unterrainer, K. Craig, B. Galdrikian, M. S. Sherwin, K. Campman, P. F. Hopkins, and A. C. Gossard, Phys. Rev. Lett. 74, 2683 (1995).
81.
K. Craig, B. Galdrikian, J. N. Heyman, A. G. Markelz, M. S. Sherwin, K. L. Campman, P. F. Hopkins, and A. C. Gossard, Phys. Rev. Lett. 76, 2382 (1996).
82.
M. Hartig, S. Haacke, P. E. Selbmann, B. Deveaud, R. A. Taylor, and L. Rota, Phys. Rev. Lett. 80, 1940 (1998).
83.
Z. Xu, P. M. Fauchet, C. W. Rella, B. A. Richman, H. A. Schwettmann, and G. W. Wicks, Phys. Rev. B51, 10631 (1995).
84.
J. Faist, F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho, Science 264, 553 (1994).
85.
F. Capasso, K. Mohammed, and A. Y. Cho, IEEE J. Quantum Electron. 22, 1853 (1986).
86.
J. Rammer, Rev. Mod. Phys. 63, 781 (1991).
87.
H. Haug and A. P. Jauho, Quantum Kinetics in Transport and Optics of Semiconductors, Springer, Berlin, 1996.
88.
C. Rauch, G. Strasser, K. Unterrainer, W. Boxleitner, E. Gornik, and A. Wacker, Phys. Rev. Lett. 81, 3495 (1998).
89.
R. C. Iotti, and F. Rossi, Phys. Rev. Lett. 87, 146603 (2001).
90.
P. Kleinert and V. V. Bryksin, Physica B304, 60 (2001).
91.
S. C. Lee and A. Wacker, Phys. Rev. B66, 245314 (2002).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH04_180_03/23/2006 Ultrafast Dynamics of Intersubband Excitations in Quantum Wells and Quantum Cascade Structures 180
Chapter Four
92.
K. Leo, J. Shah, E. O. Göbel, T. C. Damen, S. SchmittRink, W. Schäfer, and K. Köhler, Phys. Rev. Lett. 66, 201 (1991).
93.
J. Feldmann, K. Leo, J. Shah, D. A. B. Miller, J. E. Cunningham, T. Meier, G. von Plessen, A. Schulze, P. Thomas, and S. SchmittRink, Phys. Rev. B46, 7252 (1992).
94.
C. Waschke, H. G. Roskos, R. Schwedler, K. Leo, H. Kurz, and K. Köhler, Phys. Rev. Lett. 70, 3319 (1993).
95.
M. Woerner, K. Reimann, and T. Elsaesser, J. Phys.: Condens. Matter 16, R25 (2004).
96.
C. Sirtori, P. Kruck, S. Barbieri, P. Collot, J. Nagle, M. Beck, J. Faist, and U. Oesterle, Appl. Phys. Lett. 73, 3486 (1998).
97.
R. F. Kazarinov and R. A. Suris, Fiz. Tekh. Poluprovodn. 5, 797 [Sov. Phys. Semicond. 5, 707 (1971)].
98.
R. F. Kazarinov and R. A. Suris, Fiz. Tekh. Poluprovodn. 6, 148 [Sov. Phys. Semicond. 6, 120 (1972)].
99.
C. Sirtori, F. Capasso, J. Faist, A. L. Hutchinson, D. L. Sivco, and A. Y. Cho, IEEE J. Quantum Electron. 34, 1722 (1998).
100.
R. C. Iotti and F. Rossi, Appl. Phys. Lett. 76, 2265 (2000).
101.
R. C. Iotti and F. Rossi, Appl. Phys. Lett. 78, 2902 (2001).
102.
H. Page, C. Becker, A. Robertson, G. Glastre, V. Ortiz, and C. Sirtori, Appl. Phys. Lett. 78, 3529 (2001).
103.
H. Vaupel, P. Thomas, O. Kühn, V. May, K. Maschke, A. P. Heberle, W. W. Rühle, and K. Köhler, Phys. Rev. B53, 16531 (1996).
104.
S. A. Gurvitz, I. BarJoseph, and B. Deveaud, Phys. Rev. B43, 14703 (1991).
105.
F. Wolter, H. G. Roskos, P. HaringBolivar, G. Bartels, H. Kurz, K. Köhler, H. T. Grahn, and R. Hey, Phys. Status Solidi B204, 83 (1997).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_181_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
5 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
Claire Gmachl Department of Electrical Engineering and PRISM Princeton University Princeton, New Jersey
Oana Malis Bell Laboratories, Lucent Technologies Murray Hill, New Jersey
Alexey Belyanin Department of Physics Texas A&M University College Station, Texas
5.1 Introduction to Nonlinear Intersubband Optical Transitions 5.1.1
Introduction
Nonlinear optics is an extensive field of research at the intersection of optics and material science with appeal to both pure scientific pursuit as well as applicationfocused engineering. Nonlinear optics encompasses all effects describing a change of the optical properties of a material under incident light. Such changes are usually very minute in 181
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_182_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 182
Chapter Five
naturally occurring materials, and the field of nonlinear optics was hence tightly coupled to the invention of the laser and continuing advances in laser science [1]. Lasers are the only (practical and convenient) light sources capable of generating sufficiently large optical fields to noticeably change the material’s optical properties. Over the last several decades, nonlinear optics has matured from being a descriptive science, measuring, calculating, and understanding the magnitude of the optical nonlinearities in naturally occurring and purified materials (such as vapors or solidstate crystals), to becoming an engineering science, capable of designing and fabricating new (quasi) materials displaying giant optical nonlinearities. A clear theoretical, quantum mechanical understanding of nonlinear optics, written into easytouse computer codes, as well as a compelling intuitive picture has helped to quickly advance the field. Within the intuitive picture, an electron in a confining potential, such as around an excited atom or molecule in a vapor or near a dopant ion in a solidstate crystal, is accelerated in this potential under an incident electromagnetic field. The accelerated electron oscillates and radiates according to its motion in the potential. This motion is the origin of the observed optical properties of the material, such as the refractive index. If the potential is asymmetric (anharmonic) and the driving field is large enough to force the electron into the noticeably nonharmonic portion of the potential, then the reradiated light will contain noticeable fractions of higher harmonics, with the actual shape of the potential determining the relative strength of the ensuing harmonics, such as in second harmonic generation (SHG) or third harmonic generation (THG). In analogy, one can infer that an electron in this anharmonic potential driven by two different incident electric fields will radiate the sumfrequency and/or differencefrequency generation (SFG and/or DFG) of the two incident fields. For an engineer of large optical nonlinearities, the intuitive message is then to design materials with as large an anharmonicity as possible of the electronic potential, and the reward is efficient nonlinear light generation. The above intuitive picture is instructive as a first means of gauging an optical nonlinearity; this classical model does not, however, account properly for electronic potentials with discrete energy levels, for which a quantum mechanical treatment is needed. The latter is especially essential as the optical nonlinearities are usually greatly enhanced near resonances with these discrete energy levels and at frequencies resonant with optical transitions between such quantized energy levels. Nevertheless, also the quantum mechanical models have fully been worked out, including several excellent textbook discussions [2–4], and result in workable solutions, based on the density matrix approach, for the nonlinear susceptibilities of quantum mechanical systems. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_183_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
183
Concurrently with nonlinear optics, the fields of semiconductor materials, devices, and especially lasers have equally matured. Semiconductor devices for either microelectronics or optoelectronics are highly advanced, and excellent modeling tools as well as fabrication methods exist, the combination of both allowing for swift device optimization and fast innovation cycles. While most optoelectronic devices use interband optical transitions across the material bandgap for electron– light interaction, recently another class of optoelectronic devices has attracted much (partly renewed) interest [5]. These are devices based on intersubband (ISB) optical transitions, mostly of electrons within the conduction band of a semiconductor heterostructure, such as single and coupled quantum wells (QWs), and superlattices (SLs). Much of this volume is dedicated to the physics and engineering of such devices, including quantum cascade (QC) lasers [6, 7], quantum well infrared photodetectors (QWIPs) [8], and modulators. Intersubband transitions are best understood and documented for the twodimensional QW systems; however, ISB transitions have also been discussed in zerodimensional quantum dots [9] and onedimensional quantum wire systems [10]. Intersubbandbased semiconductor structures are prime examples of engineered quasimaterials for which both design and fabrication methods (i.e., epitaxial layerbylayer growth with atomic layer precision) are extremely well developed, and nearly any conceivable energylevel combination, and hence effective electron potential, can be designed and fabricated. This is a most promising situation for the design of large optical nonlinearities based on semiconductor heterostructures. 5.1.2 Intersubband transitions and optical nonlinearities
Gurnick and DeTemple were first to argue in their seminal paper in 1983 [11] that the then rapidly progressing technologies of semiconductor heterostructure growth (especially molecular beam epitaxy and metalorganic chemical vapor deposition) could be harnessed for the design and fabrication of large optical nonlinearities based on asymmetric QWs. In their work they predicted between 10 and 100 times larger secondorder optical nonlinearities compared to the lattice value for a specially shaped, “graded,” asymmetric potential AlxGa1–xAs heterostructure. This enhancement would come on top of an already relatively large optical nonlinearity for GaAs bulk material resulting from its zincblende crystal structure. Following the work by Gurnick and DeTemple, a continuous, still ongoing stream of work has been dedicated to the exploitation of resonantly enhanced optical nonlinearities in specially shaped heterostructure potentials, including ISB optical Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_184_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 184
Chapter Five
structures. Giant, i.e., by several orders of magnitude enhanced, optical nonlinearities have been engineered and demonstrated [12, 13], the large increase in the nonlinearity being the result of the resonant enhancement of the nonlinearity at the discrete energy levels, and also the result of the large optical dipole matrix elements that are achievable for ISB transitions (typically several nanometers, compared to angstroms for interband transitions), and which enter into the optical nonlinearity with higher order. A single, undisturbed QW still constitutes a highly symmetric potential without much nonlinearity; thus, several strategies have evolved since the proposal by Gurnick and DeTemple to break the symmetry of the single well, and achieve large potential asymmetry, manifested in the symmetry breaking of the electronic wave functions, a loosening of the selection rules for transitions between states, and— related to that—large optical dipole matrix elements between all confined energy levels. Figure 5.1 shows a collection of such potentials and strategies for symmetry breaking. Figure 5.1a is the proposed asymmetric potential by Gurnick and DeTemple. This proposal was quickly followed by asymmetry induced by an applied electric field [14] (Fig. 5.1b, which allows for field tunability of the nonlinearity, both by changing the dipole matrix elements and by adjusting the resonance conditions), by step QWs [15] (Fig. 5.1c) and coupled QWs [16] (Fig. 5.1d). The primary material systems employed for such bandgap engineering are GaAs/AlxGa1–x As,InxGax –1As/AlyIny –1As grown strained,
Energy
(a)
Graded composition
(b)
Electric field induced
x
(c)
Step quantum well
(d) Asymmetric coupled quantum wells
Figure 5.1 Schematics of approaches to QW potentials with an asymmetry leading to observable optical nonlinearities. (a) Gradedcomposition QWs as first proposed by Gurnick and De Temple [11]; (b) an asymmetry induced by an applied electric field [14]; (c) step QW [15]; and (d) asymmetric coupled QWs [16]. (The energy levels and wave functions are schematic only.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_185_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
185
straincompensated, or latticematched on InP, and more recently also GaN/AlxGa1–xN [17], Sb [18], and IIVI [19] related materials; and the nonlinear optical effects most commonly investigated are SHG, THG, DFG, SFG, Raman scattering, and the optical Kerr effect. Following the original proposal by Gurnick and DeTemple, several more theoretical discussions of nonlinear effects based on ISB transitions were published, with the one by J. Khurgin [20] being an excellent and rather complete example. The first experimental evidence followed in 1989. Fejer et al. demonstrated the first evidence for large secondorder susceptibility and SHG in a GaAs/AlGaAs QW under an electric field and pumped by an CO2 laser, in the midinfrared (midir) wavelength range of 9.6 to 10.8 ȝm [21]. Rosencher et al. reported the first experimental demonstration of SHG and optical rectification in a stepQW in 1989 [22] and 1990 [23], also in the midir; and Sirtori et al. demonstrated the first SHG in an asymmetric coupled doubleQW in 1991 [24]. Thirdorder optical nonlinearities were first reported in experiments by Segev et al. [25]. Nonlinear light generation in the farir and terahertz regime was reported first by Bewley et al. [26] for a semiparabolic graded QW, and by Sirtori et al. for coupled QWs [27]. Heyman et al. reported the first evidence of dynamical screening and the depolarization shift in ISB transitions [28]. Most of these examples use resonant ISB transitions in the conduction band of directgap GaAs/ AlGaAs and InGaAs/AlInAs QWs. In the early 1990s, the interest shifted partially also to the valence band, with theoretical discussions by Tsang and Chuang [29] and Li and Khurgin [30], as well as to inclusions of additional conduction band valleys such as the L valley in Sbbased QWs by Xie et al. [31]. Good examples of publications summarizing this progress can be found in Ref. 5 or 13. Aside from the intellectual challenge of designing and fabricating synthetic, engineered, novel materials with new giant optical nonlinearities, much of this work is also motivated by applications, and by supporting functions in a wider range of optoelectronic devices. A general appeal of this work follows from the wavelength coverage of ISB transitions in IIIV semiconductor materials, which coincides with the midir and farir wavelength range, for which few practical alternative materials exist. The first application, at the very heart of nonlinear optics, is wavelength conversion, i.e., the use of highperformance lasers operating in one wavelength range to generate light in another wavelength range that is not easily accessible otherwise. Excellent examples of wavelength conversion have been reported in Ref. 32 where the light of nearir semiconductor laser diodes is used to generate tunable midir light; or in Ref. 33 where nearir light is converted to terahertz light. One extremely beneficial aspect of wavelength conversion is that significant Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_186_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 186
Chapter Five
features of the pump lasers, such as a wide tuning range, are translated to the new wavelength range. As a result, nonlinear light sources often have superior tuning characteristics compared to linear light sources; this fact is amply demonstrated by the commercial availability of optical parametric amplifiers and oscillators (OPAs and OPOs). For this application, wavelength conversion, ISBbased nonlinearities are of interest simply for their giant nonlinearities, which should lead to very efficient wavelength conversion and hence compact optical systems. A second group of applications relates to refractive index modulators [34], saturable absorbers [35], optical limiters [36], and Kerr switches [37], essentially a wide range of light modulators in which the transmission of one light signal through the material is controlled by another pump signal or light beam (selfmodulation is also possible). In these applications, ISB transitions are of particular interest due to their ultrafast (about picosecond), nonlinear relaxation rates [38]. Recent work on ISB optical transitions for the communications wavelength range (~1.55 m) is a prime example of this concentration [39]. A third application is nonlinear detectors, such as nonlinear QWIPs [40]. The interest stems from the operating wavelength in the midir and the ability of phasesensitive light detection, such as upconversion autocorrelation. Another recent interest stems from the interplay between quantum optics and nonlinear optics as ISB resonances have become narrow enough (as a result of improved material quality) to display the strong coupling effects previously reserved for vapors or ions in solidstate crystals [41]. This is a recent field of interest, which includes ideas as varied as photon pair generation, electromagneticinduced transparency [42], lasing without inversion [43], and similar effects. Aside from the considerable successes that have been documented for ISBbased optical nonlinearities (such as the ones given above), several drawbacks are also inherent to them, which need specific attention. Leading among those difficulties is the fact that the nonlinearities are only strongly enhanced for light traveling inplane with the QWs, as significant optical dipole matrix elements only exist for an electric field polarized normal to the QW plane, i.e., the plane of electron confinement. As a result, for efficient nonlinear light generation or manipulation, light needs to be efficiently coupled into the inplane configuration, which is inherently more difficult than normal incidence coupling (but not impossible). A second issue is the resonant absorption accompanying most ISBbased optical nonlinearities. The strength of the optical nonlinearity is about proportional to the density of electrons in the asymmetric QW potential, assuming only one energy level, usually the lowest one, is Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_187_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
187
occupied. As this lowest energy level is a real state with real electron population, it induces strong resonant absorption of either the pump light or the nonlinear light, or even both, depending on the nature (real or virtual) and resonance condition of each subsequent energy level. Real and nearresonant energy levels show resonant enhancement of both the nonlinearity and the absorption, with the latter outweighing the former under most conditions [12, 13]. Hence, only nearresonant optical nonlinearities are used, or new methods of populating the nonlinearities with charge carriers have to be found and implemented. We show in the subsequent sections how a quantum cascade approach can be used for this implementation. The third challenge is related to phase matching. As semiconductor materials have noticeable nonzero material dispersion across the wide wavelength spans of nonlinear optics, the copropagation of linear and nonlinear light generally leads to destructive interference of the nonlinearly generated light along the propagation direction of the primary pump beam. Additionally, the fact that the optical nonlinearity is strong mostly for the inplane light favors copropagating pump and nonlinear light within a waveguide structure; this adds complexity to the situation in the form of waveguide dispersion. The commonly used IIIV materials are furthermore not (sufficiently) birefringent such that birefringence phase matching is not a viable option. Nevertheless, quasiphase matching has been demonstrated [44], and modal phase matching has also been implemented [45] and is described in greater detail in a later section. Overall, the initial shortcomings of inplane propagation, resonant absorption, and the need for phase matching have been repeatedly addressed, and with good success. The most recent solution comes from the integration of the ISB optical nonlinearities with ISB QC lasers, the main topic of the second part of this chapter. 5.1.3
Theoretical model
Before focusing on the implementation of optical nonlinearities into QC lasers, we will briefly present the theoretical framework used here to calculate the strength of the optical nonlinearities and the expected nonlinear optical output power. This theoretical model employs density matrix formalism following the calculation of the energy levels and wave functions from solving Schrödinger’s equation in the envelope function approximation. The electromagnetic fields are treated classically with Maxwell’s equations. Excellent textbook discussions of these formalisms can be found in Refs. 2, 3, and 4. We here reproduce the derivation that we presented in Ref. 48, which in itself follows the textbook of Ref. 2. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_188_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 188
Chapter Five
Figure 5.2 shows a schematic of the conduction band diagram of a coupled QW structure under an applied electric field, which was previously designed for efficient SHG [46]. This nonlinearity is populated with electrons following a cascade approach, such that under the appropriate bias energy level 3, the center level of the nonlinear level triplet is populated. This is one of the approaches that strongly reduce the absorption of the nonlinear light; it does, however, carry the penalty of pumplight absorption. Level 2 is considered practically empty of electrons, which quickly scatter through resonant longitudinal optical phonon emission into level 1 [6]. The structure is designed with large optical dipole matrix elements between all levels 2, 3, and 4; this structure “D2912” is discussed in greater detail in Ref. 48 and Sec. 5.4.2. Equations for the density matrix elements ȡmn for this multilevel system can be written in the following general form [2]: dȡmn ie + (Ȗ mn + iȦ0mn )ȡ mn = E ( zmq ȡ qn í zqn ȡmq ) dt ല q
(5.1)
dȡmm ie ^ + Rm = E ( zmq ȡqm í zqm ȡ mq ) dt ല q
(5.2)
Here Ȗmn is the relaxation rate of the offdiagonal element ȡmn of the density matrix, Ȧ0mn is the transition frequency, zmn is the optical dipole ^ moment of the transition m – n, and Rm denotes all relaxation and pumping terms that determine the population nm = ȡmm of the mth state in the absence of a radiation field; e is the electron charge, and ƫ is the reduced Planck constant. The electric component E(r, t) of the radiation field is considered to be a sum over quasimonochromatic components with slowly varying
5 4
Energy
e
3 2 1
e
x
Figure 5.2 Conduction band diagram and moduli squared of the essential wave functions of a twowell active region design suitable for laser emission (wavy line) between energy levels 3 and 2, and nonlinear light generation from the level triplet 2–3–4 (thin arrows). The thick gray arrows indicate the injection and exit of the electron flow. (Source: Ref. 46.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_189_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
189
amplitudes Fmn and frequencies Ȧmn nearly resonant to the transition frequencies Ȧ0mn : E (r, t ) = F mn (r, t )e
íiȦ mn t
+ c.c.
(5.3)
In the SHG process (see Fig. 5.2) Ȧ32 = Ȧ43 = Ȧ, and Ȧ42 = 2Ȧ, where Ȧ is the fundamental frequency of the pump laser. Similarly, F32 = F43 = EȦ and F42 = E2Ȧ. Offdiagonal elements of the density matrix can be written as
ȡmn (t ) = ı mn (t )e
íiȦ mn t
(5.4)
where the amplitude ımn is a slowly varying function of time. For the diagonal elements, ȡmm = ımm. Using the expressions in Eqs. 5.1 and 5.2, we arrive at the truncated density matrix equations dı mn ie + īmn ı mn = ( z F ı í zqn F qn ı mq ) dt ല q mq mq qn
(5.5)
dı mm ^ ie + Rm = ( z F ı í zqm Fqm ı mq) dt ല q mq mq qm
(5.6)
* * , z * Here īmn = Ȗ mn + i (Ȧ0mn í Ȧ mn ), ımn = ımn mn = zmn , and F mn = F mn . The nonlinear polarization at the second harmonic can be calculated from Eqs. 5.5 and 5.6 as
P(r, t ) = eNe z24ȡ42
(5.7)
where Ne is the volume density of electrons in the active mixing region. This polarization serves as a source for the electromagnetic field at the second harmonic. [Here we have neglected the potential presence of nonresonant lattice nonlinearities and other nearresonant nonlinearities, such as the cascade 3–4–5 in Fig. 5.2. If the latter were included (as is done later in Sec. 5.4.2 and in Ref. 46), then P(r, t) = eNe (z24ȡ42 + z35ȡ53).] In solving for the steadystate solution, all timedependent terms in the above equations are set to zero, and the calculation of ı42 is reduced to algebra. In principle, the expression for the nonlinear polarization defined by Eq. 5.7 is valid for arbitrarily strong field amplitudes and includes all resonant nonlinear effects such as saturation and power broadening. However, for weak enough fields, we can expand the solution in powers of the field amplitudes and arrive at the following expression for the amplitude of nonlinear polarization in the Ȥ(2)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_190_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 190
Chapter Five
approximation P(2Ȧ) = Ȥ(22Ȧ) Ex2(Ȧ), where Ȥ(2) is the secondorder nonlinear susceptibility: 2) Ȥ(2Ȧ =
e 3 Ne z23 z34 z24 n3 í n4 n3 í n2 P(2Ȧ) = + ī42 ī43 ī32 E x2(Ȧ) ല2
(
)
(5.8)
Here Ex(Ȧ) is the x component of the electric field at fundamental frequency Ȧ; and x is the coordinate in the growth direction [001], i.e., normal to the QW plane. Increasing the field intensity beyond the saturation value leads to the decrease in the population differences ค [1/Ex(Ȧ)2] and broadening of the line widths ī42 คEx(Ȧ)2, so that the value of Ȥ(2) decreases. The saturation intensity is on the order of 1 MW/cm2, assuming exact resonance, and increases with detuning. In the same weakfield approximation, the nonlinear polarization amplitude at the third harmonic is given by P(Ȧ) = eNe z25ı52 싉
ie 4 z23 z34 z45 z25 Ne E x3(Ȧ) ല3ī52
(5.9a)
1 n3 í n4 n3 í n2 1 n4 í n5 n3 í n4 + í í ī43 ī32 ī54 ī43 ī42 ī53
(
Ȥ(33Ȧ) = 싉
)
(
)
P(3Ȧ) E x3(Ȧ) ie 4 z23 z34 z45 z25 Ne
(5.9b)
ല3ī52 1 n3 í n4 n3 í n2 1 n4 í n5 n3 í n4 + í í ī43 ī32 ī54 ī43 ī42 ī53
(
)
(
)
5.2 Application of Intersubband Optical Nonlinearities to Quantum Cascade Lasers 5.2.1 Monolithic integration of nonlinearity and pump laser
As shown in Sec. 5.1, nonlinear optics with ISB transitions is a broad and promising field of science and engineering. Recently, these transitions have been implemented into QC lasers for the first time [47]. This integration of QC pump lasers and ISBbased optical nonlinearities has allowed the mitigation of several of the earlier drawbacks of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_191_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
191
combinations of separate ISBbased nonlinear crystals and external pump lasers, such as a CO2 laser. The realization that ISB optical nonlinearities are straightforward to implement into QC lasers stems from the fact that both are based on ISB transitions, both obey the same polarization selection rules, and hence both would couple efficiently to each other via the light field. In monolithically integrating the optical nonlinearity and the QC lasers into one laser waveguide and cavity, several clear advantages arise. First, the intracavity optical field inside a QC laser can be very high (up to few megavolts per centimeter) [48], essential for an efficient presentation of the nonlinear effects; and the overlap of the nonlinear material and the pump light field can be made large through deliberate semiconductor waveguide design [49], which is a highly mature field, for which excellent solutions and computational modeling tools exist. The integration of the optical nonlinearity with the QC laser can essentially be accomplished in one of two different ways, both of which are outlined in Fig. 5.3. First, the nonlinear region can be made a separate stack [50] of coupled or otherwise asymmetric QWs inserted into the QC laser cavity wherever the laser field is large (Fig. 5.3a). In this case, the nonlinear structure can be separately optimized from the QC laser structure, which is advantageous for both. Yet, the nonlinear region should still be made capable of conducting the current density necessary for QC laser operation. In principle, a multiterminal device can be envisioned (see Fig. 5.3b) [50], which bypasses the nonlinear region; nevertheless, despite having been demonstrated, such multiterminal devices are cumbersome to fabricate, especially for large currentcarrying devices such as the QC laser. Conversely, twoterminal devices with heterogeneous cores have repeatedly been shown to work well, even when the substacks required different local electric fields for operation [50]. A particular type of such heterogeneous integration is interleaved “interdigitated” active and nonlinear regions with matching injector regions [51]. The requirement for the nonlinear region to carry current has both an advantage and a disadvantage. On one hand, under bias it is fairly straightforward to concentrate electrons in an excited energy level by implementing a cascade scheme similar to that of QC lasers. This is done though the appropriate tailoring of the interlevel scattering times (longitudinal optical phonon scattering for midir ISB transitions). As a result, the nonlinear optical transition can be made transparent for the nonlinear light, which is clearly advantageous. On the other hand, a concomitant requirement is that the tunneling times for electrons through the heterostructure be sufficiently short to allow for a low differential resistance and hence good current and voltage stability [52]. This design criterion implies that the wave functions overlap and mix Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_192_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 192
Chapter Five
(a)
(c)
(b)
(d)
Stack of nonlinear active regions and injectors Stack of QC laser active regions and injectors Interleaved stack of nonlinear and QC laser regions Nonlinearity and QC laser in shared quantum wells Figure 5.3 Schematics of various approaches to integrate an optical nonlinearity with a
QC laser. (a) Separate serial stacks (black and gray bands) for the nonlinear and laser materials, and current is flowing through both stacks; (b) separate stacks and separate contacts for the laser and nonlinear regions; (c) interleaved laser active regions and nonlinear active regions; (d) the nonlinearity and laser active regions are implemented within the same active region (and injector) QWs.
across the structure, which generally leads to somewhat smaller optical dipole matrix elements and concomitant nonlinearities than could be achieved by using isolated asymmetric, coupled QWs. The second method of monolithically integrating the nonlinearity into the QC laser entails integrating it directly into the QC laser structure, taking advantage of the QWs in the latter. Here again, one may use QWs in the injector regions of the QC laser to form the optical nonlinearity—an approach that has, to our knowledge, not yet been tried—or directly employ the laser active region to build the nonlinear region with significant level and population sharing between the two. This approach is highly advantageous because it practically guarantees near resonance for one “leg” of the nonlinear optical transition. Conversely, because lasers and nonlinearity share significant design resources, some compromises in design may have to be made for both. Furthermore, at high optical power, high optical nonlinearity, and high lineartononlinear conversion efficiency, the pump laser transition may be bleached with direct detrimental consequences for laser operation. Nevertheless, this type of monolithic integration has been used predominantly in the literature so far and with good results [46, 47]; the nonlinear power levels are still far from where bleaching would be expected to occur. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_193_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
193
5.2.2 Phase (mis)match and nonlinear optical power
The monolithic integration of the optical nonlinearity together with the pump laser into one waveguide and cavity raises a new challenge related to the phase mismatch between fundamental and nonlinear light. Given the (usually) linear geometry of the laser cavity, both waves necessarily are copropagating in guided modes along the same waveguide. First, the waveguide (or, potentially, twin waveguide [53]) must be capable of supporting the modes of all light fields, often at very different wavelengths, involved in the nonlinear process. Yet even then, the material and modal dispersion lead to different propagation constants, and effective modal refractive indices, for the different modes. One can estimate the power of the nonlinear signal, as we demonstrate here for SHG, that can be obtained from such an integrated waveguide geometry for various conditions of mode (mis)match. As a starting point, the guided modes at the various wavelengths of the “cold” waveguide are calculated. Only the transverse magnetic (TM) modes are excited efficiently since the polarization associated with electronic ISB transitions contains only the x component, i.e., the field component normal to the QW plane. In conventional QC laser waveguides, a small number of lateral transverse modes are usually supported; i.e., the laser cavities are rarely transverse singlemode waveguides. Given the dominance of freecarrier absorption in the waveguide loss, which increases about quadratically with wavelength, the multiwavelength waveguides need to be optimized for the longest wavelength to be supported in them. As a result, for the shorter wavelengths the waveguide is “oversized,” and a large number of lateral and vertical transverse modes exist, each with its own propagation constant. For the TM modes it is convenient to use the magnetic field of the modes as a description; the magnetic field amplitude Hy(r) of a given TM mode with frequency Ȧ and longitudinal wave number k = Ȧȝ/c, where ȝ is the mode effective refractive index and c is the speed of light in vacuum, can be represented as a product of functions A(z) exp ikz, where the complex function A(z) varies slowly with coordinate z along the waveguide direction, and the transverse distribution HȦ(x, y), which satisfies the transverse Helmholtz equation for the “cold” waveguide:
( Ȧ, x, y )
(x
Ȧ2 İ (Ȧ, x , y ) + H+ í k2 H = 0 İ x y İy c2
) (
)
(5.10)
The x component of the electric field is related to Hy as Hy/z = iȦİ (Ȧ, x, y)Ex/c. Substituting the above expression for Hy into the wave equation for the second harmonic polarization, using the orthogonality of the functions H for modes of different order, and solving the resulting Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_194_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 194
Chapter Five
equation for the amplitude A2Ȧ, we arrive at the expression for the nonlinear signal power 128ʌ5 Ȉ W12 R21 + e W2 ~
íĮ 2 L
í 2R1e
ía L 2 / 2
cos( ǻk L ) (1 í R2)
˜2)(1 í R1)2 ȝ21ȝ2cȜ22( ǻk 2 + Į
(5.11)
Į = Į2 / 2(1 / L) ln(1 / R1); Į2 stands for the waveguide intensity where ˜ losses at wavelength Ȝ2 = Ȝ1/2 of the SHG signal; L is the cavity length; R1,2 and ȝ1,2 are the intensity reflection factors of one cavity facet and effective refractive indices of modes at wavelengths Ȝ1,2, respectively; ǻk = k2Ȧ – 2kȦ = 2Ȧ(ȝ2 – ȝ1)/c is the phase mismatch; and W1 is the power in the fundamental mode. We took into account only the interaction of copropagating modes and assumed that the intracavity intensity of the pump has an unsaturated exponential profile along the cavity. The nonlinear overlap factor Ȉ, which defines an effective interaction cross section Â = Ȥ(2)2/Ȉ of two TM modes, is given by =
ȝ41ȝ22
/ (
(
H22Ȧ
2
1 Ȥ ( x, y ) 2 HȦ2 H2 Ȧ d x d y İȦ ( 2)
1 2 dx d y H dx d y İȦ Ȧ
)
2

1 H2 dxd y İ2 Ȧ 2 Ȧ
)
(5.12)
where İȦ(x, y) and İ2Ȧ(x, y) are the dielectric permittivities of the waveguide at frequencies Ȧ and 2Ȧ, respectively. The values of Â are between 300 and 1000 ȝm2 for typical QC laser waveguides, depending on the thickness of the laser core, i.e., the number of linear/nonlinear active regions and injector pairs. Using Eqs. 5.8, 5.11, and 5.12, one can now estimate the expected secondorder optical susceptibility Ȥ(2) and the nonlinear conversion efficiency Ș = W2 /W12. While the particular geometry and coupling of pump laser and optical nonlinearity are evidently highly sensitive to the phase mismatch ǻk, the large number of available transverse modes allows for true modal phase matching for a particular choice of engineered waveguide and pair of modes. We discuss phase matching in Sec. 5.7. The intracavity wave mixing described here for nonlinear QC lasers has been previously proposed and recently demonstrated for interband semiconductor lasers [54] as an efficient mechanism to combine pump and mixing nonlinearity. Overall, the implementation of nonlinear active regions into QC lasers is highly advantageous as an alternative way to produce very shortwavelength (Ȝ < 4 ȝm) light in QC lasers [55]. Such short wavelengths are of importance, e.g., for trace gas sensing of lightweight Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_195_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
195
molecules [56]. Furthermore, many of the concepts discussed here are similarly valid for a much wider range of nonlinear optical effects including SFG, DFG, and higher harmonics generation, which in their entirety will significantly broaden the wavelength range and versatility of QC lasers. 5.3 SumFrequency Generation in Quantum Cascade Lasers Using Resonant Intersubband Nonlinearities The first implementation of an optical nonlinearity into a QC laser was reported in Owschimikow et al. [47]. The original goal of this work was SFG based on two basic, rather practical considerations. First, upconversion into the shortwave (3 to 5 ȝm) midir would allow using the highly sensitive InSb detector, hence improving the chances of detecting the expectedly small signals; second, SFG, given its multiple wavelengths, would prove interesting and adaptable enough to evaluate the interplay of nonlinearity and QC lasers. In fact, given the nanowatt signal levels of these early structures, the choice of upconversion was clearly fortuitous, and in addition to the sumfrequency, this early structure surprised by displaying SHG, which was later understood from the width of the ISB resonances and overall resonance conditions. The structure of Ref. 47 was chosen to be a twostack, twowavelength (Ȝ ~ 7.1 and 9.5 ȝm) QC laser [50] including a superlattice (SL) section sandwiched between the two laser stacks. The laser waveguide core contained a 500nmthick, lowdoped InGaAs buffer layer followed by a stack of 16 periods of alternating active and injector regions [7] designed to emit at 7.1ȝm wavelength. Each injector region was doped to a sheet density of 2.0 × 1011 cmí2. Separated from this stack by 25 nm of lowdoped InGaAs, an 18period SL of alternating 4.1nmthick InGaAs wells and 2.3nmthick AlInAs barriers was grown into which nine equally spaced QWs, each 2.4 nm thick, were inserted. The entire SL totals 27 QWs and is doped homogeneously to 3 × 1016 cmí3. After another 25nmthick InGaAs spacer layer, a second QC laser stack containing 19 periods of active regions and injectors designed for emission at 9.5 ȝm followed, doped to a sheet density of 1.9 × 1011 cmí2 in each injector. A 200nmthick InGaAs layer completes the waveguide core. A conventional, ternary top waveguide cladding, and the InP substrate as bottom cladding are used [49]. Figure 5.4 shows the modeintensity profiles at the two laser wavelengths as well as at the SFG wavelength, and it also shows the arrangements of the lasers and SL in the waveguide core. The effective modal indices of this structure at the various wavelengths (calculated using a Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_196_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Chapter Five
10 7.1μm laser: neff = 3.297
0
0
Superlattice 7.1μm laser
9.5μm laser: neff = 3.258
4.1μm mode: neff = 3.353 9.5μm laser
Mode intensity (arb. units)
196
5 Distance (μm)
Substrate
10
Figure 5.4 Calculated modeintensity profiles at the two laser wavelengths as well as at
the SFG wavelength of the first implementation of a nonlinear QC laser, from Ref. 47. The effective modal indices at the various wavelengths (calculated using a onedimensional model for infinitely wide waveguides) are given.
Energy (eV)
onedimensional model for infinitely wide waveguides) are clearly different; i.e. the modes are noticeably phase mismatched. This structure provides two distinct sources of resonant secondorder ISB nonlinearities, one in the SL and one in the layer structure of the 7.1ȝmwavelength laser. The designs of both structures are shown in Figure 5, and the optical transitions are indicated by the arrows. In the SL the first transition from the energy levels of the lowest miniband (1 in Fig. 5.5a) to the localized states of the inserted QWs (2) is in near resonance with the radiation of the 9.5 ȝm laser. The second transition, from these localized states (2) to the bottom of the second miniband (3), is near resonant with the 7.1ȝm radiation. We calculate the transition frequencies Ȧij (i, j = 1, 2, 3) of ƫ·Ȧ21 = 134 meV, ƫ·Ȧ32 = 171 meV, ƫ·Ȧ31 = 305 meV, and the corresponding optical dipole moments z21 = 0.4 nm, z32 = 1.3 nm, and z31 = 0.02 nm. The second optical nonlinearity can be found in the 7.1ȝm QC laser (Fig. 5.5b). While QC laser action is taking place between energy
5 4 0.5 3 3
2 1 0 0
20 (a)
2 1 Bias: 55 kV/cm 40 0 20 40 60 Distance (nm) (b)
Schematics of the conduction band diagrams of the mixing (a) SL and (b) QC laser active region incorporating the optical nonlinearity. In (a) the resonant nonlinearities result from transitions 1–2–3. In (b) the QC laser process is supported by levels 3, 2 and 1; the optical nonlinearities stem from resonant transitions 3–4–5. (Source: Ref. 47.) Figure 5.5
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_197_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
197
levels 3 and 2 [6, 7], nearresonant optical transitions of 9.5 and 7.1 ȝm can be found from level 3 to level 4 and from the latter on to level 5, respectively. Also here we calculate the relevant parameters as ƫ·Ȧ43 = 143 meV, ƫ·Ȧ54 = 164 meV, ƫ·Ȧ53 = 307 meV, z43 = 0.7 nm, z54 = 1.8 nm, and z53 = 0.4 nm. The line broadening at the pump frequencies is about 10 meV, and at a mixing frequency it is 20 to 30 meV. The presence of the nonlinearity in the QC laser region was somewhat fortuitous, and it enhanced the overall optical nonlinearity. In addition to the wafer above, a second wafer was grown, in which the SL was entirely homogeneous (alternating 4.1nmthick InGaAs wells and 2.3nmthick AlInAs barriers) and did not contain energy levels 2; in this wafer only the nonlinearity within the 7.1ȝm QC laser was active. The secondorder nonlinear susceptibilities were estimated by using the density matrix approach for the above nonlinearities, with SFG mixing at 4.1 ȝm resulting from the 7.1ȝm QC laser region providing the largest optical nonlinearity. Including all ISB transitions, a secondorder optical susceptibility of Ȥ(2) § 3.4 × 10í10 (N3/1016 cmí3) m/V was estimated, where the population N3 of state 3 changes between ~2 to ~5 × 1016 cmí3 as the current increases. This value of Ȥ(2) is approximately one order of magnitude greater than the lattice nonlinearity of the waveguide core. Deepetched ridge waveguide lasers were processed in conventional fashion [6, 7] with ridge widths ranging from 10 to 20 m and cleaved cavity lengths from ~1 to 3 mm. The lasers were mounted in a temperaturecontrolled He flow cryostat and were operated in pulsed mode with pulse widths ranging from 50 to 600 ns and at a 1.8 to 85kHz repetition rate. The laser output power was measured by using a calibrated, room temperature HgCdTe (MCT) photovoltaic detector. The laser spectra were measured by using the rapidscan mode of a Nicolet 860 Fourier transform infrared (FTIR) spectrometer and a liquidnitrogencooled HgCdTe photocurrent detector. The shortwavelength radiation was measured by using a calibrated, liquidnitrogencooled InSb photovoltaic detector fitted with a sapphire flat to suppress the longwavelength radiation. The shortwavelength spectra were obtained with the same detector and by using the FTIR spectrometer in step scan mode. We furthermore used a set of interference filters in the 4 to 6ȝmwavelength range and a wiregrid polarizer to discriminate between the various components of the emitted radiation. We performed similar measurements with other twowavelength lasers [50] to rule out spurious effects in the detection optics and electronics. Figure 5.6a shows highresolution spectra of a laser obtained at various levels of pumping current and at 10 K heat sink temperature. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_198_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
Intensity (arb. units)
198
Chapter Five
2.0 A
0 1.5 A
0 1.0 A
0
7.1
7.2 7.3 9.4 9.5 Wavelength (μm)
9.6
(a)
Intensity (arb. units)
10
ω2+ ω1
2.0 A 1.5 A 1.0 A
2ω1
2ω2
0 3
4 5 Wavelength (μm)
6
(b) Figure 5.6 (a) Highresolution spectra measured of a 10mwide, 1.6mmlong laser
under pulsed operation at various levels of peak current, as indicated. (b) Lowresolution stepscan spectra of the same device measured under the same operating conditions in the shortwavelength region. The spectra are offset with respect to one another, and the peaks are labeled in accordance with their origin, SFG and two SHG signals. The small arrow indicates the spectral cutoff of one filter used in the experiment. (Source: Ref. 47.)
Figure 5.6b shows the corresponding shortwavelength spectra. We observe SFG and SHG at 4.1 (Ȧ1 + Ȧ2) and 3.6 (2Ȧ2) and 4.75 ȝm (2Ȧ1), respectively. With increasing pumping level the relative strengths of the various components change, but we consistently observe all three components. The broad, slowly rising background, which we interpret as spontaneous emission from electrons excited into highlying energy levels and the continuum above the barriers, can also be found in conventional QC lasers under high pumping conditions. In Fig. 5.7 the light output power and voltage versus current (LIV) characteristics of the laser of Fig. 5.2 are shown, as well as the power of the nonlinearly generated radiation. The measurements have been taken at 10 K heat sink temperature. Laser threshold is reached at 550 mA approximately simultaneously for both wavelengths, and peak power is reached at 2.6 A with 90 and 60 mW for 9.5 and 7.1ȝm wavelength, respectively. Close to peak power, a sudden, strong
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_199_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
SH&SF power (nW)
Optical Nonlinearities
30
(a)
(c)
(b) 4.7 μm
4.1 μm
199
3.6 μm
20 10 0
2
0
4 0 2 0 2 4 2 2 (Laser power) (× 1000 mW ) 4
(a) 2
5
10
Bias (V)
(d)
15
0.3 100
10 5 0 0
9.5μm laser 7.1μm laser
50
2 1 Current (A)
3
0
Laser power (mW)
0 15
0.2 0.1
SH&SF power (μW)
Current density (kA/cm )
0
(b) (a – c) Optical power measured for SFG signals [open triangles in (b)] and SHG signals [filled circles and squares for (c) 7.1 and (a) 9.5 m, respectively] versus the power squared of the respective fundamental pump light. The symbols represent data, and the straight lines are from calculations. (d) Light output and voltage versus current characteristic and combined short wavelength power of the laser of Fig. 5.6. The little arrows pointing to the current axis indicate the positions where the spectra of Fig. 5.2 and the data points of parts (a) to (c) have been taken. (Source: Ref. 47). Figure 5.7
increase in operating voltage occurs, indicative of a negative differential resistance region. We interpret this behavior as domain formation in the SL [52], when the low doping level of the latter is not anymore capable of screening the applied external electric field. Such occurrence can be mitigated by higher doping or a modified design of the SL. Nevertheless, as can be seen in Fig. 5.7d, the combined shortwavelength emission reaches a power level of 180 nW. Figure 5.7a through c show a detailed measurement of the optical power in each mixing component versus the power product of its generating laser sources. These data have been deduced from stepscan spectra and the laser data of Fig. 5.7d. The nonresonant background has been subtracted; yet the limited resolution of the stepscan spectra likely leads to a slight overestimation of the power at low pumping levels. The results of our theoretical calculations are also shown in Fig. 5.7a to c. The power of each mixing signal has been obtained from solving the wave equation with the nonlinear polarization as a source, as
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_200_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 200
Chapter Five
outlined in Sec. 5.2.2, taking into account the phase mismatch of the waveguide modes and their losses due to diffraction and freecarrier absorption. Resonant losses due to resonant intersubband absorption have been neglected, first, because of the nonresonant nature of the nonlinearities, and, second, because of the dominant factor of the nonphasematched structure. Similar formulas have been obtained for the secondharmonic signals. They are all shown in Fig. 5.7a to c as theoretical curves, evaluated for N3 = 4 × 1016 cmí3, and are in good agreement with the data. However, at high pumping levels, the data display noticeable deviations from the calculated linear curves. This can be understood from several effects. First, as the current flow is increased through the structure, also the relative electron population of the upper laser level (3 in Fig. 5.5b) increases; e.g., an increase of N3 to 5 × 1016 cmí3, consistent with QC laser operation, can already explain the deviation of the experimental curves (Fig. 5.7b and c) from straight lines at high powers. Another effect concerns the dependence of the dipole moments on the applied bias. This effect, especially important for dipole moment z54, also leads to an excess of the mixing signal power as compared to the linear dependence. Finally, the frequencies of the ISB transitions also depend on the applied bias. We calculate an increase of Ȧ43 with bias, while Ȧ54 decreases, both by a few millielectronvolts over the range of applied electric fields deduced from the experiment (approximately 50 to 65 kV/cm). The change in Ȧ43 is more important since the line width Ȗ43 is the smallest of all three transitions. The susceptibility Ȥ(2) at 3.6 μm is tuned to resonance with increasing Ȧ43, while the one at 4.75 μm becomes detuned from resonance. This can explain the different behavior of the secondharmonic signals in Fig. 5.7a and c. From this early work on SFG, important lessons were learned for the continued development of the field. First, the proof of principle had been made, and a general trend of robustness (especially with respect to the width of the resonance) was discerned; i.e., even though the structure was designed for resonant SFG, both SHG signals also were measured, Second, however, it was evident from the smallness of the signal that the nonlinearities had to be improved (which was very feasible—given that the nonlinear electron potential in the SL was very “symmetric” and the nonlinearity in the QC used an abovebandedge state). Third, it appeared that using a nonlinearity within the QC laser was preferable to separate SLs to avoid domain formation in the SLs (which certainly breaks up level alignment) and limited current transport (and laser power). Alternatively, SLs designed specifically for large current transport would have to be used. Finally, the width of the ISBs provided for both SFG and SHG; therefore, just SHG would be simpler to use, allowing more of the waveguide core to be taken up by one type of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_201_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
201
nonlinearity and laser, thus strengthening the nonlinearity and increasing the laser power, and simplifying waveguide design as fewer wavelengths needed to be properly supported. As a result, subsequent work focused on optimization of the SHG signal, both in quantum design and later in phasematching approaches. 5.4 Second Harmonic Generation in Quantum Cascade Lasers Using Resonant Intersubband Nonlinearities After the first demonstration of nonlinear light emission from QC lasers, the primary focus was to increase the overall nonlinear optical power. Three different strategies are available to accomplish this: an improved quantum design of the nonlinear region, an increase in the pump laser power, and finally phase matching of nonlinear and pump light. All three strategies favor a move from SFG and separate (SL) nonlinear regions to SHG and nonlinearities implemented inside the laser active region. First, SHG provides a smaller number of wavelengths, thus simplifying phase matching (which is discussed in Sec. 5.7); second, not having to implement two pump laser wavelengths into one laser core enables more nonlinearity to be available for SHG; third, the integrated nonlinearity is more stable (as stable as QC lasers) under high current injection, and this added stability also allows for higher laser pump currents and pump power. Even after the decision is made to implement the nonlinear transition into the active laser region, several options remain; the nonlinearity can use a separate set of energy levels from the laser (as shown in Sec. 5.3), or the laser transition can be one part of the nonlinear structure. In implementing the latter, an automatic resonance of the pump light with one “leg” of the nonlinear optical transition cascade is achieved, hence maximizing one portion of the nonlinear susceptibility (e.g., by minimizing one denominator in Eq. 5.8). Furthermore, when one is implementing the nonlinearity in a cascade scheme, the electrons can be accumulated in an excited energy level, rather than the ground level, hence reducing resonant absorption for the nonlinear light. Nevertheless, such close integration of nonlinear and laser active regions may incur respective tradeoffs including bleaching of the laser transitions (however, such saturation has not yet been observed). In this section, a “secondgeneration” SHG in QC lasers, in which the QWs of the active regions simultaneously function as nonlinear oscillators, is presented. These structures were originally described in Ref. 46. In this design the essential parameters for laser performance and SHG, such as resonance conditions, optical dipole matrix Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_202_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 202
Chapter Five
elements, and carrier density, have been optimized. As a result, up to ~1 W of pump power at ~7.5 ȝm was then converted up to ~1 ȝW of SHG at ~3.75ȝm wavelength, which is a twoordersofmagnitude improvement in the nonlinear power over that presented in Sec. 5.3. The lineartononlinear power conversion efficiency was improved in devices operating at 9.1 (pump) and 4.55ȝm (SHG) wavelength also by another factor ~100. Most of these improvements are the result of proper design of the electronic level structure; phase matching and improved waveguide design are the topics of Sec. 5.7. At a minimum, highperformance QC lasers contain at least four energy levels, termed g, 3, 2, and 1, in their active regions, and can be envisioned as fourlevel laser schemes, with the laser transition set between levels 3 and 2. Examples of QC laser band structures are given in Fig. 5.8. For highest performance, the energy levels and wave functions, and the laser pumping mechanism (current), are designed such that under operation only levels 3 and g (closely coupled to 3) are occupied with electrons, and the optical dipole matrix element between levels 3 and 2 is as large as possible (usually 1 to 2 nm). These two conditions are also highly favorable for nonlinear ISB transitions, namely, a population concentrated in a single energy level (or a strongly coupled, closelevel ensemble), and large optical dipole matrix elements. In particular, as we discussed in Sec. 5.2.2, an ISB structure capable of efficient SHG contains a triplet of energy levels (i, ii, iii), in near resonance with the pump radiation at frequency Ȧ and SHG at 2Ȧ, and the product of the three optical dipole matrix elements ziii, ziiii, and ziiiii between all three levels is large. We adopt a simplified version of Eq. 5.8, the absolute value of the secondorder nonlinear susceptibility Ȥ(2), as the figure of merit of our design; the latter is given as [12] Ȥ(2) ∝ e 3 Ne
zi
(ലȦ
í Ei
í ii
í ii
í i 썉Ȗ i
z ii
í ii
í iii
zi
) 썉 (2ലȦ
í iii
í Ei
í iii
í i 썉Ȗ i
í iii
) (5.13)
where Ne is the electron density in the active region, assumed to be concentrated in energy level 3, and Ejk and 2Ȗjk are the energy difference and transition broadenings between levels j and k (j, k = i, ii, iii), respectively. Starting from the requirement that the upper QC laser level (levels 3 and g) be the only one significantly populated with electrons under laser operation, and hence must coincide with one energy level of the ISB nonlinearity, one can build the nonlinear cascade. Two separate workable design approaches are shown in the following.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_203_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
5
203
I 5 I
4 3
g
4 3 g
Energy
2 1
2
Active region
X (a)
1
Active region
(b)
Figure 5.8 Portions of the conduction band diagram, one active region sandwiched between two injector regions, and the moduli squared of the essential wave functions of designs (a) D2886 and (b) D2912. The significant energy levels are labeled 1 to 5 inside the active region and g for the ground state of the injector. The dashed lines indicate the extent of the minibands inside the injector regions. The laser transition (3 ĺ 2) is marked by a wavy arrow. The thicknesses in nanometers of the QWs and barriers of one period of active region and injector of D2886 are, from left to right (i.e., electron downstream) and starting with the injection barrier I, 4.3/1.4/1.3/6.8/1.1/5.1/2.6/3.6/2.2/3.4/2.1/3.3/ 2.1/3.3/2.5/3.2, the barriers are indicated by bold font, and the underlined layers are doped to 4.5 × 1017 cmí3. The analogous layer sequence of D2912 is 4.1/8.3/1.3/ 5.2/2.6/4.1/2.1/3.9/2.3/3.7/2.5/3.5/2.6/3.3; the doping density was 3.0 × 1017 cmí3. (Source: Ref. 46.)
5.4.1 SHG in QC lasers with threeQW active regions
In Fig. 5.8a the conduction band structure of one active region with its preceding and subsequent injector regions is shown. This QC laser active region, labeled D2886 [46], contains three coupled QWs—a thin first QW, followed by two wider ones. The latter are the essential QWs sustaining the laser transition, between levels 3 and 2. The center QW is furthermore the main origin for energy level 5, and the thin first QW mainly supports level 4. The pump radiation at the fundamental frequency is generated between levels 3 and 2. Nonlinear cascades can be found for the level triplets 2–3–4 and 3–4–5. As the energy positions of levels 3 and 5 are mainly governed by the center QW, and that of level 4 by the thin first QW, variations in the relative thicknesses of the two QWs quickly allow optimization of the resonance condition; in particular, the thin well enables adjust one to level 4 practically independently of levels 3 and 5. Furthermore, the spatial asymmetry of the QWs—from localizing them in separate but adjacent wells—ensures sizable optical dipole matrix elements [5]. The specific design parameters for the SHG structure D2886 shown in Fig. 5.8a are given in Table 5.1. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_204_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 204
Chapter Five
TABLE 5.1
Design and Device Parameters of Samples D2886 and D2912 D2886
D2912
E23 (meV) E34 (meV) E45 (meV) Ȝ1 (ȝm) z23 (Å) z24 (Å) z34 (Å) z45 (Å)
167 176 143 7.4 18 0.4 3.5 20
131 123 105 9.5 17 6 23 19
z35 (Å) Ȗ23 (meV) Ȗ24 (meV) Ȗ34 (meV)
2 12 25 15
8 10 20 15
Ȗ45 (meV) Ȗ35 (meV) Ĳ32 (ps) Ĳ3 (ps) Ĳ2 (ps) Lp (nm) Ne (cmí3)
D2886
D2912
15 25 2.6 1.2 0.3 48.2 2.0 × 1017
15 20 3.6 1.8 0.3 49.5 1.5 × 1017
Waveguide Parameters μeff,0 3.29 3.28 μ eff,2Ȧ 3.35 3.35 Į0 (cmí1) 10.5 15 Į2Ȧ (cmí1) 2 3
Thirtyone periods of active regions (containing the laser active region and the nonlinearity) and injectors were grown at the core of a lowloss QC laser waveguide with ternary top cladding, which implies an about twofold increase in each active element (laser active regions and nonlinear regions) compared to the original firstgeneration designs shown in Sec. 5.3 [46, 47]. 5.4.2 SHG in QC lasers with twoQW active regions
A closer examination of the structure of Fig. 5.8a, however, reveals some shortcomings. First, the very choice of a threeQW design also results in another energy level situated between levels 3 and 4. While out of resonance with any radiation inside the cavity, and thus not severely impeding the process, it still leads to smaller than possible dipole matrix elements for the other transitions. Such argument follows from a sum rule of the oscillator strength for intersubband transitions [57]. Therefore, we adopted a new design, labeled D2912 [46], of the QC laser active region with nonlinear cascade with only two QWs. The conduction band structure and moduli squared of the essential wave functions of one active region as well as of its preceding and following injector regions are shown in Fig. 5.8b. A detailed picture of the active region of this design is also shown in Fig. 5.2. The structure has been calculated for an applied electric field of 38 kV/cm; QC laser action again takes place between levels 3 and 2. As the first “leg” of the nonlinear cascade 2–3–4 coincides with the laser transition, i.e., the fundamental pump light, their remaining in resonance is trivial. Resonance of the second “leg” can be achieved by relative thickness variations of the two QWs and the barrier between them. It is worth noting that, in this
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_205_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
205
design of the nonlinear cascade, resonant absorption of the SHG radiation is negligible, as the freeelectron population is in level 3 rather than in level 2. The full set of device parameters for this type of design (D2912) is also given in Table 5.1. Wafer D2912 was grown with a conventional QC laser waveguide [46, 49]. Fifty periods of active regions and injectors are sandwiched between two layers of InGaAs layers. The bottom cladding is provided by the InP substrate, and the top cladding is made from an inner 2.1ȝmthick AlInAs layer doped to nSi ~ 1 × 1017 cmí3 and an outer AlInAs layer, 400 nm thick and doped to nSi ~ 2 × 1017 cmí3, which are also capped by a 350nmthick, highly doped (nSi ~ 5 × 1016 cmí3) layer of InGaAs. The calculated modal refractive indices and waveguide attenuation coefficients of all waveguides at both the fundamental (μeff,0 and Į0, respectively) and SHG (μeff,2Ȧ and Į2Ȧ, respectively) wavelengths are summarized in Table 5.1. The estimations for Ȥ(2) may be uncertain within a factor of 2 or 3, mainly because of differences between the designed and actual transition frequencies and the doping levels. We obtain Ȥ(2) = 340 and 2 × 104 pm/V, for structures D2886 and D2912, respectively. The nonlinear coefficient for D2912 is rather large, about two orders of magnitude higher than that in bulk IIIV semiconductors. In both cases D2886 and D2912, the contributions from 2–3–4 and 3–4–5 cascades turn out to be of comparable order of magnitude, but with leading contribution from the 2–3–4 cascade. In estimations of the lineartononlinear power conversion efficiency Ș, the largest uncertainty comes from Ȥ(2)2, and there are additional sources of uncertainty: the phase mismatch ǻk and overlap factor Ȉ. Variations of these parameters also cause the spread of Ș between different devices of the same structure. Nevertheless, values of Ș = 0.8 ȝW/W2 for D2886 and Ș = 300 ȝW/W2 for D2912 are calculated. These values are in reasonable agreement with the experimental values. Shu et al. [58] recently reported improved designs of nonlinearities implemented in QC laser active regions only employing the 2–3–4 resonance triplet and maximizing the optical dipole matrix elements. These designs are shown in Fig. 5.9. Design D3043 localizes and isolates the lower level of the laser transition, separating it from the injector to which it was coupled in previous designs. Decoupling the lower energy level from the injector states increases the values of the dipole matrix elements for transitions from and to this level. The coupling of the upper laser level with the injector ground level is taken into account by summing the oscillator strengths. The calculated dipole matrix elements are z12 = 22.4 Å, z23 = 22.6 Å, and z31 = 6.88 Å; and the optical nonlinear susceptibility is calculated to be Ȥ(2) = 8.8 × 104 pm/V, a factorof4 improvement in Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_206_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Chapter Five
D3056
3 2
520 meV
D3043
3 2
520 meV
206
1 1
Active region
Active region
Figure 5.9 Schematics of the conduction band diagrams of two novel QC laser designs
(D3043 and D3056) with integrated resonant optical nonlinearities [58]. The active region layer thicknesses in nanometers for D3043 and D3056 are 5.3/1.2/8.2 and 6.7/1.0/5.5, respectively, starting from the left wells. The respective laser transitions are indicated by the wavy arrows; the nonlinear transitions are indicated by dotted arrows. (Source: Ref. 58.)
optical nonlinearity over D2912, at the about same designed fundamental and SHG wavelengths of 9.2 and 4.6 m, respectively. In design D3056, optimization of the nonlinear susceptibility is achieved by isolating the uppermost level 3 of the optical nonlinearity. To accomplish this, the energy level was placed in the electronic “upstream” quantum well of the twoQW active region, away from the upper miniband where it had been located in previous designs. As a result, the upper laser level must be placed in the electronic “downstream” quantum well, a novel configuration for QC laser levels since such a design incurs a tunneling time penalty for electrons in the upper laser level and the injector ground level. The calculated dipole matrix elements are z12 = 24.1 Å, z23 = 29.3 Å, and z31 = 8.0 Å; and the optical nonlinear susceptibility is calculated to be Ȥ(2) = 1.3 × 105 pm/V, an almost oneorderofmagnitude improvement in nonlinear optical susceptibility over D2912. The designed fundamental and SHG wavelengths are 8.9 and 4.5 m, respectively. Work on both structures, especially in light of improving their laser performance, is ongoing; both are examples in which the nonlinear design was the primary goal, and laser design came second, while earlier designs had been using successful laser designs as starting points and modified them to become nonlinear crystals. Again the lasers were processed and characterized in conventional manner, as previously outlined. The cryostat was fitted with a doubly antireflection (AR) coated ZnSe window, yet control measurements have also been made using a quartz window; lenses with large numerical aperture, made from ARcoated ZnSe, Ge, or uncoated CaF, were used to collimate and refocus the highly divergent light Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_207_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
207
0.1
0.2
0
100
2
0.2
[PL (W)]
50 0 0
1
2 3 Current (A) (a)
4
0 5
49 W/W
2
( W)
0.3
600 NL
0.6
2
400
P
65 W/W
2
68 W/W
.05
0
0 0.005 0.01 2
[PL (W)]
200
0 0
1
2 3 Current (A)
4
0 5
Nonlinear power PNL (nW)
0
150
0.1 Linear power PL (W)
2
0.46 W/W
200
NL
0.1
0.4
( W)
250 0.2
2
0.86 W/W
P
Linear power PL (W)
0.6
Nonlinear power PNL (nW)
emission from the cleaved facets. Quartz, silica glass, sapphire, and an undoped InP flat were used as optical filters to discriminate between fundamental pump and SHG light. When the laser light was measured at the fundamental frequency, attenuation screens were used to avoid saturation of the detector and detection electronics, which in itself would result in erroneous nonlinear signals. After measuring the linear and nonlinear light output versus current (LI) characteristics, we deduce the external lineartononlinear power conversion efficiency by graphing the nonlinear power versus the square value of the linear power. A linear fit to this curve (where suggested) results in the external power conversion efficiency. Figure 5.10a shows the linear and nonlinear LI characteristics of a representative device of D2886; approximately 0.5 W of fundamental peak power results in about 200 nW of SHG light. The inset reports the external lineartononlinear power conversion efficiency, which is close to ~1 W/W2. The kink at about 2.4 A in the linear LI curve is a frequent occurrence with QC lasers. It is mostly attributed to the onset of higherorder transverse modes; i.e., the laser ridges are wide enough to support two, sometimes even three transverse modes in lateral direction. The kink is also reproduced in the nonlinear LI curve and the external conversion efficiency curve. As different transverse modes have different modal effective indices and attenuation coefficients, it is not surprising that the external efficiency can change noticeably at such a kink. Figure 5.10b shows the linear and nonlinear LI curves for a characteristic device of D2912. Here, about only 100 mW of fundamental peak output power is transformed to nearly 550 nW of
(b)
Figure 5.10 Linear (dashed) and nonlinear (solid) light output versus current
characteristics of two representative devices (a) D2886 and (b) D2912. The insets show the respective external lineartononlinear conversion efficiency. The numerical values inside the inset graphs have been extracted from leastsquares fits to nearlinear portions of these graphs. All data were taken in pulsed current mode at ~10 K heat sink temperature. The device of (a) was 12 m wide and 3.04 mm long; the dimensions of the device of (b) were 13 m and 2.25 mm, respectively. (Source: Ref. 46.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_208_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 208
Chapter Five
SHG light. The external power conversion efficiency is accordingly much higher than that of the device of Fig. 5.3a, from a factor of 50 to 100 higher. Lasers of D2886 showed values up to ~1 W/W2. Devices of D2912 achieved greatly increased external conversion efficiencies up to 100 W/W2. A strong spread in the values of the external conversion efficiency, which can span almost a decade, can be detected. The overall highest nonlinear power (of a nonlinear QC laser without a phasematching waveguide) was measured from a laser of D2886, as shown in Fig. 5.11, which reports the linear and nonlinear light output and voltage versus current (LIV ) characteristics of the one device of D2886. We obtained 2 W of SHG light at 1 W of fundamental peak output power. Figure 5.12a to c reports spectral data obtained from our lasers. Figure 5.12a displays large spectral range power versus wavelength data obtained with the InSb (top) and HgCdTe (bottom) detectors. These spectra demonstrate the absence of spurious signals in the power measurements of the two detectors, each targeted for its own specific (the fundamental or SHG) wavelength range. Figure 5.12b and c shows highresolution spectra of representative devices D2886 and D2912, respectively. Spectra in the region of the fundamental as well as the SHG emission are shown. The expected direct correspondence between the respective spectra is observed in the data. It is necessary to note that what we term SHG here is actually a whole set of SHGs and SFGs as each of the individual FabryPerot modes of the freerunning laser mixes with itself (SHG) and with all the other FabryPerot modes (SFG). This is so because the spectral width of the laser emission is narrower than the laser gainband width, which is the same as or narrower (for SHG) than the nonlinear transition. Many of these SHG 1.0
4
2.0
0.8
1.5
0.6 1.0
2
~ 1.4 W/W
0.4
0.5
0.2
2
~ 2.8 W/W
2
0 0
Nonlinear power (μW)
6
Linear power (W)
Voltage (V)
8
0 1
2
3
4
5
6
7
Current (A) Figure 5.11 Linear (dashed) and nonlinear (solid) light output and voltage (solid line with
separate y axis) versus current characteristics of a 10mwide, 3.04mmlong laser device of D2886. The laser was operated with 60nslong current pulses at 4.16kHz repetition rate and at 10K heat sink temperature. The external power conversion efficiencies are given in two regions. (Source: Ref. 46.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_209_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
100
1
1000
0.01
100 10
209
Power (arb. units)
Power (arb. units)
Optical Nonlinearities
1 4
6 8 Wavelength (μm)
10
(a)
Power (arb. units, offset)
7.4
7.5
7.6
9.1
9.2
(c)
(b)
3.7
9.0
3.75
3.8
4.5 4.55 4.6
Wavelength (μm) Emission spectra of QC lasers with integrated secondorder nonlinear cascades. (a) Widerange spectra of a characteristic laser of D2912. The spectrum on top has been taken in stepscan mode with an InSb detector fitted with a sapphire window and an additional quartz/silica glass filter. The bottom spectrum is taken with a HgCdTe detector; the laser radiation has been reduced with a metal screen to avoid saturation of the detector and detector electronics; no spurious electronic or optical signals are measured. (b) and (c) Highresolution spectra of representative laser devices of D2886 and D2912, respectively. The SHG (bottom) and fundamental (top) light emission is shown for both devices. (Source: Ref. 46.) Figure 5.12
and SFG combinations are degenerate due to the low dispersion and hence the observed equidistant frequency comb results. Nevertheless, close inspection of the spectra allows one to count and attribute individual modes. So far, in this section, we have demonstrated several strategies for improved quantum design of optical nonlinearities; a severalordersofmagnitude improvement and continuing improvement have been shown. These values have been obtained without any phase matching, causing large spread in data quality and limited overall output power.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_210_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 210
Chapter Five
5.4.3 Temperature performance of nonlinear quantum cascade lasers
The early implementations of nonlinear QC lasers, as discussed in Secs. 5.4.1 and 5.4.2, and potential future implementations of more elaborate effects in parametric nonlinear lasers and light sources are limited to low temperatures, generally to keep a cold electron population. Nevertheless, for applications, such as trace gas sensing, two major questions arise: (1) How is performance at high temperatures? (2) What is the singlemode performance of the system? To answer these questions, the previously discussed SHG QC lasers were presented in Ref. 59. In particular, design D2886 was used for the study of the temperature behavior, and again conventional laser processing and characterization (as briefly outlined above) were employed. In particular, the lasers were operated in pulsed mode at a very low duty cycle (< 1%) and pulse duration (50 to 100 ns), such that the measured heat sink temperature can be assumed to be practically identical to the laser core temperature. Figure 5.13 shows the linear and nonlinear light output and voltage versus current characteristics of a 10mwide and 3mmlong device of D2886 at various heat sink temperatures. Figure 5.13a shows the linear optical power at ~7.5m wavelength measured with nearly unity collection efficiency; Fig. 5.13b shows the nonlinear SHG light output at ~3.75m wavelength measured with a cooled InSb photovoltaic detector and collected with 60% collection efficiency from the same facet. From the linear and quadratic portions of the LI curves in the top and bottom panels, respectively, an external lineartononlinear power conversion efficiency can be deduced. The latter is shown as a function of the heat sink temperature in the inset of Fig. 5.13b. Figure 5.14 reports spectra taken of the same device of Fig. 5.2 at cryogenic temperature as well as at a 250 K heat sink temperature. As the heat sink temperature is raised, the nonlinear power drops quickly, a combined effect of the reduced power level of the fundamental pump laser and the reduced lineartononlinear conversion efficiency. Nevertheless, at 250 K, a clear SHG signal can be measured, as shown in Fig. 5.14b top, with a peak power level of ~50 nW. Only at 300 K had the signal disappeared into a rising shortwavelength background. The reduction of the fundamental optical power with increased heat sink and active region temperature is a wellknown effect with QC lasers (as with most semiconductor lasers). Nevertheless, QC lasers can be obtained with high optical power even at room temperature [48]. Therefore, efficient SHG should be possible with QC lasers having (linear) peak output power levels in the watt range at room
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_211_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
8
6 K 1.0 50 K 100 K
6K 300 K
0.75 150 K
4 200 K
2
250 K 0.25 300 K
2
Efficiency (μW/W )
(a)
0
0 2.0
6 K 1.2 50 K 100 K
1.0 0
0.5
0.8 0
100
200
300
150 K
Temperature (K)
(b) 0
0.4
200 K 250 K
1
2 3 Current (A)
4
Nonlinear power (μW)
Voltage (V)
6
211
Linear power (W)
Optical Nonlinearities
0
5
Figure 5.13 Linear (top, solid lines) and nonlinear (bottom) light output and voltage (top, dashed lines) versus current (LIV ) characteristics of a 10mwide, 3mmlong QC laser of D2886 at various heat sink temperatures, as indicated. The inset shows the lineartononlinear power conversion efficiency as extracted from the LIV curves versus the heat sink temperature. The solid line of the inset is a linear leastsquares fit to the data, resulting in a slope of –5 nW/(W2·K). (Source: Ref. 59.)
temperature. The deterioration of the external lineartononlinear power conversion efficiency, conversely, can be understood from a discussion of the secondorder nonlinear susceptibility Ȥ(22Ȧ) , to which it Wavelength (μW)
Power (arb. units, offset)
3.25
3.5
3.75
4.0
(a)
3.75
4.0
4.25
250 K 4.5 A
(b)
10 K 4.8 A 6.5
7.0
7.5
8.0
7.5
8.0
8.5
Wavelength (μW) Figure 5.14 Linear (bottom) and nonlinear (top) emission spectra of QC lasers with
integrated secondorder nonlinear cascades obtained at (a) 10 K and (b) 250 K and at high peak current levels, as indicated. (Source: Ref. 59.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_212_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 212
Chapter Five
is closely related through W2(2Ȧ) 싀  Ȥ(22Ȧ)  2 W1(Ȧ)2, where W1(Ȧ) and W2(2Ȧ) are the linear and nonlinear (SHG) power at frequencies Ȧ and 2Ȧ, respectively. The secondorder nonlinear susceptibility (Eqs. 5.8 and 5.13) contains several temperaturedependent quantities. First, the transition line widths of QC lasers are known to increase significantly, by ~ 50%, between 10 and 300 K [7]. We estimate values Ȗij for the line broadening (full width at half maximum) of the transitions between levels i and j of Ȗ23 = 12 meV and Ȗ24 = 20 meV for 10 K heat sink temperature and Ȗ23 = 18 meV and Ȗ24 = 30 meV for 300 K. The larger contribution to the drop of  Ȥ(22Ȧ)  with increasing temperature thereby results from the increase in Ȗ24, as the increase in Ȗ23 is partly (except for excited state absorption 3 ĺ 4) compensated by the increase in the population difference (population inversion) between the upper and lower laser levels, as a result of the increased laser threshold following the broadening of the laser gain bandwidth. Another source of reduced  Ȥ(22Ȧ)  can be found in the thermal shift of the various energy levels that may lead to a change in the resonance conditions. 5.4.4 Singlemode emission and tunability in nonlinear quantum cascade lasers
In Sec. 5.4.3 we referred to SHG of FabryPerot type spectra, which (as we pointed out) is somewhat of a misnomer, as a good fraction of the nonlinear signal is in fact SFG of many FarbyPerot modes mixing with one another. For precise determination of the nonlinearity, as well as for applications that require singlemode spectra, such singlemode performance needs to be assessed in the nonlinear domain. It has long been known how midir QC lasers can be made into singlemode and tunable lasers; one straightforward method is to fabricate the QC lasers as distributed feedback (DFB) lasers. In this section we discuss the singlemode emission and tuning of the SHG signal of a QC DFB laser. Quantum cascade DFB devices with firstorder topsurface Bragg gratings (with grating periodicity ȁB) were fabricated from wafer D2882, a design very similar to D2886, but with slightly shorter wavelength [46]. Figure 5.15 shows the singlemode emission wavelength at both the fundamental pump and SHG wavelengths as a function of the heat sink temperature for a device with ȁB = 1.1 μm. The inset shows a highresolution shortwavelength spectrum taken at cryogenic temperature. As we obtain singlemode emission for the QC lasers, the SHG signal is also singlemode. The fundamental emission wavelength ȜȦ of the QC DFB laser is given by ȜȦ = 2neff(T)·ȁB, with neff(T) being the temperaturedependent effective refractive index of the waveguide. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_213_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
213
Temperature (K) 0
50
100
150
200
250
300
1 P (arb. units)
3.51
0.1 0.01
6.98
3.49
3.44 3.48 3.52 Wavelength ( m)
6.94
3.47
6.90
Wavelength (μm)
Wavelength (μm)
7.02
3.45 0
50
100
150
200
250
Temperature (K) Figure 5.15 Singlemode emission wavelength versus temperature for a QC DFB laser
with active regions that also include nonlinear optical cascades. The solid circles indicate the emission wavelength in the fundamental wavelength range, the open triangles in the SHG wavelength range. The solid lines are fitted to the data using slopes of 0.4 and 0.2 nm/K for the fundamental and SHG wavelength range, respectively. The inset shows a highresolution spectrum of the singlemode SHG signal obtained in stepscan mode at cryogenic temperatures. (Source: Ref. 59.)
The singlemode wavelength Ȝ2Ȧ of the SHG signal is given by Ȝ2Ȧ = ȜȦ/2 = neff(T)·ȁB. Therefore, we expect a SHG tuning rate of onehalf the value of that of the fundamental mode. In fact, as shown in Fig. 5.15, we measure tuning rates of ~0.4 and ~0.2 nm/K for the fundamental pump and SHG light, respectively. The latter is very comparable to the tuning rate expected for a QC DFB laser with fundamental light emission at such short wavelength [6], which is not surprising where we take into account that the temperature coefficients of the refractive indices of the various materials are very little wavelengthdependent at energies far away from the fundamental energy gap. Nevertheless, there are technological and merely practical advantages, such as a larger grating periodicity, to obtaining a singlemode shortwavelength nonlinear emitter by fabricating the pump laser as a singlemode DFB laser. 5.5 Third Harmonic Generation in Quantum Cascade Lasers Using Resonant Intersubband Nonlinearities In earlier sections we have motivated our choice of nonlinearity that we implemented first with QC lasers; SHG and SFG were the nonlinearities of choice. The next nonlinear effect to explore was THG. Originally, THG was a byproduct of the earlier designs for SHG, which included
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_214_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 214
Chapter Five
two interleaved SHG level triplets, providing an automatic THG level cascade [46]. Aside from the auspicious presence of the THG nonlinearity, it was an intellectual challenge to test if it could be made strong enough to be of value as a means to extend the shortwavelength limit of nonlinear QC lasers. The results of this work indicated that technologically it will be unlikely that THG will result in useful power levels; nevertheless, the intellectual challenge of design and evaluation is of interest. The first observation of THG was a byproduct of the improved SHG designs of active regions D2912 which contained two strong and interleaved nonlinear cascades for SHG that added up to a nonlinear cascade 2–3–4–5, as shown in the inset of Fig. 5.16. At resonance, the ratio of the thirdorder to secondorder nonlinear susceptibility Ȥ(3)/Ȥ(2) ez25/(ƫȖ52) and the ratio of powers W3/W2 is of the order of ez25 Ex(Ȧ)/(ƫȖ52)2 . This ratio can be on the order of 0.01 if the pump field intensity is about 1 MW/cm2 and the dipole moment z25 is on order of 10 Å. In fact, the design of D2912 has nonnegligible, though in no way optimized, Ȥ(3). Figure 5.16 thus reports the highenergy emission spectrum of a representative device of D2912; a small signal at 3Ȧ (at Ȝ3Ȧ = 3.05 μm wavelength) is observed [46]. Nevertheless, after accidental observation of the THG signal in D2912, an attempt was made to improve on the THG signal with targeted design, and the results were reported in Mosely et al. [60]. Again, the design strategy was to use the active region of the laser simultaneously as the nonlinear region, and to have one leg of the nonlinearity (the lowest transition) coincide with the laser transition.
1000 Energy
Powe (arb. units)
5
100
4 3
X
10
2 1
THG
1 0.1
SHG
0.01 250
300
350
400
450
500
Energy (meV) Figure 5.16 Emission spectrum of a representative device of D2912 in the very short
wavelength range. A small THG signal is measured. The energy of the fundamental light is 136 meV (9.1m wavelength); SHG and THG are at 271 meV (4.55 m) and 407 meV (3.05 m), respectively. (Source: Ref. 46.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_215_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
215
The design was made for pump light at ~11.1 m wavelength and SHG and THG emission at 5.4 and 3.7 m, respectively, where now the SHG signal is a byproduct of a structure optimized for THG. Fiftytwo periods of QC laser active regions interleaved with injector regions have been grown with a ternary waveguide that is lowloss at the pump wavelength. The large wavelength step from the fundamental to the THG wavelength implies that the waveguide at the THG wavelength is minimally lossy (but also rather poorly confined; i.e., it is an oversized waveguide, in which a large number of transverse modes are allowed). Figure 5.17 shows the conduction band diagram for one active region sandwiched between two injector regions under an applied bias of 42 kV/cm. This field is considerably higher than the turnon electric field calculated and measured as 30 kV/cm and is more appropriate to describe the structure under high pumping conditions, where we also measure the highest optical power. The structure is designed such that energy levels 1, 2, and 3 facilitate the laser transition at the fundamental frequency, and the nonlinear processes are supported by energy levels 2, 3, 4, and 5. The energy level separations ǻE23, ǻE34, and ǻE45 are 98, 104, and 90 meV, respectively. Since our target nonlinear light generation occurs as a result of the 2–3–4–5 cascade, we are most interested in the corresponding optical dipole matrix elements. They are calculated to be z23 = 14.6 Å, z34 = 21.5 Å, z45 = 33.2 Å, and z25 = 7.0 Å, yielding a significantly greater dipole matrix element product than that of previous asymmetric coupled QW designs intended for intersubband SHG or THG in the AlInAs/GaInAs material system [12, 46], which to some extent is attributed to the smaller laser and resonance energies ǻEij. The lasers were processed and measured in conventional fashion. Figure 5.18 shows the emission spectra from the integrated device taken at cryogenic temperatures. Figure 5.18a shows a FabryPerot spectrum characteristic for the radiation at the pump wavelength; Fig. 5.18b shows the THG signal at Ȝ ~ 3.7 μm from the same device that displays a fundamental emission at Ȝ ~ 11.1 m. The spectral response of the InSb detector fitted with a shortpass filter is given as a dashed line. The small broad background emission can be attributed to background luminescence from electrons excited to high energy levels; the SHG signal is present at 5.4m wavelength. Using Eq. 5.9, the calculated dipole moments, and electron density Ne ~ 5 × 1015 cmí3, assuming that all the population is in level 3, neglecting all detunings, and assuming all gammas (Ȗmn) equal to 10 meV, except Ȗ52 ~ 20 meV, we arrive at Ȥ(3) ~ 7 × 10–8 esu, which is quite a large value. The ratio of thirdorder to secondorder susceptibilities for the same structure scales as
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_216_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 216
Chapter Five
5 4 3 2 1 Injector Active region Injector Conduction band energy diagram for one active region between two injector regions. The significant energy levels inside the active region are labeled 1 to 5. The thicknesses in nanometers of the InGaAs QWs and AlInAs barriers of one period of injector and active region are, from right to left, 3.7/2.1/3.0/2.1/3.5/2.1/3.4/3.6/3.1/1.2/ 6.4/1.3/4.7/2.6, the barriers are indicated in bold font, and the underlined layers are doped to nSi = 2.5 × 1016 cmí3. The light gray bars indicate the levels involved in THG; the dark gray bars and arrow indicate the laser transition. (Source: Ref. 60.) Figure 5.17
Ȥ (3 ) Ȥ (2 )
 
~
ez52 í3 ~ 10 ലȖ52
(5.14)
40 30 20 10 0 10
10.5 11.5 11 Wavelength (μm) (a)
12
12
(b)
10
SHG
120 100
8
80
6
60
4
40
THG
20
2 0
3
4 5 Wavelength (μm) (b)
6
signal (arb. units)
signal (arb. units)
50
Detector response (arb. units)
This gives the ratio of signal powers at second and third harmonics on the order of 0.01, which compares well with the experimental value of ~1.5 × 10í2. Nevertheless, as outlined in Mosely et al. [60], by using this reasonably optimized THG process, even a fundamental power of 100 mW will only result in 30 to 50 nW of nonlinear THG power, a power level that was consistent with the measured detector signal.
0
Emission spectra of a QC laser with integrated thirdorder nonlinear transition in the active region. (a) The spectrum of the fundamental light emission at a wavelength of 11.1 m; (b) the SHG and THG light emission from the same device, at wavelengths of 5.4 and 3.7 m, respectively. (Source: Ref. 60.) Figure 5.18
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_217_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
217
5.6 Nonlinear Light Generation in Quantum Cascade Lasers Using Lattice Nonlinearities So far, we have considered only resonant optical nonlinearities based on ISB transitions. These are advantageous, as they are much larger than the average bulk nonlinearities and thus result in high nonlinear optical power output and lineartononlinear conversion efficiency. Nevertheless, they also have two drawbacks. First, the magnitude of the nonlinearity is about proportional to the freecarrier density, but a high carrier density also increases the freecarrier loss in the cavity. Second, the nonlinearities are resonant and must be tuned by design to the correct wavelengths. Given those shortcomings, it is worthwhile to consider nonlinear QC lasers based on the bulk, i.e., lattice, nonlinearities. The GaAs and InPbased IIIV semiconductors have zinkblende lattice structure with two different atoms in the unit cell. The resulting asymmetry leads to a distinct secondorder nonlinear susceptibility tensor, with nonzero components for electric pump fields that are oriented away from the main axes of symmetry. For the usual combination of transverse magnetic polarization, due to strict selection rules, and growth on (100)oriented substrates, the secondorder nonlinearity is vanishingly small in conventional InP or GaAsbased QC lasers, much smaller than the one induced by the ISB transitions. Neverthless, Bengloan et al. [61] succeeded in growing GaAsbased QC lasers on (111) substrate. In this orientation, the TM pump field is at an angle with all the major axes, and a significant nonlinear field is generated. This nonlinear process has the advantage that it is not resonant, i.e., is largely independent of wavelength, and that it is a property of the entire lattice; i.e., the overlap with the guided modes is unity, independent of the waveguide geometry. In their work, Bengloan et al. [61] demonstrated GaAs/Al0.45Ga0.55As QC lasers emitting at ~11.5m wavelength and SHG emission at ~5.8 m. In a nonphasematched waveguide, ~200 mW of pump light was converted to ~20 W of SHG signal. The authors estimate a maximum power conversion efficiency of 1% to 10% for a phasematched structure. Giovannini et al. [62] reported SHG in nonlinear QC lasers based on a (111) lattice nonlinearity in InPbased lasers. 5.7 PhaseMatching Considerations in Nonlinear Quantum Cascade Lasers In previous sections, emphasis was put on the proof of principle of nonlinear light generation in QC lasers, and on the quantum design. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_218_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 218
Chapter Five
Yet, practically no attempt was made to phasematch the fundamental and excited nonlinear guided modes, which would be essential to reap the full benefit of the nonlinear light generation. Phase matching is particularly important, because in the simplest geometry, the fundamental and harmonic modes copropagate within the same waveguide. Nevertheless, even for the nonphasematched case, several microwatts of nonlinear light could be measured. This is partially the result of the low material dispersion for wavelengths far off the material bandgap and a particularly beneficial “side effect” of the QC laser which uses ISB instead of interband optical transitions [63]. Nevertheless, as the quantum design of the nonlinear QC laser improved, it became clear that the power was now limited by the lack of a phasematching strategy. Hence, the next development step was dedicated to implementing phase matching into the nonlinear QC laser waveguide. Before we review the various means of phase matching reported so far in the literature, a quick estimate of the magnitude of a typical phase mismatch in a conventional midir QC laser waveguide is given. For the SHG structures presented above, the mismatch factor ¨k in the structures under study is between 1000 and 1500 cmí1, which is more than 100 times larger than the modal losses Į2. Therefore, we could obtain a three to fourorderofmagnitude increase in nonlinear power efficiency by reducing the mismatch factor to the level of the optical losses. The common techniques for phase matching, such as birefringence phase matching [64] or quasiphase matching, are not practical for QC lasers due to the linear waveguide geometry. Moreover, the various schemes proposed for SHG phase matching based on refractive index matching in asymmetric double quantum well structures [65] cannot be easily applied to QC lasers because of the intrinsic waveguide dispersion, weak voltage tunability, and strict current transport requirements. 5.7.1
Modal phase matching
The technique of phase matching described here takes advantage of the flexibility in the design of the integrated QC laser waveguide and the fact that these are “large” waveguides capable of sustaining several transverse modes. These two properties allow for true matching of the fundamental (pump) and SHG modal refractive indices of different transverse order waveguide modes, i.e., true modal phase matching, while simultaneously preserving a large nonlinear overlap of the interacting modes with the nonlinear active region. While this phasematching technique was first demonstrated using SHG nonlinear QC
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_219_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
219
lasers, as reported by Malis et al. [66], we estimate that it can readily be extended to other nonlinear optical processes. The QC laser structures used in this study [66] employed the fairly optimized active region D2912 (shown in Figs. 5.8 and 5.16 and discussed previously [46]) and a waveguide, as described in Fig. 5.19a. For this structure a maximum nonlinear susceptibility of Ȥ(2) ~ 2 × 104 pm/V is calculated, assuming exact resonance for all interacting fields, while the effective interaction cross section of the fundamental and nonlinear modes with the nonlinear region Â varies between 600 and 1400 m2 as the ridge width varies between 6 and 12 m. The power transfer from the fundamental to the nonlinear signal is maximized by minimizing the phase mismatch ǻk and effective area Â, as outlined in Eqs. 5.11 and 5.12 and the related discussion in Sec. 5.2.2. For QC lasers, the phase mismatch ǻk is determined by the structure of the laser waveguide. Due to material dispersion at the two wavelengths (~9.1 and 4.55 m) used in this study, phase matching is not possible between the zeroorder transverse waveguide modes of the fundamental and SHG signals, or between the fundamental zeroorder transverse magnetic (TM00) mode and the SHG firstorder transverse mode (TM01). However, numerical analysis shows that phase matching is possible between the fundamental (TM00) and the SHG (TM02) modes. 3
cm , 10 nm Ti/Au top contact
n InGaAs, 6.5 x 10 n InAlAs, 10
17
18
3
17
17
2
3
cm , 1600 nm
Active regions and injectors 50 stages 2475 nm n InGaAs, 10
(b)
3
cm , 1300 nm
n InGaAs, 10
0
cm , 850 nm
Thickness (μm)
20
n++ InGaAs, 10
4
6
3
cm , 1500 nm 8
n InP, 15 x 10
17
3
cm , substrate 10
(a)
0 2 4 SH refractive index and mode profiles
Figure 5.19 Waveguide structure of sample D2957, a SHG nonlinear QC laser with modal phasematching waveguide. (a) The layer structure, materials, doping levels, and thicknesses; (b) refractive index profile at the SHG wavelength, and the intensity of the magnetic field profiles (arbitrary units) for the TM00 fundamental mode (solid line) and TM02 SH mode (dashed line) for this waveguide. (Source: Ref. 66.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_220_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 220
Chapter Five
When modes of different mode orders are matched, one consideration is to maximize the overlap integral of these modes with the nonlinear mixing region. Modes of different transverse order and the same frequency are exactly orthogonal. Since the frequencies differ by a factor of 2 in the SHG case, this orthogonality is partially lifted; but still the overlap integral between these modes over the transverse cross section of the waveguide can be quite small. Hence, the nonlinear region (which doubles as the laser active material) must be placed in such a position in the waveguide so that the overlap is maximized (Fig. 5.19b). The refractive indices of undoped InGaAs and InAlAs were derived by linear interpolation between the published values of the end alloys at 9.1 and 4.55 m. The complex refractive indices of the variously doped layers were then calculated, using the Drude formalism. The refractive index profile has the shape plotted in Fig. 5.19b. This profile is similar to that of the socalled M waveguides that have been proposed and demonstrated for SHG phase matching in LiNbO3 and AlGaAs in the nearir [67]. The waveguide layer thicknesses were first optimized by minimizing the phase mismatch corresponding to an infinitely wide waveguide. The difficulty of designing a phasematched waveguide lies in the uncertainty of the refractive indices for the various materials and in the inevitable differences between a designed structure and the real wafer and processed device. To keep the phase mismatch ǻk below 100 cmí1, e.g., one would need to know and control the refractive indices of the waveguide layers with an absolute accuracy better than 0.1%, which is not feasible. Therefore, we need a degree of freedom that allows one to tune the finished structure through the phasematching point. Such a degree of freedom is provided by the dependence of the effective refractive indices of the various modes on the laser ridge width. The effective refractive index of the fundamental mode decreases faster with decreasing ridge width than the SHG refractive index (inset of Fig. 5.20b). This behavior can be understood from the slightly larger overlap of the fundamental mode with the SiN insulator and metal contact layers outside the semiconductor ridge, and the different refractive indices at the two wavelengths. The crossover point, corresponding to exact phase matching, was designed to lie within the available experimental ridge width range of 4 to 16 m. The waveguide structure detailed in Fig. 5.19b (sample D2957 [66]) provides an optimal calculated phase mismatch of 367 cmí1 for an infinitely wide waveguide, a value that is theoretically reduced to zero for an 8.8mwide ridge laser. Figure 5.20a shows the LI curves at the fundamental and SHG wavelengths for an 8mwide, 1.5mmlong laser. The laser displays a nonlinear power of 240 W and a nonlinear Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_221_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
200
300
221
300
250
250
100
200
η=
50 0 0.00
150
0.02
2
2.4 mW/W
0.04
0.06
0.08
200 150
0.10
PL2(W2) 100
100
50
50
0
Nonlinear power PNL (μW)
PNL (μW)
Linear power PL (mW)
150
0 0
1
3
2 Current (A)
(a)
refractive index
Linear to nonlinear power conversion effciency η (μW/W 2)
2500
2000
1500
fundamental
3.20
secondharmonic
3.16 3.12
phasematching
3.08 3.04
4
8
12
16
20
Width (μm)
1000
500
0 4
6
8
10
12
14
16
18
20
Width (μm)
(b) Figure 5.20 (a) Fundamental (solid) and SHG (dashed line) light output power versus
current characteristics for an 8mwide, 1.5mmlong laser of wafer D2957 (see Fig. 5.19). The inset shows the SHG power as a function of the linear power squared and a fit of the curve with a straight line in the central region to obtain the external conversion efficiency. (b) Ridge width dependence of the nonlinear power conversion efficiency for wafer D2957. The solid line through the data points (triangles) represents a fit with a lorentzianlike function. The inset shows the theoretical dependence of the fundamental and SHG effective refractive indices on the ridge width. (Source: Ref. 66.)
efficiency of approximately 2.4 mW/W2. Both values are significantly (by at least two to three orders of magnitude) higher than what was Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_222_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 222
Chapter Five
possible without phase matching. The highest nonlinear conversion efficiency of 36 mW/W2 was achieved for a similar waveguide design, D2944, for a ridge width of 4 m at the lowest end of what was feasible to process. The maximum theoretical nonlinear efficiency is 2 W/W2, assuming ǻk = Į2 = 10 cmí1 and undepleted pumping. With this efficiency, pump depletion is reached when the fundamental laser power goes beyond ~200 mW. The discrepancy between the theoretical prediction and the experimental results can be explained by a 0.5 to 1m ridge width nonuniformity intrinsic to the wetchemical mesa etching process; a deviation by 0.5 m from the optimal ridge width would lead to the mismatch increase to ǻk ~ 50 cmí1. Another possible factor contributing to lower efficiency is the excitation of higherorder lateral laser modes that have much lower conversion efficiency. The ridge width dependence of the nonlinear power efficiency was studied in detail for sample D2957, and the results are shown in Fig. 5.20b. The ridge width was measured at the height of the active region with a precision of ±0.5 m. As expected from the theoretical calculations, the nonlinear conversion efficiency displays a maximum around 8 to 9 m. The line through the data points shown in Fig. 5.20b represents a fit of the data with a lorentzianlike function of the form 1/(ǻk2 + Į22), where ǻk2 is the calculated phase mismatch. The width of the experimental curve (closely related to the optical loss Į2) is considerably larger than expected from theory, most likely due to a larger experimental loss as well as to other ridgewidthdependent factors such as nonuniformity. The work by Malis et al. [66] as outlined above demonstrates that true (near) modal phase matching can be achieved for the fundamental TM00 mode and SHG TM02 modes. Such phase matching increased the nonlinear output power by a factor of 100 compared to that of nonphasematched structures with near optimized nonlinear quantum design. The third strategy to improve on the nonlinear output power is to reduce the waveguide loss, to improve the overlap factor, and to increase the overall laser power. All these requirements can be met or at least addressed by using a waveguide that employs InP for both the top and the bottom (substrate) claddings [68]. InP offers the advantage of better optical confinement, i.e., overlap, due to its lower refractive index, higher material quality, and lower optical losses at both wavelengths of interest. Hence, an effort was made to implement nonlinear QC lasers and phasematching waveguides with InP top claddings; this work was reported in Ref. 69. The thicknesses of the waveguide layers are detailed in Fig. 5.21a and were chosen to reach the phasematching condition between the fundamental TM00 and SHG TM02 modes for the waveguide ridge width of ~7.3 m; and the phase mismatch was ǻk = 538 cmí1 for an infinitely wide waveguide. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_223_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
5×1016
cm3, 1.3 μm
active regions and injectors 50 stages 2.475 μm n InGaAs, 5×1016 cm3, 1.4 μm
PNL (mW)
1.5 μm
400
300
2.0 1.5
2.0
1.0
17 mW/W2
0.5 0.0 0.00
1.5 0.04
0.08 2
0.12 2
PL (W )
200
1.0
0.5
100
0.0
0
n InP, 12×1017 cm3, substrate
Nonlinear power PN L (μW)
n InGaAs,
cm3,
Linear power PL (mW)
n InP,
1×1017
2.5
500
Ti/Au top contact n++ InP, 99%). Devices with ridge widths between 5 and 12 m were characterized, and the optimal width was found to be around 7 m, as expected from theory. Figure 5.21b shows the LI curves at the fundamental and SHG wavelengths for a 7mwide, 1.5mmlong laser measured at cryogenic temperatures. The device displays a maximum nonlinear power of 2 mW and a lineartononlinear power conversion efficiency of approximately 17 mW/W2. Both are exceptionally high values for nonlinear QC lasers; reaching the milliwatt power range is significant as such a power level is sufficient for trace gas point sensors using midir sources. The SHG farfield radiation pattern was found to have two unequal maxima located symmetrically with respect to the waveguide axis at angles of approximately 45 degrees from the normal to the laser facet in a plane perpendicular to the device layers. This is consistent with the expected farfield distribution for the TM02 mode. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_224_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 224
Chapter Five
The narrower optimal ridge width (7 m as opposed to 9 m in the previous study [6]) is also beneficial because it suppresses the turnon of higherorder inplane transversal laser modes that are not phasematched to the SHG modes. 5.7.2
Other methods of phase matching
The abovediscussed method for true modal phase matching has the advantage of being a resonant effect with strong enhancement of several orders of magnitude at true resonance. The strategy is also straightforward, as the crossing point of the waveguide dispersion curves and hence the phasematching point can be calculated and with some effort can even be made robust toward ridge width variations; i.e., the crossing of the dispersion curves (versus ridge width) can be made more oblique. It is nevertheless up to the experimenter to fabricate lasers at the precise ridge width. While this is a seemingly trivial point, a more robust technique for phase matching would be welcome. Several techniques have been proposed, many of which adapt strategies of quasiphase matching to the nonlinear QC lasers. Belkin et al. recently [44] reported on such quasiphasematched structures, where the laser waveguide was periodically modified, by removal (etching) of a significant portion of the top cladding and the metal contact layer, which periodically changes the current injection and modal refractive index along the laser ridge. The authors report an improvement in the SHG conversion efficiency for a D2912type SHG structure by a factor of about 10. Belyanin et al. [70] recently suggested a surfaceemitting approach in which the nonlinear radiation is coupled out normal to the laser surface by using a deepetched surface (or bulk) grating. The periodicity of the grating thereby corresponds to a secondorder Bragg grating for the nonlinear light, while the fundamental pump light is still coupled through the facets of the edge emitter. Berger and Sirtori [71] finally noticed that nearir and terahertz radiation in waveguides can be directly phasematched as a result of the strong materials dispersion including anomalous dispersion around the reststrahlenband and waveguide dispersion, which in fact results in similar (or at full matching, the same) refractive indices in GaAsbased waveguides for radiation around 1 and 100 m. 5.8 Other Nonlinear Effects in Quantum Cascade Lasers The abovediscussed applications of resonant optical nonlinearities in QC lasers were chosen with the particular goal of nonlinear light Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_225_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
225
generation (higher harmonics and SFG) in mind. In the following, we briefly discuss a wider spectrum of optical nonlinearities and their use in QC lasers. These include nonlinear light generation through electronic Raman scattering and the role of nonlinearities, especially the optical Kerr effect, in modelocked QC lasers. 5.8.1 Resonant Raman upconversion scattering
Raman scattering is—essentially by definition and origin—a means of wavelength conversion. While Raman scattering involving the absorption or emission of phonons is the most familiar form of Raman scattering, other means of scattering exist within this class as well. In the context of QC lasers, resonant electronic Raman scattering involving an excited ISB transition is the obvious choice. So far, Stokes Raman ISB lasing has been reported following two different approaches. Liu et al. [72] reported an optically pumped ISB laser, in which Raman lasing involving the GaAs phonon was observed. In the second report, Troccoli et al. [73] demonstrated electronic Stokes lasing based on a designed nonlinear structure; this work is the focus of Chap. 6. While Stokes lasing is an efficient means of frequency downconversion, here we briefly discuss the complementary frequency upconversion process, i.e., stimulated electronic antiStokes (AS) Raman emission in QC lasers. As nonlinear light generation from Raman processes does not require phase matching, this work [74] may constitute a more straightforward route to unstrained (i.e., latticematched) InPbased QC lasers operating at wavelengths around and below ~4 m. In this particular work [74], we chose to implement the nonlinear and QC laser regions as two separate, monolithically integrated stacks of active regions and injectors [50]. Figure 5.22 shows a schematic of the device, including the pump laser and the AS nonlinear region stacks. The ISB transitions in the nonlinear regions (also shown in Fig. 5.22 for two specific examples) were designed to include an energy level triplet 2–3–4 embedded in a cascade, such that the maximum population is again in the excited energy level 3. The optical dipole matrix elements between levels 2, 3 and 4, z43 and z42, respectively, were made as large as possible by design, to enhance the relevant thirdorder AS nonlinearity. The electrons in level 3 undergo AS Raman scattering stimulated by the pump light (resulting from the adjacent stack of QC laser active regions and injectors), emitting photons with energy hvAS = ǻE42 + į = ǻE32 + hvpump, where ǻEij is the energy separation between levels i and j and į is the detuning, defined as į = hvpump í ǻE43. Fast depletion of the lower level (2) is achieved through LO phonon enhanced scattering into the lower energy levels. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_226_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 226
Chapter Five
50
/cm
kV
(e)
1
g U
g 3
2 1
L /cm kV 45
Active region Active region
(a)
Pump region Nonlinear region
(b)
Period length 637 Å
U g
2 cm 1 0 kV/ 5
Active region Period length 485 Å
L
(c)
m V/c 30 k
(d) 88 Å
Pump
6
3 0.2
0
0
4
2 0.2 1
2 4 6 8 10
0
0
2
Refractive index
g
4 0.4 AS
P.R. NL.R.
3
(f )
0.4
Pump region NL region
4
Normalized TM mode Intensity
0.52 eV
Period length 470 Å
2 4 6 8 10
Distance (μm)
Figure 5.22 (a) and (b) Conduction band diagrams of the (a) nonlinear and (b) pump regions, respectively, in wafer D3015, a nonlinear QC laser structure for antistokes Raman upconversion. The barrier/well widths of each of the 26 periods of the nonlinear stack, in nanometers, are 4.5/3.1/2.9/3.1/2.5/3.2/3.0/3.3/1.5/3.7/1.5/4.2/1.5/4.8/1.5/2.7, with the wells given in boldface. The underlined layers are doped to 2 × 1017 cmí3. The pump laser is a conventional 20stage QC stack emitting at Ȝ ~ 8.3 ȝm. (c) and (d) Diagram of the conduction band of the (c) nonlinear region and (d) pump region, respectively, in wafer D2924. The pump is a conventional 30period QC laser emitting at Ȝ ~ 10.5 ȝm. The layer thicknesses of each of the 30 periods comprised in the nonlinear stack are 4.0/2.6/ 2.9/2.9/2.6/2.7/2.3/2.7/2.0/2.7/1.7/3.8/2.5/4.2/1.8/7.1, following the same notation as above. In (a) and (c) the black arrows indicate the Raman transition, and the levels involved are numbered. In (b) and (d), the letters U and L indicate the upper and lower pump laser levels, respectively. The ground level of the injector is labeled g in all four plots. (e) Schematic of the laser ridge showing the stacked configuration of QC laser and antiStokes Raman structure. (f) Normalized mode intensity profile and profile of the real part of the refractive index in the reverse growth direction for both antiStokes and pump fundamental modes in wafer D3015. (Source: Ref. 74.)
Stimulated AS emission—but so far no laser action—has been observed in a variety of samples, with both, positive and negative detuning. Two designs, D3015 (positive detuning) and D2924 (negative detuning), are shown in Fig. 5.22 and discussed in Ref. 74 and below. The lasers are processed in conventional fashion, with the ridges etched deeply enough to provide strong current confinement for both active stacks, AS nonlinearity and QC laser, in the waveguide core. Figure 5.22 shows the normalized mode intensity profiles of both the AS and pump laser modes in sample D3015. The normalized mode overlap of the pump mode with the AS and pump active regions is 0.32 and 0.33, respectively; the confinement factor of the AS light is 0.38 for the nonlinear region. When one is implementing the nonlinear region and QC laser in a two or potentially multistack approach, such as
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_227_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
227
here, the relative overlap of the modes with the various stacks becomes a new degree of freedom, which must be carefully tailored to maximize energy transfer without depleting (or otherwise compromising) the pump field. Figure 5.23a shows the spectra of sample D3015 measured at different peak currents above pump laser threshold. The inset shows the spectrum of the pump light for a peak current of 2 A. The main peak at 4.8 ȝm (258 meV) is attributed to stimulated AS Raman scattering [hvpump = 150 meV and ǻE32 = 110 meV, obtained from luminescence measurements below pump laser threshold, giving an expected ȜAS = 4.8 ȝm (hvAS = 260 meV)]. Electrons in level 3, when excited by the pump photons, can also easily scatter into energy level 4 and then return via spontaneous emission to level 2. This incoherent upconversion process is the likely cause of the peak observed at 5.3 ȝm (235 meV), which is truncated by the wavelength cutoff at ~5.4 ȝm of the InSb detector. The detuning, obtained from the shift between the lines corresponding to AS Raman scattering and incoherent upconversion peak, is į = 258 meV – 235 meV = +23 meV. The shortwavelength emission spectra of the sample with negative detuning, D2924, were measured at 7 K for different peak currents above the pump laser threshold and are shown in Fig. 5.23b. The main feature is a peak at around 4.5 ȝm (276 meV), which is again attributed to AS Raman scattering (hvpump = 118 meV and ǻE32 = 155 meV, from luminescence measurements below threshold, giving an expected ȜAS = 4.5 ȝm (hvAS = 273 meV). Both examples present experimental evidence of stimulated electronic AS Raman emission in QC lasers. The most beneficial feature of this process is the large frequency shifts between the AS Raman and pump photons that can be achieved, namely, over 100 meV. Nevertheless, so far no narrowing of the AS emission peak or other evidence of gain or impending laser action has been observed. Work on improved designs of the nonlinear active regions, especially in light of an optimized (smaller) detuning į, and on a better balance of the nonlinear and QC laser active regions in the waveguide, to achieve a larger pump laser power, is underway. 5.8.2 Intersubband nonlinearities in modelocked QC lasers
All the nonlinearities discussed so far in connection with QC lasers involve specially designed multilevel ISB cascades. However, even before this work, a simple twolevel ISB nonlinearity has been shown to be at work in QC lasers, namely, the Kerr nonlinearity, or intensitydependent refractive index n around the laser transition n = n0 + I · n2, where Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_228_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Chapter Five
Intensity /arb.units
228
Intensity (arb. units)
300 250 200 150
2A 3A 2.5 A 2A 1.5 A 1.25 A
8.0 8.2 8.4 8.6
Wavelength /μm 100 50 0 3
4
5 Wavelength (μm)
6
(a) Intensity (arb. units)
Intensity (arb. units)
160 120 80
1.5 A
2.5 A 2.25 A 2A
0 5 10 15 Wavelength /μm
40
1.8 A
0
3.0 3.2 3.4 3.6 3.8 4.0 4.2 4.4 4.6 4.8 Wavelength (μm)
(b) (a) Shortwavelength emission spectra of a laser of wafer D3015 above laser threshold. Peaks attributed to stimulated antiStokes emission (4.8 ȝm), and incoherent upconversion (5.3 ȝm) can be distinguished. The inset shows the spectrum of the pump laser measured at a heat sink temperature of ~90 K and 2A peak current. (b) Shortwavelength luminescence spectra, above threshold, of D2924 measured near liquid helium temperatures (~7 K). The main peak at 4.5 ȝm is attributed to antiStokes emission. The inset shows the pump spectrum measured at ~90 K and a peak current of 1.5 A. (Source: Ref. 74.) Figure 5.23
n0 and n2 are the linear and nonlinear refractive indices, respectively, and I is the mode intensity in the cavity. When the QC laser field consists of ultrashort pulses, as in actively or passively modelocked devices, such nonlinearity gives rise to selfphase modulation, which in turn introduces a characteristic oscillatory envelope in the emission spectrum. In addition, on the longwavelength side of the laser transition n2 is positive and hence leads to selffocusing of the mode in the cavity. Selffocusing in QC lasers also reduces the mode losses, as the overlap of the guided mode with the surrounding metal contact layers is reduced; therefore it provides a saturable loss mechanism which has
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_229_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
229
been invoked to explain the observation of selfmodelocked QC lasers in Ref. 75. In later work, Soibel et al. [76] combined the mode locking of QC lasers and the thenavailable knowledge on SHG in these devices to employ the latter as an analytical tool to estimate the time duration of the modelocked pulses. In particular, from the increase in nonlinear power between cw and selfmodelocked operation, a pulse duration of ~12 ps was estimated in a QC laser capable of SHG, consistent with other measurements. These examples illustrate cases in which ISB nonlinearities serve mainly supporting functions in QC lasers; they are excellent reminders that practically all ISB transitions are nonlinear to some degree, and that these properties need to be taken into account in a complete description of QC lasers and other ISBderived optoelectronic components. 5.9 Conclusions and Outlook In summary, we have reviewed here briefly ISBbased optical nonlinearities and then in greater detail the first implementation of ISB nonlinearities into QC lasers. The latter has been especially successful with the demonstration of frequency upconversion such as SHG, SFG, and THG. Such nonlinear QC lasers are an alternative route to narrowband, shortwavelength (Ȝ 4.5 m), coherent emitters, especially those grown with latticematched, unstrained heterostructures. Some steps of design optimization for nonlinear upconversion lasers have been discussed; however, given the newness of the field, several more iterations of improved quantum design of nonlinearities are likely. Similarly, phase matching has been demonstrated in several attempts, most of which require some external tuning parameter that is still difficult to control, given current processing techniques. Thus, better implementations for phase matching are expected for future developments of nonlinear QC lasers. Finally, a significant future development will be the demonstration of successful integration of downconversion optical nonlinearities into QC lasers, especially DFG and photonpair generation by parametric downconversion, as well as monolithic parametric amplification in QC lasers. 5.10 Acknowledgments The work reviewed here and originally presented in a range of publications as referenced above is the result of many fruitful and rewarding collaborations with wonderful individuals and teams with whom Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_230_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 230
Chapter Five
working has always been, and continues to be, a real pleasure. While we won’t be able to list all those who merit thanks for the work performed, we would like to especially thank the following contributors: F. Capasso, J. Chen, A. Y. Cho, R. Colombelli, A. GomezIglesias, V. Kocharovsky, H. C. Liu, T. S. Mosely, N. Owschimikow, R. Paiella, M. L. Peabody, G. Shu, A. M. Sergent, D. L. Sivco, A. Soibel, and D. Wasserman. The work performed at Princeton University was supported by the MRSEC grant at Princeton University under account NSF DMR0213706 and by NSF grant ECS0400615. Belyanin acknowledges support from NSF and AFOSR. References 1.
P. A. Franken, A. E. Hill, C. W. Peters, and G. Weinreich, Phys. Rev. Lett. 7, 118 (1961); T. H. Maiman, Nature 187, 493 (1960).
2.
Ya. I. Khanin, Principles of Laser Dynamics, Elsevier, Amsterdam, 1995.
3.
Y. R. Shen, The Princeiples of Nonlinear Optics, John Wiley & Sons, New York, 1984.
4.
R. W. Boyd, Nonlinear Optics, Academic Press, New York, 2003.
5.
H. C. Liu, and F. Capasso (eds.), Intersubband Transitions in Quantum Wells: Physics and Device Applications I and II, Semiconductors and Semimetals, vols. 62 and 66, Academic Press, New York, 2000.
6.
J. Faist, F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho, Science 264, 553 (1994).
7.
C. Gmachl, F. Capasso, D. L. Sivco, and A. Y. Cho, Rep. on Progress in Physics 64, 1533 (2001) and references therein.
8.
H. C. Liu, Physica E8, 170 (2000).
9.
J. Allam and M. Wagner, Appl. Phys. Lett. 60, 2726 (1992); S. Krishna, S. Raghavan, G. Von Winckel, A. Stintz, G. Ariyawansa, S. G. Matsik, and A. G. U. Perera, Appl. Phys. Lett. 83, 2745 (2003); P. Bhattacharya, S. Gosh, and A. D. StiffRoberts, Ann. Rev. Mat. Res. 34, 1 (2004).
10.
J. Christen, M. Joschko, O. Stier, D. Bimberg, and E. Kapon, Semicond. Sci. Techn. 9, 1939 (1994); A. Weber, O. GauthierLafaye, F. H. Julien, J. Brault, M. Gendry, Y. Desieres, and T. Benyattou, Appl. Phys. Lett. 74, 413 (1999); S. Schmult, I. Keck, T. Herrle, W. Wegscheider, M. Bichler, D. Schuh, and G. Abstreiter, Appl. Phys. Lett. 83, 1909 (2003).
11.
M. K. Gurnick and T. A. De Temple, IEEE J. Quantum Electron. 18, 791 (1983).
12.
F. Capasso, C. Sirtori, and A. Y. Cho, IEEE J. Quantum Electron. 30, 1313 (1994); C. Sirtori, F. Capasso, D. L. Sivco, and A. Y. Cho, Phys. Rev. Lett. 68, 1010 (1992).
13.
E. Rosencher, A. Fiore, B. Vinter, V. Berger, Ph. Bois, and J. Nagle, Science 271, 168 (1996).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_231_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
231
14.
L. Tsang, D. Ahn, and S. L. Chuang, Appl. Phys. Lett. 52, 697 (1988); L. Tsang, S. L. Chuang, and S. M. Lee, Phys. Rev. B41, 5942 (1990).
15.
P. Boucaud, F. H. Julien, D. D. Yang, J. M. Lourtioz, E. Rosencher, P. Bois, and J. Nagle, Appl. Phys. Lett. 57, 215 (1990).
16.
C. Sirtori, F. Capasso, D. L. Sivco, S. N. G. Chu, and A. Y. Cho, Appl. Phys. Lett. 59, 2302 (1991).
17.
J. Hamazaki, H. Kunugita, K. Ema, A. Kikuchi, and K. Kishino, Phys. Rev. B71, 165334 (2005); E. Baumann, F. R. Giorgetta, D. Hofstetter, H. Wu, W. J. Schaff, L. F. Eastman, and L. Kirste, Appl. Phys. Lett. 86, 032110 (2005); I. Friel, K. Driscoll, E. Kulenica, M. Dutta, R. Paiella, and T. D. Moustakas, J. Cryst. Growth 278, 387 (2005); C. Gmachl and H. M. Ng, Electron. Lett. 39, 567 (2003).
18.
H. Yoshida, T. Simoyama, A. V. Gopal, J. Kasai, T. Mozume, and H. Ishikawa, IEICE Trans. Electron. E87C, 1134 (2004); P. Cristea, Y. Fedoryshyn, and H. Jackel, J. Cryst. Growth 278, 544 (2005).
19.
M. Munoz, H. Lu, X. C. Zhou, M. C. Tamargo, and F. H. Pollak, Appl. Phys. Lett. 83, 1995 (2003); B. S. Li, R. Akimoto, K. Akita, and H. Hasama, J. Appl. Phys. 95, 5352 (2004).
20.
J. Khurgin, Phys. Rev. B38, 4056 (1988).
21.
M. M. Fejer, S. J. B. Yoo, R. L. Byer, A. Harwit, and J. S. Harris, Phys. Rev Lett. 62, 1041 (1989).
22.
E. Rosencher, P. Bois, J. Nagle, and S. Delaitre, Electron. Lett. 25, 1063 (1989); E. Rosencher, P. Bois, J. Nagle, E. Costard, and S. Delaitre, Appl. Phys. Lett. 55, 1597 (1989).
23.
E. Rosencher, P. Bois, B. Vinter, J. Nagle, and D. Kaplan, Appl. Phys. Lett. 56, 1822 (1990).
24.
C. Sirtori, F. Capasso, D. L. Sivco, S. N. G. Chu, and A. Y. Cho, Appl. Phys. Lett. 59, 2302 (1991).
25.
M. Segev, I. Grave, and A. Yariv, Appl. Phys. Lett. 61, 2403 (1992).
26.
W. W. Bewley, C. L. Felix, J. J. Plombon, M. S. Sherwin, M. Sundaram, P. F. Hopkins, and A. C. Gossard, Phys. Rev. B48, 2376 (1993).
27.
C. Sirtori, F. Capasso, J. Faist, L. N. Pfeiffer, and K. W. West, Appl. Phys. Lett. 65, 445 (1994).
28.
J. Heyman, K. Craig, B. Galdrikian, M. S. Sherwin, K. Campman, P. F. Hopkins, S. Fafard, and A. C. Gossard, Phys. Rev. Lett. 72, 2183 (1994).
29.
L. Tsang and S. L. Chuang, Appl. Phys. Lett. 60, 2543 (1992); D. S. Citrin, Opt. Lett. 26, 554 (2001); Z. Xu, P. M. Fauchet, C. W. Rella, B. A. Richman, H. A. Schwettman, and G. W. Wicks, Solid State Commun. 93, 903 (1995).
30.
S. Z. Li and J. Khurgin, Appl. Phys. Lett. 62, 1727 (1993).
31.
H. Xie, W. I. Wang, J. R. Meyer, and L. R. RamMohan, Appl. Phys. Lett. 65, 2048 (1994).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_232_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 232
Chapter Five
32.
C. Fischer and M. W. Sigrist, in Solid State MidInfrared Laser Sources; Topics in Applied Physics 89, 97 (2003); D. Richter, A. Fried, B. P. Wert, J. G. Walega, and F. K. Tittel, Appl. Phys. B75, 281 (2002); D. Richter, D. G. Lancaster, R. F. Curl, W. Neu, and F. K. Tittel, Appl. Phys. B67, 347 (1998).
33.
A. A. Afonenko, V. Y. Aleshkin, and A. A. Dubinov, Semicond. 38, 239 (2004); T. Kaing, J. J. Zondy, A. P. Yeliseyev, S. I. Lobanov, and L. I. Isaenko, IEEE Trans. Instr. and Measurement 48, 592 (1999).
34.
O. Wada, New J. Phys. 6, 183 (2004); A. Harwit, R. Fernandez, W. D. Eades, D. K. Kinell, and R. L. Whitney, Superlatt. and Microstruct. 19, 39 (1996).
35.
I. Vurgaftman, J. R. Meyer, and L. R. RamMohan, IEEE J. Quantum Electron. 32, 1334 (1996); M. Zaluzny, J. Appl. Phys. 74, 4716 (1993); R. Rapaport, G. Chen, O. Mitrofanov, C. Gmachl, H. M. Ng, and S. N. G. Chu, Appl. Phys. Lett. 83, 263 (2003).
36.
J. R. Meyer, I. Vurgaftman, and C. A. Hoffman, J. Appl. Phys. 81, 7662 (1997).
37.
X. H. Zhang, Z. H. Chen, D. F. Cui, G. Z. Yang, and R. Z. Wang, Appl. Phys. Lett. 69, 3164 (1996).
38.
N. Suzuki, J. Opt. Soc. Am. B21, 2017 (2004); N. Iizuka, K. Kaneko, and N. Suzuki, Electron. Lett. 40, 962 (2004); Claire Gmachl, Sergey V. Frolov, Hock M. Ng, S.N. George Chu, and A. Y. Cho, Electron. Lett. 37, 378 (2001).
39.
J. Hamazaki, S. Matsui, H. Kunugita, K. Ema, H. Kanazawa, T. Tachibana, A. Kikuchi, and K. Kishino, Appl. Phys. Lett. 84, 1102 (2004); Claire Gmachl, Hock M. Ng, SungNee G. Chu, and Alfred Y. Cho, Appl. Phys. Lett. 77, 3722 (2000); V. D. Jovanovic, Z. Ikonic, D. Indjin, P. Harrison, V. Milanovic, and R. A. Soref, J. Appl. Phys. 93, 3194 (2003); K. Kishino, A. Kikuchi, H. Kanazawa, and T. Tachibana, Appl. Phys. Lett. 81, 1234 (2002).
40.
H. C. Liu and E. Dupont, J. Nonlin. Opt. Phys. & Mat. 11, 433 (2002).
41.
H. Schmidt, K. L. Campman, A. C. Gossard, and A. Imamoglu, Appl. Phys. Lett. 70, 3455 (1997); J. F. Dynes, M. D. Frogley, M. Beck, J. Faist, and C. C. Phillips, Phys. Rev. Lett. 94, 157403 (2005); D. Dini, R. Koehler, A. Tredicucci, G. Biasiol, and L. Sorba, Phys. Rev. Lett. 90, 116401 (2003).
42.
H. Schmidt and R. J. Ram, Appl. Phys. Lett. 76, 3173 (2000).
43.
J. Faist, F. Capasso, C. Sirtori, D. L. Sivco, A. L. Hutchinson, M. S. Hybertson, and A. Y. Cho, Phys. Rev. Lett. 76, 411 (1996); H. Willenberg, G. H. Dohler, and J. Faist, Phys. Rev. B67, 085315 (2003).
44.
M. A. Belkin, M. Troccoli, L. Diehl, F. Capasso, A. A. Belyanin, and D. L. Sivco, Conference on Lasers and ElectroOptics—PostDeadline Session QPDA1, Baltimore, MD, May 22–27, 2005.
45.
A. A. Belyanin, F. Capasso, V. Kocharovsky, and M. O. Scully, Phys. Rev. A63, 053803 (2001); A. A. Belyanin, F. Capasso, V. V. Kocharovsky, Vl. V.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_233_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
233
Kocharovsky, and M. O. Scully, Phys. Rev. A63, 053803 (2001); ibid. 65, 053824 (2002). 46.
C. Gmachl, A. Belyanin, D. L. Sivco, M. L. Peabody, N. Owschimikow, A. M. Sergent, F. Capasso, and A. Y. Cho, IEEE J. Quantum Electron. 39, 1345 (2003).
47.
Nina Owschimikow, Claire Gmachl, Alexey Belyanin, Vitaly Kocharovsky, Deborah L. Sivco, Raffaele Colombelli, Federico Capasso, and Alfred Y. Cho, Phys. Rev. Lett. 90, 043902 (2003).
48.
S. Slivken, A. Evans, J. David, and M. Razeghi, Appl. Phys. Lett. 81, 4321 (2002); J. S. Yu, A. Evans, J. David, L. Doris, S. Slivken, and M. Razeghi, IEEE Photon. Techn. Lett. 16, 747 (2004); A. Evans, J. S. Yu, J. David, L. Doris, K. Mi, S. Slivken, and M. Razeghi, Appl. Phys. Lett. 84, 314 (2004); S. Forget, C. Faugeras, J. Y. Bengloan, M. Calligaro, O. Parillaud, M. Giovannini, J. Faist, and C. Sirtori, Electron. Lett. 41, 418 (2005).
49.
C. Sirtori, J. Faist, F. Capasso, D. L. Sivco, A. L. Hutchinson, and A. Y. Cho, Appl. Phys. Lett. 66, 3242 (1995).
50.
Claire Gmachl, Deborah L. Sivco, James N. Baillargeon, Albert L. Hutchinson, Federico Capasso, and Alfred Y. Cho, Appl. Phys. Lett. 79, 572 (2001).
51.
A. Straub, T. S. Mosely, C. Gmachl, R. Colombelli, M. Troccoli, F. Capasso, D. L. Sivco, and A. Y. Cho, Appl. Phys. Lett. 80, 2845 (2002); C. Gmachl, D. L. Sivco, R. Colombelli, F. Capasso, and A. Y. Cho, Nature 415, 883 (2002).
52.
H. T. Grahn, R. J. Haug, W. Müller, and K. Ploog, Phys. Rev. Lett. 67, 1618 (1991).
53.
S. Illek, W. Thulke, C. Schanen, H. Lang, and M. C. Amann, Electron. Lett. 26, 46 (1990).
54.
A. Belyanin, V. Kocharovsky, Vl. Kocharovsky, and M. Scully, Phys. Rev. A65, 053824 (2002); S. M. Wang, Y. H. Shen, J. X. Xu, L. G. Hu, J. Zhu, D. R. Yang, H. Zhang, Y. W. Zeng, and J. Q. Yao, Appl. Phys. Lett. 84, 3007 (2004).
55.
J. S. Yu, S. Slivken, S. R. Darvish, and M. Razeghi, IEEE Photon. Techn.Lett. 17, 1154 (2005); M. P. Semtsiv, M. Ziegler, S. Dressler, W. T. Masselink, N. Georgiev, T. Dekorsy, and M. Helm, Appl. Phys. Lett. 85, 1478 (2004); R. Teissier, D. Barate, A. Vicet, C. Alibert, A. N. Baranov, X. Marcadet, C. Renard, M. Garcia, C. Sirtori, D. Revin, and J. Cockburn, Appl. Phys. Lett. 85, 167 (2004).
56.
M. W. Sigrist (ed.), Air Monitoring by Spectroscopic Techniques, Wiley Interscience, New York, 1994.
57.
C. Sirtori, F. Capasso, J. Faist, and S. Scandolo, Phys. Rev. B50, 8663–8674 (1994).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_234_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers 234
Chapter Five
58.
G. Shu, E. E. Narimanov, C. Gmachl, D. L. Sivco, and A. Y. Cho, Conference on Lasers and ElectroOptics, CTuM5, Baltimore, MD, May 22–27, 2005.
59.
C. Gmachl, N. Owschimikow, A. Belyanin, A. M. Sergent, D. L. Sivco, M. L. Peabody, A. Y. Cho, and F. Capasso, Appl. Phys. Lett. 84, 2751 (2004).
60.
T. S. Mosely, A. Belyanin, C. Gmachl, D. L. Sivco, M. L. Peabody, and A. Y. Cho, Opt. Express 12, 2972 (2004)
61.
X. Marcadet, V. Ortiz, J.Y. Bengloan, S. Dhillon, M. Calligaro, and C. Sirtori, J. Vac. Sci. and Techn. 22, 1558 (2004); J.Y. Bengloan, M. Calligaro, V. Ortiz, X. Mercadet, I. Maurin, and C. Sirtori, Intersubband Transitions in Quantum Wells 2003, R65, Evolene, Switzerland, September 1–5, 2003.
62.
H. Giovannini, M. Beck, N. Hoyler, and J. Faist, Intersubband Transitions in Quantum Wells 2003, R64, Evolene, Switzerland, September 1–5, 2003.
63.
C. Gmachl, A. Soibel, R. Colombelli, D. L. Sivco, F. Capasso, and A. Y. Cho, IEEE Photon. Techn. Lett. 14, 1671 (2002).
64.
A. Fiore, V. Berger, E. Rosencher, P. Bravetti, and J. Nagle, Nature 391, 463 (1998).
65.
J. R. Meyer, C. A. Hoffman, F. J. Bartoli, and L. R. RamMohan, Appl. Phys. Lett. 67, 608 (1995); K. L. Vodopyanov, K. O’Neill, G. B. Serapiglia, C. C. Phillips, M. Hopkinson, I. Vurgaftman, and J. R. Meyer, Appl. Phys. Lett. 72, 2654 (1998).
66.
Oana Malis, Alexey Belyanin, Claire Gmachl, Deborah L. Sivco, Milton L. Peabody, A. Michael Sergent, and Alfred Y. Cho, Appl. Phys. Lett. 84, 2721 (2004).
67.
A. Chowdhury and L. McCaughan, IEEE Photon. Techn. Lett. 12, 486 (2000); K. Moutzouris, S. V. Rao, M. Ebrahimzadeh, A. De Rossi, M. Calligaro, V. Ortiz, and V. Berger, Appl. Phys. Lett. 83, 620 (2003).
68.
J. Faist, F. Capasso, C. Sirtori, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, S. N. G. Chu, and A. Y. Cho, Appl. Phys. Lett. 68, 3680 (1996).
69.
O. Malis, A. Belyanin, D. L. Sivco, J. Chen, A. M. Sergent, C. Gmachl, and A. Y. Cho, Electron. Lett. 40, 1586 (2004).
70.
A. A. Belyanin, V. V. Kocharovsky, Vl. V. Kocharovsky, and M. O. Scully, “SurfaceEmitting GratingOutcoupled Lasers for Mid/FarIR DifferenceFrequency Generation,” submitted to Appl. Phys. Lett. (2005).
71.
V. Berger and C. Sirtori, Semicon. Science and Techn. 19, 964 (2004).
72.
H. C. Liu, C. Y. Song, Z. R. Wasilewski, A. J. Spring Thorpe, J. C. Cao, C. Dharmawardana, G. C. Aers, D. J. Lockwood, and J. A. Gupta, Phys. Rev. Lett. 90, 077402 (2003).
73.
M. Troccoli, A. Belyanin, F. Capasso, E. Cubucku, D. L. Sivco, and A. Y. Cho, Nature 433, 845 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_235_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers Optical Nonlinearities
235
74.
A. GomezIglesias, D. Wasserman, C. Gmachl, A. Belyanin, and D. L. Sivco, Appl. Phys. Lett. 87, 261113 (2005).
75.
R. Paiella, F. Capasso, C. Gmachl, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, Science 290, 1739 (2000).
76.
A. Soibel, F. Capasso, C. Gmachl, M. L. Peabody, A. M. Sergent, R. Paiella, D. L. Sivco, A. Y. Cho, and H. C. Liu, IEEE J. Quantum Electron. 40, 197 (2004).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH05_236_03/23/2006 Optical Nonlinearities in Intersubband Transitions and Quantum Cascade Lasers
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_237_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
6 Raman Injection and Inversionless Intersubband Lasers Alexey Belyanin Department of Physics, Texas A&M University, College Station, Texas
Mariano Troccoli and Federico Capasso Division of Engineering and Applied Sciences Harvard University, Cambridge, Massachusetts
6.1
Introduction
Quantum cascade lasers (QCLs) are only 11 years old [1]; however, they have already reached a remarkably high level of maturity. QCLs operate due to population inversion on the intersubband transition between quantumconfined electron states in semiconductor quantum well structures. They utilize a typical fourlevel lasing scheme [2] (Fig. 6.1), in which electrons are injected to the upper laser state 3 from the upstream injector 4 by resonant tunneling, make radiative or nonradiative transition to the lower laser state 2, and then rapidly depopulate this state via phonon emission and tunneling out of the active region to the injector section downstream. The latter serves as an upstream injector for the next active stage. The active region can be formed by several coupled quantum wells (QWs) or by a superlattice. Details of different active region and laser designs are presented in Chaps. 2 through 4 of this volume. Although the scheme in Fig. 6.1 includes at least four states, there are only two states, 2 and 3, interacting resonantly with laser radiation. In this case, positive gain for the laser signal exists only in the presence 237
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_238_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 238
Chapter Six
4 3
2 1
4
Figure 6.1 Sketch of the fourlevel lasing scheme implemented in one active stage of a
conventional QCL. There are usually many stages in a device.
of population inversion between these states. Of course, population inversion should be defined by taking into account the density of states in the momentum space and the distribution function of electrons. The situation changes if one of the laser states is strongly coupled to some other state(s) by the electromagnetic field, through coherent tunneling, or even through an incoherent relaxation process. Coupling means the existence of the coherence or the offdiagonal element of the density matrix on one of the transitions. It gives rise to an additional contribution to laser gain and frequency. Under favorable conditions this contribution adds a positive gain, and amplification becomes possible in the absence of population inversion. This phenomenon has been called lasing without inversion (LWI) and has been the subject of much debate and investigation since the 1980s; see, e.g. Refs. 3 and 4 for the review and references to original works. In the “quantum” language, the origin of the effect is the quantum interference between multiple transition channels, which violates the reciprocity between the absorption and emission processes. Hereafter by states we will mean “bare” states of the hamiltonian of the electron subsystem. In most cases, the inversion exists in the basis of states “dressed” by the coupling, i.e., of the eigenstates of the total hamiltonian that includes the coherent coupling term. In some cases, the gain exists without population inversion in any meaningful basis. In the language of macroscopic electrodynamics, the effect is described by resonant polarization of the multistate system at the signal frequency. The polarization is strongly affected by the resonant coupling, which gives rise to the change in the amplification condition for the signal, accompanied by peculiar changes in the refractive index and group velocity that have been the subject of active investigation and controversy as well; see Ref. 5 for the review. Note that although the polarization can be treated as linear with respect to the weak signal, it is highly nonlinear with respect to the electromagnetic field (the “drive”) that is used to create coherent coupling. Therefore, with respect
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_239_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
239
to the total field we are dealing with resonant nonlinear optical interaction. The simplest system that already exhibits LWI consists of three states in the presence of a strong drive field. Four possible configurations are shown in Fig. 6.2. Despite obvious differences, the physics of inversionless gain in these systems is remarkably similar. In the absence of an optical drive, the signal gain is proportional to the population difference on the signal transition, and population inversion is required for amplification. When the optical drive is on, there is an additional contribution to the gain coming from the nonlinear mixing of the drive electromagnetic field and the coherent polarization oscillations at frequency resonant to transition 1–2 in Fig. 6.2a and b and transition 1–3 in Fig. 6.2c and d. This polarization, in turn, is excited selfconsistently by the interaction between the drive and signal field. Under certain conditions, this Ramantype contribution can exceed both resonant absorption on the signal transition and all other losses, leading to laser action. When all fields are close to resonance, Ramantype inversion on the twophoton transition (e.g., 1–3–2 in Fig. 6.2a and b) may or may not be present in a system. When the drive field is detuned very far from resonance with the drive transition 1–3, the gain exists only in the presence of the Raman inversion n1 – n2 > 0. Raman inversion in cascade schemes in Fig. 6.2c and d means n3 > n1. Similarly to the ȁ scheme, gain on the signal transition in cascade schemes is possible in the absence of any inversion including Raman inversion. However, we found that for realistic parameters in QC structures, the gain exceeds losses when Raman inversion is already present in the system. A similar conclusion has been reached in studies of other systems [6, 7]. 3
2 1
Es
Ed
2
1
Es
Ed 3
(a)
(b)
3
3
Ed 2
Ed
Es 1
Es
2
1 (c)
(d)
Figure 6.2 Simplest threelevel systems exhibiting the effects of Raman and inversionless
lasing of the signal field Es in the presence of a coherent drive field Ed. (a) ȁ scheme; (b) V scheme; (c) and (d) cascade, or ladder, schemes.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_240_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 240
Chapter Six
Although there have been many theoretical studies of LWI, experimental progress has not been that impressive; see Ref. 4 for the review. It has been limited to the proofofprinciple experiments with rarefied atomic vapors, in which the multilevel atomic system strongly driven by external laser field demonstrated amplification on the order of several percent at a signal frequency very close to the frequency of the drive laser. In semiconductor quantum wells, it was suggested to reach LWI by employing Fanotype interference between two states induced by tunneling to the quasicontinuum; see Ref. 8 for the review. There was also a suggestion to use coherent laser coupling to achieve LWI in a system of excitons in quantum dots [9]. As far as we know, these ideas have not been realized yet. Another issue with LWI in any material system, not only semiconductors, is the lack of a strong practical motivation. It would be very important to achieve inversionless lasing on the rapidly decaying transition when the population inversion is difficult to implement, e.g., on the Xray transitions in atomic ions or intersubband transitions in a QW. However, note that in realistic situations LWI occurs under conditions that are actually harder to implement than usual lasing with inversion [6–8]. Selection rules in atomic systems place strong restriction on the type and efficiency of the particular LWI scheme. In addition, the necessity of a strong external laser drive limits practical applications of such schemes and gives rise to additional problems related to the drive absorption, scattering, and overlap with a signal beam. For example, in many cases the drive field experiences resonant absorption at a characteristic length, which is shorter than the amplification length of the signal. The latter is especially true for semiconductor QWs in which the drive absorption on the interband or intersubband transition makes the realization of the LWI schemes with an external drive unfeasible. In Ref. 5 we argued that the above problems can be overcome if the drive field is generated in the same multilevel system that is used for inversionless amplification of the signal, as shown schematically in Fig. 6.3. This idea of resonant intracavity optical pumping is applicable not only to Raman or inversionless lasing, but also to any nonlinear optical process. Such schemes and devices can demonstrate new physics and offer significant practical benefits. QCL structures seem to be an ideal system for implementing such integration of lasing and nonlinear optical generation. Intracavity intensities of the laser field in QCLs can be quite high—many megawatts per square centimeter, which corresponds to Rabi frequencies exceeding the spectral line width of intersubband transitions. Intersubband transitions in coupled asymmetric QWs can Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_241_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
241
Integrated laser drive and nonlinear active region
Drive z y
Signal x
Figure 6.3 Integration of the conventional injection laser and the nonlinear region supporting resonant nonlinear conversion of the laser (drive) field into radiation at a signal frequency. Coordinate frame used in the equations below is indicated.
be manipulated to control their dipole moments and relaxation rates. These dipole moments are usually very large, between 1 and 10 nm, giving rise to giant resonant nonlinearities. For example, the values of Ȥ(2) ~ 106 pm/V have been demonstrated; see, e.g., Refs. 10 through (2) 13. Note that in conventional nonlinear optical crystals Ȥ is on the order of several picometers per volt. Electron transport through the structure and populations of electron states can be efficiently controlled by resonant tunneling and phonon emission. Finally, QC structures offer a great flexibility in combining several laser transitions or heterogeneous active stages designed to emit or absorb at different wavelengths [14]. In particular, lasing in QCLs at two or more frequencies has been demonstrated [15, 16]. We have recently shown [17–23] that the standard active region of a QCL can be integrated with a cascade of intersubband transitions designed for the nonlinear conversion of the laser field into coherent radiation at a different frequency. Generation of the second and third harmonics and the sum frequency has been demonstrated. Milliwatt power level for second harmonic generation has been achieved [22]. Recently the first successful experiment on Raman injection laser has been reported [23]. Here we consider the possibility to integrate a QC laser with a multipleQW nonlinear section implementing one of the schemes shown in Fig. 6.2, in which states 1, 2, and 3 are electron subbands in the conduction band. Besides discussing the physics of Raman and inversionless lasing with application to QC lasers, our goal is to identify the particular schemes that could bring meaningful practical benefits. From a practical point of view, the schemes in Fig. 6.2 could be used to implement a nonlinear conversion of the optical drive into the signal at wavelengths that can be hard to reach for standard QC lasers and that can vary in a very broad range from the terahertz region to short midinfrared and even nearinfrared region. The physical reasons Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_242_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 242
Chapter Six
underlying this advantage of nonlinear optical schemes are that (1) no resonant tunneling and even no current are required in the nonlinear section of the laser and (2) no population inversion is necessary on the signal transition. Of course, population inversion and electron transport are required in the active region supporting the drive laser. However, the drive wavelength can be chosen to lie in the “sweet spot” of QC lasers (7 to 9 m for InGaAs/AlInAs structures) where population inversion is easy to provide and where they are most powerful, efficient, and capable of continuouswave roomtemperature operation [24, 25]. In addition, one may expect new or enhanced functionalities stemming from the nature of the nonlinear optical process, e.g., electric tuning by Stark effect and wider tuning range as compared to conventional QC lasers. To summarize, the primary practical appeal of integrated devices is the potential to combine the advantages of semiconductor injection lasers (compactness, robustness, and handling convenience) with the benefits of nonlinear optical sources. We give a review of opportunities and limitations related to the simplest threelevel Raman and LWItype schemes in QCL structures, in which the laser field serves as an internally generated coherent optical drive. 6.2 Theoretical Framework 6.2.1
Electromagnetic modes
Throughout the chapter we assume that the electromagnetic field is classical and is described by the Maxwell equations. An interesting problem of the statistics of light generated in our resonant nonlinear systems is beyond the scope of this review and will be considered elsewhere. In QCL structures we are dealing with interaction of tightly confined waveguide modes. Although the nonlinear optics of waveguide modes has been considered many times in the past (see, e.g., Ref. 26), for the reader’s convenience we present the general equations in the form suitable for QC structures. For intersubband transitions close to the ī point in the conduction band, the dipole moments have only z components. Therefore, transverse magnetic (TM) polarized modes with a large z component of the electric field are preferentially excited. In Maxwell’s equations it is convenient to separate resonant intersubband polarization P from the nonresonant dielectric response described by the complex dielectric function İ (x, y, z) as follows:
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_243_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
෮ × H =
243
İ E 4ʌ P + c t c t
(6.1)
1 H c t
(6.2)
෮×E= í
In the simplest case of a planeparallel semiconductor waveguide, the dielectric function has a piecewiseconstant profile in the z direction and is constant in the y direction, with jumps on the lateral walls of the waveguide. In deriving a single wave equation for the magnetic field in the TM ˜ = (1 / İ)෮, which is mode, it is convenient to introduce a new operator ෮ equivalent to the transformation to new variables y
x
˜x = İ(x,
y, z) d x
z
˜y = İ(x,
˜z = İ( x,
y, z) d y
0
0
y, z) d z
0
Then Eqs. 6.1 and 6.2 can be combined as 4ʌ 1 ෩2 H ෩ P 2 ෮ Hí 2 = í ෮ × 2 c ෩t İ İc ෩t
( )
(6.3)
Let us further assume for simplicity that İ = İ (y, z) is independent of x, and let us expand the magnetic field over the quasiorthogonal set of the transverse waveguide modes Fj(y, z): H = h j ( x )F j ( y , z )e
iȕ j x í iȦ j t
+ c.c.
j
(6.4)
Here the functions hj(x) are slowly varying with x, and we can neglect their second derivatives. In general, hj are also the functions of time, but here we consider the continuouswave operation or pulses that are much longer than all relaxation times in a QCL. The waveguide modes are eigenfunctions of the equation İ
(
Ȧ2j İ + Fj + í ȕ2j F j = 0 2 y İ y z İ z c
)
(
)
(6.5)
The solution of Eq. 6.5 defines both the transverse profile of a given waveguide mode Fj(y, z) and its dispersion, i.e., the complex propagation constant ȕj(Ȧj) as a function of the real frequency of the mode. The modes with different index j are weakly coupled due to waveguide losses, but we neglect this coupling here, assuming the orthogonality condition
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_244_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 244
Chapter Six
1İ F F d A = į i
* j
(6.6)
ij
where the integration is over the waveguide cross section and the asterisk denotes complex conjugation. After substituting the expansion 6.4 into Eq. 6.3 and using Eq. 6.5, we arrive at j
2iȕ j iȕ x F je j İ
í iȦ j t
h j 4ʌİ ˜ P = í ෮ × x c t İ
( )
(6.7)
Multiplying Eq. 6.7 by F*k , integrating over the waveguide cross section, and using the condition 6.6, we finally obtain the equation describing the excitation of a given waveguide mode: hk 2ʌi íiȕ k x + iȦ k t ˜ P * = e İ෮ × F dA x cȕk t İ k
( )
(6.8)
The polarization that excites a given mode can be due to nonlinear optical processes involving other modes, in which case we should write the equation similar to Eq. 6.8 for each participating mode and solve the whole coupled system together with material equations for the polarization. Further simplification occurs if we recall that the intersubband electronic polarization is directed along the z axis perpendicular to the QW plane: P = Pz0. For the waveguide that is sufficiently broad in the y direction, we may also assume that the magnetic field has only a y component. Then Eq. 6.8 can be rewritten as hk 2ʌi íiȕ k x = í e cȕ x k
+ iȦ k t
1 2 P * F dA İ t x k
(6.9)
This equation has to be solved with appropriate boundary conditions on the cavity facets x = 0 and x = L, taking into account the reflection and transmission of the optical power. For a weak signal field the polarization can be expanded in series in powers of the field. For example, the terms of zeroth order with respect to the signal field describe intracavity generation of harmonics by a strong laser drive field [18, 21]. Here we restrict ourselves to the processes of true lasing, in which the weaksignal polarization is proportional to the z component of the electric field of a given mode: P = Ȥ Ez. This would lead to the exponential weaksignal gain. Note that the polarization may be linear with respect to the weaksignal field but is highly nonlinear with respect to the drive field. In fact, it has to be highly nonlinear. Indeed, the main nonlinearity Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_245_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
245
present in our system is resonant saturation nonlinearity. The expansion of the polarization in powers of the drive field breaks down when the drive field intensity approaches the saturation value (between 0.1 and 1 MW/cm2 for a strong intersubband transition). However, since the drive field is an internally generated laser field, it is inevitably close to saturation as soon as the lasing threshold is surpassed by a factor of 2. Therefore, we are in the nonperturbative regime, and in calculating the polarization, the drive field needs to be taken into account exactly. The resonant susceptibility Ȥ is a function of all three coordinates x, y, z as it depends on the position of the active layers in a waveguide and the distribution of the drive field intensity across the waveguide and along the cavity. We will, however, assume that the x dependence of Ȥ is quite smooth and neglect its x derivative in the righthand side of Eq. 6.9. Then, from Eqs. 6.1 and 6.2 one can derive the relation iȕ x í iȦ j t 2P cȤ 2 H cȤ § § í h ȕ2 F e j İ x 2 İ j j j j t x
(6.10)
If only one waveguide mode is excited at a signal frequency (because, e.g., it has the excitation threshold considerably lower than that of all other modes), we can obtain from Eqs. 6.9 and 6.10 the equation for the amplitude of this mode
h 2ʌiȦȝh Ȥ 2 F 2 d A = 2ʌiȦȤ § īh x c cȝ İ
(6.11)
where ȝ = c Re( ȕ ) / Ȧ is the effective refractive index of the given waveguide mode and
ī = ȝ2
1 2 2 F  d A İ Ȥ0
(6.12)
is the effective optical confinement factor proportional to the overlap of the Poynting vector of the mode with the active region. The integral in Eq. 6.12 is over the active layers where Ȥ 0 and Ȥ is the averaged value of Ȥ in the active region; its definition is evident from comparing Eqs. 6.11 and 6.12. We will omit the overbar hereafter. The integral in Eq. 6.12 extended over the whole waveguide cross section would give the total flux of the Poynting vector of the mode in the x direction. The real part of the coefficient before h on the righthand side of Eq. 6.11 defines the modal gain of the field
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_246_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 246
Chapter Six
gM =
2ʌȦ Im Ȥ ī cȝ
(6.13)
while its imaginary part determines the resonant frequency shift. Solving Eq. 6.3 with boundary conditions on the cavity facets leads to a set of discrete longitudinal modes of the FabryPerot cavity, spaced by ǻȞ = mʌc/L, where L is the cavity length and m is an integer. This spacing is usually much smaller than the spacing between neighboring transverse modes. For a weak signal field below saturation, when Ȥ is independent of the signal intensity, the x distribution of the total field amplitude in a cavity is the sum of two counterpropagating exponents Htot =
Hout (g í Į ) x í(g í Į ) x Re M w + e M w 1íR
(
)
(6.14)
where Įw = Im ȕ is waveguide losses, R = ( ȝ í 1) / ( ȝ + 1) is the reflection factor of the facets for the magnetic field in the TM mode, and Hout is the amplitude of the magnetic field in the outgoing radiation from one facet. We assumed the reflection factors for the two facets to be equal for simplicity. The excitation condition for a given mode has the usual form gM > Į w +
1 1 ln R 2L
(6.15)
Note that both gain and losses are defined here with respect to the field amplitude. The same quantities for the field intensity are 2 times larger. 6.2.2
Material equations
Since we are dealing with resonant optical nonlinearities, the natural way to treat the interaction of light with an electron subsystem is through the density matrix equations. It allows one to easily incorporate many interacting fields and various incoherent relaxation and scattering processes. In this approach the polarization P of the medium that serves as a source of the field in Maxwell’s equations is calculated as a trace of the density matrix P=
1 Tr (dȡ) ˂V
(6.16)
where the summation is performed over all electron states in the volume ǻV and dij = ezij are the dipole moments of the intersubband transitions i–j. The elements of the density matrix are found from the master equation of the type Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_247_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
ȡ k ȡk i = í ( H , ȡk ) + t t ല

247
(6.17) col
where the hamiltonian includes a system of electron states and its coherent interaction with the electromagnetic field, while all relaxation and scattering processes are included in the collision integral, which is the second term on the righthand side. We proceed with several important approximations as specified below. 1. We neglect most manybody effects due to Coulomb interaction of electrons. The only Coulomb effect that we include is the electric field due to charge separation in a doped structure. For average electron densities in the active region at the level of several 1016 cm–3 typical for QCLs, the neglected HartreeFock and higherorder corrections lead to the energy shift of the intersubband (ISB) transition of the order of 1 meV or less, which is insignificant compared to the line broadening and experimental uncertainty. Of greater potential importance is the effect of Coulomb interactions on the decoherence rates. There have been arguments that Coulomb interactions may actually decrease the decoherence rate of the optical polarization [27], which could be important for the coherent phenomena considered here. However, the line broadening typically observed in InGaAs/AlInAs structures in luminescence and absorption experiments is at the level of 10 to 15 meV full width at half maximum (FWHM). This value is much larger than any positive or negative effect associated with Coulomb interactions. The origin of the observed broadening is uncertain at this point. It could be homogeneous broadening related to the interface roughness [28], which is supported by an approximately lorentzian profile of the absorption lines. Another option is the inhomogeneous broadening that could be associated, e.g., with inhomogeneity of the QW structure. In any case, we treat the decoherence rates of the offdiagonal matrix elements as external parameters coming from experiment. 2. We neglect the effect of the laser field on the electron wave functions and dipole moments of the intersubband transitions. In principle, the intracavity laser intensities in QCLs can reach the level of several megawatts per square centimeter. This corresponds to the electric field of tens of kilovolts per centimeter, which is comparable to the external electric field created by a voltage bias across the contacts. Such fields could modify the electron wave functions, leading to a change in the dipole moments and scattering rates, although we are not aware of any studies of this effect for intersubband transitions. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_248_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 248
Chapter Six
This could be an interesting problem by itself, which is beyond the scope of this chapter. 3. In evaluating the dynamics of populations (diagonal terms in the density matrix), we replace the realistic spatial kinetics of electron transport through the structure with rate equations for a set of electron states, with the transition times between different states defined by phonon emission and resonant tunneling. Then the analysis can be split in two sequential steps. At the first step, the electron states are found in the absence of the optical field by solving the coupled Schrödinger and Poisson equations. The dipole moments and scattering rates are calculated. At the second step, the resonant interaction of the multifrequency laser field with a given set of electron states is studied on the basis of Maxwell’s equations coupled with density matrix equations, with the dipole moments and relaxation rates provided from the previous step. As a result, we find the electron populations, drive and signal thresholds, and drive and signal intensities as functions of the single external parameter of injection current density. Equations for the intersubband offdiagonal density matrix elements ȡmn(k) and the diagonal matrix elements ȡmm(k) can be written in the following general form [29]: dȡmn ie E ( z ȡ í zqn ȡmq ) + (Ȗ mn + iȦ mn )ȡ mn = dt ല z q mq qn
(6.18)
dȡmm ie + Rm = E ( z ȡ í zqm ȡ mq ) dt ല z q mq qm
(6.19)
Here Ȗmn(k) is the relaxation rate of the offdiagonal element ȡmn(k) of the density matrix, Ȧmn(k) is the transition frequency and zmn the dipole moment of the ISB transition between mth and nth subband states with a given inplane momentum k, and Rm denotes all relaxation and pumping terms that determine the electron distribution ȡmm(k) in the mth subband in the absence of radiation field. Since we deal with resonant interactions, the electric component Ez(r, t) of the radiation field inside the laser cavity can be represented as a sum over quasimonochromatic components with slowly varying amplitudes Emn and frequencies Ȟmn nearly resonant to the transition frequencies Ȧmn:
Ez (r, t ) = Emn (r) e
i ȕ mn x í iȞ mn t
+ c.c.
(6.20)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_249_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
249
The function Emn is related to the magnetic field amplitude hmn(x) Fmn(y, z) for a given quasimonochromatic field component through Maxwell’s equations 6.1 and 6.2. In principle, there can be several waveguide modes for each frequency Ȟmn. However, we will assume for simplicity that there is only one transverse waveguide mode excited for each frequency. Then one can write Emn § í h( x) ȝ / İ( y , z)]F ( x , z ). Here all terms on the righthand side should also have the index mn, which we dropped for simplicity. The generalization to the case of many transverse modes of different order is straightforward. Offdiagonal elements of the density matrix can be written as
ȡ mn (t ) = ı mn (t )e
íiȞ mn t
(6.21)
where the amplitude ımn is a slowly varying function of time. For the diagonal elements, ȡmm = ımm. Using the above expressions in Eqs. 6.18 and 6.19, we arrive at the truncated density matrix equations dı mn ie + īmn ı mn = ( z E ı í zqn Eqn ımq ) dt ല q mq mq qn
(6.22)
dı mm ie + Rm = ( z E ı í zqm Eqm ı mq ) dt ല q mq mq qm
(6.23)
* , and Here ī mn = Ȗ mn + i (Ȧ mn í Ȟ mn ). Note that ı mn = ı*mn , zmn = zmn * . Emn = Enm
6.3 Raman QC Laser Let us apply the above general treatment to the generic Raman process of Fig. 6.2a. Stimulated Raman scattering is a thirdorder nonlinear process that allows one, in specific materials, to generate gain at a wavelength different from the one of the incident radiation and can lead to laser emission at the peak of the Raman gain. The underlying physical mechanism is the scattering of the incident fundamental radiation by a certain eigenmode of oscillations in a material, which is selfconsistently excited by the parametric interaction between the incident and the scattered light. The wavelength shift between the fundamental and the Raman emission is determined by a resonance frequency of the internal oscillations and can be due to vibrational (phonon), rotational, plasmon, or electronic resonances. In a general scheme of the Raman Stokes process sketched in Fig. 6.4, the internal oscillations in a medium correspond to the transition
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_250_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 250
Chapter Six
3
hvL
Δ
hvS
2 1 Figure 6.4 A schematic of Raman scattering of laser light (left arrow) into a lower
frequency Stokes wave (right arrow).
between electron or molecular states 1 and 2. The incident photon of energy ƫȦd is converted into a Stokes signal photon of energy ƫȦs, where both the incident and scattered beams are usually fardetuned in frequency from state 3 and other higherlying states to avoid strong absorption. In this case, only twophoton transitions between state 1 and 2 mediated by an intermediate, very shortlived virtual state may occur. As a result, the interaction between the fundamental and scattered light is of purely parametric origin and is ultimately constrained by the ManleyRowe relation: conservation of a total number of photons in both electromagnetic modes. Stimulated Raman scattering has been observed in all kinds of media: gases, liquids, solids, and plasmas. Until now, a distinctive feature of all Raman amplifiers has been the necessity of an external optical pump. Also, existing solidstate Raman sources universally employ scattering off a vibrational (phonon) resonance in a crystal or fiber [30]. A powerful fundamental laser radiation is usually required to offset a small value of the Raman gain (several 10–9 cm/W). The possibility of Raman amplification using intersubband transitions has been theoretically discussed in Ref. 31. In Ref. 32, Raman lasing on intersubband transition in a GaAs/AlGaAs double quantum well structure optically pumped by CO2 laser has been demonstrated, although the Raman shift was still determined by a phonon resonance. In recent work [23] we demonstrated the first injectionpumped Raman laser, in which the fundamental and the Raman radiation are both generated by intersubband electronic transitions in the very same active region of a quantum cascade laser. The stimulated scattering and lasing is due to the excitation of coherent electronic polarization on the midinfrared intersubband transition 2–1. Its frequency (E2 – E1) / ƫ defines the Raman shift; it has nothing to do with phonons and can vary in a very broad range. It could be also efficiently tuned by a voltage bias since the transition 2–1 is diagonal in real space.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_251_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
6.3.1
251
Gain in the resonant ฎ scheme
Let us first consider the generic properties of resonant gain at the Stokes frequency in a system of Fig. 6.4 without specifying its implementation in a particular semiconductor heterostructure and the way the electron transport is organized. To get transparent semianalytic results, we assume for simplicity that all relevant ISB transitions are homogeneously broadened; i.e., the transition frequency between two subbands is the same for all electrons in these subbands. There are experimental indications and theoretical arguments that this may indeed be the case for QCL structures [28]. In doing this, we assume that the effects of subband nonparabolicity and inhomogeneity of the structure lead to smaller broadening than the homogeneous line width. The effects leading to inhomogeneous broadening can be easily taken into account if necessary. Then Eqs. 6.18 and 6.19 or 6.22 and 6.23 can be summed over the electron kstates in each subband, which amounts to dropping the argument k and replacing the diagonal matrix elements by the total populations of the subbands nm = ȡmm . The result is k
dı21 + ī21ı21 = í iȍ d ı*32 + iȍ*s ı31 dt
(6.24)
dı31 + ī31 ı31 = iȍ d n13 + iȍ s ı21 dt
(6.25)
dı32 + ī32ı32 = iȍ s n23 + i ȍ d ı*21 dt
(6.26)
where ī32 = Ȗ32 + i(Ȧ32 í Ȧ s ) ī31 = Ȗ31 + i(Ȧ31 í Ȧ d ) ī21 = Ȗ21 + i(Ȧ21 í Ȧ d + Ȧ s )
Here ȍd = ez13Ed / ƫ and ȍs = ez23Es / ƫ are the Rabi frequency of the drive and the Stokes mode, respectively; n12 = n1 – n2; zmn is the dipole moment of the transition m – n; and Ȧd and Ȧs are frequencies of the drive and the Stokes field modes, respectively. The polarization on the Stokes transition 2–3 that should be substituted in the righthand side of Eq. 6.9 or 6.11 is given by
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_252_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 252
Chapter Six
P = e ( z23 ȡ32 + z32 ȡ23)
(6.27)
The system of Eqs. 6.24 through 6.26 is incomplete because the drive field and the population densities n1,2,3 of electrons in states 1, 2, 3 are not free parameters. They must be calculated selfconsistently from the full set of coupled density matrix and Maxwell equations including the QCL section in which the drive field is generated; see the modeling of the specific QCL structure below. The only external parameters are the injection current density and the dephasing rates Ȗmn that are equal to the halfwidth at halfmaximum of the corresponding transition line widths. Typical values of Ȗmn are 5 to 10 meV for intersubband transitions in InGaAs/AlInAs quantum wells in the midinfrared range, which exceeds the lifetime broadening, estimated to be on the order of 1 meV. Lifetimebroadened intersubband transitions have been reported so far only in GaAs QWs at low temperature [28]. In the terahertz range the broadening is usually smaller, on the order of 2 to 6 meV FWHM. For the continuouswave operation or pulses that are much longer than all relaxation times, one can neglect the time derivatives in Eqs. 6.24 to 6.26. Then the calculation of ı32 is reduced to algebra. According to Eq. 6.13, the gain is proportional to Im Ȥ = Im(ez23ı32/ E s ). Retaining only linear terms with respect to the weak field Es, we obtain for the intensity gain (which is double the modal gain in Eq. 6.13) g1 = 2gM =
{
2 4 ʌ Ȧ s e 2 z32 īs ലcȝ s
1 × Re ī32 +  ȍ d  2 ī*21
/
 ȍ d  2 (n1 í n3) ī*21ī*31
í (n2 í n3)
}
(6.28)
where īs is the confinement factor for the Stokes mode. An expression similar to Eq. 6.28 has been obtained before in theoretical papers on LWI [33]. Note several peculiar features in it, compared to the “usual” Raman physics in existing Raman lasers and amplifiers. First, the gain is not proportional to the Raman inversion n1 – n2 between the initial and final states of the twophoton transition. Instead, there are two terms. Their origin can be seen from inspecting the general structure of Eqs. 6.24 to 6.26. It is clear that in the absence of the drive field, the density matrix element ı32 can be excited only by the first term on the righthand side of Eq. 6.26, which is proportional to the Stokes field and the population difference n2 – n3 on the Stokes transition. This term describes linear absorption of the Stokes field on the transition 2–3 (the second term in brackets in Eq. 6.28). Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_253_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
253
When the drive field is on, there is a second term iȍ d ı*21 on the righthand side of Eq. 6.26 that originates from the coherent beating between the drive field and the polarization ı12 on the transition 1–2. The latter, in turn, is excited by the coherent mixing of the Stokes field and the polarization ı31 on the drive transition 1–3, as described by the second term iȍ*s ı31 on the righthand side of Eq. 6.24. In turn, according to Eq. 6.25 the polarization ı31 is excited by the strong drive field: ı31 § in13 ȍ d / ī31 . As a result, there is a contribution to the polarization ı32 , which scales as ı32 ค ȍd ı*21 ค ȍ d ȍ s ı*31 ค ȍ d 2 ȍ s n13 . It is proportional to the drive field intensity and the population difference on the drive transition n13. This contribution gives rise to the first term in brackets in Eq. 6.28. Second, note the first term iȍ d ı*32 in Eq. 6.24 that describes the shift of the resonances for the Stokes field due to the resonant ac Stark effect. It gives rise to the term  ȍ d  2 / ī*21 in the denominator of Eq. 6.28. The net effect of the strong drive field on the propagation of a weak signal nearly resonant to the transition 2–3 can be described in terms of the splitting of the “bare” state 3 into two new states, “dressed” by the drive (Fig. 6.5). Instead of one resonance at frequency Ȧs = Ȧ32, the weak Stokes signal has two resonances with these states. If all broadenings Ȗij are equal, the dressed states are shifted from the bare state 3 by
Ȧ31 í
E± ǻ = ± 2 ല
( ǻ2 ) + ȍ  2
d
2
§
{
ǻ+
ȍ d 2 ǻ
ȍ d 2 í ǻ
(6.29)
where ǻ = Ȧ31 – Ȧd and the energies of the dressed states E± are counted from the energy of state 1. The last approximate equality in Eq. 6.29 is in the limit of ȍd:
D =
ȍs  1 í ȍd  2
 ȍ s 2 +  ȍ d 2
(6.31)
where ȍ s = ez23 Es / ല. This phenomenon has been called coherent population trapping (CPT) [34]. As a result, one can get transparency for both propagating fields, and the inversionless amplification for one of them if incoherent pumping is present. In principle, this amplification may occur in the absence of any inversion in the system including Raman inversion. However, in practice there is a very narrow range of parameters in which the absence of Raman inversion and the presence of gain for the signal field coexist. In our lasers the Raman inversion is certainly present, because state 1 is close to the ground state of a doped injector and state 2 is relatively shortlived by design. 6.3.2 General properties of the nonlinear dynamics of Raman lasing
Equation 6.28 has been derived by assuming the Stokes signal to be weak and the drive field to be constant along the cavity. In reality, one has to consider the coupled propagation of both fields along the waveguide, taking into account their absorption and nonlinear interaction. Some general features of this process can be seen without solving the equations. Using Eqs. 6.11, 6.24 to 6.26, and the relation between Hy and Ez in the TM mode, one can write the propagation equations for the normalized drive and Stokes field intensities as Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_256_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 256
Chapter Six
ı32 d Is = í Ș s Re I dx iȍ s s
(6.32)
ı31 d Id = í Ș d Re I + gd Id dx iȍ d d
(6.33)
( ) ( )
where Șs =
2 4 ʌ Ȧ s e 2 z23 īs ലȝ s c
Șd =
2 4 ʌ Ȧ d e 2 z13 īd ലȝ d c
and īs and īd are the overlap factors of the Stokes and drive modes with the Raman active region, and gd is the modal gain for the drive field due to the presence of the drive active region (see Fig. 6.8). Offdiagonal density matrix elements for arbitrarily strong fields are given by
ı32 = iȍ s
ı31 = iȍ d
( ( ( (
n23 Is + ī32 Is +
n13 Id + ī31
ī*21ī*31 í n13 Id Ȗ21Ȗ31 ī*21ī*31 Ȗ21Ȗ31
) ) ) )
+
(6.34)
ī*31 Id
ī21ī*32 í n23 Is Ȗ21Ȗ31
ī21ī*32 Id + + ī*32 Is Ȗ21Ȗ31
(6.35)
The normalized intensities are defined by Is ,d = ȍ s ,d 2 /(Ȗ21Ȗ31). In atomic systems it is possible to have very longlived Raman coherence: Ȗ21 > 1, the above equations yield d Is = Ș s ĭ Is dx d Id dx ĭ
(6.41)
= í Ș d ĭ Id + gd Id 싥
n13 Id í n23 Is
(6.42)
Ȗ32 Is + Ȗ31 Id
Population differences n13 and n23 are to be evaluated from the equations for diagonal density matrix elements. There is no conservation law of the ManleyRowe type. In the absence of the drive gain term gdId, Eqs. 6.41 and 6.42 have the first integral, which is different from Eqs. 6.38 but still corresponds to the nonlinear transfer of energy from the drive to the Stokes mode. However, the numerical analysis shows that in this limit ĭ ĺ 0 due to coherent population trapping and saturation effects, so that the coupling between the two fields becomes Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_259_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
259
suppressed. In our QCL system, this condition of strongfield electromagnetically induced transparency (EIT) can occur only when both fields are well above saturation, with intensities greater than 1 MW/cm2. In atomic systems the relaxation rate Ȗ21 of the Raman coherence can be very small, so that the strongcoupling regime Is,d >> 1 and the EIT can occur well below saturation. 6.3.3 Experimental realization of Raman QC laser
Here we consider the first realization of a Raman laser monolithically integrated with a QC laser [23]. To the best of our knowledge, this is the first Raman laser with injection pumping. One period of the Raman laser structure is shown in Fig. 6.8. In our injectionpumped resonant Raman laser, the fundamental radiation and the Stokes radiation are both generated by electronic transitions between confined states in the conduction band of the very same active region of a quantum cascade laser. The typical layout of a QC laser has been modified to include within the same band structure the ȁ scheme of three intersubband transitions designed to produce stimulated Raman scattering of laser radiation. Each period of the laser multistage structure consists of an injector, a drive laser region, and a Raman active section where lasing at the Stokes frequency takes place (Fig. 6.8). The drive section consists of a coupled well’s vertical transition active region, used in the design of stateoftheart midinfrared QC lasers [35], suitably modified for optimum coupling to the Stokes section. The drive is generated across the E76 transition, where state 6 is depleted by resonant LOphonon emission to level 5. The energy of the E13 transition is designed to be detuned by 13 meV from the intersubband resonance Ȧ31. Although the detuning lowers the gain, as shown in Eq. 6.28, we kept it on the order of the 1–3 transition full width at half maximum 2Ȗ31 = 10 meV, in order to decrease resonant absorption for the drive, to minimize the threshold current for the drive and Stokes lasers, and to be able to distinguish between Raman lasing and usual lasing due to population inversion on the transition 3–2. Laser light at 6.7 ȝm generated on the transition 7–6 serves as a resonant optical pump for lasing at the Stokes wavelength of 9 ȝm, corresponding to the twophoton resonance Ȧs = Ȧd – Ȧ21. Resonant absorption of the drive on the transition 1–3 is overcome by amplification in the drive laser section on the transition 7–6, which has 2 times larger dipole moment and larger overall cross section of the stimulated emission. The triply resonant nature of the process makes stimulated Raman scattering very efficient: peak intracavity Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_260_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 260
Chapter Six
fundamental power is only 60 mW at the threshold for Raman lasing, which implies very large material gain coefficient on the order of 2 × 10–5 cm/W per period (6 × 10–4 cm/W for the whole stack of 30 stages) and high efficiency of the nonlinear interaction. Nonlinear conversion efficiency of around 30% has been measured. The devices were based on the InGaAs/InAlAs heterostructure, grown by molecular beam epitaxy latticematched to the InP substrate. Typical emission spectra from ridge waveguide devices are shown in Fig. 6.9a. The pump wavelength (inset) at a heat sink temperature of 80 K is measured to be ȜL = 6.7 m, corresponding very well to the predicted value of ƫȦd = E76 = 186 meV. The Stokes spectrum is peaked
Optical power (arb. units)
1.5
32
1.0
6.6
0.5
0 7.5
6.7
6.8
Wavelength (μm)
8.0
8.5
9.0
9.5
10.0
10.5
Wavelength (μm) (a) Optical power (a.u.)
1.0
76 7΄3΄
32
0.5
0 100
120
140
160
180
200
220
Energy (meV) (b) Figure 6.9 (a) Measured subthreshold emission spectra (black lines) of quantum cascade Raman laser at currents of (from bottom to top) I = 2.43, 2.45, and 2.5 A, offset for clarity. The gray curve is recorded above threshold for Raman lasing (I = 2.6 A). Inset: Fundamental laser emission spectrum at I = 0.8 A. All measurements shown are performed at a heat sink temperature of T = 80 K. The vertical arrow marks the position where the emission from the transition 3–2 would be expected if level 3 were populated by optical pumping. (b) Comparison of electroluminescence (gray curve) and fundamental and Raman laser (right and left peaks, respectively) emission spectra. The vertical arrows indicate the energy of the transitions 3–2, 3–1 and 7ಾ–3ಾ as calculated from the band structure in Fig. 6.1c. All measurements were performed in pulsed operation with a repetition rate of 80 kHz and a pulse width of 100 ns.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_261_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
261
at a wavelength Ȝs = 8.9 m corresponding to the expected value ƫȦs = ƫȦd í E21 = 137 meV, and its narrowing with increased current demonstrates that it is a stimulated process. The onset of Stokes lasing is observed above a threshold current of 2.6 A, as indicated by the appearance of narrow cavity modes centered nears Ȝs. Figure 6.9b shows the electroluminescence spectrum of the same material processed into round mesa devices to prevent feedback from the facets and laser action at the same current density (J 싉 4.5 kA/cm2) as the one in laser devices at threshold for Raman lasing. We can clearly identify the main peak as the pump transition E76, while two lowintensity peaks appear at lower energies, none of which corresponds to the Stokes emission. Raman lasing has been demonstrated in all 15 tested devices. The power output characteristics of one of the devices are displayed in Fig. 6.10. The measured samples exhibit typically two thresholds, the first one around 1 kA/cm2 for the fundamental laser emission and the second one around 4.3 kA/cm2 for the Stokes emission. The three curves shown in Fig. 6.10a represent the IV curve (top curve) and the laser emission turnon of the fundamental radiation (middle curve) and Stokes (bottom curve) radiation. The Stokes laser turnon occurs when the output laser power reaches about 40 mW, and at higher currents the Stokes power reaches about 26% of the fundamental power, where the fundamental emission starts to saturate, as commonly observed in QC lasers at injection levels of several times the threshold current. This should be compared to conversion efficiencies for solidstate Raman lasers that are usually very low ( 10–3), with the exception of ultrahigh Q spherical microcavities (~ 20%) [36] and spinflip Raman lasers in InSb (~ 50%) [37]. Also shown in Fig. 6.10b are the emitted Stokes radiation and fundamental output power as a function of current on a logarithmic scale, to highlight the exponential dependence of the emission below threshold compared with the linear behavior above threshold for both laser lines. Given that the laser facet reflectivity does not change significantly in the wavelength range Ȝ = 6 to 9 m, we can consider the ratio of the emitted powers to be equal to the ratio of the internal power densities, measured by comparing the relative intensities of the laser peaks in spectra acquired over the entire midir range without any optical filtering. From these measurements, the conversion efficiency is estimated to be about 30% at currents of 4.5 A, in good agreement with the value obtained from the powercurrent curves. In response to suggestions by Faist and Colombelli [38], we conducted a detailed investigation to verify that the observed lasing at 9m wavelength is indeed due to coherent optical driving and not due to an accidental electrically pumped transition in the structure. First, we compared devices with identical stripe width very close to each other on the wafer with somewhat different pump thresholds and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_262_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Chapter Six
68 kV/cm
100
Power (mW)
80
15
IV
59 kV/cm
Pump power Stokes power
10
60
40 5
Voltage (V)
262
20 0
0
1
2
3
4
5
0
Current (A) (a)
Power (mW)
100
10
1
Laser Stokes
0.1
0
1
2
3
4
5
Current (A) (b) (a) Peak output power versus current characteristics measured for the fundamental (middle curve) and Stokes (lower curve) emissions at a temperature of 80 K. The upper curve is the IV characteristics. Measurements were performed with a 5kHz repetition rate at a 0.05% duty cycle. (b) Experimental powercurrent characteristics on a logarithmic scale, showing the exponential behavior of the emission close to threshold.
Figure 6.10
slope efficiencies. The data for two representative devices (Fig. 6.11) show that the longerwavelength lasing turns on at the same pump power (which also corresponds to the same intracavity powers for the two devices). This is direct evidence that the 9m lasing results from internal pumping by the shorterwavelength radiation rather than from direct electrical pumping. Second, highreflectivity SiO2/Au backfacet coating was deposited on part of the samples. The resulting change in the threshold between coated and uncoated devices for the pump lasing (6.7 m) and the Stokes lasing at 9 ȝm has been measured. The threshold current for the pump laser is simply proportional to the sum of the waveguide and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_263_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
263
Different samples, same stripe width
0.08
0.008 D2959A5 Bot(2)  Pump
0.07
0.007
D2959A5 Bot (2)  Stokes
0.06
0.006
D2959A5 Top(2)  Stokes
0.05
0.005
0.04
0.004
0.03
0.003
0.02
0.002
0.01
0.001
0
Stokes peak power (W)
Pump peak power (W)
D2959A5 Top(2)  Pump
0 0
0.5
1.0
1.5
2.0
2.5
3.0
3.5
4.0
4.5
Current (A) Powercurrent curves for two representative devices 1 mm apart in the wafer, denoted by filled and open squares, respectively. There are two curves for each device, corresponding to the pump (upper curve) and Stokes (lower curve) emission. Pump threshold difference is ~80 mA, Stokes threshold difference is ~0.5 A. Both Stokes lasers turn on at the same output power in both devices: ~35 mW.
Figure 6.11
p mirror losses: Jp ค Į wp + Įm . If the longerwavelength laser at 9 m is indeed optically pumped, its gain must be proportional to the intracavity energy density of the pump field Wpump
gs
ค W pump ค
JĲ p
ค
J p Į wp + Įm
which is proportional to the injection current times the pump photon lifetime Ĳp. This lifetime is inversely proportional to the total pump losses. The superscript p in the losses in the equation above refers to the pump. From this relation we obtain that the current at Raman threshold scales as
Js
ค gs(Įwp + Įmp) ~ (Įws + Įms )(Įwp + Įmp)
where the superscript s refers to the Stokes field. p s Both Į m and Įm decrease in the coated samples approximately by onehalf, according to Įm =
1 ln L
1 R1 R2
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_264_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 264
Chapter Six
where the cavity length L ~ 1.25 mm, reflection factors are R1 = R2 = 0.27 in the uncoated sample, and R1 = 0.96 in the coated one for both wavelengths. Therefore, one should expect a greater decrease in the threshold current for the optically pumped Raman laser compared to an electrically pumped laser emitting at the Stokes wavelength Ȝs = 9 m. The measurements show that the reduction in threshold is ~12% to 15% for the pump radiation and ~25% to 28% for the Stokes radiation. These data are consistent with the optical pumping hypothesis and tend to rule out electrical pumping as the origin of the longwavelength lasing. We have also performed measurements of the corresponding changes of the slope efficiency and power. These data clearly show that after application of the coating, the slope efficiency of the Stokes lasing increases by a factor of 5.5 to 6, significantly more than that of the pump laser, which increases by a factor of 1.6. These results also point in the direction that the 9m lasing arises from internal optical pumping rather than electrical. However, a quantitative analysis predicts the lower magnitude of the effect. Third, the rolloff of the pump and Stokes lasers occurs at the same current, which also suggests a strong correlation between them and contradicts the hypothesis of unrelated electrically pumped lasers. Finally, analysis of the band structure of Raman devices does not reveal any transition that could have a significant population inversion in the whole range of applied voltages and could be a potential candidate for the electrically pumped laser at 9 m. 6.3.4 Theoretical modeling of Raman QC laser
The simplest model of a system shown in Fig. 6.8 should include states 1, 2, 3, 6, and 7 coupled by two laser fields. We assume that the injector states remain undepleted and do not need to be included directly. This assumption is believed to work reasonably well for QC lasers; it can be easily dropped if necessary. Then the density matrix equations for the populations read n1 = j1 + r31n3 + r21n2 í r12n1 í r1(n1 í n1T ) í 2 Im (ı31ȍ*d ) t
(6.43a)
n2 = j2 + r32n3 + r12n1 í r21n2 í r2(n2 í n2T ) í 2 Im (ı32ȍ*s ) t
(6.43b)
n3 = í r3n3 + 2 Im (ı32ȍ*s ) + 2 Im (ı31ȍ*d ) t
(6.43c)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_265_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
265
n6 = j (1 í Ș ) + r76n6 í r6(n6 í n6T ) í 2 Im (ı76ȍ *L) t
(6.43d)
n7 = j Ș í r7n7 + 2 Im (ı76ȍ *L) t
(6.43e)
Here j is the total current density and j1,2 are the densities of current flowing through states 1 and 2. We will assume that j1 + j2 = j, although this may not necessarily be the case. The factor Ș is the efficiency of injection to the upper drive laser state 7; we again assume that the rest of the current goes to state 6, although this may not be the case. Quantities niT are equilibrium populations in the absence of current injection and the optical fields. Equilibrium populations of states 3 and 7 are neglected. The relaxation rate ri is the inverse time during which state i reaches equilibrium with the injector; we assume that the injector remains undepleted and has Fermi distribution of electrons at temperature T. The relaxation rate rij is the inverse time of the transition from state i to state j. Then we need Eqs. 6.24 through 6.26 for the offdiagonal density matrix elements that have to be supplemented by the equation dı76 + ī76ı76 = iȍ Ln67 dt
(6.44)
for the optical polarization on the laser drive transition. Note that since the dipole moments of the transitions 7–6 and 3–1 are different, the Rabi frequencies ȍ L = ez67 Ed / ല and ȍ d = ez13 Ed / ല are also different despite the fact that the drive field is the same. It is the Rabi frequency—not the amplitude of the field itself—that determines the strength of the coupling between the field and the transition of interest. This provides an important flexibility in designing the integrated devices: The same field interacts differently with the drive laser transition 7–6 and with the drive transition 3–1 in the Raman cascade. Finally, we need two coupled equations for the drive and Stokes field amplitudes that can be written as 2 ȍs 2 ʌ iȦ s e z z23 ī s ı32 = x cȝ s ല
(6.45)
2 2 ȍd 2 ʌ iȦ d e 2 z13 2 ʌ i Ȧ d e 2 z67 ī d ı31 + ī Lı76 = x cȝ d ല cȝ d ല
(6.46)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_266_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 266
Chapter Six
The factor īL is the transverse overlap of the drive mode with the drive laser active region; for our structure its value is very close to īd. However, in the alternative design where the stacks of the Raman and drive laser active regions are separated, these two factors can be very different. The density matrix elements ıij on the righthand sides of Eqs. 6.45 and 6.46 are averaged with the transverse mode distribution over the cross section of the active layer, according to Eq. 6.11. The above set of equations 6.24 to 6.26 and 6.43 to 6.46 can also be used to describe the shortpulse regime after replacing /x ඎ /x + ( ȝ / c )(/t ). In this chapter, we are interested in the continuouswave or longpulse regime when the pulse duration is much longer than all relaxation times; therefore, we may put all time derivatives equal to zero in Eqs. 6.24 to 6.26 and 6.43. An important feature of our system compared to many previous studies of LWI is that it is open: The sum of populations of states 1, 2, and 3 is not conserved. One can control them quite efficiently by a combination of scattering and tunneling processes, i.e., through the control of electron transport. This adds flexibility and significantly broadens the range of parameters under which the lasing is possible, compared to simple threelevel schemes. There are several parameters in the above equations that we know with a large degree of uncertainty or do not know at all: the electron temperature, relaxation rates Ȗij of the offdiagonal density matrix elements, and the efficiencies of current injection. We checked the sensitivity of the results to these parameters. It was found that the drive laser threshold is quite sensitive to the thermal population n6T of the lower laser state 6 and the efficiency Ș of injection to the upper state 7. As expected, it increases with increasing n6T and increases sharply with decreasing Ș—by a factor of 3 when Ș changed from 1 to 0.8. The Stokes threshold is not sensitive to n6T, but increases significantly (by 50%) with the above decrease in Ș. The Stokes threshold is also not very sensitive to the change in the injection efficiency to states 1 and 2: It increases by only 20% when j2/j increases from 0 to 1. The reason is that in our structure state 1 is very close in energy to the ground state of the doped injector; therefore it always stays filled. State 2 is elevated above the Fermi level of the injector by only 34 meV, so its thermal population is also nonnegligible. Therefore, the variation in the distribution of the injection current over these states does not lead to strong changes in the Stokes threshold. At the same time, the latter shows a significant dependence from the thermal population of state 2 and the line widths of all transitions. This is clear from the expression for the gain spectrum in Eq. 6.28. It is also clear from Eq. 6.28 that having a large population of state 1 and narrow line widths is beneficial for the Stokes laser. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_267_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
267
Figure 6.12 shows the output powers of the drive and Stokes lasers calculated for Ș = 1, j2/j = 0.2, and electron temperature T = 10 meV. The total nonresonant losses for the drive and the Stokes modes were taken to be 12 and 13 cm–1, respectively, according to the measurements and in agreement with calculations of the waveguide and cavity losses for TM00 modes. The line widths (FWHM) were assumed to be 8 meV for transitions 1–3 and 2–3, and 5 meV for transition 1–2. For this choice of parameters the agreement with experimental values of both thresholds is very good. Increasing Ȗ21 by a factor of 2 increased the Stokes threshold by 30%. Decreasing the electron temperature by 50% decreases the Stokes threshold by 25%, while the same relative increase in temperature boosts the Stokes threshold by more than a factor of 2. Figure 6.6 shows the gain spectrum for the Stokes field. The peak gain is achieved close to the twophoton resonance, because the Stark shift is very small: The Rabi frequency of the drive is only about 2 meV. Figure 6.13 shows this peak value of the gain as a function of current. Experimental LI curves (Fig. 6.10) show the rolloff of the drive laser power at a current several times above the drive threshold. Such rollover is not seen in our simulations. It is unlikely to result from the nonlinear interaction between the drive and Stokes fields. Such interactions are included in the model, but they become important at much higher Stokes powers. A plausible hypothesis is that the drive laser deteriorates with current due to decreasing efficiency of injection to state 7, which can originate from increasing misalignment between this state and the upstream injector. We can model this effect by including the dependence of efficiency on current Ș = 1 í aj, where a is a free parameter. The result for a = 1 indeed shows the behavior similar to that of the experimental curve, although there is not much predictive power in such empirical modeling. Another feature of the measured lightcurrent curves that we were not able to reproduce accurately is their slope. In general, the slope is much more sensitive to the uncertainties in the above input parameters
Power (mW)
100
50
1
2
3
Current (A)
4
Figure 6.12 Calculated drive (upper curve) and Stokes (lower curve) powers as functions of injection current.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_268_03/23/2006 Raman Injection and Inversionless Intersubband Lasers
Maximum gain (cm1)
268
Chapter Six
30 20 10 2
3
4
5
6
7
Current (A)
Figure 6.13
Maximum gain of the Stokes mode as a function of injection current.
than are the laser thresholds. The modeling predicts considerably higher power for both lasers compared to the measurements. Also, the drive laser curve in Fig. 6.12 demonstrates an increase in the slope when the Stokes laser turns on, while we observed only a decrease in the slope for all our simulations. An interesting question involves the choice of the optimal detuning ǻ of the drive field. The denominator in Eq. 6.28 is minimized when all detunings are equal to zero. At the same time, at zero detuning the resonant absorption of the drive field on the transition 1–3 is maximized, leading to an increase in both the drive and Stokes threshold. Figure 6.14 shows the dependence of both thresholds on the drive field detuning. It is clear that the designed value of ǻ = 13 meV is close to the optimum. Finally, both Fig. 6.6 and our experimental results in Fig. 6.9 indicate that there is no net gain or conventional lasing on the transition 2–3 at the current corresponding to the Stokes threshold. However, for the drive field intensities about 2 times higher than those reached in these experimental devices, the optical pumping should lead to population
Current at Stokes and pump threshold versus detuning of the drive Pump
5 4.5 4 3.5
2.5
10
20
30
Δ (meV) (a)
40
Current (A)
Current (A)
Stokes 2.5 2 1.5 10
20
30
Δ (meV)
40
(b)
Figure 6.14 Threshold current for (a) Stokes and (b) drive field as a function of the drive
field detuning.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_269_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
269
inversion n3 > n2. In this case one could expect lasing to start around the frequency Ȧs = Ȧ32. The laser modes will experience strong electrical and optical coupling, resulting in complex multimode dynamics. To summarize, our calculations demonstrate reasonable robustness and good agreement with experiment with respect to laser thresholds. The details of the powercurrent curves turned out to be more difficult to reproduce, and their modeling has a low predictive power. 6.3.5
AntiStokes Raman laser
The physics of resonant antiStokes generation is similar to that of the Stokes case, but the specific implementation in the QCL structure is of course very different. Figure 6.15 shows one example of such a design. Here the electrons need to be injected to a relatively longlived initial state 2 and drained from the final state 1 by, e.g., resonant optical phonon emission, in order to maintain a large population difference on the drive transition 2–3 and decrease the resonant absorption of the signal on transition 1–3. The expression for the gain spectrum is similar to Eq. 6.28, after permutation of indices and changing of the phases of complex detunings: g1 = 2 gM = × Re
{
2 4 ʌ Ȧ s e z z13 īs ലcȝ s
ī31 +
1 ȍ  d 2 / ī21
 ȍ d 2 (n2 í n3)
ī21ī32
í (n1 í n3)
}
(6.28a)
Here ȍd = ez23 Ed / ƫ and ȍs = ez13 Es / ƫ are the Rabi frequency of the drive and signal mode, respectively; the subscript s now relates to the antiStokes mode and means “signal” in order to avoid introducing new notation. The above analysis of the gain optimization and the nonlinear dynamics of the Stokes lasing is directly applicable here. Some practical benefits are discussed below.
3
Ed
Es
2 1
Figure 6.15
A schematic of the antiStokes laser.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_270_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 270
Chapter Six
One feature of the antiStokes laser is that initial state 2 of the Raman transition is elevated, and its population is mainly controlled by injection current. State 1 should stay as empty as possible, which means that it should also be elevated above the ground state of the injector. This puts some additional constraint on the design, but also adds flexibility in manipulating the populations by current. 6.3.6
Optically pumped laser
In the ȁ scheme of Figs. 6.8 and 6.15, and in all other schemes in Fig. 6.2, the role of the drive field is twofold. On one hand, it helps to excite the Raman coherence between the initial and final states of the twophoton transition (states 1 and 2 in the ȁ scheme) which creates maximum gain at the twophoton resonance Ȧs = Ȧd í Ȧ21. (We will discuss the Raman Stokes scheme for definiteness, although the same reasoning applies to all other systems.) On the other hand, it transfers populations to states 3 and 2 by onephoton absorption on the drive transition with subsequent incoherent relaxation. Both effects are included in the expression 6.28 for the gain and similar equation 6.51 for the cascade scheme below. Under certain conditions, this optical pumping creates population inversion on the Stokes transition 3–2, and the second term in brackets in Eq. 6.28 may become dominant, while all effects related to the twophoton transitions and Raman coherence become less significant. This gives rise to the gain peaked at the frequency Ȧs = Ȧ32 and conventional lasing with inversion on this transition. Of course, an intermediate case is also possible, when both contributions are comparable. A natural question to ask is, What are the optimal conditions for one of these contributions to become dominant? This question has been addressed in Ref. 39 on the basis of simplified rate equations and an approximate expression for the Raman gain, valid for large detunings of the drive field from the transition 1–3 or very low drive powers, when the depletion of state 1 is neglected and only the twophoton Raman transitions through a virtual state are taken into account. By using Eqs. 6.24 to 6.26, 6.28, and 6.43, it is easy to consider the general case of arbitrary detuning and field strength. The population differences n13 and n23 that enter the gain expression 6.28 can be expressed as a function of the optical drive intensity as n13 =
n1T + j1 / r1 1
1 + I [ 1 + ( r3 í r31 / r1)
n23 = n 2T +
(
j2 r32 í I n13 1 í r2 r2
)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_271_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
271
where I = 2  ȍ d 2 Ȗ31 / r3(Ȗ231 + ǻ2) is the drive intensity normalized by saturation intensity, and we neglected the term r21n2 í r12n1 in Eqs. 6.43 for simplicity. This term is small in our case; it can be easily included if necessary. In the experimental device described in Ref. 23, state 2 was only 34 meV above the Fermi level of the injector. Also, there was inevitable current injection into this state, although its rate was difficult to quantify. Even with small injection, we had n23 § n2T > In13 at the signal threshold for electron temperature above 10 meV. As a result, the gain was primarily due to the excitation of Raman coherence, and lasing started at the Stokes frequency. Theoretically, we can consider a hypothetical structure optimized for the optical pumping, in which state 2 has negligible equilibrium population and current injection, and very short lifetime: r2 >> r32. In this case the transition 3–2 can be inverted by the optical pumping: n32 § In13. Exactly at resonance, when ǻ = 0, the gain in Eq. 6.28 has a single maximum at Ȧs = Ȧ32 where both terms in Eq. 6.28 are positive and the ratio of the second to the first term is equal to ȍ d 2 n13 / (Ȗ21Ȗ31n23) = r3 / Ȗ21. This ratio is generally less than 1, although the transition 2–1 can be forbidden and have a relatively narrow line width. Very far from resonance, when ǻ is much larger than all line widths and the Rabi frequency of the drive, the gain at the Stokes frequency is equal to
 ȍ d 2 n12
g (Ȧ s = Ȧ d í Ȧ21) 싌 Ș
Ȗ21ǻ2
The gain at the frequency of the transition 3–2 is g (Ȧ s = Ȧ32) = Ș
 ȍ d 2 n13 Ȗ32ǻ
2
(
Ȗ31 í1 r3
)
Note that the first term in Eq. (6.28) is negative at this frequency, contributing the í1 term in the above expression. Here the factor 2 Ș = 4 ʌ Ȧ32e 2 z32 ī s / (ലȝ s c ). The ratio of the two peak gains is g (Ȧ s = Ȧ d í Ȧ21) g (Ȧ s = í Ȧ32)
=
Ȗ32 Ȗ21(Ȗ31 / r3 í 1)
When all line broadenings are equal, this ratio is about 0.3 to 0.5 for realistic laser structures. Therefore, in a structure optimized for the optical pumping, Raman gain is always lower by a factor of 2 to 3, and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_272_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 272
Chapter Six
lasing is expected to start at the frequency of the transition 3–2. Note that this conclusion depends sensitively on the relaxation rate of the Raman coherence Ȗ21, as should be expected. If this rate is low, Raman gain can win. 6.4
Vertical Cascade Schemes
Now we turn to other threelevel laser schemes shown in Fig. 6.2. Among these, the cascade, or ladder, schemes in Fig. 6.2c and d turned out to be of the greatest potential importance for integration with QC lasers. The most interesting and potentially useful feature of these cascade schemes is that when the drive field is tuned to resonance to the drive transition 2–3, the coherent twophoton contribution to the signal gain is positive when there is population inversion on the drive transition and is negative otherwise. This pattern is reversed for large detuning of the drive, when, however, the gain is small. Therefore, it has been suggested in Ref. 6 that one can use the threelevel cascade scheme for simultaneous generation of the drive field on the inverted transition 3–2 and inversionless lasing on the transition 2–1. Then one does not need a separate active region for generation of the drive field. This saves space in the laser core, maximizes the modal overlap, eliminates drive absorption in the active region for the signal, and eliminates the problem of tuning the drive field to resonance with the drive transition. Of course, the design similar to the one in Fig. 6.8, when these two active regions are separate, is always a possibility. Two possible arrangements for a completely integrated design are sketched in Fig. 6.16a and b. In the scheme of Fig. 6.16a there is population inversion between states 2 and 1 due to a very fast depletion of state 1 and the relatively long lifetime of state 2. The laser field generated on the transition 2–1 serves as a coherent drive for the inversionless lasing on a fastdecaying transition 3–2. Block arrows show the injection current of electrons. In the scheme of Fig. 6.16b the roles of transitions 1–2 and 2–3 are interchanged. Now the transition 3–2 is inverted and supports the drive laser generation, while the signal is generated on the fastdecaying transition 1–2 in the absence of population inversion on this transition. Note that an attempt to have lasing with inversion on both transitions 3–2 and 2–1 reported in Ref. 14 resulted in lasing on only one of these transitions. The physics of the two schemes is similar. In both the drive field is generated automatically at resonance with the drive transition. As a result, the peak gain is also reached at resonance with the signal transition. Obviously, there is no problem with resonant absorption of the drive that has been a serious factor for the ȁ scheme. This is a very Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_273_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
3
3
Signal
Fast decay
2 Slow decay
Pump laser
Slow decay
Pump laser
1
273
2 Fast decay
1 (b)
(a)
Two cascade schemes showing gain without inversion on the signal transition and lasing with inversion on the drive transition.
Figure 6.16
important advantage of the cascade configuration. Below we concentrate on the scheme shown in Fig. 6.16b. The set of the density matrix equations for this scheme is given by ı21 + ī21ı21 = iȍ s n12 + iȍ*d ı31 dt
(6.47a)
ı31 + ī31ı31 = iȍ d ı21 í iȍ s ı32 dt
(6.47b)
ı32 + ī32ı32 = iȍ d n23 í iȍ*s ı31 dt
(6.47c)
n1 = r31n3 + r21n2 í r21n1 í r1(n1 í n1T ) í 2 Im (ı21ȍ*s ) t
(6.48a)
n 2 = j (1 í Ș ) + r32n3 + r12n1 í r2(n2 í n2T ) t + 2 Im (ı21ȍ*s ) í 2 Im (ı32ȍ*d ) n3 = jȘ í r3n3 + 2 Im (ı32ȍ*d ) t
(6.48b)
(6.48c)
where ī32 = Ȗ32 + i (Ȧ32 í Ȧ d ) ī31 = Ȗ31 + i (Ȧ31 í Ȧ d í Ȧ s ) ī21 = Ȗ21 + i (Ȧ21 í Ȧ s )
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_274_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 274
Chapter Six
Here ȍd = ez23 Ed / ƫ and ȍs = ez12 Es / ƫ are the Rabi frequency of the drive and signal mode, respectively, and Ȧd and Ȧs are frequencies of the drive and signal modes, respectively. All other notations are the same as in Eqs. 6.43. Wave equations for the field amplitudes are simpler than in the case of Raman generation, because there is no separate active region for the drive field. Most importantly, there is no absorption of the drive in the active region for the signal: 2 ȍ s 2ʌiȦ s e 2 z12 ī s ı21 = x cȝ s ല
(6.49)
2 ȍ d 2ʌiȦ d e 2 z23 ī d ı32 = x cȝ d ല
(6.50)
The smallsignal gain is given by the expression generally similar to the one in Eq. 6.28: g1 = 2gM = × Re
{
2 4ʌȦ s e 2 z12 īs
ī21 +
ലcȝ s 1  ȍ d  2 / ī31
 ȍ d  2 (n3 í n2) ī31ī32
í (n1 í n2)
}
(6.51)
An example of the gain spectrum is plotted in Fig. 6.17 for the parameters corresponding to a real QCL structure, currently under investigation. The maximum gain is reached exactly at resonance, when all īij are real and equal to Ȗij. Similarly to the Stokes generation, resonant absorption of the signal can be overcome by a twophoton coherence term proportional to the population difference on the drive transition and the drive intensity. However, in the present case, population inversion of the drive transition is required. There is not much flexibility in controlling the population difference on the drive transition and the resulting gain. In the linear approximation with respect to the signal field, the population inversion n32 is fixed at its value on the drive laser threshold. For a homogeneously broadened transition n32 =
cȝ d ലȖ32Į d 2 4ʌȦ d e 2 z23 īd
(6.52)
where Įd is the total cavity losses for the drive mode. The drive field intensity is given by Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_275_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
275
Gain, cm1 8 6 4 2 30
20
Figure 6.17
10
2
10
20
30
ωs  ω 21 , meV
Gain in the scheme of Fig. 6.16b.
( )
n 32 í1  ȍ d 2 =  ȍ dsat  2 n32
(6.53)
sat where  ȍ d  ~ r2Ȗ32 is the value of the Rabi frequency that saturates the transition 2–3. It is a cumbersome function of relaxation rates. In Eq. 6.53, n 32 is the population inversion supported by injection pumping in the absence of both drive and signal field. One can see from the above expressions that as long as  ȍ d  싨 Ȗ21Ȗ31 and onephoton absorption due to n12 is smaller than the twophoton term, the signal gain increases with current proportionally to n 32. The factor ȍ d 2 / Ȗ31Ȗ32 before n32 in brackets in Eq. 6.51 is smaller than or on the order of 1. Therefore, to overcome the resonant absorption on the transition 1–2 one needs n32 > n12. This means (1) that state 1 cannot be the ground state and (2) that the threshold for the drive laser should not be too low, so there is a tradeoff between the drive and signal lasers. When the opposite inequality is satisfied and the drive field is very strong, the factors ȍ d 2 in the numerator and denominator of Eq. 6.51 cancel each other, and the ratio of the signal gain to signal losses becomes equal to 2 ȝ d Ȧ s z12 īs Įd g1 § >1 2 ī Į Įs ȝ s Ȧ d z23 d s
(6.54)
where the last inequality is required for lasing. This inequality seems to be easy to satisfy when Ȧs > Ȧd. In the opposite case of the frequency downconversion, all ratios in Eq. 6.54 except the ratio of the dipole moments are smaller than or on the order of 1; therefore one needs z12 to be significantly larger than z23 in order to reach the lasing threshold for the signal.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_276_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 276
Chapter Six
The above semiqualitative conclusions are confirmed by numerical results. We have also found that by the time the signal laser threshold is reached, the population of state 3 is greater than or very close to the population of state 1. This means that the twophoton Ramantype inversion is usually required for lasing. This is not surprising, since the condition n32 > n12 mentioned above corresponds to Raman inversion n3 > n1. If the transition 1–3 has a strong dipole moment, one can get lasing on this transition as well. Two signal modes resonant to the transitions 1–2 and 1–3, respectively, can actually help each other to turn on. The analysis of the amplification of such a bichromatic signal presented in Ref. 6 shows that in this case the threshold can be significantly lower than that for a monochromatic signal. However, one needs to put extra effort into the design to provide fast depopulation of both state 1 and state 2 simultaneously and strong enough dipole moment on the transition 1–3. 6.5
Practical Considerations and Benefits
The experiment reported in Ref. 23 was mainly a proof of principle. The natural question to ask is, Does this kind of device have any potential benefits compared to standard QC lasers? One can envision at least several benefits that are usually associated with nonlinear optical sources: 1. Generation at wavelengths that are not easily accessible for QC lasers in general, or within a given material system: for example, in the terahertz range or at short wavelengths below 3 to 4 m. 2. Significantly better tunability and wavelength agility compared to standard QC lasers. 3. Higher operating temperature, which is essentially defined in our devices by the operating conditions for the drive laser. The drive wavelength can be chosen to fit within the “sweet spot” of the QC lasers (7 to 9 m for InGaAs/AlInAs structures) where they are most powerful, efficient, and capable of the continuouswave room temperature operation. 4. Other benefits, such as small beam divergence or generation of light with interesting statistical properties, e.g., squeezed or entangled light. Below we consider some examples from the above list.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_277_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
277
6.5.1 Frequency downconversion to the terahertz region
Inversionless or Ramantype lasing could be especially valuable in the situations in which the population inversion is difficult to reach. One example of such a situation is the lasing in the terahertz spectral region. With decreasing energy separation between subbands it becomes increasingly difficult to provide selective injection to the upper laser state, and selective depopulation of the lower state and to prevent backfilling of the lower state. These factors limit operation of existing terahertz QC lasers to cryogenic temperatures. The nonlinear optics may provide an alternative to usual lasing. Two possible ȁtype schemes for terahertz generation are shown in Fig. 6.18. In the scheme of Fig. 6.18a, the separation between states 2 and 3 is below the optical phonon energy, and the drive field is generated in a separate active region. If these states are high enough above the ground state, their population is only due to the optical pumping. They are likely to have comparable lifetimes; therefore, the transition 2–3 has the population difference close to zero or even inverted due to the selective optical pumping to state 3. The twophoton term in the gain expression in Eq. 6.28 is proportional to the population difference n1 – n3 that can be quite large if state 1 is the ground state or close to it. Therefore, potentially the Stokes gain in the terahertz range can be much larger than the gain for standard lasing with inversion on the transition 2–3 and much larger than the gain in the midir QC laser. Plugging the typical numbers into Eq. 6.28, we obtain the following scaling formula for the gain: g=
( z32 / 5 nm)2(n13 / 3 × 1016cmí3) (ī s / 0.3) (Ȝ / 100 ȝm) (Ȗ32 / 2 meV)
3 Es
( )
1 130 cmí1 Ȗ21Ĳ3
3 2
Es
Ed
2 1 (a)
Ed
1 (b)
Figure 6.18 Terahertz Raman lasing (a) at resonance with the terahertz intersubband transition and (b) at large detunings from the midinfrared intersubband transition.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_278_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 278
Chapter Six
This estimate is obtained for the optimal value of the average drive intensity in the Raman active region ȍ d 2 Ĳ3/Ȗ31 ~ 1 corresponding to the drive power of ~50 to 100 mW. Of course, care should be taken to avoid too strong absorption of the drive on the transition 1–3, especially when this field is close to resonance. In particular, the dipole moment of the laser transition in the drive active region should be larger than z13 by at least a factor of 2. In the scheme of Fig. 6.18b, the transition 2–3 may be in the midir, but the drive field is far detuned from state 3 to shift the Stokes wavelength to the terahertz region. An advantage of this scheme is negligible resonant absorption of the drive field. However, the gain is smaller in this case, which imposes more stringent limitations on the maximum terahertz losses in the waveguide. For the cascade schemes in Fig. 6.16, the requirement imposed by Eq. 6.54 makes it very difficult to reach the threshold when the ratio of the signal to drive field frequencies is on the order of 0.1 or less. Therefore, it makes sense to have separate active regions for the drive and signal lasers. Population inversion on the drive transition in the cascade scheme is still required; however, its magnitude and the drive field amplitude are not controlled by the drive lasing threshold. As a result, the gain can be significantly enhanced, although extra space is needed for the drive active region. The main challenge with realization of the Ramantype terahertz laser is a more complicated waveguide design. The waveguide needs to accommodate both midir and terahertz modes and to provide a good overlap between them. Probably the simplest way to achieve it is to have a doublemetal or surfaceplasmon terahertz waveguide [40–43] and group the active region for the drive and Stokes fields in two separate stacks. Then the whole Raman stack may be an injectorless doped multipleQW region or a superlattice, since we do not need any current injection to excited states (and actually no current at all) to obtain Raman Stokes lasing. The Raman active region needs only optical pumping. The injectorless design saves space in the waveguide and helps to increase the optical confinement factors; see also Ref. 44. One example of such a design is shown in Fig. 6.19. The terahertz losses are inevitably higher than in terahertz QC lasers, because both active regions must be doped in the range of 1016 cm–3 to provide high gain for both the drive and the Stokes fields. Typical numbers in the devices we modeled range between 40 and 100 cm–1. These losses are expected to be compensated by a higher gain.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_279_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
279
0
Cladding
4
Drive laser active region Raman active region
8 12
InP substrate
Figure 6.19 A sketch of the InGaAs/AlInAs Raman terahertz laser with a doublemetal waveguide and separately stacked active regions for the drive and Stokes laser. Transverse profiles of the magnetic fields squared of the midir drive (Ȝd = 7 m) and terahertz Stokes (Ȝs = 70 m) laser modes are shown with dashed and solid lines, respectively. Metal layers are shaded.
6.5.2
Frequency upconversion
Frequency upconversion is in general easier to realize than downconversion, because freecarrier losses decrease with frequency, and there is no need in a special waveguide design. The practical motivation is the possibility to shift the operating frequency to the region close to the band offset of a given material system, when the usual lasing becomes difficult to achieve. For the InGaAs/AlInAs material system, this means lasing at wavelengths shorter than about 4 to 5 ȝm, although lasing at wavelengths as short as 3.5 m [45] and room temperature pulsed operation at ~3.8 m [46] has been demonstrated in straincompensated heterostructures. The antiStokes scheme shown in Fig. 6.15 is suitable for this purpose. As is clear from the figure and Eq. 6.28a, the upper state 3 can be arbitrarily close to the band offset or even in the continuum, because its population is unimportant. There is no need to provide resonant tunneling to the highlying state 3; therefore, almost full band offset can be utilized. Moreover, one can implement this scheme for the frequency upconversion into the nearinfrared range by using heterostructures with large conduction band discontinuity, such as InGaAs/AlAsSb, in which the presence of lowlying L and X valleys creates a fundamental problem for conventional injectionpumped QC lasers. Evidently, lateral valleys are not a problem for the optically pumped Raman process that does not require any electron current through the excited state 3. 6.5.3
Tunability issues
Conventional QC lasers are based on resonant tunneling structures. They “resist” any tuning by Stark effect above laser threshold, after the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_280_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 280
Chapter Six
alignment between the injector and the upper laser state is reached. In practice, QC lasers can only be tuned over a limited range by changing the temperature or using an external cavity. Tunability in conventional Raman lasers or amplifiers has been associated with tuning the external optical pump, while the amount of frequency shift has remained fixed and determined by the phonon frequency. Here we have an opposite situation: The drive laser serving as an optical pump for the Raman laser is internally generated, and its tunability is limited; at the same time, the Raman shift is not fixed. It is determined by the energy separation between subbands denoted by 1 and 2 in Fig. 6.8 or 6.15. If the transition 1–2 is diagonal in space (which is a desirable feature for the Raman laser anyway), its energy can be efficiently tuned by the electric field. To increase the electric tuning range and flexibility, the Raman active region should be grouped in a separate stack from the drive laser, so that it can be independently contacted and biased. This design is shown in Fig. 6.20. Note that the device is expected to generate TM1 modes that have zero field at the position of a strongly doped side contact layer, thus minimizing the losses. Also, the TM1 mode provides better confinement factors and the overlap of the drive field with the Raman region. The Raman active region of the device in Fig. 6.20 can be an injectorless stack of coupled QWs, such as shown in Fig. 6.21. This structure has large dipole elements z13 = 15 nm and z23 = 14 nm, while the transition 2–1 is diagonal in space and partially suppressed. Changing the electric field from 0 to 15 kV/cm shifts the Stokes frequency by as much as 15 meV, or by 120 cm–1. At the same time, the frequency detunings of both drive and Stokes fields from their respective vertical transitions 1–3 and 2–3 remain practically unchanged: Their shift is only 3 meV. The dipole moments of these transitions are also changed very little — by 0.2 nm. Moreover, these 0
Cladding
2
Drive section
4 8
Substrate
6
Raman section
10 Figure 6.20 Design of a broadly tunable Raman laser with independent biasing of the drive and Raman sections. Also shown are the magnetic field squared of the TM1 mode (solid line) and TM0 mode (dashed line) at the drive laser wavelength of 6 m.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_281_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
281
0.8
Energy
0.6
0.4
3 2
0.2
1 0 400
300
200
100
0
Position Figure 6.21 One stage of the Raman active region in an InGaAs/AlInAs structure. The
drive field (solid arrow) is nearly resonant to the transition 1–3, while the Stokes field (dashed arrow) is generated at frequency Ȧs = Ȧd í Ȧ21 and close to resonance with the transition 2–3.
small changes in the detunings and dipole moments can partially compensate one another in expression 6.28 for the Raman gain. Therefore, the electric tuning of the Stokes field is not accompanied by a significant modulation of the output intensity. This is a very important advantage of the proposed broadly tunable laser. 6.6 Acknowledgments It is our pleasure to acknowledge numerous helpful discussions with our colleagues and collaborators M. Belkin, R. Colombelli, J. Faist, C. Gmachl, O. Kocharovskaya, V. Kocharovsky, O. Malis, Y. Rostovtsev, M. Scully, C. Sirtori, A. Tredicucci, and B. Williams. This work has been supported by the Air Force Office for Scientific Research and the National Science Foundation. References 1.
J. Faist, F. Capasso, D. L. Sivco, C. Sirtori, A. L. Hutchinson, and A. Y. Cho, Science 264, 553 (1994).
2.
O. Svelto, Principles of Lasers, Plenum Press, New York, 1998.
3.
M. O. Scully and M. S. Zubairy, Quantum Optics, Cambridge Univ. Press, U.K., 1997.
4.
J. Mompart and R. Corbalán, Quant. & Semiclass. Opt. 2, R7 (2000).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_282_03/23/2006 Raman Injection and Inversionless Intersubband Lasers 282
Chapter Six
5.
A. B. Matsko, O. Kocharovskaya, Y. Rostovtsev, G. R. Welch, A. S. Zibrov, and M. O. Scully, Adv. in Atom., Mol. and Opt. Phys. 46, 191–242 (2001).
6.
A. A. Belyanin, C. Bentley, F. Capasso, O. Kocharovskaya, and M. O. Scully, Phys. Rev. A64, 013814 (2001).
7.
J. Khurgin and E. Rosencher, IEEE J. Quantum Electron. 32, 1882–1896 (1996).
8.
J. Faist, C. Sirtori, F. Capasso, et al., Quantum interference effects in intersubband transitions, in Intersubband Transitions in Quantum Wells: Physics and Device Applications I, H. C. Liu, and F. Capasso (eds.), Academic Press, San Diego, 2000.
9.
W. W. Chow, H. C. Schneider, and M. C. Phillips, Phys. Rev. A68, 053802 (2003).
10.
M. K. Gurnick and T. A. De Temple, IEEE J. Quantum Electron. 19, 791 (1983).
11.
M. M. Fejer, S. J. B. Yoo, R. L. Byer, A. Harwit, and J. S. Harris, Phys. Rev. Lett. 62, 1041 (1989).
12.
C. Sirtori, F. Capasso, D. Sivco, S. N. G. Chu, and A. Y. Cho, Appl. Phys. Lett. 59, 2302 (1991).
13.
F. Capasso, C. Sirtori, D. L. Sivco, and A. Y. Cho, Nonlinear optics in coupledquantumwell quasimolecules, in Intersubband Transitions in Quantum Wells: Physics and Device Applications II, H. C. Liu, and F. Capasso (eds.), Academic Press, San Diego, 2000.
14.
C. Sirtori, A. Tredicucci, F. Capasso, et al., Opt. Lett. 23, 463 (1998).
15.
C. Claire, D. L. Sivco, and J. N. Baillargeon, Appl. Phys. Lett. 79, 572 (2001).
16.
C. Gmachl, D. L. Sivco, R. Colombelli, et al., Nature 415, 883–887 (2002).
17.
N. Owschimikow, C. Gmachl, A. Belyanin, V. Kocharovsky, D. L. Sivco, R. Colombelli, F. Capasso, and A. Y. Cho, Phys. Rev. Lett. 90, 043902 (2003).
18.
C. Gmachl, A. Belyanin, D. L. Sivco, Milton L. Peabody, N. Owschimikow, A. M. Sergent, F. Capasso, and A. Y. Cho, IEEE J. Quantum Electron. 39, 1345 (2003).
19.
C. Gmachl, N. Owschimikow, A. Belyanin, A. M. Sergent, D. L. Sivco, M. L. Peabody, F. Capasso, and A. Y. Cho, Appl. Phys. Lett. 84, 2751 (2004).
20.
O. Malis, A. Belyanin, C. Gmachl, D. L. Sivco, M. L. Peabody, A. M. Sergent, and A. Y. Cho, Appl. Phys. Lett. 84, 2721 (2004).
21.
T. S. Mosely, A. Belyanin, C. Gmachl, D. L. Sivco, M. L. Peabody, and A. Y. Cho, Opt. Express, 12, 2972 (2004).
22.
O. Malis, A. Belyanin, D. L. Sivco, J. Chen, A. M. Sergent, C. Gmachl, and A. Y. Cho, Electron. Lett. 40, 1586 (2004).
23.
M. Troccoli, A. Belyanin, F. Capasso, E. Cubukcu, D. L. Sivco, and A. Y. Cho, Nature 433, 845 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_283_03/23/2006 Raman Injection and Inversionless Intersubband Lasers Raman Injection and Inversionless ISB Lasers
283
24.
A. Evans, J. S. Yu, S. Slivken, and M. Razeghi, Appl. Phys. Lett. 85, 2166 (2004).
25.
S. Blaser, D. A. Yarekha, L. Hvozdara, Y. Bonetti, A. Muller, M. Giovannini, and J. Faist, Appl. Phys. Lett. 86, 041109 (2005).
26.
A. Yariv, The coupledmode formalism in guidedwave optics, in Proc. of the NATO Advanced Study Institute on Fiber and Integrated Optics, D. B. Ostrowsky, ed., Plenum Press, New York, 1978.
27.
D. Nikonov, A. Imamoglu, and M. Scully, Phys. Rev. B59, 12,212 (1999).
28.
J. Faist, C. Sirtori, F. Capasso, L. Pfeiffer, and K.W. West, Appl. Phys. Lett. 64, 872 (1994).
29.
Ya. I. Khanin, Principles of Laser Dynamics, Elsevier, Amsterdam, 1995.
30.
H. M. Pask, Progress in Quantum Electron. 27, 3–56 (2003).
31.
G. Sun, J. Khurgin, L. Friedman, and R. A. Soref, J. Opt. Soc. Am. B15, 648 (1998).
32.
H. C. Liu et al., Appl. Phys. Lett. 78, 3580 (2001).
33.
O. Kocharovskaya, Yu. V. Rostovtsev, and A. Imamoglu, Phys. Rev. A58, 649–654 (1998).
34.
E. Arimondo and G. Orriols, Nuovo Cim. Lett. 17, 333 (1976).
35.
F. Capasso, C. Gmachl, R. Paiella, A. Tredicucci, A. L. Hutchinson, D. L. Sivco, J. N. Baillargeon, A. Y. Cho, and H. C. Liu, IEEE J. Select. Topics Quantum Electron. 6, 931–947 (2000).
36.
S. M. Spillane, T. J. Kippenberg, and L. J. Vahala, Nature 415, 621–623 (2002).
37.
Y. R. Shen, The Principles of Nonlinear Optics, John Wiley & Sons, New York, 1984.
38.
J. Faist and R. Colombelli, private communication.
39.
J. Khurgin, G. Sun, L. R. Friedman, and R. A. Soref, J. Appl. Phys. 78, 7398 (1995).
40.
R. Koehler, A. Tredicucci, F. Beltram, H. E. Beere, E. H. Linfield, A. G. Davies, D. A. Ritchie, R. C. Iotti, and F. Rossi, Nature 417, 157 (2002).
41.
B. S. Williams, S. Kumar, Q. Hu, and J. L. Reno, Opt. Express 13, 3331 (2005).
42.
B. S. Williams, S. Kumar, H. Callebaut, Q. Hu, and J. L. Reno, Appl. Phys. Lett. 83, 2124 (2003).
43.
G. Scalari, N. Hoyler, M. Giovannini, and J. Faist, Appl. Phys. Lett. 86, 181, 101 (2005).
44.
M. C. Wanke, F. Capasso, C. Gmachl, et al., Injectorless quantum cascade lasers, Appl. Phys. Lett. 78, 3950 (2001).
45.
J. Faist, F. Capasso, D. L. Sivco, et al., Appl. Phys. Lett. 72, 680 (1998).
46.
M. P. Semtsiv, M. Ziegler, S. Dressler, W. T. Masselink, N. Georgiev, T. Dekorsy, and M. Helm, Appl. Phys. Lett. 85, 1478 (2004).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH06_284_03/23/2006 Raman Injection and Inversionless Intersubband Lasers
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_285_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
7 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response
H. C. Liua Institute for Microstructural Sciences National Research Council Ottawa, Ontario, Canada
Harald Schneiderb FraunhoferInstitute for Applied SolidState Physics D79108 Freiburg, Germany
7.1 Introduction Similar to all other devices discussed in this book, the quantum well infrared photodetector (QWIP) makes use of intersubband transitions between quantized states within (commonly) the conduction band. The most popular materials system is GaAs/AlGaAs because of its maturity in fabrication techniques, e.g., grown by molecular beam epitaxy (MBE). For a given materials system, the conduction band offset or bandgap discontinuity is limited to a given range. For example, the wavelengths covered by GaAs/AlGaAs QWIPs are longer than about 3 m. Nearly 20 aElectronic bPresent
mail: [email protected].
address: Institute of IonBeam Physics and Materials Forschungszentrum Rossendorf, D01314 Dresden, Germany.
Research, 285
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_286_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 286
Chapter Seven
years of research and development activities have placed QWIP arrays into the market for thermal imaging applications in the two atmospheric transmission windows of 3 to 5 and 8 to 12 ȝm in wavelength. The physics [1] and applications [2–4] of GaAs/AlGaAs QWIPs are well established. Thermal imaging is the main existing application of QWIPs fabricated into arrays [2]. For detecting weak signals, the device parameters are chosen to obtain the highest possible sensitivity and background limited infrared performance (BLIP) temperature. To reduce and in most cases eliminate the noise caused by dark current, the devices are cooled to cryogenic temperatures. For example, for a 10m cutoff QWIP viewing the usual room temperature background, the operating temperature is about 77 K. The design principles for this existing application are reviewed in Ref. 1. Presently QWIP arrays are on the verge of infiltrating existing applications and more importantly finding new ones [5, 6]. A schematic illustration of the QWIP operation is shown in Fig. 7.1. The intrinsic detector response time is limited by either the photoelectron lifetime or the total transit time, whichever is smaller. The transit time is usually much longer than the lifetime, leading to an intrinsic response time of about 5 ps due to the fast intersubband scattering processes by electronphonon, electronimpurity, or electronelectron interactions. To turn to the subject of this chapter, QWIPs are also well suited for highfrequency and highspeed applications. A distinct advantage of QWIPs over standard detectors made of HgCdTe is their high intrinsic speed. This is related to the inherent short carrier lifetime Ĳ ~ 5 ps as inferred both from heterodyne experiments [7, 8] showing a cutoff frequency of about 30 GHz and from timeresolved photocurrent measurements [9–11]. In this chapter, we review a simple way to achieve high absorption and demonstrate the highspeed capability. For characterizing short laser pulses, an autocorrelation technique is commonly used. This can be done either by a second harmonic generation crystal plus a linear detector or by a twophoton detector. We investigate the nonlinear behavior of QWIPs having three energetically equidistant energy levels. Resonantly enhanced nonlinear absorption, six orders of magnitude higher compared to typical bulk semiconductors, leads to a threshold power density for quadratic detection as low as 0.1 W/cm2 and femtosecond time resolution. The approach enables dynamic characterization of the optical light field of infrared (ir) emitters with unprecedented sensitivity. We demonstrate that secondorder autocorrelation measurements of ultrashort midinfrared laser pulses in the picojoule regime can be performed by using these ultrasensitive twophoton detectors. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_287_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
287
Zero bias
hν Emitter nGaAs AlGaAs nGaAs
Under bias Collector Schematic conduction band edge profile of a GaAs/AlGaAs QWIP under zero (above) and finite (below) bias. The electron population in the ntype wells is provided by doping using silicon. The emitter and collector contact layers are doped with silicon. Electrons occupy the ground state subband. Photons (hȞ) excite electrons from quantum wells, causing a photocurrent.
Figure 7.1
7.2 Pictures of Intersubband Transition and Photoconductivity The success of QWIPs has been made possible by the semiconductor crystal growth technology such as MBE [12] and by the device concepts using bandgap engineering [13]. Semiconductor structures with atomic layer control are now routinely fabricated by MBEs. Several introductory textbooks on quantum well physics have been written, e.g., by Bastard [14], Weisbuch and Vinter [15], Shik [16], and Harrison [17]. The term intersubband transition, abbreviated as ISBT hereafter, refers to the electronic transition between the confined states in quantum wells. The physics related to the optical ISBT in quantum wells is treated in great detail by Helm [18]. Other materials of specific relevance to QWIPs can be found in Refs. 1, 19, and 20. Here, we discuss only ISBT in the conduction band. Examples presented here are all on samples made by GaAsbased MBE. For this system, a polarization selection rule was established in the early days [21]: Only the light polarized in the growth direction can cause ISBT. The selection rule is valid for quantum wells where the single isotropic effective mass
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_288_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 288
Chapter Seven
approximation holds. Since the argument is based on the effective mass approximation, the selection rule is naturally not rigorous. As band mixing is the cause of the breakdown of the selection rule, physical intuition tells us that the accuracy of the selection rule should be related to the ratio of the energy scales involved. The closest band to the conduction band (at least for the GaAs case) is the valence band. The relevant energy ratio is then En/Eg, where En are the eigenenergies of the confined states in the conduction band quantum well and Eg is the bandgap. (Note that the reference point—zero energy—for En is chosen at the conduction band edge of the well.) For common quantum wells used in QWIPs (see, e.g., Ref. 1) the ratio is small, and therefore the selection rule is expected to be quite accurate, with a deviation of at most 10% level, as shown experimentally [22]. Because of the selection rule, a normalincidence geometry (i.e., light incident normal to the wafer and along the growth direction) is not suited. A commonly employed 45degree edge facet geometry is shown in Fig. 7.2, as first used in Levine et al. [23]. For unpolarized light, this geometry “throws away” onehalf of the power, but is simple and convenient and is usually used to obtain a detector performance benchmark. This geometry is also suited for highspeed applications involving lasers. The majority of applications of QWIPs require large twodimensional (2D) arrays where the facet geometry is not suited. For imaging arrays where the incident infrared is normal to the wafer, a diffraction grating is fabricated on each pixel to bend the light. Within the singleband effective mass approximation, the Schrödinger equation reads í
ല2 2 ෮ ȥ +V ȥ = E ȥ 2m
(7.1)
where m is the effective mass and V is the potential. If we choose the quantum well direction as the z axis, the potential V depends only on z, and the wave function is separable into lateral xy plane and z parts. The lateral part is simply a plane wave.
Mesa device P S
GaAs substrate
IR Figure 7.2 A 45degree edge facet light coupling geometry. The figure is not drawn to scale. The semiinsulating GaAs substrate thickness is usually in the range of 400 to 700 m. For testing individual detector performance, mesa devices of areas from about 1002 to 10002 m2 are used. The infrared (IR) light is shone normal to the facet surface. The P and S polarizations are defined with respect to the light incidence on the quantum wells.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_289_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
289
To obtain a simple picture of ISBT, much of the physics can be illustrated by using the simplest model of an infinitely highbarrier square quantum well [24]; that is, V = 0 for 0 z Lw and V = for z < 0 and z > Lw, where Lw is the well width. In this case the eigenstate wave function and energy are trivial: ĺ
ȥn (k x y ) = ĺ
2 Lw A
En (k x y ) =
sin
ĺ ĺ ʌnz exp (ik x y 썉 x) Lw
(
2 ല2 ʌ2n + kx2y 2m L2w
)
(7.2)
(7.3)
where A is the normalization area in the xy plane, n is a positive ĺ integer, k x y is the inplane wave vector, and m is the effective mass in the well. Equation 7.3 explains the reason for the term subband instead of a single state. For a given quantized state, one can put many electrons occupying different inplane momenta. For the ground state in equilibrium, the occupation of electrons leads to a Fermi energy determined by n2D = (m/ʌʄ2 )Ef, where n2D is the 2D quantum well carrier density and m/ʌʄ2 is the 2D density of states. The dipole matrix moment between any two states (say, n and nƍ) with opposite parity is e < z> n ,nƍ = eL w
nnƍ 8 2 2 ʌ (n í nƍ2)2
(7.4)
Note that the inplane momentum remains the same between initial and final states. The oscillator strength is f Ł
2mȦ n 2nƍ2 64 2n ,nƍ = 2 ല ʌ (n 2 nƍ2)3
(7.5)
The absorption probability for an ir beam polarized in the plane of incidence and propagating at an angle of ș with respect to the growth axis is Ș =
sin2 ș ǻE e2h 1 n2D f ʌ 4İ0nr mc cos ș ( En,nƍ í ലȦ)2 + (ǻE )2
(7.6)
where İ0 is the vacuum permittivity, nr is the index of refraction, c is the speed of light, En,nƍ Ł En – Enƍ, and ¨E is the broadening halfwidth. The line shape associated with broadening is modeled by a lorenzian. At the peak (En,nƍ = ƫȦ) the absorption is inversely proportional to ǻE. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_290_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 290
Chapter Seven
For a given n2D, the absorption is inversely proportional to m; that is, the smaller the effective mass, the larger the absorption. Note that for a given Ef, however, the absorption is independent of m since n2D = m / (ʌല2) E f . Note also that the integrated absorption is independent of ¨E. The derivation of Eq. 7.6 is straightforward by using a dipole interaction hamiltonian and Fermi’s golden rule (see, e.g., Helm [18]). The factor sin2 ș in Eq. 7.6 comes from the polarization selection rule discussed before. The factor cos ș seems to give an unphysical result when ș ĺ 90°. However, since the meaning of Ș is the absorption probability of light passing through the well, in this extreme the passing length becomes infinitely long, resulting in an infinitely large absorption. If one had considered a quantity of absorption constant Į defined by Ș = Į × length, where length = L w / cosș is the propagation length, this quantity would have been always finite. For a real quantum well with finite barrier height, it would be more physical to choose the length using the quantum well structure thickness (including barriers) instead of only Lw taken here. Let us put some typical numbers into Eq. 7.6 to get a feeling for how strong the ISBT absorption is. For a typical 8 to 12ȝm peaked QWIP, the halfwidth is about ǻE = 0.01 eV. For ground state to first excited state transition, the oscillator strength is f = 0.961 (see Eq. 7.5 with nƍ = 1 and n = 2). For 77 K operation, the carrier density is set to about n2D = 5 × 1011 cmí2. For GaAs well, the reduced effective mass is m* = 0.067 (m = m* × me, where me is the free electron mass), and the refractive index is about nr = 3.3. With these values and for a 45degree angle (ș = 45°), the absorption for a single quantum well is Ș = 0.54% (for polarized light). Let us also evaluate the absorption constant for the case of ș = 90°, with other parameters the same as above. Taking a quantum well structure thickness of 50 nm (including barriers), we find the peak absorption constant is Į = 1520 cmí1. For a standard QWIP, the optimum well design is the one having the first excited state in resonance with the top of the barrier. This configuration gives at the same time both a large peak absorption (similar to the bound state to bound state transition discussed above) and a rapid escape for the excited electrons. The optimum design configuration has been experimentally proved [25, 26]. To design a quantum well for a given QWIP wavelength, one needs to know how the barrier height (conduction band offset) relates to heterosystem parameters, i.e., the Al fraction x in the GaAs/AlxGa1íxAs case. Surveying many samples by comparing the calculated transition energy with the experimental peak absorption, we find a range of values for the conduction band offset ǻEc = (0.87 ± 0.04) × x eV, where x is the Al fraction. The calculation is a simple eigenenergy calculation of a square quantum well. Higherorder effects, such as band nonparabolicity and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_291_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
291
manybody effects, influence the precise values of the calculation (as discussed by Helm [18]). To describe the photocurrent from a QWIP, the standard photoconductivity formulas can be used. The current responsivity (in amperes per watt) is written as Ri =
e Șg hȞ
(7.7)
where Ș now is the total absorption quantum efficiency and g is the photoconductive gain given by g = Ĳlife/Ĳtrans, where Ĳtrans is the total transit time and Ĳlife is the excited carrier lifetime or more specifically for QWIP the capture time into the quantum well. The noise in a common QWIP is of a generation recombination nature and is therefore given by 2 inoi se = 4egI B
(7.8)
where I is the device current (including dark current and photocurrent) and B is the measurement bandwidth. Given the incident photon power, the photocurrent is calculated by Eq. 7.7, while the dark current can be estimated by the simple expression
Jdark = eN3Dv
(7.9)
where v is the drift velocity for carriers in the barrier region and the threedimensional (3D) mobile carrier density in the barrier is estimated by
(
N3D § 2
mb kBT 2ʌല
2
)
3/2
exp
(
í Eact kBT
)
(7.10)
where mb is the barrier effective mass. Eact is the thermal activation energy, which equals the energy difference between the top of the barrier and the top of the Fermi sea in the well. We have assumed that Eact /(kBT ) 싯 1, appropriate for most practical cases. 7.3 HighAbsorption QWIPs As shown later, especially for the case of heterodyne detection, a high absorption efficiency directly translates to a high sensitivity and is therefore of critical importance. In this section, we show experimental results to demonstrate the highabsorption capability. We also show that these devices can work at elevated temperatures either within the thermoelectric cooling range (> 200 K) or near room temperature.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_292_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 292
Chapter Seven
7.3.1
Absorption measurements
Starting from a standard QWIP structure, the simplest way to enhance absorption is to dope the wells more heavily and to grow more wells [27, 28]. At 45degree incidence and for polarized light, the absorption per quantum well per pass is about 0.54% per well for a standard GaAs/AlGaAs QWIP with 5 × 1011 cmí2 doping. For a doping density of 1.5 × 1012 cmí2, the onewell, onepass absorption is expected to be Ș1 § 1.6%. If a 90% QWIP absorption is desired, the number of wells needed is determined by exp(í2NȘ1) = 10%, which gives N = 72. (The factor of 2 in the exponential accounts for the double passes in the 45degree facet detector geometry.) In the following experiments, we have chosen N = 100 to ensure high absorption. All QWIP wafers were grown in a MBE system. Here we show three examples with different detection wavelengths centered at about 10, 8, and 5 m. The period of the 100repeat multiplequantumwell structure consists of a GaAs well and AlxGa1íxAs barriers. The GaAs well center region is doped with Si to give an equivalent 2D density of 1.5 × 1012 cmí2. The top and bottom GaAs contact layers are 400 and 800 nm thick, doped with Si to 2 × 1018 cmí3. Other device parameters are listed in Table 7.1. Mesa devices were fabricated by standard GaAs processing techniques. All devices were packaged into the 45degree edge facet geometry for optical coupling. With the high well doping densities used in these QWIPs, we expect a large increase in dark current [29]. Using a set of samples having similar cutoff wavelengths but different doping densities of 5 × 1011, 1.0 × 1012, 1.5 × 1012, and 2.0 × 1012 cmí2, measurements on currentvoltage (IV) characteristics at 77 K show approximately a factorof10 increase between consecutive samples. The increase is mainly caused by the increase in the well Fermi energy ǻEf which raises the dark current by exp ǻE f / (kBT ) . Measurements of the BLIP temperature show that TBLIP is degraded with increasing doping and TBLIP § 60, 45, and 30 K for 1.0 × 1012, 1.5 × 1012, and 2.0 × 1012 cmí2 doping samples, respectively. An optimized QWIP (with about 4 × 1011 cmí2 doping) covering the same wavelength range would have a TBLIP of about 77 K
TABLE 7.1 Sample Parameters The doping in the well is Si, įdoped at the center to 1.5 × 1012 cmí2. The number of periods is 100. The symbols are Ȝp for peak detection wavelength, x for Al fraction, Lw for well width, and Lb for barrier thickness.
Sample
Ȝp (m)
x
Lw (nm)
Lb (nm)
QWIP10 QWIP8 QWIP5
10.0 8.4 5.0
0.19 0.24 0.48
6.6 5.9 5.0
25 24 22
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_293_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
293
for a 2ʌsolidangle field of view. Highdoping devices are therefore far from optimum for the detection of weak signals. To show the anticipated high absorption, Fig. 7.3 presents the measured doublepass polarized 45degree incident transmission spectra for the three samples. For samples QWIP10 and QWIP8, the high absorption is clearly demonstrated. Ideally, QWIP5 should have a similar absorption, and it is not clear why a somewhat lower absorption is obtained. Nevertheless, a 70% absorption is still quite high. In a separate experiment on a set of 10ȝm QWIPs [27], it was noted that if the doping was further increased from 1.5 × 1012 to 2.0 × 1012 cmí2, then the peak absorption did not increase and only a broadening in the spectral width was seen. The same experiment also indicated that a doping of 1.0 × 1012 cmí2 is sufficient for the 10ȝm QWIP to have 90% absorption. 7.3.2
Detector characteristics
Figure 7.4 shows the spectral response curves for the three samples, covering the designed wavelength regions. A further goal of these samples is to attempt operation on them at elevated temperatures. To maximize the dark current limited detectivity, it has been established [1] that the well doping density should be such that the Fermi energy is Ef = 2kBT, where T is the desired operating temperature. The doping in the well is assumed to be completely ionized; i.e., doping density equals electron density (n2D). The Fermi energy relates to n2D by n2D = m / (ʌല2 ) E f , where m is the well effective mass. For T = 80 K, the required density is about 4 × 1011 cmí2 for GaAs wells. It is then 1.0
Transmission
0.8
0.6
0.4 QWIP5 0.2 QWIP10 0.0
QWIP8
Room temperature 45° incidence double pass
1000 1500 2000 Wavenumber (cm1)
Doublepass 45degree incidence transmission spectra at room temperature and with polarized light.
Figure 7.3.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_294_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 294
Normalized response
1.0
Chapter Seven
QWIP10
QWIP8
QWIP5
80 K
0.8 0.6 0.4 0.2 0.0 500
1000
1500 2000 2500 Wavenumber (cm1)
3000
Normalized spectral response curves at 80 K and 3 V. The device geometry is equivalent to that of Fig. 7.3 so that the absorption efficiency is represented by Fig. 7.3.
Figure 7.4.
expected that the doping range of 1 to 2 × 1012 cmí2 is where QWIPs may operate near room temperature, albeit with a reduced sensitivity. Measured results at various temperatures using a CO2 laser tuned to 10.6 ȝm are shown in Fig. 7.5 for sample QWIP10. It is clear that the device does work up to room temperature. It is interesting to note that with increasing temperature, the responsivity first goes up and then comes down for a given bias voltage. Since the responsivity is proportional to the mobility, this behavior is attributed (in a large part) to the temperature dependence of the mobility. It is well known that the impurity scattering limited mobility increases with temperature whereas the phonon scattering limited mobility decreases. The two scattering effects result in the observed behavior [29]. For elevatedtemperature operation where the QWIP resistance is low, a high responsivity is highly desirable to overcome the large noise associated with the low resistance and the 50ȍ termination. It is difficult to accurately measure the responsivity when the device resistance is low and comparable to contact and/or series resistance. The low resistance causes a “short circuit” for the photocurrent, leading to an apparent low responsivity. The values in Fig. 7.5 for high temperatures (> 200 K) could be somewhat lower than reality. Given the measured IV, responsivity, and absorption, the detectivity D * is easily evaluated. Using the relations R i = e / ( hȞ) gȘ and D * = R i A / 4egI , where Ri is the responsivity, Ȟ is the photon frequency, g is the photoconductive gain, A is the device area, and I is the device current, the dark current limited detectivity at 10.6 ȝm and for polarized light is calculated and plotted in Fig. 7.6 for various temperatures. A stateoftheart QWIP for the same wavelength would have a D * value of over 1010 cm·Hz1/2/W at 80 K. The present device is Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_295_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
295
0.25
Responsivity (A/W)
0.15 0.10 0.05 0.00
QWIP 10 @ 10.6 μm
140 130 120 110 100 90 80 K
0.20
1.5x1012cm2 doping 6
5
4
3
2
1
0
1
2
3
4
5
6
0.12 150 160 170 180 190 200 210 K
Responsivity (A/W)
0.10 0.08 0.06 0.04 0.02 0.00 1.5
1.0
0.5
0.0
0.5
1.0
1.5
Responsivity (A/W)
0.04 220 230 240 250 260 270 280 290 300 K
0.03
0.02
0.01
0.00 0.6
0.4
0.2
0.0
0.2
0.4
0.6
Voltage (V) Responsivity versus applied voltage under a CO2 laser (10.6 ȝm) illumination and at various temperatures for sample QWIP10.
Figure 7.5.
(again) then far from optimum for lowsignal and lowtemperature use. Comparing with a room temperature thermal detector having a D* value of about 108 cm·Hz1/2/W, which is commonly used in a Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_296_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 296
Chapter Seven
109
Detectivity (cm Hz1/2/W)
80 K 90 110
108
130 150 170 200 240
QWIP10 @ 10.6 μm 10
290 K
7
5 Figure 7.6
4 3 2 1 0 1 Voltage (V)
2
3
4
5
Detectivity at 10.6 ȝm for sample QWIP10 and at various temperatures.
midinfrared spectrometer system, we see the present device needs to be cooled to about 150 K to achieve the same D *. Note that temperatures about 200 K and higher are attainable by thermoelectric cooling. Operation at elevated temperatures implies high dark currents. To overcome the dark current noise at room temperature, a laser power of about 10 mW is required for a 10 × 10 ȝm2 activearea device; and similarly at 200 K a power of about 5 mW is needed. Highspeed operation requires small device capacitances. The present approach employing a large number of quantum wells makes the device thicker than a typical QWIP and hence of lower capacitance. For the present devices with a thickness of about 3 ȝm, an active area of about 50 × 50 ȝm2 or smaller is sufficient for operation at 30 GHz or higher. Similarly, the detectivity for sample QWIP5 is shown in Fig. 7.7. For this shorterwavelength device, a higher detectivity is obtained, making this device well operable with a thermoelectric cooler. 7.4 HighSpeed and HighFrequency QWIPs Thanks to the intrinsic short carrier lifetime, QWIPs are well suited for highspeed and highfrequency applications. Highspeed detectors may create new applications, e.g., environmental remote sensing of molecules [30] and CO2 or quantum cascade laserbased communication [31], as well as laboratory and instrumentation [32–36]. For these applications, there is commonly a strong signal or a powerful local oscillator, in most cases employing lasers. Under such circumstances, a high dark current can be tolerated to a large degree, and a high absorption and high operating temperature are desirable. Note also that
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_297_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
10
297
11
Detectivity (cm Hz1/2/W)
QWIP5 @ 5 μm 80 K
1010 110
109
10
130
210 K
8
10
Figure 7.7
5
0 Voltage (V)
5
170
10
Detectivity at 5 ȝm for sample QWIP5 and at various temperatures.
the polarization sensitivity of the ntype QWIP is no longer a disadvantage for (polarized) laserbased systems. The intrinsic detector response time is limited by either the photoelectron lifetime or the transit time, whichever is smaller. For a large number of QWs, the total transit time is usually much longer than the lifetime, leading to a lifetimelimited intrinsic response time of about 5 ps. If, on the other hand, a QWIP has a small number of QWs (for example, 10 or less), photoexcited carriers will be swept out before capture, resulting in a transit timelimited situation. At present, QWIPs hold the unique position of having highspeed, highfrequency capability and high absorption for the thermal infrared region. There are no competitive alternatives. The measurement of highspeed and highfrequency characteristics can be done in either the frequency [7, 8, 37] or the time [9–11] domain. In this section, we discuss the physics and show results in the frequency domain. 7.4.1
Microwave rectification
As a simple way to measure the QWIP highfrequency behavior, we first discuss the microwave rectification technique [37]. We apply a microwave signal to the QWIP and measure the change in its direct biasing current. This is complementary to the optical heterodyne technique, which involves generating a microwave signal within a QWIP at the difference frequency of two optical beams [7]. The rectification in the QWIP relies on its inherent nonlinear IV characteristic and therefore probes its transport properties. The smallsignal rectified direct current is given by Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_298_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 298
Chapter Seven
Irect =
1 IƎ Vȝ2 4
(7.11)
where IƎ is the second derivative of the IV curve and Vȝ is the amplitude of the microwave voltage applied to the device. Both IƎ and Vȝ depend on the microwave frequency Ȧ. The dependence of IƎ on Ȧ reflects the frequency rolloff behavior of the intrinsic transport mechanism and therefore is expected to behave as 1/[1 + (ȦĲ)2], where Ĳ is some characteristic time. This Ĳ is expected to be approximately the excited electron lifetime or the photoconductive lifetime. Given a constant output power from a microwave source, Vȝ varies as a function of frequency because of the circuit limited by the device capacitance and differential resistance, and other parasitics. We then rewrite Eq. 7.11, separating out the frequency dependencies: Irect =
1 I ƎV 2 Į(Ȧ) ȕ(Ȧ) 4 0 ȝ0
(7.12)
1 1 + (ȦĲ)2
(7.13)
where Į(Ȧ) =
Here ȕ(Ȧ) is the circuit dependence, and I0Ǝ and Vȝ0 are the lowfrequency limiting values of IƎ and Vȝ, respectively. The experiment is schematically shown in Fig. 7.8. QWIPs were connected to the end of a 50ȍ coplanar transmission line by a short wire bond. The dc bias is applied through a biasT. The microwave power is supplied by a microwave source capable of frequencies up to 40 GHz. The QWIP is modeled by a parallel resistancecapacitance V
bias Measure current
50 _ Ω line
Microwave source Bias T QWIP L
R
C
Figure 7.8 Schematic of the microwave rectification experiment. The QWIP is mounted at the end of a 50ȍ transmission line. The QWIP is modeled by a parallel resistancecapacitance equivalent circuit, and the parasitic inductance is caused by the short wire bond.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_299_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
299
(RC) equivalent circuit, and the parasitic inductance L is caused by the wire bond. Given the equivalent circuit of the device and its parasitic inductance (Fig. 7.8), the microwave voltage across the device is straightforward Vȝ2 =
8R L 2
2
(1 í Ȧ LC ) + Ȧ2( R LC + L / R)2
Pout
(7.14)
where RL = 50 ȍ is the line impedance, R = 1/Iƍ is the device differential resistance, Iƍ is the derivative of the IV curve, and Pout is the output power from the microwave source. We have made the approximation R + RL § R because RL 싮 R for a typical QWIP. For Ȧ ĺ 0 we get 2 Vȝ0 = 8R L Pout
(7.15)
and by comparison with Eq. 7.12 ȕ(Ȧ) =
1 (1 í Ȧ2 LC )2 + Ȧ2( R LC + L / R)2
(7.16)
The L ĺ 0 limit of the above gives the usual RC rolloff: 1/[1 + (ȦRLC)2]. We show experimental results on three samples listed in Table 7.2. The samples differ mainly by the number of quantum wells. All experiments were carried out with the sample at 77 K. The relevant device parameters of these samples are listed in Table 7.3. The expected RC characteristic frequency is fRC = 1/(2ʌRLC) for RL = 50ȍ TABLE 7.2 Sample Structural Parameters The Si doping density in the two contact layers was 1.5 × 1018 cmí3, and the center Si įdoping density in the wells was 9 × 1011 cmí2 for all samples.
Sample
x
Lw (nm)
Lb (nm)
Repeats
16W 8W 4W
0.265 0.260 0.276
5.7 5.9 6.0
23.7 24.6 24.6
16 8 4
TABLE 7.3 Sample Device Parameters The device size is 10 × 10 ȝm2. Here Ltot is the total active device thickness, C is the device capacitance, fRC = 1/(2ʌRLC), RL = 50 ȍ, fmax is the lifetimelimited cutoff frequency, and Ĳ = 1/(2ʌ fmax).
Sample
Ltot (ȝm)
C (fF)
fRC (GHz)
fmax (GHz)
Ĳ (ps)
16W 8W 4W
0.49 0.27 0.15
21.5 39.4 72.2
148 81 44
33 §33 §33
4.8 §4.8 §4.8
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_300_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 300
Chapter Seven
load resistance. The estimated carrier lifetime Ĳ and the intrinsic cutoff frequency fmax [defined by Ĳ = 1/(2ʌfmax)] are discussed next. Figure 7.9 shows the measured (dots) and calculated (lines) rectified current versus frequency for the three samples. The 3dB point from the maximum fmax for the 16well sample (sample 16W) is about 33 GHz. For this sample, the RClimited frequency is much larger than 33 GHz, and hence the rolloff here directly relates to Ĳ, resulting in a value of 4.8 ps. However, for the 4 and 8well samples, the RC effect is clearly seen. The rectified current starts to roll off at a lower frequency and with a much slower rate. The calculated curves in Fig. 7.9 used the expressions given above with the inductance L determined by the length of the wire bond. Further details are given in Ref. 37. 7.4.2
Heterodyne detection
Although very well suited, heterodyne detection using QWIPs has received limited attention [38, 39, 7, 8, 32]. Heterodyne detection involves a local oscillator (LO), commonly a laser, at a slightly different wavelength from that of the signal. The differencefrequency signal (often referred to as the IF—the intermediatefrequency signal) is measured. 104
16 Wells
5
Rectified current (A)
10
106 104
73 kV/cm
(c)
8 Wells 10
5
106 71 kV/cm
(b)
107 104
4 Wells
105 106
68 kV/cm
(a) 0
10
20
30
40
Frequency (GHz) Rectified current versus frequency for (a) the 4well, (b) the 8well, and (c) the 16well samples. The solid lines are calculated. The bias voltages were chosen to give approximately the same electric field of 70 kV/cm. All device areas were 10 × 10 ȝm2. The device temperature was 77 K. The microwave power was 1.0 mW. Figure 7.9
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_301_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
301
This method is also used to characterize the highfrequency behavior by beating two lasers and measuring the IF as a function of the frequency. The advantage of heterodyne detection is well known and described [40]. The key point is that with a sufficiently high LO power, the ideal detection limit can be reached, and the sensitivity [e.g., the noise equivalent power (NEP)] depends only on the absorption quantum efficiency for a given wavelength. The argument can be easily constructed for a photoconductive QWIP as follows. As established, the detector current responsivity is written as Ri =
e Șg hȞ
(7.17)
where Ș is the absorption quantum efficiency and g is the photoconductive gain. Under a strong LO power PLO, i.e., LOinduced current I LO dominates over dark current, the gr noise current power spectral density is
Si = 4egILO = 4egR i PLO
(7.18)
By using Eq. 7.17, Eq. 7.18 becomes Si = (2eg )2
Ș P hȞ LO
(7.19)
Hence the noise current is Ș P B hȞ LO
i noise = Si B = 2eg
(7.20)
where B is the measurement bandwidth. The heterodyne current for a signal power of Psig is ihet = 2R i PLO Psig = 2eg
Ș PLO Psig hȞ
(7.21)
The last step used Eq. 7.17. The minimum detectable signal occurs when inoise = ihet; from Eqs. 7.20 and 7.21, we then have Psig,min hȞ = Ș B
(7.22)
which leads to the following definition [38, 39]:
(NEP)het =
hȞ Ș
(7.23)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_302_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 302
Chapter Seven
The NEP is measured in watts per hertz (not in the common unit of W/ Hz1/2 for the usual detection scheme). It is shown from Eq. (7.23) that the heterodyne NEP depends only on the absorption Ș and photon quantum hȞ, and is independent of gain g. This of course is in the regime where LOinduced current is dominant, referred to as photon noise limited. The direct measurement of IF signal is limited to frequencies up to the capability of the available spectrum analyzer. To achieve higher frequencies, we can employ mixing in the QWIP to downconvert the IF signal generated by the optical heterodyne [8]. This again (as in the rectification case) relies on the nonlinear IV characteristic as in rectification. We apply to the QWIP not only the two ir beams, as in a conventional heterodyne experiment, but an additional microwave excitation. Specifically, let fir1 and fir2 denote the two ir frequencies, and fȝwave be the microwave frequency. Then the ir heterodyne frequency is fhet = fir1 – fir2, while the downconverted signal frequency is fhet – fȝwave. In this scheme, one can reach very high fhet frequencies by using a standard spectrum analyzer at the output of the QWIP. Of course, when fhet and fȝwave are both sufficiently small, we also observe the upconverted signal at fhet + fȝwave on the spectrum analyzer. The device used in this experiment was a 100well QWIP with a GaAs well width of 4.5 nm and an Al0.21Ga0.79As barrier width of 40 nm. The center 2.5 nm of each well was doped with Si to 2.5 × 1018 cmí3. The ir sources were either two CO2 lasers [41] or a CO2 laser and a leadsalt temperature tunable diode laser (TDL) [42]. The microwave or millimeterwave radiation was generated by either a microwave source tunable up to 40 GHz or a Gunn oscillator mechanically tunable in the range of 91 to 94 GHz. The CO2 lasers were operating in the neighborhood of 10.3 ȝm on individual lines selected by gratings with a separation between adjacent lines of about 41 GHz. The TDL was used only for fhet < 26.5 GHz, which was the limit of our spectrum analyzer. A schematic of the experimental techniques is shown in Fig. 7.10. The experimental results covering the frequency range of about 1 to 100 GHz are shown in Fig. 7.11. The curves are the expected rolloff behavior due to the device RC time constant and the photocarrier lifetime, again using Ĳ ~ 5 ps. The optical heterodyne data were taken with a CO2 laser and the TDL laser [7]. We have normalized the signal for a constant incident power of about 0.2 mW from each of the ir lasers and 0.3 mW from the microwave source. The five data points [8] shown in Fig. 7.11 for the mixing experiment were taken using different sources and different microwave coupling schemes. For the first three points at fhet = 1.83, 5.37, and 15.5 GHz, we used one CO2 laser, the TDL, and the microwave source at frequencies of fȝwave = 9, 15, and 10 GHz, respectively, and measured the sum signals of fhet and fȝwave. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_303_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
V
bias
Bias T Co2 Tunable diode
303
Preamp
Spectral analyzer
QWIP
Microwave source V
10dB Directional coupler Co2 Tunable diode or another Co2
bias
Bias T
Preamp
Spectral analyzer
QWIP
A schematic of heterodyne detection experiment: (above) direct measurement of the IF and (below) mixing on QWIP for extending the measurement frequencies.
Figure 7.10
20 30
Heterodyne
Signal (–dBm)
40 50 Up & down converted
60 70 80
80 K
90
100well QWIP 100 1
10 Frequency (GHz)
100
Figure 7.11 Direct infrared heterodyne and mixed heterodyne frequency with microwave frequency signal versus heterodyne frequency for a bias voltage of 2 V. The curves show the expected rolloff behaviors. The heterodyne frequency is defined as the difference between the two infrared frequencies. The incident powers from the two infrared sources and the microwave source are normalized to about 0.2 and 0.3 mW, respectively. The device temperature was about 80 K.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_304_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 304
Chapter Seven
The point at 41.42 GHz was obtained by using two CO2 lasers separated by fhet = 41.42 GHz and the microwave source at fȝwave = 20 GHz, and measuring the difference signal at 41.42 – 20 = 21.42 GHz. The point at 82.16 GHz was obtained by using two CO2 lasers separated by this frequency and a Gunn oscillator mechanically tuned in the range of 91 to 94 GHz. The difference signal in the range of 9 to 12 GHz was measured. For this data point, the millimeterwave radiation was coupled into the device through free space. To crosscheck the consistency between results measured in frequency and time domains, both microwave rectification and timeresolved photocurrent measurements were made on one of our QWIPs. The Fourier transform of the timeresolved photocurrent is compared with the microwave rectification curve in Fig. 7.12. For this experiment, we used a QWIP very similar to the sample QWIP10 in Sec. 7.3, but with a doping concentration of 1012 cmí2. The details of this sample are given in Ref. 27. The plot in Fig. 7.12 exhibits an excellent quantitative agreement between the two experimental methods. There was a defect in the packaging of this device, resulting in a drop in the frequency response at about 8 GHz. Recently we have made substantial advances in both fabrication and packaging of highfrequency devices and in measurement techniques [43]. The air bridge and coplanar waveguide are monolithically integrated with QWIP, eliminating the wire bond. Direct measurements of heterodyne signal over coaxial cables have been performed up to 110 GHz and from cryogenic to room temperatures. Data measured on a 100well QWIP with 1012 cmí2 well doping are shown in Fig. 7.13, representing a substantial improvement over the results in Fig. 7.11.
microwave rectification Fourier Transform of the photocurrent transient
Spectral density (a.u.)
0.2
0.1
T = 80 K 0.0 0
10
20 30 40 Frequency (GHz)
50
60
Figure 7.12 Comparison of the Fourier transform of the photocurrent transient and the frequency dependence obtained from the microwave rectification method.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_305_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
Figure 7.13
305
Normalized heterodyne signal taken at 80 K (circles) and 300 K (dots).
7.5 TwoPhoton QWIPs 7.5.1 Equidistant threelevel system for quadratic detection
While the highspeed detection methods discussed so far need to take into account the residual capacitance and inductance of the QWIP device and its packaging, much faster signals can be studied by exploiting the intrinsic nonlinearity. Since such nonlinear spectroscopy usually suffers from a lack of detection sensitivity, an artificial threelevel system has been realized by energetically equidistant subbands [44, 45], as indicated in Fig. 7.14a. Subbands 1 and 2 are bound in the QW, whereas state 3 is a continuum resonance located close to the barrier energy. In an external electric field, the carriers excited into the continuum are swept out of the QW and give rise to a photocurrent. According to numerical simulations, a 7.6nmthick GaAs QW, sandwiched between Al0.33Ga0.67As barriers, is optimized for a transition wavelength of 10.2 ȝm, whereas operation at 7.9 ȝm is achieved by using a 6.8nm In0.10Ga0.90As QW and Al0.38Ga0.62As barriers. Figure 7.14b summarizes the spectral characteristics of a twophoton QWIP comprising 20 GaAs QWs of 7.6nm width, Sidoped to an electron concentration of n2D = 4 × 1011 cmí2, and Al0.33Ga0.67As barriers (device 1). The spectral dependence of the optical transition from the first to the second subband (1 ĺ 2) is obtained through intersubband absorption measurements in a Brewsterangle geometry at 77 K. The 2 ĺ 3 transition was studied through photocurrent measurements at 130 K, where the thermal population of the second subband causes a signal. The spectral dependence of the twophoton photocurrent at
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_306_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 306
Chapter Seven
Absorption 1 → 2 Photocurrent 2 → 3 TP Signal 1 → 3
NORMALIZED SIGNAL
1.0
E3 E2
0.8 0.6 0.4 0.2
E1 0.0
9
(a)
10 WAVELENGTH (μm) (b)
11
(a) Schematics of the twophoton QWIP. (b) Normalized absorption at 77 K in Brewsterangle geometry, photocurrent at 130 K due to excitation from thermally populated subband 2 into subband 3, and twophoton photocurrent at 77 K under excitation by a continuouswave CO2 laser versus excitation wavelength. (Source: Ref. 44.) Figure 7.14
Photocurrent Density (A/cm2)
77 K has been measured with a wavelengthtunable CO2 laser. Remarkably, all three experimental curves point to identical peak wavelengths (10.4 ȝm), indicating perfectly equidistant subband energies (E2 í E1 = E3 í E2 = 119 meV). The spectrum associated with CO2 laser illumination is narrower than the absorption spectrum, which reflects the quadratic nature of the twophoton transition [46]. Figure 7.15 shows the photocurrent versus the power density P upon CO2 laser illumination at 10.2 ȝm. The photocurrent exhibits a linear increase with P up to about 0.1 W/cm2 at 70 K (up to 1 W/cm2 at 90 K) followed by a quadratic increase. Closer investigation at different temperatures up to 160 K reveals thermally activated behavior of the 103 70 K 82 K 90 K
104 10
5
106 107 108
∝P
2
∝ P
109 0.01
0.1 1 10 Power Density (W/cm2)
Figure 7.15 Photocurrent density under continuouswave illumination at a wavelength of 10.3 ȝm and 1.5V detector bias versus power density at different temperatures, as indicated. (Source: Ref. 44.)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_307_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
307
photocurrent in the linear regime, with an activation energy of 104 meV. This result allows us to conclude that the linear regime is caused by thermal population of E2. Quadratic behavior can be achieved even below 0.1 W/cm2 when the device is operated at lower temperatures. From the data of Fig. 7.15, the twophoton absorption coefficient ȕ can be readily determined. In a twophoton detector with an absorbing region of thickness L, the associated quantum efficiency Ș2P is given by Ș2P = ȕPLfș. Here the parameter fș relates to the selection rule for intersubband transitions. If ș is the angle between light propagation and the sample normal, we have fș = sin4 ș/cos ș for twophoton absorption, whereas the corresponding factor in the linear case is sin2 ș/cos ș. Using the usual definition of responsivity, the twophoton photocurrent density j2P is thus expressed as j2P =
eg ȕL f ș P 2 hȞ
(7.24)
For a doublepass at ș = 45°, the light traverses 2N = 40 absorbing QWs with a total thickness of L = NLw § 0.3 ȝm. The gain as determined from noise measurements amounts to g = 0.3 at 1.5 V. Equation 7.24 thus yields a twophoton absorption coefficient of 1.3 × 107 cm/GW. This nonlinearity is six orders of magnitude higher than that in typical bulk semiconductors (Si, ZnSe, GaAs), where values of ȕ § 10 cm/GW are observed. These results also indicate a huge increase of ȕ compared to the detuned twophoton QWIP [47], where ȕ takes a value of about 5 × 103 cm/GW. 7.5.2 Autocorrelation of subpicosecond optical pulses
We now demonstrate the use of this detection scheme for quadratic autocorrelation measurements of ultrashort optical pulses. With a Michelson interferometer, the pulses are split into two parts separated by a variable time delay. While quadratic intensity autocorrelation measurements have been studied in Ref. 45, we concentrate here on interferometric autocorrelation. The interference between the pulses contains additional information associated with the relative phase between the pulses. The optical pulse source used for the experiment is generated by the difference frequencies between the signal and idler pulses of an optical parametric oscillator pumped by a femtosecond Ti:sapphire laser [48]. The pulse source is wavelengthtunable from 6 to 18 m, with 10pJ pulse intensity, 160fs pulse width, and 76MHz repetition rate. Due to the high sensitivity of the present twophoton
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_308_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 308
Chapter Seven
Signal
QWIP, interferometric autocorrelation measurements can be performed in spite of the low optical power. The upper part of Fig. 7.16 shows an autocorrelation trace measured at 77 K on a device with 6.8nm In0.10Ga0.90As quantum wells and Al0.38Ga0.62As barriers. From these data, important information both on the temporal width of the optical pulses and on the dynamic properties of the twophoton QWIP can be obtained. While the interference fringes around zero time delay correspond to those of a nearly ideal autocorrelation of the optical field, two additional signatures are associated with intrinsic time constants of the detector. First, the amplitude of the interference fringes toward increasing positive and negative delay times shows an exponential rather than gaussianlike decay. This behavior is attributable to the decay time T2 (dephasing time) of the coherent intersubband polarization between the first and second subbands. Second, after the disappearance of the fringes, the signal still decreases exponentially with delay time toward its asymptotic value. The associated time constant T1 is due to intersubband relaxation of electrons from the second back to the first subband. Using the model function of Nessler et al. [49], we have carried out a numerical leastsquares fit of the measured autocorrelation (lower part of Fig. 7.16). The procedure is facilitated because the dephasing time associated with the continuum resonance 3 is negligibly small. The fit yields T1 = 0.46 ps and T2 = 0.10 ps, which agrees with typical values obtained from degenerate fourwavemixing experiments [50]. The value of T2 corresponds to a broadening with a fullwidth at half
5
Experiment
Signal
0 5
Theoretical Fit
0 1.0
0.5
0.0 Delay time (ps)
0.5
1.0
Twophoton photocurrent autocorrelation of femtosecond optical pulses at 8.0 ȝm (upper part) and numerical fit (lower part) versus delay time. The signal is normalized to its value at a large delay time above 10 ps. (Source: Ref. 44.)
Figure 7.16
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_309_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
309
maximum of ī12 = h/(ʌT2) = 13 meV. Since the absorption line width of this sample has a similar value (11 meV), we conclude that the 1 ĺ 2 transition is homogeneously broadened. We note that similar time constants T1 = 0.53 ps and T2 = 0.13 ps have been obtained for the sample of Fig. 7.14b [45]. Theoretically, two different mechanisms give rise to photoemission involving two absorbed photons. One mechanism is a coherent twophoton transition which, like degenerate fourwave mixing, is 3 associated with the thirdorder nonlinear susceptibility Ȥ . Within secondorder perturbation theory, it gives rise to the twophoton absorption coefficient ȕȤ3 =
(
e2 4İ0nr mc
)
2
n2 D f f 2T 2T L w hȞ 12 23 2 e
(7.25)
with the well width Lw, the refractive index nr, and the dimensionless oscillator strengths f12 and f23 associated with the 1 ĺ 2 and 2 ĺ 3 transitions, respectively. Here Te is the time constant associated with the broadening of state 3, which is attributed to the escape time. Equations 7.25 (together with Eq. 7.24) can be seen as a generalization of the twophoton quantum efficiency Ș(2) to the case of N quantum wells. The other mechanism is a sequential twostep absorption ȕ2step =
(
e2 4İ0nr mc
)
2
n2D f f 4T T T L w hȞ 12 23 1 2 e
(7.26)
where the population of subband 2 either is excited into 3 or decays with the time constant T1. While the two processes cannot be distinguished in a continuouswave experiment, they have different signatures in the autocorrelation traces in Fig. 7.16. In fact, the Ȥ 3 process manifests itself by interference fringes, limited with increasing time delay by the decay time T2 of the coherent intersubband polarization. Sequential absorption produces the “slow” decrease in the autocorrelation trace, prominent at larger time delays when the coherence has been lost. Interestingly, expressions 7.25 and 7.26 take the same value if the decoherence of the 1 ĺ 2 transition is entirely due to relaxation (i.e., absence of pure dephasing [50]), and the relation T2 = 2T1 holds. In the present experiment, the coherence loss is mainly caused by pure dephasing, such that ȕ2step is almost an order of magnitude larger than ȕ3Ȥ . Using an estimated value of Te = 50 fs (consistent with the line width of the measured 2 ĺ 3 absorption), Eq. 7.26 in fact yields a value of 1 × 107 cm/GW, which is in excellent agreement Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_310_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 310
Chapter Seven
with the experimentally observed twophoton absorption coefficient. 3 Even though ȕȤ 3 싮 ȕ2step, the Ȥ process is still dominant at short delay times, as Eqs. 7.25 and 7.26 refer to the timeintegrated response. 7.6 Conclusion In this chapter, we summarized the highspeed and nonlinear properties of QWIPs. We have shown that QWIPs can have high absorption, contrary to popular belief. Our study indicates that a 100well QWIP with 1 to 1.5 × 1012 cmí2 well doping is close to the optimum. Decreasing the doping leads to a reduction in absorption, while increasing the doping seems to only result in a spectral broadening. A further advantageous point of high doping is that it shortens the carrier lifetime, but this also leads to a disadvantageous point of lower photoconductive gain and lower responsivity. We have also shown that these highabsorption QWIPs can operate at elevated temperatures, even near room temperature. Furthermore, we have shown by various experimental techniques that QWIPs have high intrinsic speeds. It is also possible to go even higher (> 30 GHz) by, e.g., using an even shorter lifetime system such as the ptype valence band quantum well. Since limited work on QWIPs for highabsorption and nearroomtemperature operation has been carried out so far [51, 27, 28], further work will surely lead to better performance and will help to create new applications. We have also shown that by properly designing a doubleresonance quantum well, nonlinear absorption (ȕ = 1.3 × 107 cm/GW) is enhanced by more than three orders of magnitude higher than in previous, nonresonant devices. In this equidistant threelevel system, both coherent and sequential twophoton absorptions are necessarily present, and they manifest themselves through different experimental signatures, which also allow us to determine the dephasing time T2 and the intersubband relaxation time T1. This approach enables quadratic detection at much lower radiation density, and it is thus expected to make a substantial impact on the characterization and development of novel infrared and terahertz radiation sources. Twophoton QWIPs based on resonant optical transitions between three energetically equidistant subbands allow us to study the autocorrelation of weak infrared sources with unprecedented sensitivity and femtosecond temporal resolution. 7.7
Acknowledgments
We thank many of our coworkers and colleagues at both the National Research Council of Canada and FraunhoferInstitute for Applied SolidState Physics in Freiburg, Germany. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_311_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
311
References 1.
H. C. Liu, “Quantum well infrared photodetector physics and novel devices,” in Intersubband Transition in Quantum Wells: Physics and Device Applications I, H. C. Liu and F. Capasso, eds., Academic Press, San Diego, 2000, Semiconductors and Semimetals, vol. 62, chap. 3, pp. 126–196.
2.
S. D. Gunapala and S. V. Bandara, “Quantum well infrared photodetector focal plane arrays,” in Intersubband Transition in Quantum Wells: Physics and Device Applications I, H. C. Liu and F. Capasso, eds., Academic Press, San Diego, 2000, Semiconductors and Semimetals, vol. 62, chap. 4, pp. 197–282.
3.
H. Schneider, T. Maier, J. Fleissner, M. Walther, P. Koidl, G. Weimann, W. Cabanski, M. Finck, P. Menger, W. Rode and J. Ziegler, Electron. Lett. 40, 831 (2004).
4.
H. Schneider, T. Maier, J. Fleissner, M. Walther, P. Koidl, G. Weimann, W. Cabanski, M. Finck, P. Menger, W. Rode, and J. Ziegler, SPIE 5726, 35 (2005).
5.
M. A. Fauci, R. Breiter, W. Cabanski, W. Fick, R. Koch, J. Ziegler, and S. D. Gunapala, Infrared Phys. Technol. 42, 337 (2001).
6.
W. A. Cabanski, R. Breiter, W. Rode, J. Ziegler, H. Schneider, M. Walther, and M. A. Fauci, SPIE 4721, 165 (2002); in E.L. Dereniak and R.E. Sampson, eds., Infrared Detectors and Focal Plane Arrays VII.
7.
H. C. Liu, G. E. Jenkins, E. R. Brown, K. A. McIntosh, K. B. Nichols, and M. J. Manfra, IEEE Elect. Dev. Lett. 16, 253 (1995).
8.
H. C. Liu, J. Li, E. R. Brown, K. A. McIntosh, K. B. Nichols, and M. J. Manfra, Appl. Phys. Lett. 67, 1594 (1995).
9.
S. Ehret, H. Schneider, J. Fleissner, P. Koidl, and G. Böhm, Appl. Phys. Lett. 71, 641 (1997).
10.
S. Steinkogler, H. Schneider, R. Rehm, M. Walther, and P. Koidl, Appl. Phys. Lett. 81, 3401 (2002).
11.
S. Steinkogler, H. Schneider, M. Walther, and P. Koidl, Appl. Phys. Lett. 82, 3925 (2003).
12.
A. Y. Cho, ed., Molecular Beam Epitaxy, American Institute of Physics, New York, 1994.
13.
F. Capasso, Science 235, 172 (1987).
14.
G. Bastard, Wave Mechanics Applied to Semiconductor Heterostructures, Les Éditions de Physique, Les Ulis, France, 1988.
15.
C. Weisbuch and B. Vinter, Quantum Semiconductor Structures, Academic Press, Boston, 1991.
16.
A. Shik, Quantum Wells, World Scientific, Singapore, 1997.
17.
P. Harrison, Quantum Wells, Wires and Dots: Theoretical and Computational Physics, Wiley, New York, 1999.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_312_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response 312
18.
Chapter Seven
M. Helm, “The basic physics of intersubband transitions,” in Intersubband Transition in Quantum Wells: Physics and Device Applications I, H. C. Liu and F. Capasso, eds., Academic Press, San Diego, 2000, Semiconductors and Semimetals, vol. 62, chap. 1, pp. 1–99.
19.
B. F. Levine, J. Appl. Phys. 78, R1 (1993).
20.
K. K. Choi, The Physics of Quantum Well Infrared Photodetectors, World Scientific, Singapore, 1997.
21.
D. D. Coon and R. P. G. Karunasiri, Appl. Phys. Lett. 45, 649 (1984).
22.
H. C. Liu, M. Buchanan, and Z. R. Wasilewski, Appl. Phys. Lett. 72, 1682 (1998).
23.
B. F. Levine, K. K. Choi, C. G. Bethea, J. Walker, and R. J. Malik, Appl. Phys. Lett. 50, 1092 (1987).
24.
L. C. West and S. J. Eglash, Appl. Phys. Lett. 46, 1156 (1985).
25.
A. G. Steele, H. C. Liu, M. Buchanan, and Z. R. Wasilewski, Appl. Phys. Lett. 59, 3625 (1991).
26.
H. C. Liu, J. Appl. Phys. 73, 3062 (1993).
27.
H. C. Liu, R. Dudek, A. Shen, E. Dupont, C.Y. Song, Z. R. Wasilewski, and M. Buchanan, Appl. Phys. Lett. 79, 4273 (2001).
28.
T. Oogarah, H. C. Liu, E. Dupont, Z. R. Wasilewski, M. Byloos, and M. Buchanan, Semicond. Sci. Technol. 17, L41 (2002).
29.
H. C. Liu, R. Dudek, A. Shen, E. Dupont, C.Y. Song, Z. R. Wasilewski, and M. Buchanan, J. High Speed Electronics and Systems 12, 803 (2003).
30.
E. R. Brown and K. A. McIntosh, U.S. Patent 5,304,805, Apr. 19, 1994.
31.
R. Martini, R. Paiella, C. Gmachl, F. Capasso, E. A. Whittaker, H. C. Liu, H. Y. Hwang, D. L. Sivco, J. N. Baillargeon, and A. Y. Cho, Electron. Lett. 37, 1290 (2001).
32.
R. K. Richards, D. P. Hutchinson, C. A. Bennett, M. L. Simpson, H. C. Liu, and M. Buchanan, ECS Proc. 9821, 95 (1998); in S. S. Li, H. C. Liu, M. Z. Tidrow, and S. D. Gunapala, eds., Long Wavelength Infrared Detectors and Arrays: Physics and Applications VI.
33.
R. Paiella, F. Capasso, C. Gmachl, D. L. Sivco, J. N. Baillargeon, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, Science 290, 1739 (2000).
34.
R. Paiella, F. Capasso, C. Gmachl, H. Y. Hwang, D. L. Sivco, A. L. Hutchinson, A. Y. Cho, and H. C. Liu, Appl. Phys. Lett. 77, 169 (2000).
35.
T. Kondoh, Y. Miura, S. Lee, R. K. Richards, D. P. Hutchinson, and C. A. Bennett, Rev. Sci. Instrum. 74, 1642 (2003).
36.
R. K. Richards, D. P. Hutchinson, C. A. Bennett, T. Kondoh, Y. Miura, and S. Lee, Rev. Sci. Instrum. 74, 1646 (2003).
37.
H. C. Liu, J. Li, M. Buchanan, and Z. R. Wasilewski, IEEE J. Quantum Electron. 32, 1024 (1996).
38.
E. R. Brown, K. A. McIntosh, F. W. Smith, and M. J. Manfra, Appl. Phys. Lett. 62, 1513 (1993)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_313_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response Quantum Well Infrared Photodetector
313
39.
E. R. Brown, K. A. McIntosh, K. B. Nichols, F. W. Smith, and M. J. Manfra, “CO2laser heterodyne detection with GaAs/AlGaAs MQW structures”, in Quantum Well Intersubband Transition Physics and Devices, H. C. Liu, B. F. Levine, and J. Y. Andersson, eds., Kluwer, Dordrecht, Netherlands, 1994, pp. 207– 220.
40.
R. H. Kingston, Detection of Optical and Infrared Radiation, SpringerVerlag, New York, 1978.
41.
K. J. Siemsen and H. D. Riccius, Appl. Phys. A35, 177 (1984).
42.
T. Koizumi, H. Tashiro, K. Nagasaka, and S. Namba, Jpn. J. Appl. Phys. 23, L809 (1984).
43.
P. D. Grant, R. Dudek, L. Wolfson, M. Buchanan, and H. C. Liu, Electron. Lett. 41, 69 (2005).
44.
H. Schneider, T. Maier, H. C. Liu, M. Walther, and P. Koidl, Opt. Lett. 30, 287 (2005).
45.
T. Maier, H. Schneider, M. Walther, P. Koidl, and H. C. Liu, Appl. Phys. Lett. 84, 5162 (2004).
46.
H. C. Liu, E. Dupont, and M. Ershov, J. Nonlin. Opt. Phys. Mat. 11, 433 (2002).
47.
A. Zavriyev, E. Dupont, P. B. Corkum, H. C. Liu, and Z. Biglov, Opt. Lett. 20, 1886 (1995).
48.
S. Ehret and H. Schneider, Appl. Phys. B66, 27 (1998).
49.
W. Nessler , S. Ogawa, H. Nagano, H. Petek, J. Shimoyama, Y. Nakayama, and K. Kisho, J. Electron. Spectrosc. Rel. Phenom. 88, 495 (1998).
50.
R. A. Kaindl, K. Reimann, M. Woerner, T. Elsaesser, R. Hey, and K. Ploog, Phys. Rev. B24, 161308 (2001).
51.
H. Schneider, C. Schönbein, G. Bihlmann, P. van Son, and H. Sigg, Appl. Phys. Lett. 70, 1602 (1997).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH07_314_03/23/2006 Quantum Well Infrared Photodetector: HighAbsorption and HighSpeed Properties, and TwoPhoton Response
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_315_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
8 Intersubband Transitions in Quantum Dots
Pallab Bhattacharya, Xiaohua Su, and Subhananda Chakrabarti Department of Electrical Engineering and Computer Science University of Michigan Ann Arbor, Michigan
Adrienne D. StiffRoberts Department of Electrical and Computer Engineering Duke University Durham, North Carolina
Carl H. Fischer M.I.T. Lincoln Laboratory Lexington, Massachusetts
8.1 Introduction Bulk semiconductor materials are optically sensitive to a large portion of the electromagnetic spectrum, with their bandgap energy Eg ranging from the ultraviolet to the infrared (ir). However, the lowbandgap materials appropriate for detection and emission in the longand farir ranges ( 8 m) are inherently soft and brittle, and it can be difficult to epitaxially grow and fabricate ir devices with bulk active regions based on these materials. In addition, intrinsic long/farir photodetectors have limited applicability. However, many more options for extending the ir detection and emission ranges of compound 315
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_316_03/23/2006 Intersubband Transitions in Quantum Dots 316
Chapter Eight
semiconductors exist if the advantages of an extrinsic scheme are realized. As a result, largebandgap materials that are more amenable to various fabrication techniques become an option. An important extrinsic scheme is the reduced dimensionality of semiconductor active regions so that intersubband transitions are possible. Through epitaxial growth techniques, active region heterostructures with threedimensional (3D) quantum confinement, called quantum dots (QDs), can be realized. In this chapter, the strainedlayer epitaxy of a typical QD material system is described, the optoelectronic properties of intersubband transitions in QDs relevant to ir absorption and emission are discussed, and current research related to QD ir detectors and emitters is reviewed. 8.2 Molecular Beam Epitaxy of SelfAssembled Quantum Dots The rapid improvement of epitaxial growth techniques, such as molecular beam epitaxy (MBE) and metalorganic chemical vapor deposition (MOCVD), has enabled the routine growth of excellent compound semiconductor materials [1]. In particular, the epitaxial growth of quantumconfined heterostructures has been pursued for decades due to enhanced performance of electronic and optoelectronic devices using such materials in the active region. While MBE is well suited for the growth of quantum wells, in which the active region experiences quantum confinement in the growth direction only, achieving the 3D quantum confinement required for devicequality QDs is much more challenging. Currently, the most successful approach to achieve defectfree, multiplelayer, highdensity QD ensembles is the heteroepitaxy of coherently strained, 3D, selfassembled islands [2–9], a process referred to as the StranskiKrastanow (SK) growth mode [10, 11]. 8.2.1
StranskiKrastanow growth mode
Strainedlayer epitaxy is controlled by the strain energy between the substrate and the epitaxially grown overlayer, or epilayer. Typically, the epilayer is biaxially strained in the plane of the substrate and uniaxially strained in the perpendicular direction. For a thick substrate, the biaxial strain is determined from the bulk lattice constants of the substrate material as and the epilayer material al [12]: İ =
as í1 al
(8.1)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_317_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
317
When strain is incorporated into the epitaxial crystal coherently, the lattice constant of the epilayer parallel to the interface is forced to be equal to the lattice constant of the substrate. Consequently, the lattice constant of the epilayer perpendicular to the substrate is changed by the Poisson effect [12] İ 쌩= í
İ ı
(8.2)
where ı is the Poisson ratio. Therefore, compressive strain (al > as) reduces the parallel lattice constant of the epilayer and increases the perpendicular lattice constant, while tensile strain (al < as) increases the parallel lattice constant and reduces the perpendicular lattice constant. The strainedlayer epitaxy of the SK growth mode is limited by both the strain energy and the dislocation formation energy. In other words, for a lattice mismatch in the range from 1.8% to 10%, it is possible to grow a pseudomorphic, 2D epilayer, or wetting layer, that is latticematched to the substrate for very small thicknesses. Beyond some critical thickness, the strain energy in the system is relaxed by the formation of misfit dislocations at the epilayer/substrate interface. However, as long as the epilayer is below the critical thickness, the strain is absorbed coherently and minimal dislocations are produced by the formation of coherently strained 3D islands on the epilayer surface. Thermodynamic considerations have demonstrated that the minimum Helmholtz freeenergy surface configuration in a coherently strained system is not atomically flat, but has a 3D form [13]. Thus, selfassembled QDs result from the minimization of the Helmholtz free energy during strainedlayer epitaxy such that thermodynamic equilibrium is achieved in the heterostructure. Note that thermodynamic equilibrium includes the effect of microscopic, kinetic processes of adatoms on the crystal surface, such as diffusion. Thermodynamic equilibrium is achieved when the total free energy is minimized, given a fixed amount of deposited material. The driving forces for achieving equilibrium in these selfassembled QDs are elastic relaxation at the facet edges, straininduced renormalization of the surface energy at the facets, and interaction between neighboring islands via the substrate. 8.2.2 Standard MBE growth technique for InAs/GaAs QDs
The lattice mismatch at the interface of an InAs epilayer and a GaAs substrate is
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_318_03/23/2006 Intersubband Transitions in Quantum Dots 318
Chapter Eight
f =
aInAs í aGaAs aGaAs
§ 7%
(8.3)
where the lattice constant in InAs is 6.06 Å and the lattice constant in GaAs is 5.65 Å. Therefore, the SK growth mode for the selfassembly of 3D islands will occur under appropriate growth conditions. The typical InAs growth rate is 0.1 ML/s, and the GaAs substrate temperature is usually cooled to 500ºC. This slow rate, coupled with the low substrate temperature, enables the selfassembly of QDs since surface kinetics are minimized and thermodynamic equilibrium by the coherent incorporation of strain can be achieved more easily. The wetting layer thickness in the InAs/GaAs QD system is 1.7 monolayers (ML), where 1 ML ~ 2.83 Å for IIIV materials. The transition from the 2D wetting layer to 3D islands is observed by using in situ reflection highenergy electron diffraction (RHEED), in which a streaky pattern gives way to a spotty pattern when QDs begin to form. Once this transition is observed, InAs overgrowth occurs for 2 to 5 s to provide enough InAs charge (2.2 ML) for pyramidal QDs, and a 30s growthinterrupt pause is used to allow the complete formation of QDs. After this pause, an intrinsic GaAs cap layer (~25 to 60 nm) is grown on top of the InAs QDs, thereby completing the QD potential barrier. This sequence of growth can be repeated to achieve a specified number of QD layers. For a given volume of a coherently strained island, there exists an equilibrium shape. For growth along the [100] direction in the InAs/ GaAs QD system, the selfassembled QDs can be lens or pyramidshaped with a base in the (100) plane [14]. For typical growth parameters used in MBE or MOCVD, an ensemble of InAs/GaAs QDs has lateral sizes ranging from 15 to 25 nm and heights ranging from 5 to 8 nm. The surface density of InAs/GaAs QDs ranges from 109 to 1011 cmí2. An AFM image of an ensemble of InAs/GaAs QDs grown by MBE at 500°C at a rate of 0.1 ML/s is shown in Fig. 8.1. From this image, the dot density is estimated to be 1 × 1011 cmí2. While the SK growth mode is well established, having been reported first in 1938, there is still much to learn about the controlled growth of selfassembled QDs, particularly those with devicequality electrical and optical properties. In particular, since the SK growth mode is a random process, QD ensembles suffer from large inhomogeneous line width broadening, which adversely affects photonic device properties. In addition, the nonuniform size distribution of the QD ensemble makes it difficult to control the intersubband spacing for ir transitions. The SK growth mode also introduces challenges due to the buildup of strain for repeated dot layers. Thus, the selfassembly of QDs is a complicated process, subject to many parameters for controlling epitaxial growth.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_319_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
319
Figure 8.1 AFM image of 2.2ML InAs quantum dots on GaAs grown at 500°C (1m
scale).
8.3
Quantum Dot Intersubband Transitions
In this section, the optoelectronic properties of intersubband transitions in QDs are discussed, including boundstate energy levels, density of states, intersubband transition rates, and the phonon bottleneck. The determination of these quantities is complicated since the strain field at the heterojunction heavily influences the potential barrier and the resulting electronic band structure. However, it is important to understand these quantities as they are responsible for important differences in the performance of intersubband photonic devices featuring quantum well and quantum dot active regions. 8.3.1
Optoelectronic properties
Boundstate energy levels. The eightband k·p theory is used to deter
mine the electronic band structure in semiconductor heterostructures near the band edge only. For devices that operate using carrier phenomena near the band edge, the k·p perturbation theory not only is simple, but also yields very accurate results. An important advantage of this approach is the inclusion of the influence of remote bands. This is particularly important for strained systems such as QD heterostructures since the conduction band and valence band cannot be decoupled Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_320_03/23/2006 Intersubband Transitions in Quantum Dots 320
Chapter Eight
in the presence of large strain fields. In the eightband k·p model, only the nearest eight bands with sufficiently small energy differences from the given state are assumed to contribute to the solution [12]. In applying the k·p theory to selfassembled QDs, it is necessary to take into account the unique strain distribution of these coherently strained, quasizerodimensional heterostructures. As has been demonstrated experimentally, the large builtin strain of the QDs causes a significant change in the properties of the electronic band structure. For example, the bandgap of InAs/GaAs QDs has been measured to be ~1.05 eV, even though the intrinsic bandgap of bulk InAs is 0.4 eV [14]. Thus the effect of strain is incorporated into the energy band structure of a semiconductor by (1) determining the elastic strain energy of the system and (2) including this energy in the hamiltonian as an additional perturbation through deformation potential theory. Jiang and Singh [14] have used the valence force field (VFF) model [15, 16] to determine the strain distribution in selfassembled InAs/GaAs QDs for the eightband k·p calculation of the electronic band structure. To find the strain tensor in selfassembled QDs, they begin with an arbitrary choice of the atomic position and minimize the system energy, using the hamiltonian for the elastic strain energy. This determines the appropriate configuration of the atoms for calculating the strain distribution, yielding a very detailed strain tensor for QDs and the surrounding barrier material. They then use the finitedifference method to solve the matrix equation for the perturbed, k·p hamiltonian. By using the eightband k·p model developed by Jiang and Singh, the first four bound states in the conduction band of pyramidal InAs/GaAs QDs with dot height of 6.8 nm and base width of 13.5 nm have been calculated. The spatial dependence of the electron wave functions for the four doubledegenerate energy levels is shown in Fig. 8.2a. The listed energy levels are assumed to be from the InAs valence band edge. In Fig. 8.2b, the QD intersubband energy levels in the conduction band are shown schematically, assuming that the bandgap in strained InAs is 1.05 eV. According to this calculation, boundtobound transitions from the QD ground state to the top excited state correspond to 9.25 ȝm. Thus, the electron intersubband energies can vary greatly (from ~50 to 500 meV) depending on the QD size, composition, and heterostructure band offsets. Another unique property of QDs is the zerodimensional density of states, which leads to favorable carrier dynamics in photonic devices. In the case of QDs, kspace is zerodimensional and can be represented by a point. As a result, the density of states in kspace is infinite for each state of constant energy. Thus, unlike bulk
Density of states.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_321_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots ε0=1.327 eV
Ec
ε1=1.406 eV
GaAs
ε2=1.411 eV
ε3=1.461 eV
321
ε3 = 0.411 eV ε2 = 0.361 eV
ε1 = 0.356 eV ε0 = 0.277 eV
InAs (a)
(b)
Figure 8.2 Calculated energy levels using eightband k·p model for InAs/GaAs QD with height of 6.8 nm and base width of 13.5 nm. (a) Spatial variation of the electron wave function for the first four boundstate energy levels (with respect to the InAs valence band edge); (b) schematics of InAs QD intersubband energy levels in the conduction band assuming an InAs bandgap of 1.05 eV in strained QDs.
material or quantumconfined structures in one and two dimensions, the QD does not have a continuous density of states for any direction. However, this infinite density of states is for an ideal QD. In reality, the size of QDs varies spatially such that the density of states is actually represented by inhomogeneously broadened į functions in a gaussian distribution. For instance, the joint density of states can be written as N(ലȦ) =
(E fi í ലȦ)2 1 exp 2ʌı 2ı2
(8.4)
where Efi is the energy separation between states f and i and ı is the gaussian line width of the transition. The QD electronic density of states and corresponding electron distribution are shown schematically in Fig. 8.3a and b, respectively. Despite such inhomogeneous broadening, the discrete nature of the density of states leads to significant results in terms of the carrier N (E )
Ec
Quantum dot
E
c
E1
E2 (a)
E2
 
E1
 
E (b)
Figure 8.3 Schematic diagrams of (a) the density of states in QDs and (b) the corresponding carrier distribution in QDs.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_322_03/23/2006 Intersubband Transitions in Quantum Dots 322
Chapter Eight
dynamics in QDs. It is clear that as the dimensionality of the active region is reduced, the energy levels and density of states become quantized. In addition, the electron distribution is maximized near the conduction band edge, and it is independent of temperature to a large extent. However, at room temperature, highenergy states of QDs become occupied, where the density of states is threedimensional and continuous. Thus, as the temperature increases, the advantages that result from quantum confinement become less pronounced. Fermi golden rule. The Fermi golden rule, derived by using firstorder, timedependent perturbation theory, determines the transition rate of electrons from some initial state i to some final state f . In the case of electron interactions with an electromagnetic field, this transition occurs due to the absorption or emission of a photon. The Fermi golden rule for these processes is
W(i) =
2ʌ  f  H1 i 2 į(E f í Ei ലȦ) ല f
(8.5)
where the minus sign indicates absorption and the plus sign indicates emission. Here H1 represents the firstorder perturbation to the hamiltonian in the timedependent Schrödinger equation H1 =
íe ieല ^ A썉 ෮ = A썉 p mc mc
(8.6)
where e is the electron charge, c is the velocity of light, and A is the vector potential whose direction is equal to that of the electric field. Thus, the momentum matrix element between the initial and final p i must be evaluated in the direction of the vector states p fi 싥 f p potential a or, equivalently, the polarization of the electric field. The momentum matrix element for intersubband transitions is calculated by using the electron wave functions determined by the eightband k·p model in pyramidal QDs
p fi = f  p i = ĳ fj ĳ ik u j p uk + ĳ fj p ĳij j, k
j
(8.7)
where ĳ and u are the envelope and centralcell functions, respectively. Due to considerable band mixing in QDs, the first summation term is nonzero, as is often the case in intraband transitions in quantum wells, and therefore cannot be excluded from the calculation. An important aspect of the momentum matrix element is that, in conjunction with the polarization of the electric field, it determines the selection rules for permitted transitions in which photons are absorbed (or emitted). In contrast to quantum wells, quantum dots are sensitive to both normal Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_323_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
323
and lateral incident radiation, which is an important advantage for photonic devices. Once the rate of photon absorption Wabs is known, it is relatively straightforward to determine the absorption coefficient Į by considering the continuity equation for the photon density nph under steadystate conditions: Į=
Wabs cnph
(8.8)
In the case of a QD ensemble, the absorption coefficient for photons with energy ƫȦ is Į(ലȦ) =
ʌe 2ല 1  a썉p fi2 N(ലȦ) 2 İ0n0cm0Vav fi ലȦ
(8.9)
where İ0 is the permittivity of free space, n0 is the index of refraction, Vav is the average dot volume, and N(ʄȦ) is the intersubband joint density of states for QDs. Given the gaussian distribution of this density of states, the absorption coefficient can be calculated as a function of the photon energy or, equivalently, the incident wavelength. Therefore, typical absorption spectra have a peak absorption coefficient at the wavelength corresponding to the average intersubband transition and a line width that depends on the uniformity of the QD ensemble. Phonon bottleneck. The carrier dynamics in 3D, quantumconfined het
erostructures differ significantly from those of bulk materials and quantum wells. The most significant scattering processes for electrons occupying the excited energy levels in QDs have been identified as [17] electronphonon scattering due to a singlephonon process, electronmultiphonon scattering, electronhole scattering, and electronelectron scattering. In addition to these carrier relaxation processes, transport mechanisms play integral roles in determining: (1) the carrier relaxation time from a QD excited state to the ground state, (2) the carrier capture time from the continuum to a QD bound state, and (3) the effective carrier lifetime, which describes the time elapsed before a photoexcited carrier falls into the ground state of any QD. Note that while firstorder, electronphonon interactions cause rapid relaxation in bulk and quantum well semiconductor materials, electronphonon coupling is suppressed in QDs due to the magnitude of the intraband energy spacing between confined levels in QDs [18, 19]. More specifically, the intraband energy spacing is > 50 meV for practical QD sizes, while the longitudinal optical (LO) phonon energy is < 40 meV [20]. Thus conservation of energy cannot be satisfied with the emission Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_324_03/23/2006 Intersubband Transitions in Quantum Dots 324
Chapter Eight
of a single LO phonon. Similarly, single longitudinalacoustic (LA) phonon emission (achieved by coupling with the deformation potential) is reduced for intraband energy spacings greater than a few millielectronvolts [21]. This reduction of electrophonon scattering for QDs, which leads to longer electron lifetimes in QDs (and increased photoconductive gain in detectors), is known as the phonon bottleneck. Several experiments have been conducted to confirm the existence of the phonon bottleneck, including electroluminescence and timeresolved photoluminescence measurements of InGaAs/GaAs QDs [22], highfrequency electrical impedance measurements in In0.4Ga0.6As/ GaAs QD lasers [23], and timeresolved differential transmission spectroscopy (DTS) measurements of In0.4Ga0.6As/GaAs QDs [24]. Thus, the suppression of phonon scattering in QDs suggests that electron relaxation lifetimes are significantly longer than those in quantum wells (QWs) (~1 to 10 ps) [25], which are dominated by scattering due to the emission of single optical phonons. The phonon bottleneck also affects the effective carrier lifetime in QDs, resulting in unique carrier dynamics that are beneficial to the operation of both intersubband detectors and emitters. For detectors, the long lifetime of the carriers in the higherenergy dot states ensures that photoexcited carriers will contribute to the photocurrent. In intersubband light emitters, a long effective lifetime in the upper states implies that the intersubband stimulated emission time can also be large, and therefore the threshold current can be low. In addition, the phonon bottleneck is also promising for temperatureindependent performance since the electrons are energetically decoupled from the optical phonon, whose properties depend very heavily on temperature. Note that the carrier configuration in QDs, i.e., geminate versus nongeminate, significantly influences the effect of the phonon bottleneck. For a geminate QD configuration in which electrons and holes are present simultaneously, electronhole scattering increases due to the strong overlap between the two carriers. However, for a nongeminate QD configuration in which only electrons or only holes are present, electronhole scattering is reduced. As a result, the phonon bottleneck contributes to increased gain in QD intersubband detectors since the carrier density is low and nongeminate configurations dominate. In the case of bipolar QD intersubband emitters, the carrier density is much higher, leading to geminate configurations and increased electronhole scattering that can dominate the effect of the phonon bottleneck. 8.3.2
Intersubband absorption
Intersubband absorption in QDs spans a broad spectrum of ir wavelengths, including the nearir (NIR) from 1 to 3 m, the midir (MIR) Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_325_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
325
from 3 to 5 m, the longir (LIR) from 8 to 14 m, and the farir (FIR) for wavelengths greater than 14 m. The first observation of intersubband absorption in QDs [26] reported absorption in the 13 to 15m spectral range. Since then, intersubband absorption has been reported throughout the ir spectrum by varying the QD heterostructure through epitaxial growth conditions, QD material composition, and/or modification of the QD barrier layer [27–34]. In general, there are two types of intersubband transitions that can originate in the QD. The first type of transition, in which ground state electrons are photoexcited to excited states of the QD, is called a boundtobound (BB) transition. The second type of transition is called boundtocontinuum (BC), and in this case an electron in a ground or excited state is photoexcited out of the QD into the continuum of energy levels near the barrier bulk material band edge. For either case, the intersubband absorption process requires the presence of electrons in a bound state of the QD. Electrons can be introduced in the QD by direct doping [35], modulation doping [36], or capture of injected electrons from the device contact [37]. It has been shown that quantum dot infrared photodetector (QDIP) performance has a distinct tradeoff between, and dependence on, QD density and dopant concentration [38]. For this reason, it is customary to design QDIPs with doping such that there are approximately two electrons per QD. The dark current increases for higher dopant densities, and the absorption efficiency decreases for lower dopant densities. The absorption coefficient is an important quantity for determining the applicability of a given QD active region to the detection of ir light in that it determines, in part, both the quantum efficiency of the device and the spectral response. The QD absorption spectrum is generally broad due to the size variation of QDs comprising the active region of a device. Therefore, QD ir photodetectors experience a tradeoff between absorption strength and absorption line width. For example, a perfectly uniform QD ensemble will have large peak absorption and a narrow absorption line width since all the dots experience peak absorption at the same wavelength. However, a nonuniform QD ensemble will have reduced peak absorption and a broad absorption line width since many dots with varying sizes experience peak absorption at different wavelengths. Thus, even though each QD individually has sharp atomlike electronic states, for an ensemble of QDs the inhomogeneous gaussian line width of the density of states ı (measured in millielectronvolts) significantly influences the absorption. Specifically, the peak absorption coefficient Į (measured in cmí1) is inversely proportional to the line width [39] Įѩ
3.5 × 105 ı
(8.10)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_326_03/23/2006 Intersubband Transitions in Quantum Dots 326
Chapter Eight
8.3.3
Intersubband emission
The greatest challenge to controlling intersubband transitions in QDs for ir emitters is the achievement of population inversion between ground and excited states. For population inversion to occur, the energy relaxation time between the upperlevel excited states and the ground state Ĳu1 should be as long as possible, and the lifetime of electrons in the ground states Ĳ1 should be very short. Providing a high density of coherent photons in the cavity, which can greatly reduce the interband electronhole recombination time Ĳstim, can decrease the lifetime of the electron in the ground state. By using a bipolar scheme, a high density of coherent photons can be made available in the intersubband laser cavity by simultaneous interband lasing due to current injection. To examine population inversion between the ground state and the excited dot states, the following rate equations are solved selfconsistently: dnu dt
=
Șin í
dn1 dt
=
J nu gu(1í f 1) n1 g1(1í f u) í + e Ĳ1u Ĳu1
nu gu f u f h nphunu gu(1í f uí f h) + =0 Ĳu Ĳu
( 1íȘin )
í
nu gu(1í f 1) n1 g1(1í f u) J + í e Ĳu1 Ĳ 1u
(8.11)
n1 g1 f 1 f h nph1n1 g1(1í f 1í f h) + =0 Ĳ1 Ĳ1
where Șin is the injection efficiency; nph1 and nphu are the densities of photons that are involved in the lasing process from the ground states and the excited states, respectively; n1 and nu are the densities of electrons in the ground states and excited states, respectively; and f1 and fu are the occupational probabilities of the ground states and excited states, respectively. The degeneracy of the ground state (g1 = 2) and the excited states (gu = 4) [14] is taken into account in the rate equation calculations. Interband recombination times for the ground state Ĳ1 (= 700 ps) and the excited state Ĳu (= 250 ps) have been derived from timeresolved photoluminescence measurements [40], and an intersubband relaxation time of Ĳu1 = 60 ps is assumed. A thermal distribution of holes is used (fh = 0.45). When nph1 is zero, f1 > fu for all values of the injection current, and no population inversion is possible. However, when nph1 is increased to 50, f1 is pinned at a value of
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_327_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
327
~0.5, whereas fu increases linearly with the current. Similarly, when nphu is increased to 50, f1 > fu for all values of injection. This is consistent with the fact that if nphu = 50, interband lasing occurs from the excited state in the dot and no MIR emission results. The intersubband population inversion and lasing processes, together with the bipolar recombination, are illustrated in Fig. 8.4.
Ee2
FIR Ee1
~1 μm Ehh Figure 8.4 Schematic illustration of electronic bound states, carrier relaxation processes, and intersubband population inversion in QDs.
8.4 Quantum Dot Intersubband Photonic Devices Quasizerodimensional QD heterostructures with intersubband transitions in the ir are important for numerous military, commercial, and scientific photonic device applications. The ir detectors and the resultant imaging capability are useful for military targeting and tracking, law enforcement, medical diagnoses, and space science, while ir emitters can be used for optical spectroscopy, pointtopoint atmospheric communication, fiberoptic telecommunication, and optical radar. In particular, intersubband photonic devices comprising QDs offer several favorable attributes due to their threedimensional quantum confinement. Quantum dot infrared photodetectors are inherently sensitive to normalincidence light, can achieve hightemperature operation (> 150 K), and have low dark currents. Quantum dot infrared emitters benefit from advantages such as hightemperature operation, low threshold current, and high modulation bandwidth. 8.4.1
Quantum dot infrared detectors
QD active region heterostructures result in several advantages that should enhance ir detection in QDIPs [30, 35, 41–50]. The 3D quantum
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_328_03/23/2006 Intersubband Transitions in Quantum Dots 328
Chapter Eight
confinement of electrons leads to low dark currents in QDIPs. The boundstate, atomlike energy levels that depend on QD size and shape provide tunability of the ir absorption wavelengths and of the spectral responsivity. The carrier distribution that results from the zerodimensional density of states in QDs is beneficial in that it reduces the temperature dependence of the QDIP characteristics. The phonon bottleneck in QD carrier relaxation leads to increased gain, quantum efficiency, and responsivity. In addition, QDIPs are inherently sensitive to normalincidence ir radiation due to the polarization selection rules. Finally, since electrons and holes are localized due to quantum confinement, in general photonic devices with QD active regions exhibit better defect and radiation tolerance. Both the increased electron lifetime and the reduced dark current indicate that QDIPs should be able to provide hightemperature operation ( 150 K). Several QDIP heterostructure designs have been investigated for use as ir photodetectors in addition to the standard InAs/GaAs QDIP. As an example, InAs QDs embedded in a strainrelieving InGaAs quantum well are known as dotinawell (DWELL) heterostructures. QDIPs using a DWELL heterostructure not only permit greater control over wavelength tunability, but also have demonstrated excellent device performance [51–54]. QDIPs using an undoped active region of InAs quantum dots grown directly on AlGaAs with a GaAs cap layer have also demonstrated promising device performance [37]. Other IIIV material systems under investigation include InAs/InAlAs QDs grown on InP [55] and InGaAs/InGaP QDs grown on GaAs [56–58]. Intersubband transitions in the ir have also been observed in the valence band of Ge/Si QDs [59–64]. Three QDIP designs demonstrating stateoftheart performance are discussed in greater detail in the following sections. Some 70 layers of InAs/GaAs QDs were grown by MBE in an attempt to increase the absorption, and thereby the quantum efficiency, in QDIPs [65]. Including 70 QD layers in the InAs/GaAs QDIP increased the amount of absorbed ir light and contributed to better detector performance. In addition, 50nm GaAs barriers required for reducing dislocation propagation in the large QD stack contribute to extremely low dark currents in the 70layer QDIP. Schematic diagrams of the device heterostructure and conduction band profile under bias are shown in Fig. 8.5a and b, respectively. Figure 8.6a shows the dark current densities for T = 140, 160, and 200 K (measured at the Jet Propulsion Laboratory), demonstrating extremely low dark currents at elevated temperatures (Jdark = 2.3 × 10í6 A/cm2, Vbias = í2.0 V, T = 160 K). The spectral responsivity, as
The 70layer InAs/GaAs quantum dot infrared photodetector.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_329_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
200nm GaAs n+ contact
329
GaAs n+ contact
40nm Al0.3Ga0.7As buffer (i)
x 70
50nm GaAs barrier (i)
x 70
Al0.3Ga0.7As barrier
GaAs barrier
2.2ML InAs QDs (n+) 50nm GaAs buffer (i) 500nm GaAs n+ contact
InAs QDs GaAs n+ contact
S.I. GaAs substrate
(b)
(a)
Schematic diagrams of (a) the MBE device heterostructure and (b) the conduction band profile under bias in the 70layer InAs/GaAs QDIP. Figure 8.5
Peak responsivity (A/W)
Dark current density (A/cm2)
0.40
T = 200 K
103
T = 160 K
105 107 109
T = 140 K
1011
T = 150 K
4.0 V 0.30
3.0 V
0.20
2.0 V 0.10
1.0 V 0.00
3
2
1
0
1
2
3
2.0
3.0
4.0
5.0
Bias voltage (V)
Wavelength (μm)
(a)
(b)
6.0
Figure 8.6 (a) Dark current density as a function of bias voltage for T = 140, 160, and 200 K; (b) measured spectral peak responsivity for different bias voltages at T = 150 K in the 70layer InAs/GaAs QDIP.
shown in Fig. 8.6b, peaks at 0.34 A/W for Ȝpeak = 3.65 ȝm at Vbias = 4.0 V and T = 150 K. Using the measured dark current and spectral responsivity, the peak specific detectivity and the noiseequivalent temperature difference were estimated for the 70layer InAs/GaAs QDIP. The peak detectivity, shown in Fig. 8.7 as a function of temperature, is ~1011 cm·Hz1/2/W at T = 100 K and ~6 × 109 cm·Hz1/2/W at 200 K. These expected detectivities indicate that the 70layer QDIP will provide hightemperature performance, currently unattainable in ir photodetectors, due to the simultaneous reduction of dark current by the GaAs barrier and increase of responsivity by the 70layer absorption region. Therefore, by carefully designing the 70layer InAs/GaAs QDIP heterostructure to minimize dark current and maximize absorption, this device provided low dark current and relatively high responsivity at elevated operating temperatures. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_330_03/23/2006 Intersubband Transitions in Quantum Dots
Peak detectivity (cm • Hz1/2/W)
330
Chapter Eight
1012
Vbias = 2.0 V 1011
1010
109 100 Figure 8.7
120
140 160 180 Temperature (K)
200
Estimated peak specific detectivity in the 70layer InAs/GaAs QDIP.
Highresolution and highsensitivity imaging using ir focal plane arrays requires multicolor detectors. The performance characteristics of In0.4Ga0.6As/GaAs QDIPs with peak wavelength responses at ~3.5, 7.5, and 22 ȝm have been reported. This was the first report of multiwavelength detection in QDIPS, with operating temperatures as high as 120 k, based solely on intersubband transitions within the QDs [66]. The In0.4Ga0.6As/GaAs QDIP heterostructure is shown schematically in Fig. 8.8. The use of n+ substrates minimized multiple reflections in the substrate. The active region of the device consists of 20 QD layers separated by 50nm GaAs barrier layers. The measured threecolor spectral response is shown in Fig. 8.9 and its inset. The origin of the three peaks, centered at 3.5, 7.5, and 22 m, can be understood from the electronic states of the InGaAs quantum dots calculated with an eightband k·p formulation [12]. The peak centered at 22 ȝm arises due to transitions of photoexcited electrons Multicolor In0.4Ga0.6As/GaAs quantum dot infrared photodetector.
0.2μm n+ GaAs (n = 5 × 1018 cm3) 500Å GaAs barrier × 20 6ML In0.4Ga0.6As/GaAs QDs 500Å iGaAs spacer 0.2μm n + GaAs buffer (n = 5 × 1018 cm3) n + GaAs substrate (n = 1019 cm3) Figure 8.8
MBE.
Schematic of the 20layer In0.4Ga0.6As/GaAs QDIP heterostructure grown by
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_331_03/23/2006 Intersubband Transitions in Quantum Dots
1.0
Photoresponse (arb.units)
Photoresponse (arb.units)
Intersubband Transitions in Quantum Dots
0.5
T = 80 K
331
2.0 V
1.0 V
1.5
3.5 5.5 7.5 Wavelength (μm)
0 1
6
11
16
21
26
Wavelength (μm) Figure 8.9 Spectral response of the 20layer InGaAs/GaAs QDIP at T = 20 K. The inset shows the normalized twocolor response at 80 K.
0.1
T = 80 K λ = 7.5 μm
0.08
Detectivity (cm•Hz1/2/W)
Peak responsivity (A/W)
from the ground states to the first excited states (ǻE ~ 50 to 60 meV) while the one at 7.5 ȝm (155 meV) is believed to be due to transitions from the dot ground states to the GaAs barrier states or the wetting layer states. The broad response with peak at 3.5 ȝm is probably due to boundtocontinuum transitions from the dot ground states to dot levels in the continuum. The peaks at 7.5 and 22 ȝm, resulting from transitions between quasibound states, are narrower (ǻȜ/Ȝ ~ 0.2) than the one at 3.5 ȝm resulting from boundtocontinuum transitions (ǻȜ/Ȝ ~ 0.79). The 22ȝm transition is observed distinctly at very low temperatures (~20 K) and disappears with an increase of temperature as the excited states become more populated and thereby the rate of transitions into these states decreases. The peak responsivity of the 20 dotlayer device for the 7.5ȝm photoresponse, plotted in Fig. 8.10a as a function of bias for T = 80 K, is adequately high for application in focal plane arrays. The specific detectivity D* was obtained from the measured peak responsivity and
0.06 0.04 0.02 0 1
2 3 Voltage bias (V)
(a)
4
5.E+10
T = 80 K λ = 7.5 μm
4.E+10 3.E+10 2.E+10 1.E+10 0.E+00 1
2 3 Voltage bias (V)
4
(b)
Measured (a) peak responsivity and (b) peak detectivity as a function of applied bias for the 7.5ȝm response at T = 80 K in multicolor In0.4Ga0.6As/GaAs QDIPs.
Figure 8.10
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_332_03/23/2006 Intersubband Transitions in Quantum Dots 332
Chapter Eight
noise density spectra at different temperatures and applied biases. These measured values of D* are plotted in Fig. 8.10b as a function of bias for the 7.5ȝm response at 80 K. Detectivity D* reaches a maximum of 4.8 × 1010 cm·Hz1/2/W at 3 V and decreases thereafter, due to the monotonic increase of the dark current with bias. These values of D* are among the highest measured for QDIPs in the LWIR range and are attributed to the extremely low dark currents measured in these devices. Resonant tunneling In0.4Ga0.6As/GaAs quantum dot infrared photodetector. In the commonly investigated vertical QDIPs, with or
without confined dot layers, the dark current is determined by thermionic emission and fieldassisted tunneling. The dark current can be effectively reduced by increasing the dot confinement potential, by increasing the thickness of the active region, or by incorporating additional energy barriers. Unfortunately, these measures also reduce the photocurrent, since the transport paths of the carriers are identical. It is therefore essential to explore device designs by which the dark current can be decoupled from the thermal background which enhances thermionic emission at high operating temperatures, but the device photocurrent is not affected. The properties of a novel QDIP design in which a resonant tunneling heterostructure is incorporated with each QD layer have been reported recently [67–69]. The heterostructure and conduction band diagram of a single period of the active region are schematically shown in Fig. 8.11a and b respectively. The resonant tunneling double barrier is designed so that the electron tunneling probability is unity at the energy of the final state of the photoexcited electrons. At energies sufficiently removed from this resonance, the tunneling probability is small; thus the transport of the carriers contributing to the dark current, which have a broad energy distribution at high temperatures, will be reduced. A single Al0.1Ga0.9As barrier is also included on the side of the dots opposite to the tunnel barriers. The inclusion of this layer creates a quantum well and quasibound final states for the photoexcited electrons from the QDs. These states are designed to resonate with the tunnel states in the doublebarrier heterostructure. Furthermore, the energy position of the states in the well can be tuned by varying the distance of the AlGaAs barrier from the quantum dot layer, thereby providing tunability of the absorption peak wavelength. In Fig. 8.12 measured dark current data at 140 K are compared with calculated values for both conventional and tunnel QDIPs (TQDIPs). It is evident that there is good agreement between calculated and measured dark currents, and there is a significant reduction in dark currents with the incorporation of the resonant tunnel filters. The Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_333_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
0.3μm n+ GaAs 40Å Al0.1Ga0.9As
333
Al0.3Ga0.7As Al0.1Ga0.9As
40Å GaAs In0.4Ga0.6As QDs
Photocurrent path
10Å GaAs 30Å Al0.3Ga0.7As 40Å In0.1Ga0.9As
0
×10
73 meV
30Å Al0.3Ga0.7As
102 meV
400Å GaAs
161 meV
0.5μm n+ GaAs S.I. GaAs substrate
In0.1Ga0.9As
GaAs
InGaAs/GaAs quantum dot
(a)
(b)
Figure 8.11 (a) Schematic heterostructure and (b) conduction band profile of an InAs/
GaAs TQDIP with a GaAs/Al0.3Ga0.7As resonant tunneling heterostructure under an applied bias. The calculated energy levels in the well and dot are indicated.
Dark current density (A/cm2)
100
T = 140 K
QDIP
102
104 TQDIP
106 Calculated Measured
108 0
0.5
1.0 Bias voltage (V)
1.5
2.0
Figure 8.12 Comparison of calculated and measured dark current densities as a function of bias voltage at T = 140 K for conventional and tunneling QDIPs using In0.4Ga0.6As/ GaAs quantum dots.
disagreement at large bias values is due to nonequilibrium conditions which were neglected in our calculation. Figure 8.13a and b depicts the midir spectral response of the TQDIP for different bias values and different ambient temperatures (up to 300 K), respectively. The peak wavelength is in excellent agreement
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_334_03/23/2006 Intersubband Transitions in Quantum Dots 334
Chapter Eight
0.05
4.0 V
T = 80 K
0.6
0.4
3.0 V
0.2
2.0 V 0
3
5
7
Wavelength (μm)
(a)
9
Responsivity (A/W)
Responsivity (A/W)
0.8
0.04
Bias = 1.0 V
200 K
0.03 0.02
240 K 300 K
0.01 0
3
5
7
9
Wavelength (μm)
(b)
Figure 8.13 Measured spectral responsivity of the TQDIP: (a) in the bias range 2–4 V at 80 K and (b) in the temperature range 200–300 K under 1V bias.
with the designed and calculated transition energy of 161 meV for the photoexcited electrons from the ground state in the QD to the quasibound state in the well. The spectral response exhibits closely spaced dual peaks with an energy separation of ~15 meV. The dual peaks arise from coupling and splitting of the wave functions of the quantum well states and the bound states of the doublebarrier heterostructure and provide evidence of resonant tunneling in the operation of the device. From the data of Fig. 8.13a and b, the peak responsivity is 0.75 A/W (4V bias at 80 K) and ~0.01 A/W (1V bias at 300 K). Longir response at 17 ȝm is observed in the TQDIPs at higher temperatures, as shown in Fig. 8.14. This 17ȝm response peak intensity increases with temperature, and at 300 K its peak responsivity is higher than that of the 6ȝm peak. With reference to the calculated energies of the bound and quasibound states in the dot and well, shown in Fig. 8.11b, this peak results from transitions from the second excited state of the dot to the well state (ǻE = 73 meV). The transition line width of ~26 meV is close to the inhomogenenous broadening of the QD states at 300 K. We believe that the longir transition is dominant at high temperatures because the probability of occupation of the dot excited states increases with temperature. Due to the symmetry of the dot geometry, the excited states have a higher degeneracy than the ground state. Additionally, for the same incident power, there are more photons at 17 ȝm than at 6 ȝm. It is extremely important to note that it is the low dark current in the TQDIP that makes detection possible at these high temperatures. The measured values of D* for midir peaks at T = 80 K reach a maximum value of 2.4 × 1010cm·Hz1/2/W at 2 V and decrease again due to the monotonic increase of the dark current with bias. The values of
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_335_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
335
0.20 T = 300 K Bias = 2.0 V Responsivity (A/W)
0.15
0.10
0.05
0
10
12
14 16 Wavelength (μm)
18
20
Figure 8.14 Measured spectral responsivity of the TQDIP in the long wavelength range
at 300 K under a bias of 2 V.
D* for the 17ȝm response at a bias of 1 V are in the 107 cm·Hz1/2/W range and are reasonable at these high temperatures. 8.4.2
Quantum dot infrared emitters
The use of selfassembled QDs in the active region of intersubband emitters is expected to improve ir sources in two fundamental ways: (1) Threedimensional electron confinement enables surfacenormal light emission due to polarization selection rules, and (2) the inhomogeneously broadened, deltalike density of states in QDs introduces strict energy conservation rules that significantly reduce phonon or carriermediated scattering. These scattering processes are a significant limiting factor in the efficiency of modern longwavelength sources, especially for efficient CW laser operation at room temperature. Yet, favorable relaxation times in the excited states of QDs invoke the possibility of intersubband lasing. This was first suggested by Singh [70], who proposed the use of an external interband laser to rapidly depopulate the ground state electrons by stimulated emission, thus creating a favorable nonequilibrium carrier distribution between the ground and excited states for MIR emission. Kastalsky et al. have theoretically analyzed a similar dualcolor laser by using a threelevel carrier rate equation [71]. Also, Krishna et al. have demonstrated intersubband stimulated emission in interband QD lasers [72]. Bipolar quantum dot intersubband emitters. Spontaneous emission at 12 m, resulting from intersubband transitions in In0.4Ga0.6As/GaAs QDs [72], has been reported. The output from the surfaceemitting device
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_336_03/23/2006 Intersubband Transitions in Quantum Dots 336
Chapter Eight
was measured at 80 and 300 K. The device was essentially a fourdot layer interband laser heterostructure. The interband lasing occurring in the device at 1 m due to ground state electronhole recombination helped to deplete the electron ground state in the dots and to establish a population inversion between the excited states and the ground state. The farir signal was enhanced after the interband transition reached threshold at 300 K. To determine the possibility of stimulated emission and lasing with this scheme, the condition for intersubband population inversion was determined from the carrier and photon rate equations. In addition, the intersubband gain was calculated as a function of the inhomogeneous line width broadening of the transition, demonstrating that gains as high as 150 cmí1 can be achieved. For observing stimulated emission, plasmonenhanced waveguides were designed and grown by MBE. Edgeemitting devices were fabricated using standard photolithography, liftoff, and a combination of dry and wet etching, followed by ohmic contact formation. The width of the waveguide was varied from 20 to 60 m, and the length was varied from 800 to 1200 m. Therefore, the devices are multimode laterally. The output spectrum is broad and multimode, with a more distinct peak at 13 m which, in all probability, originates from the electron transitions from higher QD excited levels to the ground state, separated by ~90 to 100 meV. Theoretical calculations have confirmed the presence of these excited states [20]. The threshold in the FIR output occurs at 1.6 times the interband laser threshold. The additional carriers injected after the interband laser reaches threshold recombine to provide for high coherent photon density required for intersubband gain. In essence, the device converts the more readily available nearir photons to the more difficult to obtain midir photons. Unfortunately, device heating prevents measurements at higher injection currents. However, these devices demonstrate intersubband gain and stimulated emission. The polarization dependence of the farir emission, measured by using a farir polarizer, is found to be strongly TE polarized, as shown in Fig. 8.15. Unipolar quantum dot cascade lasers. While quantum cascade devices have hitherto been designed with quantum well active regions, it is of interest to investigate QD active regions for the two reasons just mentioned: (1) polarization selection rules allow surfacenormal emitting devices, and (2) reduced phonon coupling in selfassembled QDs, compared to bulk material or quantum wells, promises hightemperature operation. Note that the bipolar device described in the previous section, while adequate to demonstrate intersubband light emission, is not suitable for achieving significant stimulated emission and lasing. However, a unipolar cascade design, in which the ground state of the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_337_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
T = 285 K I = 770 mA L = 0.8 mm Ridge = 50 μm
TE TM
FIR emission (arb.units)
337
TE
TM 8.5
12.5
16.5
λ (μm) Figure 8.15 Farir (FIR) emission from the bipolar QD emitter, showing the intersubband transition to be strongly TE polarized.
QD is depopulated by tunneling to the excited state of the next dot (as shown in Fig. 8.16a) should provide stimulated emission [73]. This approach allows multiple photons to be emitted for each injected electron, and it eliminates the need for interband transitions. To facilitate tunneling between ground and excited states of adjacent QD layers, a chirped superlattice (CSL) structure must be designed to create a narrow miniband connecting these states. It has been established that injected electrons preferentially occupy the excited dot states and wetting layer states at high temperatures due to the higher density of states in these regions, suggesting that population inversion can be readily obtained. Measured and calculated carrier lifetimes in dot excited states are in the range of tens to hundreds of picoseconds, 1.
hν 3.
E2B E1B
Chirped SL 5 to 50x
(a)
Transmission of CSL
300
hν
QD layer
Energy (meV)
E2A 2. E1A
Fth
250 200 150 100 6
5
4
3
2
log(1/T ) (unitless)
1
0
(b)
Figure 8.16 (a) Conduction band schematic of a QD cascade emitter. Dashed lines show the steps an electron follows through the device. (b) Transmission characteristics of a 4period GaAs/GaAs0.96N0.04 chirped superlattice. The miniband is centered at 114 meV and the minigap extends to roughly 225 meV.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_338_03/23/2006 Intersubband Transitions in Quantum Dots 338
Chapter Eight
depending on excitation and bias conditions [74]. In contrast, the upperstate lifetime in quantum well cascade lasers is a few picoseconds, determined by phonon scattering. It is therefore expected that the threshold current will be low in unipolar QD cascade lasers. If In0.4Ga0.6As/GaAs QDs are to be used for the active region, GaAsN is an excellent choice for quantum wells in the CSL for three major reasons. First, GaAsN has a large negative conduction band offset to GaAs, thus allowing the electron to tunnel from the ground state of the QD. Second, advances in the growth of lownitrogencomposition GaAsN have led to its use as laserquality material [75]. Finally, since GaAsN is in tensile strain on a GaAs substrate, it can compensate for the compressively strained InGaAs QDs and permit more periods in the cascade structure. Using the measured conduction band shift in MBEgrown GaAs0.96N0.04, the design for a GaAs/GaAs0.96N0.04 CSL with over 40 dB of contrast between ground and excited state transmission is shown in Fig. 8.16b. Figure 8.17a shows lightcurrent (LI) measurements made on edgeemitting devices at 90 K. Since the injector region is designed to operate under a bias of ~60 mV per period (660 mV over the entire device structure), the “turnon” slightly above this bias, as illustrated by the dashed lines, is expected. The polarizationresolved electroluminescent spectra for the same device at 18 K, as measured by FTIR, are shown in Fig. 8.17b along with the predicted quantum dot energy transitions
24.8
Wavelength (μm) 12.4 8.3 6.2
200 100 0 0 10 20 Position [nm]
30
T = 90 K Pulsed bias 0
50
100
150
200
250
FTIR signal (arb.units)
Intensity (arb.units)
Energy [meV]
E31
300
TE TM
E21
50
5.0
18 K I = 200 mA
100
150
200
Current (mA)
Photon energy (meV)
(a)
(b)
250
(a) Lightcurrent characteristics from an edgeemitting broadarea (300 ȝm × 2 mm) QD cascade device at 90 K. A distinct injector “turnon” is evident, illustrated by the dashed lines. The inset shows the solution to the coupled Schrödinger–Poisson equations for the chirped superlattice at 60 mV/period with the quantum dot states from from an 8band k·p model superimposed on left. (b) Polarizationdependent spectral measurements for the broadarea device at 18 K showing dominant TE polarization. Theoretically predicted energies for first and secondexcited to groundstate transitions are indicated (as E21 and E31) for comparison.
Figure 8.17
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_339_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
339
described above. Background spectra were collected with the device unbiased and subtracted from the biased data. All TE polarized outputs show the same three emission peaks, while none of the TM polarized outputs exhibit these features. Two peaks (57 and 90 meV) agree well with first and second excited to ground state transitions, while a third peak (115 meV) arises, most likely, from wetting layer to ground state transitions. The dominant TE polarization agrees with theory [74]. Unlike in quantum wells, the oscillator strength in quantum dots arises from the centralcell part of the wave function. Strong biaxial strain in dots leads to band intermixing, which results in a larger momentum matrix element for TE polarized light. Total integrated output power for all three peaks is estimated to be 90 nW. 8.5
Conclusions
Intersubband transitions in QDs for ir detectors and emitters are positioned to become an important technology for the type of hightemperature, lowcost, highyield photonic devices required for highly sophisticated sensing and imaging applications. The 3D confinement of QD heterostructures provides important advantages in ir optoelectronic properties compared to quantum wells, such as surfacenormal detection and emission, extended carrier lifetimes due to the phonon bottleneck, and temperature invariance due to the deltalike density of states. Significant challenges exist in reaching the full potential of such devices, due in large part to the nonuniformity of selfassembled QDs. However, continued advances in epitaxial growth and device simulation should enable the desired device improvements. References 1.
E. H. C. Parker, in The Technology and Physics of Molecular Beam Epitaxy. New York: Plenum Press, 1985.
2.
L. Goldstein, F. Glas, J. Y. Marzin, M. N. Charasse, and G. LeRoux, “Growth by molecular beam epitaxy and characterization of InAs/GaAs strainedlayer superlattices,” Applied Physics Letters, vol. 47, pp. 1099– 101, 1985.
3.
S. Fujita, Y. Matsuda, and A. Sasaki, “Blue luminescence of a ZnSeZnS0.1Se0.9 strainedlayer superlattice on a GaAs substrate grown by lowpressure organometallic vapor phase epitaxy,” Applied Physics Letters, vol. 47, pp. 955–957, 1985.
4.
P. R. Berger, K. Chang, P. K. Bhattacharya, and J. Singh, “A study of strainrelated effects in the molecularbeam epitaxy growth of InxGa1íx As on GaAs using reflection highenergy electron diffraction,” Journal of Vacuum Science and Technology B, vol. 5, pp. 1162–1166, 1987.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_340_03/23/2006 Intersubband Transitions in Quantum Dots 340
Chapter Eight
5.
M. Tabuchi, S. Noda, and A. Sasaki, “Strain energy and critical thickness of heteroepitaxial InGaAs layers on GaAs substrate,” Journal of Crystal Growth, vol. 115, pp. 169–173, 1991.
6.
D. Leonard, M. Krishnamurthy, C. M. Reaves, S. P. Denbaars, and P. M. Petroff, “Direct formation of quantumsized dots from uniform coherent islands of InGaAs on GaAs surfaces,” Applied Physics Letters, vol. 63, pp. 3203–3205, 1993.
7.
Q. Xie, P. Chen, A. Kalburge, T. R. Ramachandran, A. Nayfonov, A. Konkar, and A. Madhukar, “Realization of optically active strained InAs island quantum boxes on GaAs (100) via molecular beam epitaxy and the role of island induced strain fields,” Journal of Crystal Growth, vol. 150, pp. 357–363, 1995.
8.
D. Bimberg, M. Grundmann, and N. N. Ledentsov, “Growth, spectroscopy, and laser application of selfordered IIIV quantum dots,” Materials Research Society Bulletin, vol. 23, pp. 31–34, 1998.
9.
P. Bhattacharya, K. Kamath, J. Phillips, and D. Klotzkin, “Selforganized growth of In(Ga)As/GaAs quantum dots and their optoelectronic device applications,” Bulletin of Material Science, vol. 22, pp. 519–529, 1999.
10.
I. N. Stranski and L. Krastanow, “Theory of orientation separation of ionic crystals,” Sitzungsberichte, vol. Abteilung IIb. 146, pp. 797–810, 1938.
11.
D. Bimberg, M. Grundmann, and N. N. Ledentsov, Quantum Dot Heterostructures. Chichester: John Wiley & Sons, 1999.
12.
J. Singh, Physics of Semiconductors and Their Heterostructures. New York: McGrawHill, 1993.
13.
P. R. Berger, K. Chang, P. Bhattacharya, J. Singh, and K. K. Bajaj, “Role of strain and growth conditions on the growth front profile of InxGa1íx As on GaAs during the pseudomorphic growth regime,” Applied Physics Letters, vol. 53, pp. 684–686, 1988.
14.
H. Jiang and J. Singh, “Strain distribution and electronic spectra of InAs/ GaAs selfassembled dots: an eightband study,” Physical Review B, vol. 56, pp. 4696–4701, 1997.
15.
P. N. Keating, “Effect of invariance requirements on the elastic strain energy of crystals with application to the diamond structure,” Physical Review, vol. 145, pp. 637–645, 1966.
16.
R. M. Martin, “Elastic properties of ZnS structure semiconductors,” Physical Review B, vol. 1, pp. 4005–4011, 1970.
17.
H. Jiang and J. Singh, “Selfassembled semiconductor structures: electronic and optoelectronic properties,” IEEE Journal of Quantum Electronics, vol. 34, pp. 1188–1196, 1998.
18.
U. Bockelmann and G. Bastard, “Phonon scattering and energy relaxation in two, one, and zerodimensional electron gases,” Physical Review B, vol. 42, pp. 8947–8951, 1990.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_341_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
341
19.
H. Benisty, C. M. SotomayorTorres, and C. Weisbuch, “Intrinsic mechanism for the poor luminescence properties of quantumbox systems,” Physical Review B, vol. 44, pp. 10,945–10,948, 1991.
20.
P. Bhattacharya, K. K. Kamath, J. Singh, D. Klotzkin, J. Phillips, H. Jiang, N. Chervela, T. B. Norris, T. Sosnowski, J. Laskar, and M. R. Murty, “In(Ga)As/GaAs selforganized quantum dot lasers: DC and smallsignal modulation properties,” IEEE Transactions on Electron Devices, vol. 46, pp. 871–883, 1999.
21.
B. Ohnesorge, M. Albrecht, J. Oshinowo, and A. Forchel, “Rapid carrier relaxation in selfassembled InxGa1íxAs/GaAs quantum dots,” Physical Review B, vol. 54, pp. 11,532– 11,538, 1996.
22.
K. Mukai, N. Ohtsuka, H. Shoji, and M. Sugawara, “Phonon bottleneck in selfformed InxGa1íxAs/GaAs quantum dots by electroluminescence and timeresolved photoluminescence,” Physical Review B, vol. 54, pp. R5243– R5246, 1996.
23.
D. Klotzkin, K. Kamath, and P. Bhattacharya, “Quantum capture times at room temperature in highspeed In0.4Ga0.6AsGaAs selforganised quantumdot lasers,” IEEE Photonics Technology Letters, vol. 9, pp. 1301– 1303, 1997.
24.
J. Urayama, T. B. Norris, J. Singh, and P. Bhattacharya, “Observation of phonon bottleneck in quantum dot electronic relaxation,” Physical Review Letters, vol. 86, pp. 4930–4933, 2001.
25.
D. Klotzkin and P. Bhattacharya, “Temperature dependence of dynamic and DC characteristics of quantumwell and quantumdot lasers: a comparative study,” Journal of Lightwave Technology, vol. 17, pp. 1634– 1642, 1999.
26.
D. Pan, Y. P. Zeng, M. Y. Kong, J. Wu, Y. Q. Zhu, C. H. Zhang, J. M. Li, and C. Y. Wang, “Normal incident infrared absorption from InGaAs/GaAs quantum dot superlattice,” Electronics Letters, vol. 32, pp. 1726–1727, 1996.
27.
S. Sauvage, P. Boucaud, F. H. Julien, J.M. Gérard, and J.Y. Marzin, “Infrared spectroscopy of intraband transitions in selforganized InAs/ GaAs quantum dots,” Journal of Applied Physics, vol. 82, pp. 3396–3401, 1997.
28.
J. Phillips, K. Kamath, X. Zhou, N. Chervela, and P. Bhattacharya, “Photoluminescence and farinfrared absorption in Sidoped selforganized InAs quantum dots,” Applied Physics Letters, vol. 71, pp. 2079– 2081, 1997.
29.
K. W. Berryman, S. A. Lyon, and M. Segev, “Electronic structure and optical behavior of selfassembled InAs quantum dots,” Journal of Vacuum Science and Technology, vol. 15, pp. 1045–1050, 1997.
30.
S. Maimon, E. Finkman, G. Bahir, S. E. Schacham, J. M. Garcia, and P. M. Petroff, “Intersublevel transitions in InAs/GaAs quantum dots
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_342_03/23/2006 Intersubband Transitions in Quantum Dots 342
Chapter Eight
infrared photodetectors,” Applied Physics Letters, vol. 73, pp. 2003–2005, 1998. 31.
Q. D. Zhuang, J. M. Li, H. X. Li, Y. P. Zeng, and L. Pan, “Intraband absorption in the 812 ȝm band from Sidoped vertically aligned InGaAs/ GaAs quantumdot superlattice,” Applied Physics Letters, vol. 73, pp. 3706–3708, 1998.
32.
L. Chu, A. Zrenner, G. Böhm, and G. Abstreiter, Applied Physics Letters, vol. 75, p. 3599, 1999.
33.
I. Mukhametzhanov, Z. H. Chen, O. Baklenov, E. T. Kim, and A. Madhukar, Physica Status Solidi B, vol. 224, p. 697, 2001.
34.
Z. Chen, E.T. Kim, and A. Madhukar, Applied Physics Letters, vol. 80, p. 2490, 2002.
35.
J. Phillips, K. Kamath, and P. Bhattacharya, “Farinfrared photoconductivity in selforganized InAs quantum dots,” Applied Physics Letters, vol. 72, pp. 2020–2022, 1998.
36.
N. Horiguchi, T. Futatsugi, Y. Nakata, N. Yokoyama, T. Mankad, and P. M. Petroff, “Quantum dot infrared photodetector using modulation doped InAs selfassembled quantum dots,” Japanese Journal of Applied Physics, vol. 38, pp. 2559–2561, 1999.
37.
Z. Chen, O. Baklenov, E. T. Kim, I. Mukhametzhanov, J. Tie, A. Madhukar, Z. Ye, and J. C. Campbell, “Normal incidence InAs/AlxGa1íxAs quantum dot infrared photodetectors with undoped active region,” Journal of Applied Physics, vol. 89, pp. 4558–4563, 2001.
38.
J. Phillips, “Evaluation of the fundamental properties of quantum dot infrared detectors,” Journal of Applied Physics, vol. 91, pp. 4590–4594, 2002.
39.
J. Singh, Electronic and Optoelectronic Properties of Semiconductor Structures. New York: Cambridge University Press, 2003.
40.
K. Kamath, N. Chervela, K. K. Linder, T. Sosnowski, H. T. Jiang, T. Norris, J. Singh, and P. Bhattacharya, “Photoluminescence and timeresolved photoluminescence characteristics of InxGa1íxAs/GaAs selforganized single and multiplelayer quantum dot laser structures,” Applied Physics Letters, vol. 71, p. 927, 1997.
41.
V. Ryzhii, “The theory of quantumdot infrared phototransistors,” Semiconductor Science and Technology, vol. 11, pp. 759–765, 1996.
42.
K. W. Berryman, S. A. Lyon, and M. Segev, “Midinfrared photoconductivity in InAs quantum dots,” Applied Physics Letters, vol. 70, pp. 1861–1863, 1997.
43.
D. Pan, E. Towe, and S. Kennerly, “Normalincidence intersubband (In, Ga)As/GaAs quantum dot infrared photodetectors,” Applied Physics Letters, vol. 73, pp. 1937–1939, 1998.
44.
S. J. Xu, S. J. Chua, T. Mei, X. C. Wang, X. H. Zhang, G. Karunasiri, W. J. Fan, C. H. Wang, J. Jiang, S. Wang, and X. G. Xie, “Characteristics
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_343_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
343
of InGaAs quantum dot infrared photodetectors,” Applied Physics Letters, vol. 73, pp. 3153–3155, 1998. 45.
J. Phillips, P. Bhattacharya, S. W. Kennerly, D. W. Beekman, and M. Dutta, “Selfassembled InAsGaAs quantumdot intersubband detectors,” IEEE Journal of Quantum Electronics, vol. 35, pp. 936–943, 1999.
46.
D. Pan, E. Towe, and S. Kennerly, “Photovoltaic quantumdot infrared detectors,” Applied Physics Letters, vol. 76, pp. 3301–3303, 2000.
47.
H. C. Liu, M. Gao, J. McCafferey, Z. R. Wasilewski, and S. Fafard, “Quantum dot infrared photodetectors,” Applied Physics Letters, vol. 78, pp. 79–81, 2001.
48.
S. Y. Wang, S. D. Lin, H. W. Wu, and C. P. Lee, “Low dark current quantumdot infrared photodetectors with an AlGaAs current blocking layer,” Applied Physics Letters, vol. 78, pp. 1023–1025, 2001.
49.
A. D. Stiff, S. Krishna, P. Bhattacharya, and S. Kennerly, “Normalincidence, hightemperature, midinfrared InAsGaAs vertical quantumdot infrared photodetector,” IEEE Journal of Quantum Electronics, vol. 37, pp. 1412–1419, 2001.
50.
S. Krishna, A. D. StiffRoberts, J. D. Phillips, P. Bhattacharya, and S. W. Kennerly, “Hot dot detectors: infrared quantum dot intersubband photodetectors are a promising technology for multiwavelength IR detection,” IEEE Circuits & Devices, vol. 18, pp. 14–24, 2002.
51.
E.T. Kim, Z. Chen, and A. Madhukar, “Tailoring detection bands of InAs quantumdot infrared photodetectors using InxGa1íxAs strainrelieving quantum wells,” Applied Physics Letters, vol. 79, pp. 3341–3343, 2001.
52.
S. Raghavan, P. Rotella, A. Stintz, B. Fuchs, S. Krishna, C. Morath, D. A. Cardimona, and S. W. Kennerly, “Highresponsivity, normalincidence longwave infrared (Ȝ = 7.2 m) InAs/In0.15Ga0.85As dotsinawell detector,” Applied Physics Letters, vol. 81, pp. 1369–1371, 2002.
53.
S. Krishna, S. Raghavan, G. V. Winckel, P. Rotella, A. Stintz, C. P. Morath, D. Le, and S. W. Kennerly, “Two color InAs/InGaAs dotsinawell detector with backgroundlimited performance at 91 K,” Applied Physics Letters, vol. 82, p. 2574, 2003.
54.
U. Sakoglu, J. S. Tyo, M. M. Hayat, S. Raghavan, and S. Krishna, “Spectrally adaptive infrared photodetectors with biastunable quantum dots,” Journal of Optical Society of America B, vol. 21, pp. 7–17, 2004.
55.
A. Weber, O. GauthierLafaye, F. H. Julien, J. Brault, M. Gendry, Y. Désieres, and T. Benyattou, “Strong normalincidence infrared absorption in selforganized InAs/InAlAs quantum dots grown on InP(001),” Applied Physics Letters, vol. 74, pp. 413–415, 1999.
56.
S. Kim, H. Mohseni, M. Erdtmann, E. Michel, C. Jelen, and M. Razeghi, “Growth and characterization of InGaAs/InGaP quantum dots for midinfrared photoconductive detector,” Applied Physics Letters, vol. 73, pp. 963–965, 1998.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_344_03/23/2006 Intersubband Transitions in Quantum Dots 344
Chapter Eight
57.
J. Jiang, K. Mi, S. Tsao, W. Zhang, H. Lim, T. O'Sullivan, T. Sills, M. Razeghi, G. J. Brown, and M. Z. Tidrow, “Demonstration of a 256 × 256 middlewavelength infrared focal plane array based on InGaAs/InGaP quantum dot infrared photodetectors,” Applied Physics Letters, vol. 84, pp. 2232–2234, 2004.
58.
J. Jiang, S. Tsao, T. O'Sullivan, W. Zhang, H. Lim, T. Sills, K. Mi, M. Razeghi, G. J. Brown, and M. Z. Tidrow, “High detectivity InGaAs/InGaP quantumdot infrared photodetectors grown by low pressure metalorganic chemical vapor deposition,” Applied Physics Letters, vol. 84, pp. 2166– 2168, 2004.
59.
J. L. Liu, W. G. Wu, A. Balandin, G. L. Jin, and K. L. Wang, “Intersubband absorption in borondoped multiple Ge quantum dots,” Applied Physics Letters, vol. 74, pp. 185–187, 1999.
60.
P. Boucaud, V. L. Thanh, S. Sauvage, D. DéBarre, and D. Bouchier, “Intraband absorption in Ge/Si selfassembled quantum dots,” Applied Physics Letters, vol. 74, pp. 401–403, 1999.
61.
J. L. Liu, W. G. Wu, A. Balandin, G. Jin, Y. H. Luo, S. G. Thomas, Y. Lu, and K. L. Wang, “Observation of intersublevel transitions in modulationdoped Ge quantum dots,” Applied Physics Letters, vol. 75, pp. 1745–1747, 1999.
62.
A. I. Yakimov, A. V. Dvurechenskii, Y. Y. Proskuryakov, A. I. Nikiforov, O. P. Pchelyakov, S. A. Teys, and A. K. Gutakovskii, “Normalincidence infrared photoconductivity in Si pin diode with embedded Ge selfassembled quantum dot,” Applied Physics Letters, vol. 75, pp. 1413–1415, 1999.
63.
C. Miesner, O. Röthig, K. Brunner, and G. Abstreiter, “Midinfrared photocurrent measurements on selfassembled Ge dots in Si,” Physica E, vol. 7, pp. 146–150, 2000.
64.
A. I. Yakimov, A. V. Dvurechenskii, A. I. Nikiforov, and Y. Y. Proskuryakov, “Interlevel Ge/Si quantum dot infrared photodetector,” Journal of Applied Physics, vol. 89, pp. 5676–5681, 2001.
65.
S. Chakrabarti, A. D. StiffRoberts, P. Bhattacharya, S. Gunapala, S. Bandara, S. B. Rafol, and S. W. Kennerly, “Hightemperature operation of InAs/GaAs quantum dot infrared photodetectors with large responsivity and detectivity,” IEEE Photonics Technology Letters, vol. 16, pp. 1361–1363, 2004.
66.
S. Chakrabarti, X. H. Su, P. Bhattacharya, G. Ariyawansa, and A. G. U. Perera, “Characteristics of a multicolor InGaAs/GaAs quantum dot infrared photodetector,” IEEE Photonics Technology Letters, vol. 17, pp. 178–180, 2005.
67.
X. H. Su, S. Chakrabarti, A. D. StiffRoberts, J. Singh, and P. Bhattacharya, “Quantum dot infrared photodetector design based on doublebarrier resonant tunneling,” Electronics Letters, vol. 40, pp. 1082– 1083, 2004.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_345_03/23/2006 Intersubband Transitions in Quantum Dots Intersubband Transitions in Quantum Dots
345
68.
P. Bhattacharya, X. H. Su, S. Chakrabarti, G. Ariyawansa, and A. G. U. Perera, “Characteristics of a tunneling quantum dot infrared photodetector operating at room temperature,” Applied Physics Letters, vol. 86, pp. 191,106–191,108, 2005.
69.
X. H. Su, S. Chakrabarti, P. Bhattacharya, G. Ariyawansa, and A. G. U. Perera, “A resonant tunneling quantum dot infrared photodetector,” IEEE Journal of Quantum Electronics, vol. 41, pp. 974–979, 2005.
70.
J. Singh, “Possibility of room temperature intraband lasing in quantum dot structures placed in highphoton density cavities,” IEEE Photonics Technology Letters, vol. 8, p. 488, 1996.
71.
A. Kastalsky, L. E. Vorobjev, D. A. Firsov, V. L. Zerova, and E. Towe, “A dualcolor injection laser based on intra and interband carrier transitions in semiconductor quantum wells or quantum dots,” IEEE Journal of Quantum Electronics, vol. 37, p. 1356, 2001.
72.
S. Krishna, P. Bhattacharya, J. Singh, T. Norris, J. Urayama, P. J. McCann, and K. Namjou, “Intersubband gain and stimulated emission in long wavelength (l = 13 mm) intersubband quantum dot emitters,” IEEE Journal of Quantum Electronics, vol. 37, pp. 1066–1074, 2001.
73.
C.F. Hsu, J.S. O, P. Zory, and D. Botez, “Intersubband quantumbox semiconductor lasers,” IEEE Journal of Selected Topics in Quantum Electronics, vol. 6, pp. 491–503, 2000.
74.
B. Kochman, A. D. StiffRoberts, S. Chakrabarti, J. D. Phillips, S. Krishna, J. Singh, and P. Bhattacharya, “Absorption, carrier lifetime, and gain in InAsGaAs quantumdot infrared photodetectors,” IEEE Journal of Quantum Electronics, vol. 39, pp. 459–467, 2003.
75.
A. Jackson, Electronics Letters, vol. 37, pp. 355–356, 2001.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH08_346_03/23/2006 Intersubband Transitions in Quantum Dots
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_347_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
9 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells
Hans Sigg Paul Scherrer Institut, Villigen PSI, Switzerland
9.1 Introduction The investigation of intersubband transitions in silicon and germaniumbased quantum wells has attracted considerable interest over the past 15 years. Such investigations have helped to improve the atomic layer growth of group IV materials on silicon, and were crucial in the development of the detailed knowledge we have now of the complex band structure of strained SiGe quantum structures, particularly for the valence bands. Additionally, Sibased intersubband systems have generated interest because of their potential applications in infrared detection and emission. In particular, the integration of such systems into the powerful silicon microelectronics platform promises the development of optical devices with complex functionalities. For example, monolithic integration of a chip containing large arrays of intersubband detectors with associated electric drivers and logic circuitries for signal analysis may allow the production of sophisticated infrared focal plane arrays (FPAs) at low cost. Furthermore, if the quantum cascade laser concept is successfully transferred from IIIV to group IV semiconductors, silicon, in spite of its unfavorable indirect band structure, could become a competitive player in optoelectronics. Sibased quantum cascade lasers could be designed for emission in the midinfrared and may provide a cheaper 347
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_348_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 348
Chapter Nine
alternative to IIIV and IIVI based midinfrared laser sources for applications such as environmental sensing and process diagnostics. The other targeted energy range for Sibased intersubband emitters is the terahertz region, which is important for gas tracing and security surveillance, e.g., at airports. Combined with sensitive and fast photodetectors, applications of Sibased quantum cascade lasers to onchip signal processing as well as chiptochip data communications may also be considered. The operating wavelength of such systems would certainly not reach the 1.5m telecommunication band because of the fairly low band offsets, but since for chiptochip communications freespace transmission rather than fiber coupling is required, the restriction to the midinfrared (5 to 10 m) is of less importance. As we will show, the bottleneck and thus a mandatory prerequisite for all these developments will be further progress in the deposition techniques of strained SiGe layers, in particular using molecular beam epitaxy (MBE) on virtual substrates. The understanding of the band structure, and in particular the complex multibands of the valence band, however, is now well developed. Intersubband spectroscopy is used routinely for the characterization of the epilayer quality. For example, studies are conducted to verify the abruptness and thermal stability of Si/SiGe heterointerfaces as well as to measure band structure parameters such as the straindependent heterojunction band offsets. Pioneering studies were devoted to the investigation of twodimensional electron and hole gases in Si inversion and accumulation layers in the late 1970s and 1980s [1]. During this period, many of the fundamental effects and theoretical considerations concerning the intersubband resonances, such as manybody effects, interface scattering, and coupling to plasmons, were demonstrated. This is remarkable as these studies were undertaken long before intersubband transitions were explored in group IIIV materials, such as the latticematched GaAlAs [2] and InGa/AlAs systems. In common with the quantum Hall effect, discovered in Si inversion layers but more widely explored in GaAs/AlGaAs heterostructures, the rapid development of intersubband devices in the late 1980s and 1990s was mainly realized with IIIV quantum structures [3, 4]. However, judging from the substantial progress made recently in the epitaxy of Si/SiGe heterostructures deposited on straincompensating relaxed buffer substrates, similar device developments can be expected in the near future with Sibased intersubband systems. The high standard of today’s Si/Ge epitaxy is demonstrated by the highresolution transmission electron microscopy (HRTEM) study, shown in Fig. 9.1. The depicted Si/SiGe multiquantumwell structure has been grown on relaxed buffer substrate by lowtemperature MBE. Uniform and abrupt interfaces were obtained, and intersubband absorption studies revealed transitions with narrow line width (~14 meV), as shown below. The Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_349_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
349
Si0.5Ge0.5
Si0.5Ge0.5
Si Si
Si0.5Ge0.5
Si0.2Ge0.8
100 nm
Figure 9.1 Highresolution crosssectional TEM image of a 10period Si/Si0.2Ge0.8
multiplequantumwell structure grown on a relaxed SiGe buffer layer at 300°C. The structure is strainsymmertrized as the average Ge concentration of the 12Åthick Si barriers and 40Åthick SiGe wells adds up to that of the relaxed buffer (50%). (Source: E. Müller, PSI, Switzerland.)
ultimate goal of this area of research—and the ultimate proof of the progress made in the epitaxial growth and band structure engineering of group IV materials—is the development of Sibased quantum cascade lasers. How far we are from this milestone remains an open question. This chapter aims to look into this question and give an overview of the state of the research. We review the main progress that has been made in the past few years in intersubband spectroscopy and device development with Sibased quantum structures. Specifically we emphasize those aspects of intersubband physics that are most important for Si/SiGe systems, such as the polarization selection rules of intersubband transitions in the multivalley conduction bands and strongly mixed valence bands. Sections 9.2 and 9.3 are devoted to the theoretical background, experimental methods, and results of various intersubband spectroscopy studies performed on Sibased quantum wells (QWs) and quantum dots (QDs). Section 9.4 then discusses the main device applications of these systems, namely, photodetectors and quantum cascade emitters. 9.2 Theoretical Background of Intersubband Transitions in Si/SiGe Quantum Wells Depending on the substrate material and the strain configuration, various options are available to realize an intersubband system with Si/SiGe QWs. For example, when these layers are grown on a Si substrate, most of the band offset will occur in the valence bands, and only the holes will be effectively confined in the SiGe layers, while the Si layers form the barriers. By growing on top of a thick relaxed buffer layer of SiGe, valley splitting in the strained Si (or Ge) layers enables Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_350_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 350
Chapter Nine
sufficient confinement for the electrons to be achieved as well. The most commonly used layer sequences, for ntype and ptype intersubband systems, are schematically shown in Fig. 9.2. From the numerous investigations published since the 1990s, our knowledge of intersubband absorption in Si/SiGe QWs has reached a high level of maturity. The driving force for these studies has been the prospect of developing infrared detectors that can be integrated with largescale Si circuits. Consequently, the main effort has been to elucidate the dependence of the intersubband absorption coefficient on the direction of light polarization. In particular, the possibility of absorption at normal incidence to the sample surface (defined in the following as the z direction), which is important for the realization of focal plane arrays, is of great interest. For the description of valence band states and intersubband dipolar matrix elements in strained Si/SiGe multiple QWs, envelope wave function approaches using k·p models of various complexity have been applied [5–17]. Experiments and theory have shown that normalincidence intersubband absorption (i.e., with light polarized parallel to the QWs, or in the xy plane) is possible in both ntype and ptype Si/SiGe QWs. For the Conduction band
(a)
(b) Δ4
Ge
(d) HH
SiGe
SO
Valence band
SiGe relaxed
LH
Si
Si
z
SiGe relaxed
Si
SiGe
Energy
(c)
L
Si (100)
SiGe relaxed
Δ2
Figure 9.2 Schematic representation of the band structure of frequently explored SiGe
intersubband systems. (a) Si QW grown on top of a SiGe relaxed buffer. Electrons in the ground state belong to the twofold conduction band minima ǻ2. (b) Ge QW on a (100) relaxed SiGe substrate; electrons occupy the threefold minima in the L direction, i.e., along [111]. Due to the tilt of the constant energy ellipsoids relative to the (100) growth direction, intersubband transitions couple to the xy as well as to the z polarization components. (c) Valence band SiGe QW coherently strained to a Si (001) substrate. The ground state belongs to the heavyhole (HH) band. At the ī point of the Brillouin zone, i.e., at kpar = 0, this HH band is decoupled from the lighthole (LH) and splitoff (SO) bands. (d) Strainsymmetrized SiGe QW grown on a (100) relaxed SiGe buffer layer: the compressively strained SiGe QW is embedded by tensilestrained Si barrier layers. The HH levels are much more strongly confined than the LH/SO levels.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_351_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
351
case of transitions between conduction subbands, the coupling to the xy polarization component is provided by the ellipsoid shape of the constantenergy surfaces, but only when the z (i.e., growth) direction does not match any of the main axes of the ellipsoids [5, 6]. This requirement is a drawback for ntype Si QWs (type A, Fig. 9.2a), because the sixfold degenerate Si conduction band minima at the ǻ point are oriented along the [100] direction, which is the preferred growth direction in Si microelectronics. Better compatibility to Si electronics is thus obtained from Ge QWs (type B, Fig. 9.2b) as their minima are at the L point of the Brillouin zone and thus are oriented along the [111] directions [5]. For hole intersubband transitions, the main difference from the conduction band QW states is the presence of the nearly degenerate (on the scale of typical confinement energies) heavyhole (HH), lighthole (LH), and spinorbit splitoff (SO) bands at the ī point of the valence band. Due to the reduced crystal symmetry caused by the QW potential and the strain in the QW layers, the valence band QW states are mixtures between these bands. The coupling of xypolarized light to intersubband transitions is a direct consequence of this multiband structure of the valence band. As demonstrated by Fromherz et al. [7], transitions between states belonging to the same subspace (for example, HHtoHH transitions) couple exclusively to the z polarization for vanishing inplane momentum kpar. However, transitions between the HH and LH/SO subspace couple also to the xy polarization. In both cases, the strength of these transitions is determined by the dipole matrix element between the respective initial and final QW states. For finite inplane wave vector, these selection rules are relaxed, as transitions between the subspaces of the QW states with nonvanishing overlap integral become allowed for both directions of polarization [7]. As valence band mixing (e.g., the admixture of LH/SO into the HH band) depends on strain and confinement and is increasing with increasing kpar, the actual coupling strength for the two polarizations depends on sample parameters such as temperature, doping concentration, and Ge concentration in the QW. In practice, for weakly to moderately doped systems with Fermi wave vector kF ~ 0.03 Å–1 [which corresponds to a twodimensional (2D) carrier density n2D ~ 1012 cm–2], this mixing is weak, particularly for the HH ground state. Excited HH levels may show mixing with the LH/SO bands, particularly in case of near degeneracy of the levels, as shown below. At the low carrier densities, energy level calculations based on a 6 × 6 k·p LuttingerKohn hamiltonian offer accurate results. However, for kF 0.05 Å–1 the contributions from the remote conduction bands at the ī point should be included to higher than second order, as shown in a comparison between the 6 × 6 and the 14 × 14 k·p hamiltonians by El Kurdi et al.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_352_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 352
Chapter Nine
[8]. Note, however, that some of the thus required k·p coupling parameters for the higher conduction bands are not accurately known, and their determination by intersubband experiments is difficult because of the broad intersubband resonances measured, particularly at high carrier densities. A comparison between simulations based on the 6 × 6 hamiltonian and experiments is shown in Fig. 9.3 for valence band QWs of type C [7] (as in Fig. 9.2c) and D [18] (as in Fig. 9.2d). Good agreement is obtained in both cases by using the same model with the same band parameters, taken from Refs. 19 and 20. In addition, the theory is found to give an accurate description of the resonant line shapes and explains in detail the rich substructures appearing in the tails of the absorption peaks of QWs of type D [21]. In this latter work, the Ge concentration dependence of the Luttinger parameters as given in Ref. 22 has been used. From the good agreement with the experiment it is concluded that the control of the growth as well as the modeling seems highly accurate and thus should allow the realization and simulation of highly complex intersubband systems, such as those needed for the development of efficient quantum cascade emitters. 0.75 TM
∆ T/T(%)
0.625
44Å, 31%
0.5
TE
0.375
QW 35 Å
0.25 0.125
47Å, 25% Transmission
0
150 200 250 300 350 400 450 500 550 600
(b)
40% 1
Absorption (cm )
1000
49Å, 21%
12
p = 1.2 × 10 s
0
500
1000
1500
2000 1
Wave number (cm ) (a)
2
cm
2500
TM
800
QW 35 Å 12
p=10
600
cm
2
400
TE
200 0
0
100
200
300
400
500
600
700
Energy (meV) (c)
Figure 9.3 Comparison of valence band intersubband absorption spectra of Si/SiGe modulationdoped QWs with corresponding simulations based on a 6 × 6 k·p hamiltonian. (a) TMpolarized spectra and calculations for a multipleQW structure grown on a Si (100) substrate (QW of type C). [Source: Fromherz et al., Phys. Rev. B50, 15073 (1994).] (b) TMand TEpolarized spectra obtained by carrier density modulation of a strainbalanced Si/ SiGe/Si structure (QW of type D). (c) Simulated spectra are given for comparison. [Source: Diehl et al., Appl. Phys. Lett. 3274 (2002).]
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_353_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
353
Another important aspect, particularly for the development of quantum cascade devices, is knowledge of the intersubband energy relaxation processes, since lasing requires the lifetime of the upper state to be longer than that of the lower state. The first attempt to design efficient intersubband emitters in the SiGe material system can be found in earlier work by Sun and Friedman [23]. Later, Reimann, Kaindl, and Woerner [24] developed a detailed picture of deformationpotential scattering of holes in QW structures. By symmetry, the deformationpotential scattering occurs predominantly between subbands of different types, e.g., between HH and LH subbands. The corresponding scattering rates were calculated for a Si/Si0.5Ge0.5 QW pseudomorphically grown on Si (100). Distinct scattering onsets were found at well widths between 5.5 and 4.5 nm, where the separation between the HH2 and the LH1 levels becomes equal to the optical phonon vibrational energies of the Ge–Ge, Si–Ge, and Si–Si bonds. This is illustrated in Fig. 9.4. For the deformationpotential scattering, it appears that the scattering rate increases monotonically with
6.2
4
Well width (nm) 5.5 5 4.5
4
3.6
Si0.5Ge0.5/Si QW SiSi 0.3
SiGe
0.5
2 HH2 → LHSO1
HH2 lifetime (ps)
Scattering rate (ps1)
3
GeGe 1
1
1.5 2
HH2 → HH1 0 0.08
0.10 0.12 0.14 0.16 HH2 – HH1 distance (eV)
0.18
Figure 9.4 Calculated scattering rates (left scale) and lifetimes (right scale) at zero temperature from opticalphonon deformation scattering in Si0.5Ge0.5/Si multiple QWs as a function of the HH2HH1 energy separation (varied by changing the well width, see upper scale). The arrows show the threshold for scattering by GeGe, SiGe, and SiSi type optical phonons. [Source: Reimann et al., Phys. Rev. B65, 045302 (2001).]
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_354_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 354
Chapter Nine
intersubband separation energy, as more relaxation channels become available, due to scattering to higherkpar states. This is fundamentally different from the case of polaropticalphonon scattering, where the scattering rate is largest for momentum transfers close to zero. These considerations must be incorporated into the design of Sibased quantum cascade lasers to get efficient depopulation of the lower state, while keeping the upper state sufficiently long lived. The resulting design strategies depend on the desired emission wavelength as described in greater detail below. 9.3 Intersubband Spectroscopy 9.3.1
Experimental techniques
The experimental techniques used to study intersubband absorption in SiGe QWs are very similar to those applied for the study of IIIV intersubband systems. In most cases, the samples contain multiple QWs and, to increase the intersubband absorption signal, are investigated in the waveguide geometry shown in Fig. 9.5a. Infrared light is coupled in and out of the wedged facets of the parallelogramshaped sample and undergoes multiple passes through the undoped substrate and doped QW layers. The input polarization is set by a wire grid polarizer to be aligned normal (TM polarization) or parallel (TE polarization) to the deposited layers. The absorption in such layers is strongly reduced for TEpolarized light if a metallic film is evaporated on the sample top surface. Conversly, a metallic layer increases the absorption for TM light [7]. Due to the oblique incidence, this coupling scheme does not provide light coupling in pure z polarization. In the TM configuration z and xy polarization is mixed, while in the TE configuration only the xy polarization is applied. The z polarization coupling without admixture of xy polarization could be obtained by attenuated total reflection geometry via a germanium prism tightly pressed on the sample surface [25]. The transmitted light is analyzed with a Fourier transform infrared (FTIR) spectrometer. The sensitivity of such experiments is strongly enhanced by modulating the carrier density with an electric field, applied between a Schottky front gate and the electrically contacted QW layers (c.f. Fig. 9.5b). Phasesensitive detection of the modulated signal while stepping the interferometer allows resolution of the intersubband absorption spectrum of a single QW [26]. Carrier density modulation can also be obtained by photoexcitation of the samples with abovebandgap light, as shown in Fig. 9.5c. Due to the long electronhole recombination lifetimes in indirect bandgap semiconductors such as Si and Ge, carrier densities exceeding 1018 cmí3 in bulk samples and 1011 cmí2 in QWs are obtained at moderate light Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_355_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
355
TM TE
(a) Vbias
TM TE
(b) hv > Egap
TM TE
(c) Figure 9.5 Frequently used sample configurations for intersubband transmission experiments in waveguide geometry for transverse magnetic and transverse electric polarization. (a) Samples with a top metallic layer offer good overlap of the TM mode with the multipleQW layers near the surface. TE transmission provides the reference signal. (b) Carrier density modulation with a Schottky gate gives improved signaltonoise performance, enabling detection of intersubband absorption of single wells, and gives the means to study the intersubband absorption under the influence of an E field. (c) Carriers are provided by abovebandgap optical excitation. Because of the long interband carrier lifetime in Si at low temperatures (> microseconds), substantial carrier densities are obtained at moderate excitation intensities.
intensities of 1 W/cm2 [27]. However, FabryPerot interference in the multipleQW stack due to refractive index variations and from the Drude freecarrier absorption by photogenerated carriers is found to complicate the interpretation of the spectra [28]. In doped SiGe QWs, the photoexcited intersubband absorption is found to differ from the direct absorption, which has been attributed to the fact that this method is sensitive to excess carriers located above the Fermi energy EF and away from the Brillouin zone center [29]. Thus far, only hole intersubband absorption has been observed with this technique. This can be attributed in part to weak confinement in the conduction band, at least in systems that are pseudomorphically strained to Si. For systems grown on relaxed buffers with larger conduction band
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_356_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 356
Chapter Nine
offsets, the measurement of electron intersubband absorption in the presence of photoexcitation should be possible as well. In addition to these linear spectroscopy techniques used to determine the intersubband energy separations, nonlinear and timeresolved measurements have been performed to explore the dynamics of intersubband transitions in SiGe QWs. Early pumpprobe experiments were carried out with 3nmthick ptype Si0.8Ge0.2 QWs using a freeelectron laser source, and they revealed intersubband relaxation lifetimes of between 400 and 700 fs [30]. By using 150fslong midinfrared pulses generated by parametric amplification in a GaSe crystal, intersubband relaxation processes with a time constant of 250 fs were subsequently resolved in 4.4nmthick, ptype Si0.5Ge0.5 multiple QWs [31]. Longer relaxation times were observed in wider wells [32], where the intersubband energy separations are small compared to the optical phonon energies (c.f. Fig. 9.4). This makes these systems convenient for studies with freeelectron laser sources, as demonstrated by Murzyn et al. [33] and Kelsall et al. [34]. As an alternative to pumpprobe techniques, the upperstate lifetime in quantum cascade structures can be determined from the quantitative analysis of their emission efficiency. Note, however, that this method can produce reliable results only if the detector response, the collection efficiency Șopt of the experimental setup, and the optical matrix element of the intersubband transition are known, and if an appropriate injector is built into the structure to provide efficient carrier injection into the upper state. The technique is based on the expression for the quantum efficiency ȘQC (i.e., the number NP of emitted photons per period divided by the number of carriers in the excited state NX) in terms of the radiative and nonradiative lifetimes ȘQC =
Ĳ nrad NP P e = = Ș opt N h Ȟ J NX Ĳ nrad + Ĳ rad
where hȞ is the photon energy, J is the current, N is the number of periods in the cascade structure, P is the detected power spectrally integrated over the resonance, and unit injection efficiency, that is, NX ~ J/e, is assumed. Since Ĳrad can be calculated from the dipole matrix element, Ĳnrad can be obtained from the equation above. Regardless of its restrictions, this method has been found to be very useful to determine the nonradiative lifetime of the upper state [35, 36] and to estimate the achievable gain in SiGe quantum cascade structures [37]. 9.3.2
SiGe and SiGeC quantum wells
As mentioned above, intersubband spectroscopy is an effective tool to investigate the interface quality of the layers forming the QWs and thus Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_357_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
357
is of great use to characterize and optimize layer deposition techniques. Initial intersubband spectra of Sibased heterostructures were from ptype Si/SiGe multiple QWs grown by MBE [38–40]. Since these samples were doped in the wells, the spectra were very broad, independent of the actual QW dimensions, and only the fundamental HH resonance could be identified. Subsequently, normalincidence absorption was demonstrated [41], and the intersubband spectra were simulated [42]. Betterresolved intersubband transitions were measured in ntype Si wells grown by MBE on a relaxed (100) Si0.7Ge0.3 buffer layer [43]. The barriers were formed by Si0.5Ge0.5 layers doped with Sb by secondary ion implantation techniques. The intersubband resonances were found to shift from 7 meV to approximately 30 meV as the well width was varied from 100 to 50 Å. Through simulations, this shift was found to be compatible with a discontinuity of 310 meV between the doublydegenerate ǻ2 conduction band minima in the symmetrically strained Si and Si0.5Ge0.5 layers. The intersubband line width and mobility of this sample were about 3 meV and 15 m2/(V· s), respectively, depending on the doping concentration and well width. Electron intersubband absorption has been investigated in 50Åthick welldoped SiGe/Si/SiGe QWs grown by MBE on relaxed (110) SiGe substrate layers [42]. At the doping densities of ~1020 cm–3 used in these samples, exchange and depolarization energy shifts were found to contribute considerably to the measured intersubband transition energy of ~200 meV. As expected for (110) oriented substrates, these QWs showed intersubband absorption of a similar strength for both the inplane (TE) and the outofplane (TM) polarization [44]. Comparable electron intersubband absorption of TEpolarized light at similar wavelengths (near 7 m, that is, ~200 meV) was also obtained in deltadoped Ge QWs grown on relaxed (100) SiGe substrate layers [45]. The coupling to the TE polarization component is provided in this case by the tilted energy ellipsoids of the Ge L valleys [5]. In addition, intersubband studies have been undertaken to investigate the interfacial smearing in narrow Si/SiGe multiple QWs grown by MBE using Sb to control the interface abruptness by suppressing the Ge surface segregation [46]. From the close agreement between the observed and calculated transition energies versus QW thickness (c.f. Fig. 9.6) the authors concluded that the Ge segregation was suppressed to less than 0.4 nm. Incidentally, in these samples the exchange and depolarization shifts were found to give a relatively small (< 10 meV) contribution to the intersubband transition energy, consistent with the chosen carrier concentration of ~2 × 1018 cm–3. Similar conclusions regarding the interface abruptness were obtained for Si/SiGe QWs grown using hydrogen as a segregantassist in Si gassource MBE [47]. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_358_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 358
Chapter Nine
0.4 Si / Si 0.4Ge0.5 MQW
( eV )
100 K
2.0 nm
2.6 nm
0.1
0.1
10 %
100 K
0.2
0
0 0.1
0.2 0.3 Photon energy (eV)
0.4
0
1 2 Well Width
3 ( nm )
Line width ( eV )
1.8 nm
peak
energy
0.3
Absorption
Transmittance
(arb. units)
1.4 nm
4
Figure 9.6 (a) Intersubband study of the heterointerface quality in Si/Si0.4Ge0.6 multiple
QWs prepared by segregantassisted growth with Sb. (b) Well width dependence of the peak intersubband absorption energy (circles) and resonance line width (squares). The solid line shows the intersubband transition energy calculated with a KronigPenney model. The shadow marks the formation of minibands in the multiple QWs. (Reprinted with permission from [46]. Copyright 1992, American Institute of Physics.)
Regarding intersubband transitions in the valence bands, a detailed study was carried out in pseudomorphically strained SiGe QWs with well thickness and Ge concentration ranging from 26 to 65 Å and from 20% to 50%, respectively [7]. The spectra measured with TMpolarized light could be accurately described by an envelope function band structure calculation and subsequent dielectric simulations of the multilayer stack. In this work, a line width of ~20 meV was observed for HH transitions in QWs with wellconfined excited states, which represents the narrowest value ever published for ptype QW structures pseudomorphically grown on Si. The sensitivity of the measurement was not sufficient to resolve the TE component of the intersubband absorption. In a later work by the same group with a Si/SiGe multipleQW stack capped by a 1.2mthick Si overlayer, TE absorption was observed and found to be in qualitative and quantitative agreement with theory [46]. In the same work, the difference in polarization dependence between intersubband absorption and photoconductivity was addressed. The latter process showed a stronger Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_359_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
359
response to TE than TM polarization, in contrast to the case of absorption, indicating the importance of the subsequent transport processes for the photocurrent [48]. To our knowledge, the thus far smallest line width value for intersubband transitions in ptype SiGe is ~14 meV and is realized in 60Åwide QWs of 75% Ge concentration grown on 50% relaxed buffer substrate [21]. Intersubband absorption spectra for both TE and TM polarization have also been investigated in ptype Si1íxGex (x = 0.2) QWs grown by ultrahighvacuum chemical vapor deposition (CVD) [49]. Using the phenomenological Drude model, the contributions from freecarrier absorption and intersubband absorption were separately identified in these measurements. The resulting line width of the fundamental HH resonance was approximately 30 meV. This larger value compared to the MBEgrown QWs of Ref. 7 is likely related not to the growth technique but rather to the weaker confinement of the QWs used in this work. This leads to a broadening of the intersubband absorption peak due to the mixing of the HH2 subband with the continuum. The observed pronounced contribution from freecarrier absorption may also be related to the use of shallow QWs. The growth of SiGeC QWs by CVD has been studied in a comparison of the photoinduced intersubband absorption of 3nmthick Si1íxíyGexCy (x = 17%, y = 1%) QWs and carbonfree reference QWs [50]. Similar spectra were obtained from these two systems, indicating effective substitutional incorporation of the carbon atoms and highquality epitaxial growth. However, in both systems high photopumping levels (> 100 W/cmí2) were required to discriminate intersubband absorption from freecarrier absorption, and the resonance peaks were rather broad. In addition, polarizationresolved intersubband absorption has been used in combination with photoluminescence [51] and Raman spectroscopy [52] to study the thermal stability of pseudomorphically grown Si/SiGe multiple QWs. In general, the Ge and Si atoms in these systems undergo some interdiffusion, which blurs the rectangular shape of the QWs. In turn, this reduces the confinement strength and changes the Ge distribution and thus the strain profile of the heterostructure. As this effect acts differently on the HH, LH, and SO subbands, the thermal relaxation process due to interdiffusion can be observed in the ratio of the TM and TE polarized spectra, which are sensitive to transitions between different pairs of such valence subbands. This behavior has been experimentally observed [51], and was later interpreted with k·p simulations [52]. From Raman and infared studies, the activation process during annealing of pseudomorphic Si/SiGe QWs was proposed to occur in two steps, first by strain relaxation (starting at ~750°C) and then by Ge/Si interdiffusion (from ~ 900°C on) [53]. However, interdiffusion in Si/SiGe Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_360_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 360
Chapter Nine
multilayers on relaxed SiGe pseudosubstrate observed by means of in situ Xray reflectivity has been found to occur at T > 790°C [54], in agreement with Refs. 51 and 52. The magnitude of the intersubband absorption signal in the presence of abovebandgap photoexcitation—and its dependence on the photoexcitation intensity and modulation frequency—have also been investigated to study the recombination kinetics in pseudomorphic ptype Si/SiGe QWs [27]. This method provides a direct measure of the excess carrier density because the intersubband absorption strength depends on the density of confined holes. From this experiment, an interband decay rate of 2.5 s at 80 K was obtained. Furthermore, the contributions from linear (monomolecular) and quadratic (bimolecular) recombination mechanisms were identified from the modulation frequency dependence of the intersubband absorption signal. The latter mechanism is mainly due to nonradiative recombination of the (thermally excited) holes with the electrons distributed in the wells. This description accurately reproduces the experimental dependence of the photoexcitation efficiency on temperature. The need for thick (~ micrometer) multilayer QW structures to achieve quantum cascade structures which provide high gain and good optical mode overlap in infrared waveguides has triggered the interest of the community in straincompensated growth on relaxed SiGe buffer layers. Strain compensation is obtained by balancing the number of tensile layers (e.g., the Si layers) with compressive layers (the SiGe layers). Fortunately, the source material (and time) demanding growth of the relaxed SiGe buffer can be avoided these days, as epitaxyready pseudosubstrates consisting of Si (100) covered by multimicrometerthick relaxed buffer layers have recently become available. Such growth templates have been developed mainly for the realization of highly conducting electron channels in strained Si for highspeed applications in mainstream electronics [55, 56]. The relaxed buffer layers are usually deposited by a fast chemical vapor deposition process on largesize Si (100) substrates. After the epitaxy, planarization by chemical mechanical polishing is sometimes performed. To verify band parameters, such as the band offsets, the Luttinger effective mass parameters, and the deformation potential, in straincompensated SiGe systems, and to prove the accuracy of stateoftheart band structure calculations as well as the growth quality on Gerich pseudosubstrates, detailed intersubband absorption studies and intersubband modeling of ptype Si/ Si1íxGex QWs (x varied from 70% to 85%) grown by MBE on Si0.5Ge0.5 buffer layers were performed [18, 22]. Ge content and layer thicknesses were accurately determined by Xray measurements [22]. By using the Schottky gate modulation technique, the intersubband absorption signal was observed up to Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_361_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
361
room temperature for both TM and TE polarizations. The large HH band offset (> 0.5 eV) results in the observation of wellresolved resonances with transition energies in excess of 300 meV. As mentioned previously, the energy of the fundamental HH transition, as well as the main characteristics of the TM and TE spectra, was found to be in good agreement with model calculations (c.f. Fig. 9.3). This indicates that the growth and modeling of straincompensated SiGe QWs are well under control, opening new possibilities for the realization of elaborate quantum structures such as quantum cascade emitters, as described in the section entitled “MidInfrared Injection Devices.” The importance of resonant intravalence band mixing has been addressed in a recent study of the polarization dependence of the fundamental intersubband resonance in similar strainbalanced ptype SiGe QWs [57]. The mixing is found to become strongest in samples where the HH2 level develops into degeneration with the LH/SO ground state. This situation occurs for Si0.2Ge0.8 QWs approximately 6 nm wide, grown on 50% relaxed buffer substrate. Under these conditions, strong anticrossing occurs, repulsing the levels by as much as 30 meV, which goes along with the transfer of oscillator strength from the TM to TE polarizations, and vice versa. Experimentally, the mixing is observed by the growing intensity of the TE absorption of the HH1toHH2 transition as well as apparent TM coupling of the HH1toLH1 transition, as shown in Fig. 9.7. The Schottky gate modulation technique not only offers high sensitivity by discriminating carrierinduced absorption from the background, but also allows the study of intersubband transitions under an applied electric field. By using this technique, the coupling between confined states in a double QW consisting of symmetrized Si/SiGe layers has been investigated [26]. This structure was grown by MBE on a relaxed buffer substrate of 50% Ge and is shown in Fig. 9.8b. By tuning the voltage between the twodimensional (2D) hole gas and the gate between +1 and –0.5 V, oscillator strength is transferred from the direct to the diagonal transition while the transition energies show anticrossing (c.f. Fig. 9.8a). The experimental data could be accurately reproduced by calculations based on a simple oneband model, assuming depletion from the Ti gate corresponding to an electric field of 130 kV/cm. In particular, the observed coupling strength of 40 meV, obtained from the minimal energy difference between the two resonances (c.f. Fig. 9.8c), is in agreement with the calculated value, assuming a 10.9Åthick square Si barrier. The nominal thickness of this layer was 11 Å, which again demonstrates the high level of accuracy provided by today’s Si MBE technology. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_362_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Chapter Nine
Energy (meV)
362
0.8 T = 12 K
0.7
500 400 300 200 100
0.6
0
10 Å
0.5
(b)
0.4
+0.5 V / +2.5 V
0.3
+0 V / +2.5 V
0.2 +0.5 V / +2.5 V
0.1
+1 V / +2.5 V (x 2)
0 150
200
250 300 Energy (meV) (a)
350
450
Transition energy (meV)
∆T/T (%)
600
Electric field (kV/cm) 260
100
130
160
190
240 220
Theory Experience
200 180 0.50 0.25 0
0.25 0.50 0.75 1.0
Gate voltage (V) (c) Figure 9.7 (a) Schottky biasdependent absorption spectra of a Si0.2Ge0.8/Si/ Si0.2Ge0.8
doubleQW structure. The spectra are referenced to the spectrum taken at +2.5V bias when the QW is depleted. (b) Band structure of the doubleQW structure under flat band condition. (c) Comparison of experimental and calculated transition energies. In the calculations the electric field (upper scale) is taken to consist of the external field determined by the gate voltage and the constant depletion field assumed to be 130 kV/cm. [Source: Diehl et al., Appl. Phys. Lett. 84, 2498 (2004).]
9.3.3
Quantum dots
Intersubband spectroscopy of selfassembled semiconductor quantum dots (QDs) is a subject of interest both for fundamental studies and for the development of infrared photodetectors and lasers. Compared to (twodimensional) QWs, the use of (zerodimensional) QDs for intersubband infrared devices has some advantages, such as their sharp deltalike density of states, reduced intersubband relaxation rates, favorable polarization properties, as well as lower dark current and hence lower noise in photodetectors. These features, combined with the relatively high band offsets and suitability for monolithic integration with Si signal processing and readout electronics, make Ge islands on Si particularly attractive. For a comprehensive review of Si/Gebased QDs and nanostructures, see Ref. 58. Such QDs are formed by the deposition of several (five to nine) monolayers (MLs) of germanium onto a Si (100) substrate. The dot dimensions and densities depend on the growth parameters, such as the substrate temperature [59]. In the lateral direction, typical diameters are between 20 and 80 nm, while heights span from 1.5 to
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_363_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
Frequency (cm1) 2000 3000
4000
500
0.8
T = 15 K
so2
so1
Ih2
TE x5
Si Ge Si QWs 0.2
S6: 7.0 nm
TM Ih1
hh2
1000
hh2
400
hh1so2
hh1so1
Peak position energy (meV)
so2
so1
TE x5
hh2
Ih1
Ih2
S5: 5.5 nm
S4: 4.5 nm
so1
TM
Ih2
hh2
Ih1
Ih2
so1
TM
TE x5
S3: 3.5 nm TE x5
Ih1
Singlepass absorption
TM
363
300 hh1so2
hh1lh2
200 hh1hh2
Ih2
so1
hh2
100 S1: 2.5 nm
hh1lh1
TE x 10
TM x 2
0.2%
0 100
200 300 400 Photon energy (meV) (a)
500
2
3 4 5 6 7 Quantum well thickness (nm) (b)
8
Figure 9.8 (a) TM and TEpolarized intersubband absorption spectra of strain
compensated Si0.2Ge0.8/Si QWs measured at 15 K for well width thicknesses between 2.5 and 7.0 nm. (b) Dependence of peak positions on QW thickness. The solid curve shows transition energies calculated by a selfconsistent sixband k·p model. The dotted curves show the transition energies calculated at the band edge (kpar = 0) where the mixing between HH and LH/SO states is absent. At resonance, when the LH1 level is approaching the HH2 level, the transitions from the HH1 ground state to the HH2 and LH1 appear at equal strength, as is found for sample S7 in TM and in sample S6 in TE. [Source: Tsujino et al., Phys. Rev. B72, 153315 (2005).]
10 nm. Therefore, quantum confinement is strongest along the growth direction. Dot densities exceeding 1011 cm–2 have been obtained [60]. As is typical for systems grown in the StranskiKrastanov mode, a wetting layer of approximately 3 ML of Ge develops before the dots are formed. Due to strain fields, ordered stacking is obtained for adjacent dot layers. During overgrowth with Si, the Ge islands flatten and their Ge concentration tends to decrease due to intermixing. When lowtemperature capping at about 300°C is used, segregation and intermixing of Ge are reduced, as shown by a redshifted photoluminescence [61, 62]. The first intersubband absorption spectra from borondoped multiple Ge QDs grown by MBE showed broad resonances (~100 meV) centered Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_364_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 364
Chapter Nine
at 200 to 250 meV [63]. The absorption signal was significantly stronger for TMpolarized input light compared to TE polarization. This behavior is similar to the case of transitions between HH states in a QW, which suggests that the dots were flattened as expected because of the rather high growth temperature of 650°C used in this study. In a subsequent work with selfassembled ptype Si/Ge QDs grown by MBE at 525°C, the fundamental TM resonance was found at a similar energy (about 250 meV) but with onehalf the spectral width [64]. Through the application of a bias in the lateral direction, using TiAu electrodes evaporated as interdigitated fingers with a 60m spacing, the normalincidence photoconductivity was also investigated in the same samples. Compared to the absorption, the spectral weight was found to be shifted to higher energies (400 meV), which is explained by boundtocontinuum transitions. At a bias of 1 V, the boundtobound HH transition was also observed. This photoconductivity response at normal incidence, i.e., for the “forbidden” xy polarization, is evidence of the relaxation of the QW selection rules caused by the threedimensional hole confinement in the QDs. The strong measured photocurrent due to boundtocontinuum transitions is promising for applications in largearea photodetectors [65]. Si/Ge selfassembled QDs grown by CVD at 550°C have been investigated by Boucaud et al. [66]. Their photoinduced infrared intersubband absorption spectra showed a distinct resonance at approximately 300 meV. Since this resonance appeared to be active for xy polarization, and its energy closely matched the experimental energy difference between the Si bandgap (1.155 meV) and the QD photoluminescence energy (845 meV), it was attributed to the transition between the QD ground states and the continuum states. Furthermore, the photoinduced infrared absorption in these samples was found to saturate at a pump intensity of 10 mW/cm2, which was attributed to filling of the QD ground states, i.e., the creation of two holes per QD. From the estimated dot density of 2 × 109 cm–2, the observed absorption modulation (ǻT/T ~ 0.3%) was calculated to correspond to an interband cross section of ı ~ 2 × 10–13 cm2, which is three orders of magnitude larger than the experimental value found by the same group for InAs/GaAs QDs [67]. However, no physical interpretation was given for this apparent giant cross section. An underestimation of the dot density may in part explain the unexpected result. In Fig. 9.9 is shown the saturation of the photoinduced infrared absorption observed in a dense array of Ge QDs, however at the much higher pump intensity of 110 mW/cm2 [60]. In this study, 10 Ge layers were deposited by MBE at a low growth temperature of 300°C. The Si
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_365_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells
Photoinduced absorption
Interband pump
FWHM (meV) Transition energy (meV) Int absorption (105 eV)
Intersubband Transitions in Si/SiGe Quantum Structures
Dot layers P
(mW/cm2
): 140
Infrared 110 100
0.2%
90 75 40
60
70
80
90
100
110
365
12
8
4 90 80 70
25 20 15 30
70
110
Energy (meV)
Pump intensity (mW/cm2)
(a)
(b)
150
(a) Photoinduced absorption spectra of a dense array of Ge selfassembled QDs measured at quasinormal incidence for different values of the pump power. The crosses show a calculated inhomogeneously broadened absorption line, assuming 20% size inhomogeneity. The experimental data at the incident pump power of 110 mW/cm2 are fitted with a lorentzian (dashed line). (b) From top to bottom: dependence on pump intensity of integrated absorption, transition energy, and absorption line full width at half maximum (FWHM). [Source: Yakimov et al., Phys. Rev. B62, 9939 (2000).] Figure 9.9
capping layers were deposited while the temperature was ramped up to 500°C, leading to good preservation of the island shape and large QD density. The saturation was again attributed to the occupation of two holes per QD. With the assumption that essentially all the photogenerated holes were trapped in the QDs, due to the extremely long electronhole recombination lifetime in Si, an interband absorption cross section ı on the order of 1016 cm2 (as in InAs/GaAs QDs) was correspondingly estimated. Furthermore in this study, the photoinduced infrared resonance was found to become narrow and to shift from 70 to 85 meV as the pump intensity was increased from 40 to 110 mW/cm2, as shown in Fig. 9.9b. This effect was attributed to dynamic screening by the inplane polarized collective excitation [60]. Such description reminds one of the results obtained by numerical simulations of intersubband absorption due to disorder localized electrons in a centerdoped QW [68, 69] and by interlevel electromagnetic response calculations for a rectangular lattice of Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_366_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 366
Chapter Nine
individual spherical quantum dots [70]. For these systems, similar shifts and line narrowing with increasing electron density have been predicted. Note, however, that in a perfect planar situation, the inplane polarized dipole interaction would result rather in a redshifted collective absorption peak [68]. The apparent blue shift may thus be related to the fact that in Yakimov’s experiment [60] with stacked quantum dot arrays the dynamic dipole interaction is dominated by interlayer coupling. In analogy to the situation of the z dipole momentum interaction of inplane distributed intersubband excitations, the dipole coupling then is repulsive and the collective resonance thus blueshifted. A more recent study considered the infrared absorption properties of 20 layers of selfassembled Si/Ge islands embedded in a pin structure [71]. This active region was set in a midinfrared waveguide formed by 3mthick SiGe layers with 2% Ge concentration. Both active region and waveguide were grown by CVD at a total vapor pressure and substrate temperature of approximately 140 mbar and 700°C, respectively. Under a positive bias, carriers in this structure are injected into the QDs, giving rise to absorption in the midinfrared, as well as enhanced interband transmission at nearinfrared wavelengths related to band filling in the Ge islands. A longwavelength resonance at 185 meV was observed and assigned to the boundtocontinuum transition between HH bound levels and the wetting layer ground state. This resonance was found to saturate at a current density of 20 A/cm2. By comparing the observed HH absorption strength with the calculated absorption cross section and mode filling factor, the carrier density in the active region at saturation was found to be 3 × 1018cm–3. At such high carrier concentrations, Auger recombination becomes important, and an estimate for the Auger recombination rate was obtained, slightly enhanced (by a factor of 3 to 4) with respect to bulk Si. Except for Ref. 60, interlevel spectroscopy thus far has been performed on capped Ge QD systems grown at relatively high temperatures T > 500 K. The Si overgrowth at these temperatures leads to interdiffusion of Si into the dots, which reduces the confinement energies and makes the system similar to QWs. Consequently, future investigations should be conducted on betterdefined QDs with high Ge concentration. Issues of interest include depolarization effects for xy polarized excitations and the study of dot size and carrier density dependencies. The latter may be investigated by applying the Schottky gate technique (using transparent gates) or optical modulation.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_367_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
367
9.4 Toward Applications 9.4.1
Infrared photodetectors
Infrared photodetectors are undisputedly one of the most important potential applications of intersubband transitions in Sibased materials. Therefore, as described in the previous section, several investigations of intersubband absorption in these QW and QD systems have addressed detectorrelated issues such as normalincidence response and wavelength tuning. It turns out that among the investigated systems the most promising candidates for device applications are ptype SiGe QWs and Ge QDs. These systems can be grown pseudomorphically on Si (100), and thus they are compatible with Si microelectronics. Moreover, they offer a large band offset for wavelength tuning and bandgap engineering. Quantum well infrared photodetectors (QWIPs) in Si/Ge systems commonly utilize intersubband transitions from the HH ground state to excited states that are close to or above the Si barriers. Thus, as proposed originally [72], the photoexcited holes can give rise to a photocurrent which is collected under the appropriate bias conditions by the doped contact layers above and underneath the multipleQW structure. For a recent review of the fundamental concept and performance of QWIPs (mainly in IIIV semiconductors), see Ref. 73. Typical performance values for SiGe QWIPs, based on a 10period stack of 30Åthick Si/Si1íxGex (x = 35%) QWs [74], are peak responsivities of 50 mA/W at 5 m under normal incidence. The 50nmthick Si barrier layers were used in this structure to suppress the dark current due to tunneling, yielding a 300 K background limited performance at TBLIB = 85 K, similar to QWIPs made of ptype GaAs/AlGaAs QWs. However, at present, ntype GaAsbased devices with appropriate coupling schemes for quasinormal incidence perform much better than any ptype QWIP [73]. Recent development efforts of Si/Ge infrared detectors have focused on dark current suppression schemes, multiwavelength detection, laterally biased photoconductivity, and the use of multiple QD layers. For instance, with the introduction of a pdoped, 30nmwide SiGe emitter layer in a Si/Si1íxGex (x = 23%) QWIP structure, the dark current was reduced considerably even at high bias voltages of up to 5 V [75]. Such an emitter layer establishes an ohmic contact to the top p++ Si contact layer but forms a Schottkytype contact to the SiGe multipleQW region. Probably because of the reduced barrier height in this structure, the peak responsivity was found to be shifted to a lower energy (~200 meV) and a lower value (7 mA/W). The TM response (as measured in the 45 degree waveguide geometry) was found to exceed Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_368_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 368
Chapter Nine
w1 w2 w3 w4 w5
400 300
(a)
1.5 T = 77 K
E
qf
7 6
1
200 Responsivity (mA/W)
Energy (meV)
Energy (meV)
the TE response at wavelengths around 8 m. (~150 meV). The TE component was strongest between 3 and 4.5 m (400 and 250 meV). Widerange wavelength tuning of the peak responsivity has been demonstrated by utilizing charge transfer from a deep to a shallower well in an externally applied electric field [76] (c.f. Fig. 9.10). This QWIP structure consists of several repetitions of a fundamental unit containing five coupled QWs. Depending on the bias, the carriers populate the ground state of the first or the fifth QW in each unit. As these QWs differ in Ge concentration, the spectral onsets of their photocurrent response, which are related to transitions from their ground states to continuum states, differ as well. When the ground states of the five QWs in each unit become energetically aligned (miniband formation), at a bias of around í1 V, a photocurrent starts to flow in the direction of carrier escape. In the wavelength range from 5.9 m (at +5 V) to 3.3 m (at –5 V), a peak responsivity of order 1 mW/A and TBLIP = 80 K resulting in a D * ~ 109 cm Hz / W were measured in this device. Infrared photodetectors based on QDs (QDIPs) are particularly promising because dots are intrinsically suited to normal incidence, their band offsets can generally be larger than in QWs of the same materials, and, finally, they can provide reduced dark currents and
100 0 w1 w2 w3 w4 w5
400 300
(b)
Eqf
5
0.5
4 3 2
0
1 0 1
0.5
4 6
200
8
1
100 0
1.5
100 0
10
20
30
40
50
Growth direction (nm)
60
70
0
100
200
300
400
500
Energy (meV) (c)
(a) Contour plot of the squared moduli of the wave functions and band edge profiles for the HH (dashed), LH (full), and SO (dashed dotted) valence bands for an externally applied bias of –1 V. (b) Similar contour plot but of the excited states integrated over the inplane dispersion and weighted by their contribution to the absorption of normalincident radiation. (c) Responsivity spectra of a cascade injector QWIP measured at T = 77 K and at voltages corresponding to the indicated labels. [Source: Rauter et al., Appl. Phys. Lett. 83, 3879 (2003).] Figure 9.10
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_369_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
369
higher internal gains. Because the carrier confinement is effective in all three spatial dimensions, QD layers can be used to fabricate devices with photocurrent flowing in the vertical direction, similar to QWIPs, but also in the inplane (lateral) direction. A comparison of midinfrared photocurrent generation in Ge QDs embedded in vertical and lateral detector structures has been reported in Ref. 77. Apart from a 40meV red shift (to 284 meV) of the peak response in the lateral detectors, the photoresponse was found to be very similar in the two types of devices. The responsivity of all devices was found to extend to above 600 meV but showed a steep edge at about 250 meV. In the lateral devices, when a 0.5V bias was applied over the 60m spaced interdigitated contacts, peak responsivities of 10 mA/W were obtained. The vertical devices showed onehalf this responsivity at the same bias, which of course corresponds to a much higher electric field. In a subsequent paper [78], the same group presented the intraband response of devices where the QD layers were grown adjacent to Si1íxGex (x = 25%) QWs. The inplane photoresponse was found to increase with decreasing separation d between the QD and QW layers. For d = 10 nm, the responsivity at 20 K increased to 90 mA/W. Above 20 K, however, the responsivity decreased rapidly, and at 40 K it had already dropped by a factor of 10. This loss of sensitivity was attributed to thermal excitation of the holes to the Si valence band continuum, which decreases the hole lifetime and thus the photoresponse. The photoconductivity of the previously mentioned highdensity (3 × 1011 cm–2) SiGe dot arrays [60] has also been investigated [79]. To study their photocurrent response, the dot arrays were embedded in p++ contact layers, with doping provided by boron delta sheets separated from the dot layers by 10nmthick intrinsic Si spacers. The photoresponse was measured under normal incidence in a single pass at room temperature. Two peaks at around 65 and 135 meV were observed and ascribed to transitions from the ground states to excited bound states. In spite of the low measured quantum efficiency of ~0.1%, the detectivity D * at the resonance energies was found to be in the 108 cm Hz / W range, which is comparable to uncooled thermal pyroelectric detectors, demonstrating the potential of this type of Ge dot array detectors for room temperature applications. Stateoftheart D * figures for QD systems are on the order of 1010 cm Hz / W, as measured in photoconductor devices based on InAs QDs operating above liquid nitrogen temperature [80, 81]. To obtain similar D * figures, the Ge dot devices need to be operated at much lower temperatures. This was confirmed in a study of QDIPs containing large dots of 20nm height and 200nm diameter, where the significance of the Si barrier thickness to reduce the dark current and the importance of the bias to tune the wavelength response were investigated [82]. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_370_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 370
Chapter Nine
Using thick Si barriers under low bias, operation from 0.15 to 0.6 eV (9 * to 2 m) was demonstrated with Dmax near 2 × 1010 cm Hz / W, but these values were obtained at T = 30 K. Under a bias of 1 V, the response could also be tuned to the 20m regime (0.06 eV), with a D * of about 109 cm Hz / W. Similarly, the need for lowtemperature operation to reduce the dark current was found in systems consisting of stacks of selfassembled QD layers grown by CVD [83]. In these devices, the 300 K background limited operation required a temperature of 25 K [84], which again is exceedingly low for many practical applications. To summarize, the limitations of Sibased QWIPs concerning dark current and spectral response can be partly solved by using QDs. The main remaining problem is the very low operation temperature. Systematic studies to investigate the temperaturedependent properties of Si/Ge QDIPs would thus be highly valuable. What is interesting to note at this point is the wellbehaved response at 300 K for both midinfrared and longerwavelength devices. 9.4.2
Quantum cascade lasers
The demonstration of a Sibased quantum cascade (QC) laser would represent an important technological achievement from the point of view of both fundamental and applied semiconductor research. Such a device would combine the speed and computing power of microprocessors with the enormous communication bandwidth of optics, and therefore it could have a huge impact on the Si microelectronics industry. In addition, midinfrared and terahertz QC lasers are technologically important for many applications including chemical sensing (e.g., in explosive detection), freespace atmospheric optical communications, and medical analysis. Si would be cheaper than anything else because of the mature, costeffective, and large scale Si processing. Thus Si QC lasers may successfully compete with the present IIIV devices. Moreover, SiGe QC lasers are particularly interesting for the wavelength region around 30 m (~40 meV), which is essentially inaccessible to IIIV semiconductors because of their reststrrahlen band in this spectral range. So far QC lasers have only been realized with IIIV semiconductors, and they utilize electron transitions between conduction subbands. In these devices, depopulation of the lower laser states is controlled by resonant phononassisted energy relaxation, which is particularly fast due to the polar nature of IIIV compounds. On the other hand, Si and Ge are nonpolar materials, and furthermore quantum confinement of conduction band electrons in most types of SiGe QWs is limited due to the small band offsets and the large effective masses (m* ~ m0) for vertical transport. Thus, the challenge in developing a Si/SiGe QC laser Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_371_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
371
is to design a suitable active material based on the quasidegenerate HH, LH, and SO subbands, and to find an alternative mechanism for the depopulation of the lower laser states. Additionally, because of the large effective masses of the SiGe valence bands (m*Si G e ~ 0.2m0 versus m*GaAs ~ 0.07m0 for electrons), the energy levels and the electrical transport are more sensitive to thickness fluctuations, because the well and barrier layers need to be considerably thinner than in IIIV based QC structures. Finally, the optical losses due to freecarrier absorption in the doped contact and QW layers are significant. QC active layers are among the most complex structures ever prepared by epitaxial techniques. This is especially true in the case of the Si/SiGe system because of a number of characteristic features of these materials, namely, the strong affinity of Si and Ge with oxygen, the strong tendency of Ge atoms to segregate and diffuse at the interface, and the possibility of island formation driven by the large strain fields. As a result, low growth temperatures are required for the epitaxy of Si/SiGe QC structures. The challenge is to realize uniform and abrupt interfaces while maintaining the electrical and optical high quality of the crystal. Many groups all over the world are currently working toward this goal, and after the first demonstration of intersubband emission in a Sibased cascade structure [35], further progress is been reported. For clarity, in the following the development of QC emitters in Si is presented in two parts. The section “MidInfrared Injection Devices” is based on boundtobound or boundtocontinuum intersubband transitions in active stages similar to those of the more traditional IIIV midinfrared QC lasers. The section “LongWavelength Emitters” describes terahertz emitters employing transitions between closely spaced subbands within a well or between neighboring wells in simple multipleQW structures. As the spacing between the relevant energy levels in this case is less than the optical phonon energies (for example, 37 meV for the GeGe optical vibrational modes), the intersubband scattering lifetimes can become very long, which is favorable to achieve high emission efficiency in the terahertz range and, eventually, population inversion. Longwavelength emitters. Sibased QC structures are considered to be
particularly well suited for the realization of terahertz radiation sources [85]. This follows from the experimental observation of strong electroluminescence at farinfrared wavelengths and of long upperstate lifetimes; furthermore, theoretical studies have predicted that large population inversions can be obtained in these structures. The first demonstration of terahertz emission with Sibased QC devices was carried out with a simple structure consisting of 30 periods Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_372_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 372
Chapter Nine
of 5nmwide Si barriers and 8nmwide Si1íxGex (x = 28%) wells, grown by CVD on a relaxed buffer substrate with 23% Ge concentration [86]. Band structure calculations were utilized to interpret the measured spectral features. An emission peak at around 100 m (12.4 meV, 2.9 THz) was observed and assigned to vertical transitions between the firstexcited LH and the HH ground state. In a similar structure [consisting of 100 periods of 2.2nmthick Si barriers and 4.4nmthick Si1íxGex (x = 28%) wells on a relaxed buffer substrate with 21% Ge concentration], the observed emission features were attributed to diagonal interwell transitions [87]; c.f. Fig. 9.11a. In both of these structures, the analysis of the emission spectra is complicated by the appearance of impurity lines, which, by their spectral position, were unambiguously assigned to boron (B) acceptors in silicon [87]. Given the low Si content and large strain of the active layers in these samples, such impurity lines probably originate from the substrate, and consequently they cannot be explained by direct carrier injection because no current flows through the substrate. Instead, the impurity signals seem to be related to blackbodytype of emission. In any case, these lines were found to disappear at T > 40 K where thermal ionization sets in. A systematic analysis of the emission spectrum may be required for comparsion of the knowledge of the absorption spectrum. Such data are, however, not available for these structures, possibly due to experimental difficulties related to the wide frequency spread of the oscillator strength. Despite these complications, the polarizationresolved features in the complex emission spectra of the second structure were assigned to transitions from HH1ƍ to LH1 (at 8 meV), LH1ƍ to LH1 combined with HH1ƍ to HH1 (at 25 meV), and LH1ƍ to HH1 (at 40 meV); c.f. inset of Fig. 9.11a (here the primes denote subbands in the QW upstream). In the experiment, the lowestenergy resonance was found to shift from 5 to 8 meV as the bias voltage was varied from 3.8 to 6.5 V [87], as shown in Fig. 9.11b. This shift represents only a fraction of the applied voltage divided by the period number (10 mV per 1V bias), which calls into question the assumptions made regarding the current flow and/or field distribution. The stark shift may also be reduced due to contact resistances. Calculations of the energy levels, scattering processes, and vertical transport in these SiGe terahertz emitters have been carried out by Ikonic et al. [88–90]. The relative importance of nonpolaroptical and acoustic phonon scattering relative to alloy scattering has been discussed in relation to temperature and intersubband transition energies [88]. It was found that alloy scattering is the dominant mechanism, particularly for lowenergy transitions at low temperature. Under these conditions, upperstate population lifetimes on the order Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_373_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells
HH1
5
LH1
HH1 LH1
4
Experiment Theory
HH1 LH1
HH1 LH1
(b′)
3 (c′)
2
8.0 7.5 7.0 6.5 6.0 5.5 5.0 3.5
LH1
HH1
4.5 5.0
4.0
0
10
40 20 30 Energy (meV) (a)
5.5
6.0
6.5
Voltage (V) (b)
LH1
1 0
373
HH1
(a′)
50
60
Current (A)
Spectral power (arb. units)
6
Peak energy (meV)
Intersubband Transitions in Si/SiGe Quantum Structures
0.9 0.8 0.7 0.6 0.5 0.4 0.3 3
4
5
6
7
8
Voltage (V) (c)
Figure 9.11 (a) Longwavelength edge emission from a 100period Si/SiGe multipleQW cascade structure measured under an applied bias of 6.4 V (10% duty cycle) at 4.2 K (point dashed line) and theoretical predictions (solid line). The spectral features are assigned to interwell intersubband transitions from the HH1 and LH1 states in each well to the HH1 and LH1 states in the QW downstream; c.f. inset. Spectral features labeled by (aƍ) through (cƍ) are identified as impurity transitions involving B acceptors in bulk Si. (b) Peak energy versus applied voltage for the lowenergy resonance. (c) Currentvoltage characteristics of the device. [Source: Bates et al., Appl. Phys. Lett. 83, 4092 (2003).]
of 3 to 10 ps were predicted. To include carrier dynamics and transport in this theoretical description, the same authors have employed the method of the selfconsistent energy balance [89] and Monte Carlo (MC) simulations [90]. For both methods, the assumption is made that the electric field is uniform across the active region, and holehole scattering, interface roughness, and scattering into the nextnearest neighboring wells have all been neglected thus far in the modeling. From their analysis of the biasdependent subband occupation probabilities in structures with a single QW per period (similar to the design that was investigated experimentally in Ref. 87), population inversion between HH1ƍ and LH1 at high electric fields (~80 keV/cm) was predicted [89]. In fact, the calculation predicts that independent of the bias, the population of HH1 is higher than in LH1. According to the authors, such a stable population relation between HH1 and LH1 is plausible because of the better confinement of the HH1 states—due to the higher band offset of HHs compared to LHs—which leads to a longer dwell time of carriers in HH1. In theory, the performance of these structures is found to be much better than that of structures based on the inverted mass feature of the LH1 inplane dispersion [91]. Unfortunately, in an experiment where only spontaneous emission is
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_374_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 374
Chapter Nine
measured [87, 88], no conclusive statement concerning population inversion can be made, and thus experimentally this prediction has not yet been verified. Moreover, the calculated currents are found to disagree with experiment. When the HH1ƍ and LH1 levels become aligned (at approximately 42 keV/cm2), current densities of ~5kA/cm2 are predicated, while experimentally the current flowing through the 240m × 240m mesa at 4.2 K and for a 5V bias was 0.55 A (or 0.65 kA/ cm2) (c.f. Fig. 9.11c). The current is monotonically increasing with bias, different from the case of Si MBEgrown strainbalanced Si/SiGe superlattices, where negative differential resistances due to resonant tunneling as well as the sign of domain formation have been indicated [92]. It appears that model predictions of the state lifetimes are in fair agreement with experiments on unbiased QW structures. In a recent work, Kelsall et al. [34] reported a degenerate pumpprobe experiment carried out on multiQW structures made of alternating 2.2nmthick Si barriers and SiGe wells of 6.6nm (4.4nm) thickness and 34% (25%) Ge concentration. In contrast to earlier measurements with multipleQW structures where the QWs were isolated from one another by SiGe spacer layers [33], in this case the decay was well fitted by a single exponential. This confirmed the hypothesis [33] that the previously observed dual exponential decay arose from scattering into intermediate states in the spacer layers. The measured absorption recovery times were found to lie between 2 and 25 ps, with the time increasing with decreasing LH1toHH1 separation [34]. This observation confirms the importance of the deformation potential scattering which gets suppressed for reduced subband spacing below the energy of the GeGe optical phonon mode. The temperature dependence was weak, which is explained by alloy scattering dominating phonon scattering. Finally, it should be mentioned that the realization of SiGe terahertz lasers will require the development of appropriate waveguide structures [93]. Toward this goal, the use of buried tungsten silicide layers for confinement of the optical mode has been investigated [94]. Midinfrared injection devices. Intersubband electroluminescence from
Sibased QC emitters was first observed in pseudomorphically grown Si/SiGe shortperiod superlattices consisting of five QWs per period [35]. These superlattices were designed to achieve a strong overlap of the lowest HH miniband states in the active wells at an electric field of 50 keV/cm (c.f. Fig. 9.12, left panel). Consistent with this design, the emission spectrum, also shown in the figure, was found to be centered at the calculated HH1HH2 transition energy of 130 meV; furthermore, the light output was purely TM polarized, as expected for transitions between HH states. The corresponding full width at half maximum was Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_375_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
0.08
Energy (eV)
0
Sample QCI Si/Six1Gex HH1 Injector
0.1 0.2
LH HH
HH2
w5 w4 w3/0.32 w2/0.32 w1/0.32 w5/0.21 w4/0.21 w3/0.32
0.3 0.4 100
Growth direction 50kV/cm
0 100 200 300 400 500 600
E.L. intensity (pW/meV)
0.1
L (pW)
375
V (V)
10 8 6 4
0.06
4
2 0 0.0
0.04
0.02
2 0.4
I (A) TM TE
0.8
0
0.00 100
150
200
250
Position (Å)
Energy (meV)
(a)
(b)
300
Figure 9.12 (a) Schematics of the valence band potential energy profile of a Si/SiGe QC
emitter consisting of five wells per period at the electric field of 50 kV/cm. The emission involves transitions between the HH1 and HH2 states, whose wave functions squared are shown by the solid lines. The wave functions of HH injector miniband states are given by the dotted lines. The shadowed areas denote the energy levels of the injector miniband as well as the intermediate LH states. (b) Electroluminescence spectra measured at T = 50 K and I = 250 mA with 50% duty cycle (dark solid line). The polarization dependence is investigated at 760 mA and T = 85 K. Practically no signal is obtained with TEpolarized light (dotted curve), giving strong evidence of transitions between the HH2 and HH1 states. [Source: Dehlinger et al., Science 290, 2278 (2000).]
only 22 meV, close to the best values obtained for pseudomorphic ptype SiGe QWs in linear absorption [7]. The emission efficiency of these structures was measured, using an FTIR setup that was calibrated for absolute intensities with an InGaAs/AlInAs intersubband LED of wellknown radiative and nonradiative lifetimes. The radiative emission efficiency and the nonradiative lifetime were found to depend strongly on the design of the active QW. Design issues include the blocking of the carrier escape to the continuum and the actual nonradiative decay time from the upper to the lower state. This issue has been addressed in a subsequent study where the emission efficiencies of cascade structures with 45Åwide Si1íxGex active QWs of x = 32% and 41% (QC1 and QC2) were compared to those of a cascade structure with 39Åwide (x = 42%) QWs (QC3) [95]. The quantum efficiency of QC1 and QC3 was found to be relatively low, while that of QC2 was reasonably high. The deduced nonradiative lifetime was on the order of 500 fs [35]. To explain these observations, it is necessary to consider the main nonradiative decay paths in these structures, illustrated schematically in Fig. 9.13. The direct relaxation from the injector to the HH ground state (path 1 in Fig. 9.13) primarily depends on the barrier thickness, and thus should not differ much among the three structures. The escape to the continuum (path 2 in Fig. 9.13) should be similar for QC2 and
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_376_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 376
Chapter Nine
Valenceband Energy
3 1 2
1
direct relaxation
2
escape continuum
3
phonon emission
Schematic representation of the possible energy relaxation paths in SiGe QC structures (only the two main QWs of each period are shown, i.e., the adjacent injector and emitter wells). (1) Nonradiative relaxation from the injector to the emitter ground state; (2) escape to the continuum; and (3) relaxation via an intermediate LH level by opticalphonon emission.
Figure 9.13
QC3, given their similar Ge content in the active wells, and thus is also not likely related to the higher efficiency of QC2. Therefore, the process that appears to give the dominant contribution to the nonradiative relaxation time is the emission of optical phonons via the deformation potential. As predicted in Ref. 24, this scattering mechanism is most efficient between subbands of different symmetry, such as HHtoLH subbands. In QC1 and QC3 the energy separation between subbands HH2 and LH1 is larger than, and relatively close to, the energy of the SiSi phonon mode (~60 meV). Thus, phonon emission is very efficient in these structures. And vice versa, in QC2 the separation between HH2 and LH1 is about 40 meV, so that phonon emission is essentially disallowed except for the lowest but also weakest GeGe mode. From Fig. 9.4, taken from Ref. 24, we find that the lifetime in systems where only the lowest phonon mode (GeGe) is available for emission is about 0.5 to 1 ps, consistent with the measured value in QC2. The current and temperaturedependent emission characteristics of similar SiGe cascade structures but with seven QWs per period have been measured and compared to the results of a k·p calculation by Bormann et al. [96]. The theory was found to give an appropriate description of the observed polarization selection rules, confinement energies, and lowenergy emission line broadening at high currents. The emission was again ascribed to HH transitions. For this structure a lifetime of 400 fs was calculated, but no comparison with experiments was possible, since the setup used was not calibrated to measure absolute efficiencies. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_377_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
377
The question of the upperstate lifetime was addressed by the same group in a subsequent study where the emission efficiency associated with diagonal transitions was determined as a function of barrier width and corresponding oscillator strength [36]. For several QC structures, these authors computed the ratio of the measured emission efficiency divided by the calculated oscillator strength, from which they obtained the upperstate lifetime to within a multiplicative constant. This result is plotted in Fig. 9.14, compared with calculated values. A significant increase of scattering time with increasing barrier width is observed, consistent with calculations. Compared to the case of vertical transitions, the scattering time in this system can be increased by more than one order of magnitude. Unfortunately, the oscillator strength— and hence the optical gain—are correspondingly reduced by a similar factor. The authors thus concluded that diagonal transitions may enable intersubband population inversion, but at the price of a reduced optical matrix element. A further drawback to the use of diagonal transitions in SiGebased QC structures is the considerable line width increase, e.g., from 26 to 39 meV [36], due to interface roughness scattering. This is analogous to the case of intersubband absorption in coupled wells reported in Ref. 26, where the line widths of vertical and diagonal transitions were 21 and 36 meV, respectively. Recent research on Sibased QC emitters has focused on the midinfrared electroluminescence from straincompensated structures with high Ge concentration, prepared on relaxed buffer substrates. This step
Scattering time t2 (ps)
dsi 10
1 Experimental Calculated
0
5
20 25 10 15 Si barrier layer width (Å)
30
35
Figure 9.14 Comparison between calculated and experimental nonradiative scattering
times as derived from electroluminescence intensities in Si/SiGe cascade emitters with optically active diagonal transitions across Si barriers of variable width. The experimental points (relative values) have been scaled to match the calculated result for the structure with a 15Åwide Si barrier. [Source: Bormann et al., Appl. Phys. Lett. 83, 5371 (2002).]
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_378_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 378
Chapter Nine
was needed to overcome the strain limitations concerning the number of QWs per period (five to seven) and the number of periods (10 to 15) in the active layer. In principle, the resulting increase in design freedom allows one to fabricate more complex cascade structures with improved carrier extraction from the lower states. The first midinfrared emitters using the strain symmetrization concept were realized by Diehl et al. [97] with Si/Si1í xGex (x = 80%) cascade structures grown on 50% SiGe relaxed buffer substrates. As can be recognized from the band structure shown in Fig. 9.15a, these QC emitters are based on the boundtocontinuum design; i.e., the excited state is confined in the active well, but the lower state extends over several QWs and belongs to a broad miniband. The main advantage of this design is that the various relaxation paths within the miniband allow for fast depopulation of the lower state. In the device of Fig. 9.15, the Ge concentration averaged over one cascade period corresponds to that of the relaxed buffer substrate (50%), so that the accumulated strain in each period is almost compensated. It is not exactly compensated because Vegard’s law does not apply for the elastic constants, as demonstrated for the case of the AlGaAs system [98]. Within the period, the strain averaged over neighboring Si and SiGe layers is changing gradually, as shown in Fig. 9.15b, but the strain forces stay well below the limit imposed by strain relaxation. For example, the maximal thickness of the Si layers in the above structure (25 Å) is much less than the critical thickness for a Si layer on a 50% relaxed buffer layer to form misfit dislocations, which is 10 nm. Similarly, on the length scale of a cascade period (40.4 nm for the structure above) the Ge concentration does not deviate from the average by more than 2.5%, as shown in Fig. 9.15b. On the other hand, on this length scale SiGe layers with even a 20% mismatch would be stable against the spontaneous formation of misfit dislocations. Emission from this structure was found to occur at 176 meV, in good agreement with the calculations. The current voltage (IV) characteristics measured at 80 K show a clear onset, corresponding to the voltage required to align the minibands leading to a noticeable current flow through the structure. This onset occurs at a lower bias than the design value, but was found to scale well among three identical samples with 3, 15, and 30 periods, indicating that the current is flowing through the QW states and not through the dislocations present in the structure. The full width at half maximum of the intersubband emission was about 45 meV, measured close to the emission onset, and has been ascribed to scattering due to interface roughness. Using interface roughness parameters estimated from Xray reflectivity, from highresolution crosssectional transmission electron microscopy, and from the measured relation between thickness and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_379_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
379
Injection barrier (25 Å)
Energy
70 kV/cm
m)
0n
e
1p
(a) 20
2.5
0
0
2.5
 50% Si/Si0.2Ge0.8 doublelayer average
 50% Summation over single period
5
(4 riod
20 5
1 period (40 nm)
(b) Figure 9.15 (a) Schematic diagram of a Si/SiGe QC structure of the boundtocontinuum
type, which is straincompensated to a relaxed buffer with 50% germanium content. The moduli squared of the wave functions of the HH states relevant for the optical transition and of some of the interdispersed LH states are given by the solid and dashed lines, respectively. Note that the energy axis is upside down. (b) Ge concentration averaged over one cascade period, given in relation to the 50% Ge concentration of the relaxed buffer substrate. The peak values of the Ge concentration averaged over one period (dashed line, lefthand scale) and averaged over adjacent Si and Si0.2Ge0.8 layers are noncritical, i.e., the respective length scales—period length (40 nm) and layer thicknesses (4 Å < t < 25 Å)—are considerably smaller than the critical layer thicknesses for which, at corresponding Ge concentrations, dislocations would be formed. This makes it possible to grow many periods of this structure. [Source: Diehl et al., Physica E16, 315 (2003).]
lowtemperature Hall mobility in Si/SiGe QWs [99], Tsujino et al. calculated the electroluminescence line width of the emitters as a function of the correlation length of the interface roughness in the vertical (i.e., growth) direction [100]. As shown in Fig. 9.16, the measured line width could be reproduced, assuming a vertical correlation length in the range of 1.4 to 2.2 nm. This implies that partial cancellation of the interface roughness does occur in the investigated cascade structures, as the active QWs are separated by less than this amount.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_380_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 380
Chapter Nine
100 F = 70 kV/cm
Si 0.6 nm
Intersubband broadening (eV)
= 2.3 nm
Si 0.5 nm Si 0.4 nm
10
1
Si 2.5 nm Δ = 0.4 nm Si 1.7 nm Si 1.6 nm Si 1.5 nm
102
Δ = 0.3 nm
Si 1.3 nm Si 1.2 nm Si 1.1 nm Si 1.0 nm
103 0.1
1 Vertical correlation length
К
10 (nm)
(b)
(a) Figure 9.16 (a) Calculated line width of the intersubband electroluminescence spectrum of the SiGe/Si QC structure shown on Fig. 9.15a, assumed to be limited by interface roughness scattering, plotted as a function of the vertical correlation length ț. The values for the lateral roughness and lateral correlation length used in this plot, 0.3 nm < ǻ < 0.4 nm and ȁ = 2.3 nm, respectively, were taken from Hall measurements and transmission electron microscopy (TEM). The observed emission line broadening of ~45 meV is consistent with interfaces that are correlated at separations up to 1.8 nm ± 0.4 nm. (b) TEM cross section showing the Si barriers (bright) and the Si0.2Ge0.8 wells (dark). [Source: Tsujino et al., Appl. Phys. Lett. 86, 062,113 (2005).]
A detailed analysis of the lifetime performance and current limitations of midinfrared Sibased QC structures grown on relaxed buffer layers and based on the boundtocontinuum design has been presented recently by Borak et al. [37]. From the measured emission efficiencies of 10–5 to 10–6 such devices and calculated radiative lifetime of ~95 ns, an upperstate lifetime between 10 and 100 fs was deduced, assuming a 100% injection efficiency. The emission efficiency started to level off at current densities of ~6.5 kA/cm2. From these data, an upper bound for the gain coefficient G per period was estimated at ~1 to 2 cmí1. This is a very low number, particularly in relation with the freecarrier absorption (FCA) coefficient of the active layer itself. By using the effective mass m* = 0.2m0 and a momentum relaxation time of ~10 fs [corresponding to a mobility of ~100 cm2/(V· s)] the FCA coefficient
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_381_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
381
was estimated to be ~15 cm–1 at the device emission photon energy of ~200 meV and carrier concentration of 5 × 1017 cm–3. Therefore, a substantial performance improvement is required to surmount the freecarrier losses as well as the additional losses in a laser waveguide device. Varying the doping density may not be an effective strategy in this respect, since for a parabolic dispersion the ratio G/FCA is approximately independent of carrier concentration. Rather, a substantial increase in upperstate lifetime and/or a reduction of the line width, e.g., by reducing the effect of nonparabolicity by working closer to kpar = 0, will likely be required to improve the gain and hence achieve lasing. A possible approach to achieve the required performance improvement is to design structures in which the overlap of the upper emission state with the LH/SO states is decreased and/or the energy separation between these states is reduced to below the optical phonon energies. This turns out to be difficult, because the LH/SO states tend to disperse when the HH states align and form a miniband. Further improvements may be obtained by using nonvertical transitions to extend the upperstate lifetime, as in the work by Bormann et al. [36]. The results presented by Tsujino et al. [100], showing the effect on the emission line width of vertical correlations in interface roughness, also provide important guidelines in the design of improved Sibased QC structures. Aside from these considerations relating to the active layer, several aspects of the device physics also have to be addressed and optimized before intersubband laser action can be demonstrated in Si/SiGe QWs. These include the design of the optical waveguide to obtain high mode filling, uniform carrier injection, and minimal optical losses from the electrical contacts. A detailed discussion of these aspects is, however, beyond the scope of this chapter. 9.5 Summary and Outlook Progress over the last 15 years of intersubbandbased spectroscopy and applications of the Si/SiGe system is reviewed. Technical details of various intersubband experiments covering linear absorption, emission, modulation by electric and light fields, and timesolved spectroscopy are introduced. Most of the investigations discussed involve ptype intersubband systems because of the favorable (compared to the conduction band systems) large band offsets and low confinement masses in the valence band. Corresponding polarizationdependent selection rules of intersubband and intralevel transition within and between the multivalence band are summarized, and experiments are presented that demonstrate level mixing and crossing. Measurement configurations are elucidated for which normalincidence absorption is taking place. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_382_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 382
Chapter Nine
Advanced Si epitaxy, in particular for growth on relaxed buffer substrate, is demonstrated by narrow intersubband line width. Excellent agreement is found for band structure calculation exposed to detailed intersubband studies of ptype Si/SiGe QWs grown straincompensated on relaxed buffer substrate. Advances in Sibased infrared detection are illuminated by giving examples from pseudomorphic QW systems to QD systems with twodimensional hole channels to improve responsivity. It is concluded that the application potential of Sibased infared photodetectors is still valid, provided that reduction of dark currents at temperatures beyond 30 K can be realized. A detailed summary is given of recent efforts to develop a Sibased intersubband laser. Systems presented include, for the terahertz regime, singleQW superlattices and, for midinfrared emission, multiperiod cascade structures, consisting of tunneling injector, active QWs for vertical or diagonal emission, and continuumtype depopulation sections. Presently, a gain deficit due to interfaceroughnessbroadened emission and short upperstate lifetimes, due to immersed LH/SO states, combined with strong freecarrier absorption is hindering the latter system from successfully lasing. It is argued that formation of electric field domains is occurring in the biased superlattices, in contradiction to the implications made for modeling of the highfieldcurrent transport. Research opportunities are suggested for the study of depolarization and manybody effects in the intersubband absorption of QWs and interlevel transitions in QDs. The latter systems resemble a strongly disordered twodimensional system, for which phase locking of the distributed dipoles by the electromagnetic field is predicted to generate large depolarization shifts: toward the blue for perpendicular (to the QW) polarization and toward the red for parallel polarization. However, interlevel absorption performed on Ge island arrays shows a blue shift for increasing level population. Exploring light modulation techniques to study the intersubband resonances of two and threedimensional strainfield ordered arrays of Ge QD islands—obtained by lowtemperature Si capping—may allow clarification of this matter by experiment. 9.6 Acknowledgments The author wishes to thank A. Borak, P. Bouceaud, T. Fromherz, R. Paiella, and D. Paul for critical reading of and suggestions on essential parts of the manuscript. I would like also to acknowledge the many collaborators working with me over the last 10 years on the topics presented here. For frequent discussion of the presented material, I wish to thank S. Tsujino. Finally, I would like to thank
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_383_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
383
G. Abstreiter, T. Fromherz, D. Paul, K. Reimann, and A. Yakimov for permission to use various figures presented in this chapter. References 1.
For a review see T. Ando, A. B. Fowler, and F. Stern, Rev. Modern Phys. 54, 437 (1982).
2.
L. C. West and S. J. Eglash, Appl. Phys. Lett. 46, 1156 (1985).
3.
For a review see “Intersubband Transitions in Quantum Wells,” E. Rosencher, B. Vinter, and B. Levine, eds., Proceedings of a NATO Advanced Workshop CY, Sept. 9–14, 1991, CL Cargèse, France, 1992.
4.
M. Helm, in Intersubband Transitions in Quantum Wells: Physics and Device Applications I, H. C. Liu and F. Capasso, eds., Semiconductors and Semimetals 62, 99 (2000).
5.
S. K. Chun, and K. L. Wang, Phys. Rev. B46, 7682 (1992).
6.
W. I. Xu, Y. Fu, M. Willander, and S. C. Shen, Phys. Rev. B49, 13760 (1994).
7.
T. Fromherz, E. Koppensteiner, M. Helm, G. Bauer, J. F. Nutzel, and G. Abstreiter, Phys. Rev. B50, 15073 (1994).
8.
M. El Kurdi, G. Fishman, S. Sauvage, and P. Boucaud, Phys. Rev. B68, 165333 (2003).
9.
Cho, S. M. Lee, H. H., Journ. Appl. Phys. 73, 1918 (1993).
10.
G. Hionis, M. Tsetseri, A. Zora, and G. P. Triberis, Superlattices and Microstructures 28, 151 (2000).
11.
W. L. Xu, Y. Fu, M. Willander, and S. C. Shen, Phys. Rev. B48, 11477 (1993).
12.
A. Kahan, M. Chi, and L. Friedman, J. Appl. Phys. 75, 8012 (1994).
13.
T.S. Liou, T. Wang, and C.Y. Chang, J. of Appl. Phys. 77, 6646 (1995).
14.
S. Ridene, K. Boujdaria, H. Bouchriha, and G. Fishman, Phys. Rev. B64, 1 (2001).
15.
K. Boujdaria, S. Ridene, S. B. Radhia, O. Zitouni, H. Bouchriha, and G. Fishman, J. Appl. Phys. 92, 2586 (2002).
16.
D. E. Weeks, S. H. Yang, M. R. Gregg, S. J. Novotny, K. D. Greene, and R. L. Hengehold, Phys. Rev. B65, 195314 (2002).
17.
Y.Y. Lin, and J. Singh, J. Appl. Phys. 96, 1059 (2004).
18.
L. Diehl, H. Sigg, G. Dehlinger, D. Grützmacher, E. Müller, U. Gennser, I. Sagnes, T. Fromherz, Y. Campidelli, O. Kermarrec, D. Bensahel, and J. Faist, Appl. Phys. Lett. 80, 3274 (2002).
19.
C. G. Van der Walle Phys. Rev. B39, 1871 (1989).
20.
M. M. Rieger and P. Vogl, Phys. Rev. B48, 14276 (1993).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_384_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 384
Chapter Nine
21.
T. Fromherz, M. Meduna, G. Bauer, A. Borak, C. V. Falub, S. Tsujino, H. Sigg, and D. Grützmacher, J. Appl. Phys. 78, 044501 (2005).
22.
R. Winkler, M. Merkler, T. Darnhofer, and U. Rössler, Phys. Rev. B53, 10858 (1993).
23.
G. Sun, and L. Friedman, Phys. Rev. B53, 3966 (1996).
24.
K. Reimann, R. A. Kaindl, and M. Woerner, Phys. Rev. B65, 045302 (2002).
25.
H. Sigg, M. H. Kwakernaak, B. Margot, D. Erni, P. van Son and K. Köhler, Appl. Phys. Lett. 67, 2827 (1995).
26.
L. Diehl, A. Borak, S. Mentese, D. Grützmacher, H. Sigg, U. Gennser, I. Sagnes, Y. Campidelli, O. Kermarrec, D. Bensahel, and J. Faist, Appl. Phys. Lett. 84, 2497 (2004).
27.
E. Dekel, E. Ehrenfreund, D. Gershoni, P. Boucaud, I. Sagnes, and Y. Campidelli, Phys. Rev. B56, 15734 (1997).
28.
L. Wu, P. Boucaud, J.M. Lourtioz, F. H. Julien, I. Sagnes, Y. Campidelli, and P.A. Badoz, Appl. Phys. Lett. 67, 3462 (1995).
29.
P. Boucaud, L. Gao, Z. Moussa, F. Visocekas, F. H. Julien, J.M. Lourtioz, I. Sagnes, Y. Campidelli, and P.A. Badoz, Appl. Phys. Lett. 67, 2948 (1995).
30.
P. Boucaud, F. H. Julien, R. Prazeres, J.M. Ortega, I. Sagnes, and Y. Campidelli, Appl. Phys. Lett. 69, 3069 (1996).
31.
R. A. Kaindl, M. Wurm, K. Reimann, M. Woerner, T. Elsaesser, C. Miesner, K. Brunner, and G. Abstreiter, Phys. Rev. Lett. 86, 1122 (2001).
32.
W. Heiss, E. Gornik, H. Hertle, B. Murdin, G. M. H. Knippels, C. J. G. M. Langerak, F. Schaffler, and C. R. Pidgeon, Appl. Phys. Lett. 66, 3313 (1995).
33.
P. Murzyn, C. R. Pidgeon, J.P. R. Wells, I. V. Bradley, Z. Ikonic, R. W. Kelsall, P. Harrison, S. A. Lynch, D. J. Paul, D. D. Arnone, D. J. Robbins, D. Norris, and A. G. Cullis, Appl. Phys. Lett. 80, 1456 (2002).
34.
R. W. Kelsall, Z. Ikonic, P. Murzyn, C. R. Pidgeon, P. J. Phillips, D. Carder, P. Harrison, S. A. Lynch, P. Townsend, D. J. Paul, S. L. Liew, D. J. Norris, and A. G. Cullis, Phys. Rev. B71, 115326 (2005).
35.
G. Dehlinger, L. Diehl, U. Gennser, H. Sigg, J. Faist, K. Ensslin, D. Grützmacher, and E. Müller, Science 290, 2277 (2000).
36.
I. Bormann, K. Brunner, S. Hackenbuchner, G. Abstreiter, S. Schmult, and W. Wegscheider, Appl. Phys. Lett. 83, 5371 (2003).
37.
A. Borak, S. Tsujino, C. V. Falub, M. Scheinert, L. Diehl, E. Müller, H. Sigg, D. Grützmacher, U. Gennser, I. Sagnes, S. Blunier, T. Fromherz, Y. Campidelli, O. Kermarrec, D. Bensahel, and J. Faist , MRS Symp. Proc. 832, F4.2.1 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_385_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
385
38.
R. P. G. Karunasiri, J. S. Park, K. L. Wang, and LiJen Cheng, Appl. Phys. Lett. 56, 1342 (1990).
39.
R. P. G. Karunasiri, J. S. Park, Y. J. Mii, and K. L. Wang, Appl. Phys. Lett. 57, 2585 (1990).
40.
J. S. Park, R. P. G. Karunasiri, Y. J. Mii, and K. L. Wang, Appl. Phys. Lett. 58, 1083 (1991).
41.
J. S. Park, R. P. G. Karnasiri, and K. L. Wang, Appl. Phys. Lett. 61, 681 (1992).
42.
S. K. Chun, D. S. Pan, and K. L. Wang, Phys. Rev. B47, 15638 (1993).
43.
H. Hertle, G. Schuberth, E. Gornik, G. Abstreiter, and F. Schaffler, Appl. Phys. Lett. 59, 2977 (1991).
44.
C. Lee, and K. L.Wang, Appl. Phys. Lett. 60, 2264 (1992).
45.
C. Lee, and K. L. Wang, Appl. Phys. Lett. 64, 1256 (1994).
46.
K. Fujita, S. Fukatsu, Y. Shiraki, H. Yaguchi, and R. Ito, Appl. Phys. Lett. 61, 210 (1992).
47.
D. K. Nayak, N. Usami, S. Fukatsu, and Y. Shiraki, Appl. Phys. Lett. 63, 3509 (1993).
48.
T. Fromherz, P. Kruck, M. Helm, G. Bauer, J. F. Nutzel, and G. Abstreiter, Appl. Phys. Lett. 68, 3611 (1996).
49.
J. M. Berroir, S. Zanier, Y. Guldner, J. P. Vieren, I. Sagnes, Y. Campidelli, P. A. Badoz, and B. Gil, and R.L. Aulombard, Proceedings of Semiconductor Heteroepitaxy: Growth Characterization and Device Applictions CY July 4–7 1995, CL Montpellier, France, P.314, 1995.
50.
P. Boucaud, J.M. Lourtioz, F. H. Julien, P. Warren, and M. Dutoit, Appl. Phys. Lett. 69, 1734 (1996).
51.
P. Boucaud, L. Wu, C. Guedj, F. H. Julien, I. Sajnes, Y. Campidelli, and L. Garchery, J. Appl. Phys. 80, 1414 (1996).
52.
R. Oszwaldowski, and G. Fishman, Molecular Physics Reports CT National Symposium on Crystalline Microstructures CY July 2–4 1997, CL Poznan, Poland, vol. 21, p. 99, 1998.
53.
B. Adoram, D. Krapf, J. Shappir, A. Sa’ar, M. Levy, R. Beserman, S. G. Thomas, and K. L. Wang, Appl. Phys. Lett. 75, 2232 (1999).
54.
M. Meduna, J. Novak, C. V. Falub, G. Chen, G. Bauer, S. Tsujino, D. Grutzmacher, E. Muller, Y. Campidelli, O. Kermarrec, D. Bensahel, and N. Schell, J. Phys. D. Appl. Phys. 38, A121 (2005).
55.
M. Y. A. Yousif, O. Nur, M .Willander, C. J. Patel, C. Hernandez, Y. Campidelli, D. Bensahel, and R. N. Kyutt, SolidState Electronics 45, 1869 (2001).
56.
G. Isella, D. Chrastina, B. Rossner, T. Hackbarth, H. Herzog, U. Konig, and H. von Känel, SolidState Electronics 48, 1317 (2004).
57.
S. Tsujino, A. Borak, C. V. Falub, T. Fromherz, L. Diehl, H. Sigg, and D. Grützmacher, Phys. Rev. B72, 153315 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_386_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 386
Chapter Nine
58.
K. Brunner, Reports on Progress in Physics 65, 27 (2002).
59.
Y.–W. Mo, D. E. Savage, B. S. Swartzentruber, and M. G. Lagally, Phys. Rev. Lett. 65, 1020 (1990).
60.
A. I. Yakimov, A. V. Dvurechenskii, N. P. Stepina, and A. I. Nikiforov, Phys. Rev. B62, 9939 (2000).
61.
U. Denker, M. Stoffel, O. G. Schmidt, and H. Sigg, Appl. Phys. Lett. 82, 454 (2003).
62.
M. Stoffel, U. Denker, G. S. Kar, H. Sigg, and O. G. Schmidt, Appl. Phys. Lett. 83, 2910 (2003).
63.
J. L. Liu, W. G. Wu, A. Balandin, G. L. Jin, and K. L. Wang, Appl. Phys. Lett. 74, 185 (1999).
64.
T. Fromherz, W. Mac, A. Hesse, G. Bauer, C. Miesner, K. Brunner, and G. Abstreiter, Appl. Phys. Lett. 80, 2093 (2002).
65.
C. Miesner, O. Rothig, K. Brunner, and G. Abstreiter, Appl. Phys. Lett. 76, 1027 (2000).
66.
P. Boucaud, V. Le Thanh, S. Sauvage, D. Debarre, and D. Bouchier, Appl. Phys. Lett. 74, 401 (1999).
67.
S. Sauvage, P. Boucaud, J.M. Gerard, and V. ThierryMieg, Phys. Rev. B58, 10562 (1998).
68.
C. Metzner, and G. H. Döhler, Physica E7, 718 (2000).
69.
R. N. Riemann, C. Metzner, and G. H. Döhler, Phys. Rev. B65, 115304 (2002).
70.
V. Bondarenko, M. Zaluzny, and Y. Zhao, Phys. Rev. B71, 115304 (2005).
71.
M. El Kurdi, P. Boucaud, S. Sauvage, F. Aniel, G. Fishman, O. Kermarrec, Y. Campidelli, D. Bensahel, G. SaintGirons, I. Sagnes, and G. Patriarche, J. Appl. Phys. 97, 83525 (2005).
72.
B.F. Levine, J. Appl. Phys. 74, R1 (1993).
73.
H.C. Liu, in Intersubband Transitions in Quantum Wells: Physics and Device Applications, H. C. Liu, and F. Capasso, eds., Semiconductors and Semimetals 62, 129 (2000).
74.
P. Kruck, M. Helm, T. Fromherz, G. Bauer, J. F. Nutzel, and G. Abstreiter, Appl. Phys. Lett. 69, 3372 (1996).
75.
D. Krapf, B. Adoram, J. Shappir, A. Sa’ar, S. G. Thomas, J. L. Liu, and K. L. Wang, Appl. Phys. Lett. 78, 495 (2001).
76.
P. Rauter, T. Fromherz, G. Bauer, L. Diehl, G. Dehlinger, H. Sigg, D. Grützmacher, and H. Schneider, Appl. Phys. Lett. 83, 3879 (2003).
77.
C. Miesner, K. Brunner, and G. Abstreiter, Physica Status Solidi B, Basic Research 224, 605 (2001).
78.
D. Bougeard, K. Brunner, and G. Abstreiter, Physica E, LowDimensional Systems & Nanostructures 16, 609 (2003).
79.
A. I. Yakimov, A. V. Dvurechenskii, A. I. Y. Y. Proskuryakov, J. Appl. Phys. 89, 5676 (2001).
Nikiforov,
and
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_387_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells Intersubband Transitions in Si/SiGe Quantum Structures
387
80.
J. Jiang, S. Tsao, T. O’Sullivan, W. Zhang, H. Lim, T. Sills, K. Mi, M. Razeghi, G. J. Brown, and M. Z. Tidrow, Appl. Phys. Lett. 84, 2166 (2004).
81.
S. Chakrabarti, A. D. StiffRoberts, P. Bhattacharya, S. Gunapala, S. Bandara, S. B. Rafol, and S. W. Kennerly, IEEE Photonics Technol. Lett. 16, 2004 (2004).
82.
Y. H. Peng, C. C. Chen, C. H. Kuan, and H. H. Cheng, SolidState Electron. 47, 1775 (2003).
83.
N. Rappaport, E. Finkman, T. Brunhes, P. Boucaud, S. Sauvage, N. Yam, V. Le Thanh, and D. Bouchier, Appl. Phys. Lett. 77, 3224 (2000).
84.
N. Rappaport, E. Finkman, P. Boucaud, S. Sauvage, T. Brunhes, V. Le Thanh, D. Bouchier, and S. E. Schacham, Infrared Phys. & Technol. 44, 513 (2003).
85.
A. Borak, Science 308, 638 (2005).
86.
S. A. Lynch, R. Bates, D. J. Paul, D. J. Norris, A. G. Cullis, Z. Ikonic, R. W. Kelsall, P. Harrison, D. D. Arnone, and C. R. Pidgeon, Appl. Phys. Lett. 81, 1543 (2002).
87.
R. Bates, S. A. Lynch, D. J. Paul, Z. Ikonic, R. W. Kelsall, P. Harrison, S. L. Liew, D. J. Norris, A. G. Cullis, W. R. Tribe, and D. D. Arnone, Appl. Phys. Lett. 83, 4092 (2003).
88.
Z. Ikonic, P. Harrison, and R. W. Kelsall, Phys. Rev. B64, 245311 (2001).
89.
Z. Ikonic, P. Harrison, and R. W. Kelsall, J. Appl. Phys. 96, 2004 (2004).
90.
Z. Ikonic, R. W. Kelsall, and P. Harrison, Phys. Rev. B69, 235308 (2004).
91.
L. Friedman, G. Sun, and R. A. Soref, Appl. Phys. Lett. 78, 401 (2001).
92.
S. Tsujino, S. Mentese, L. Diehl, E. Müller, B. Hass, D. Bächle, S. Stutz, D. Grützmacher, Y. Campidelli, O. Kermarrec, and D. Bensahel, Appl. Surf. Science 224, 337 (2004).
93.
Z. Ikonic, R. W. Kelsall, and P. Harrison, Semiconductor Sci. and Technol. 19, 76 (2004).
94.
R. W. Kelsall, Z. Ikonic, P. Harrison, S. A. Lynch, P. Townsend, D. J. Paul, D. J. Norris, S. L. Liew, A. G. Cullis, X. Li, J. Zhang, M. Bain, and H. S. Gamble, Opt. Materials 27, 851 (2005).
95.
H. Sigg, G. Dehlinger, L. Diehl, U. Gennser, S. Stutz, F. Faist, D. Grützmacher, K. Ensslin, and E. Müller, Physica E CT Rutherford Memorial Workshop on Semiconductor Nanostructures CY Feb. 5–9, 2001 CL, Queenstown, New Zealand, vol. 11, no. 2–3, pp. 240 (2001).
96.
I. Bormann, K. Brunner, S. Hackenbuchner, G. Zandler, G. Abstreiter, S. Schmult, and W. Wegscheider, Appl. Phys. Lett. 80, 2260 (2002).
97.
L. Diehl, S. Mentese, E. Müller, D. Grützmacher, H. Sigg, U. Gennser, I. Sagnes, Y. Campidelli, O. Kermarrec, D. Bensahel, and J. Faist, Appl. Phys. Lett. 81, 4700 (2002).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH09_388_03/23/2006 Intersubband Transitions in Si/SiGe Heterojunctions, Quantum Dots, and Quantum Wells 388
Chapter Nine
98.
S. Gehrsitz, H. Sigg, N. Herres, K. Bachem, K. Köhler and F. K. Reinhart, Phys. Rev. B60, 11601 (1999).
99.
S. Tsujino, C. V. Falub, E. Müller, M. Scheinert, L. Diehl, U. Gennser, T. Fromherz, A. Borak, H. Sigg, D. Grützmacher, Y. Campidelli, O. Kermarrec, and D. Bensahel, Appl. Phys. Lett. 84, 2829 (2004).
100.
S. Tsujino, A. Borak, E. Müller, M. Scheinert, C. V. Falub, H. Sigg, D. Grützmacher, M. Giovannini, and J. Faist, Appl. Phys. Lett. 86, 62113 (2005).
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_389_03/23/2006 Source: Intersubband Transitions in Quantum Structures
Chapter
10 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures
Arup Neogi Department of Physics and Materials Engineering University of North Texas Denton, Texas
10.1 Introduction The International Technology Roadmap for Semiconductors has reported the presence of a potential “red brick wall” or “100nm wall” that by 2010 could block further scaling of integrated electronic circuits, as predicted by Moore’s law [1]. A novel photonic technology that goes beyond the diffraction limit is thus likely to be needed to meet the demands of the future semiconductor industry. At the same time, communication networks currently operating in the 10 to 40 Gb/s range are expected to exceed 10 Tb/s by 2015, creating new challenges in transmission, switching, and networking [1]. This will necessitate ultrafast and subwavelengthscale photonic integrated circuits including devices such as switches, sources, and interconnects, e.g., to accommodate 1000 × 1000 channels on a single substrate, and to process each channel at much higher data rates than allowed by conventional electronics [2, 3]. To address the issue of physical scaling, novel functionalities are being explored based on local electromagnetic interactions between 389
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_390_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 390
Chapter Ten
nanometric elements and an optical nearfield wave, which are not limited by the principles of conventional wave optics such as interference and diffraction. Devices with fundamentally different physical principles, e.g., based on the concepts of surface elementary excitations and nanofabrication technology, are being developed that can overcome fundamental constraints in transmission or emission of light from nanoscale structures. At the same time, there is a strong tendency to replace “slow” electronic devices with “fast” photonic ones (Fig. 10.1) [4]. This drive is especially evident in the areas of computing and communications. It requires the development of an optical analog of an electronic integrated circuit capable of routing, controlling, and processing optical signals. The use of optical and optoelectronic devices for ultrafast switching and their integration in photonic circuits in turn require novel approaches to light manipulation. In particular, it will require (active) nonlinear photonic elements capable of performing, in the optical domain, logic operations analogous to their electronic counterparts without opticaltoelectrical and electricaltooptical signal conversion (Figs. 10.1b and 10.2). The fundamental understanding and exploitation of quantum and nonlinear optical effects for the development of such optical switches and modulators promise to revolutionize the field of nanophotonic devices and systems. A particularly interesting example, discussed in this chapter, is nonlinear devices based on intersubband transitions in semiconductor quantum wells, whose development integrates in a novel way aspects of quantum physics, optoelectronics, material science, and telecommunication engineering. 10.2 Femtosecond AllOptical Switches: The Challenge and Present Status Electronic circuits conventionally used for data switching are limited in their speed due to either the carrier’s transit times and lifetimes or RC time constants. Switching devices for ultrafast operation in the picosecond and femtosecond regimes must be alloptical, so that any limitation of the electronic nature can be avoided. Such ultrafast alloptical switches are a prerequisite for future optical timedivision multiplexing (OTDM) systems. Also, in the wavelengthdivision multiplexing (WDM) architecture, the development of highspeed all optical switches is of great importance to realize networks with wavelength transparency. At the optical nodes of such networks, various optical signal switching and routing elements are required to carry out functions such as add/drop multiplexing (ADM) and crossconnect. Thus, different types of switching devices suitable for
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_391_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
10
391
4
Sy
10 10 em 0T Installed Tb b/s t h /s system 1 T ro b/s ug hp Electronics speed limit ut :
st
Multiplex number
10
10
3
10
0G
b/s
Wavelength management limit
2
10
10
Gb
/s
1G
Femtosecond optoelectronics
WDM
b/s
TDM
1 0.1 G
OTDM
100 G 1T 10 G Signal bit rate (b/s)
1G
10 T
(a) Function
Key devices
Generation
Transmission
Femtosecond laser Optical regenerator
Distribution
Control
Alloptical switch (space, time and wavelength)
Ultralow dispersion waveguides Basic technique
Mode locking Dispersion control
Ultrafast relaxation Optical nonlinearity enhancement
Control of optical field and electron states Physics
Microcavity
Quantum wires and dots
Intersubband transition
Photonic band
Exitonpolariton
Spin relaxation
(b) (a) Different approaches to improve system throughput shown in a space of channel multiplex number as a function of signal bit rate per channel. (b) Key femtosecond devices required for future ultrahighthroughput system operation, elementary functions, and basic techniques as well as novel material and semiconductor physics, which can be used in the development of these devices. Figure 10.1
operation in the time, space, and wavelength divisions need to be developed. The essential features required for all these devices include an ultrafast response time, high repetition rate, low switching energy, high extinction ratio, and low insertion loss. A few different approaches can be used to develop practical, ultrafast alloptical switches with the abovementioned characteristics. One approach is to develop new device structures that enable ultrafast operation without relying on the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_392_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 392
Chapter Ten
Various approaches for ultrafast recovery
Problem in conventional semiconductor Femtosecond control pulse
Femtoseconds Nanoseconds Optical Output nonlinear material
Signal pulse
Slow recovery (lifetime limit) Weak response (nonlinearity limit)
1. Novel device structure MZ interferometer 2. Novel ultrafast phenomena Intersubband transition Fourwave mixing NIDRES, etc. 3. Novel nonlinear materials Organic film Quantum dots
Overview of ultrafast optical switching.
Figure 10.2
material’s intrinsic speed but at the expense of device complexity, i.e., symmetric MachZehnder (SMZ) interferometers [5]. The second approach is to utilize novel materials that exhibit ultrafast relaxation, such as organic materials [6] and lowtemperaturegrown multiple quantum well (MQW) structures [7]. The use of novel ultrafast phenomena in semiconductors, such as spin polarization switching due to the D’yakonovPerel interaction [8] or intersubband (ISB) optical switching, is a third approach, which opens up new possibilities of using more mature (and hence more reliable) materials in a novel way. To summarize the present status of alloptical switching device development, various switches are displayed in a space of power per bit versus switching time in Fig. 10.3 [4, 9]. A large number of existing devices, including electronic transistors, Josephson junction devices, and optoelectronic switches such as SEEDs [10], are included in this
10
0
Electronic
10
3 6
Quantum limit
h
10
tc wi
rs
Power/bit (W)
3
we po w
10
CDQW MQW OSE FPC  PTS VCD SOA pin DFB  WG CSN DC
Alloptical
Lo
10
6
Josephson kT (300 K)
10
9
10
15
10
1 μJ
Optoelectronic
12
1 fJ
1 aJ
10
9
1 nJ
1 pJ Photon number limit
10
6
10
3
10
0
Switching time (s) A plot of switching power per bit versus switching time for a variety of devices including alloptical, electronic, optoelectronic, and Josephson junction devices.
Figure 10.3
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_393_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
393
figure for comparison. Alloptical devices include symmetric MachZehnder switches [11], polarizationdiscriminating SMZ (PZSMZ) switches [12], lowtemperaturegrown surface reflection alloptical switches (LOTOS) [13], spin polarization switches based on MQWs (SPSMQW) [14], bistable devices based on semiconductor optical amplifiers (SOAs) [15], conventional MQW etalons [16], optical Stark effect (OSE) devices operating at low temperature [17], and currentinduced directional coupler (CIDC) switches [18]. In addition, recent studies using ISB transitions (ISBTs) in coupled double quantum wells (CDQWs) [19, 20] and MQWs [21] have demonstrated very promising results of switching operation in the femtosecond regime and with switching energy on the order of 10 pJ or less. While impressive results have already been achieved in the development of these alloptical switching devices, further improvements mainly directed toward the reduction of the switching energy are needed. These may be obtained through the enhancement of the optical nonlinearities utilized in the switching process, by the introduction of novel physics and materials, and by novel device structures and system architectures. In general, intrinsic material nonlinearities tend to be weak, but can in some cases be strongly enhanced through careful material engineering. Specifically, to maximize the nonlinear optical susceptibilities, one needs to maximize the products of the dipole moments of the relevant optical transitions, and to minimize the detunings between the energies of the photons participating in the nonlinear interaction and the transition energies [22, 23]. Compared to optical transitions in discrete atomic or molecularlevel systems, bandtoband transitions in semiconductors are generally offresonant due to the electron and hole dispersions within the parabolic conduction and valence bands. As a result, semiconductor materials exhibit relatively weak optical nonlinearities; however, these can be substantially improved by using discrete states in lowdimensional structures such as quantum wells (QWs) and quantum dots (QDs). In particular, ISBTs in these systems have been recognized early on as very promising for nonlinear optical devices due to their remarkable design flexibility. To optimize the efficiency and speed of alloptical switching, we combine two approaches to enhance optical nonlinearities. One is resonance enhancement via eigenfunction engineering: We design a structure whose geometric properties enhance the ISB nonlinear interaction in the communication wavelength regime, in particular using the wideconductionbandoffset InGaAs/AlAsSb QW system. The second approach is to engineer the ISB scattering rate in a multilevel quantum confined system by manipulating the doping level, which changes the switching speed as well as the on/off contrast ratio of the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_394_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 394
Chapter Ten
switching process. Nonlinear Kerr coefficients 12 orders of magnitude larger than in bulk AlGaAs have been measured in such systems [24]. 10.3 Interband and Intersubband Transitions in WideConductionBandOffset Materials Recently investigated microphotonic techniques for alloptical communications utilize optical nonlinearities based on carrierinduced ISBTs in semiconductor QWs. Intersubband transitions have several advantages for device applications compared to the more conventional bandtoband transitions originating from both exciton recombination and freecarrier processes. These advantages include the ability to control the ISBT energies independently of the material bandgap and to obtain resonance enhancement of ISB optical nonlinearities, as well as the giant ISB dipole moment matrix elements. In addition, ISBTs are characterized by ultrafast (< 1ps) lifetimes due to longitudinal optical (LO) phonon scattering. In the past few years, several groups including ours have successfully demonstrated ultrafast ISB carrier relaxation at 1.55 m, an important milestone for alloptical modulation and switching in QWs [25–29]. Motivated by these advantageous features of ISBTs, current activities to extend the transmission capacity of fiberoptic networks beyond 1 Tb/s include the development of bandgapengineered ISB systems [30] with transition wavelengths in the near infrared. These can be realized with QWs and QDs based on wideconductionbandoffset semiconductor systems, such as III nitrides [31], IIVI compounds (for example, CdS/ZnSe/BeTe) [26], and antimonides [32]. In conventional semiconductor optoelectronic devices, bandtoband transitions (interband transitions, or IBTs) are used, whose response time is limited by the electronhole recombination lifetime (~nanoseconds) [34]. For ultrafast alloptical switching in future OTDM systems, the use of ISBTs in QWs [34–38] or QDs [39] is advantageous, primarily because of the very fast ISB relaxation times. These lifetimes are determined by LOphonon scattering and are typically in the range of ~50 fs to 3 ps (depending on the electron effective mass), that is, two to three orders of magnitude faster than the interband carrier lifetime. Following several investigations of ISB alloptical switching, recently the operation of digital (NOR) gates for ultrafast alloptical data processing has also been demonstrated, based on a combination of ISB and IB transitions in QWs [40]. Alloptical NOR gating had already been demonstrated using optical fibers [41] or interband SOAs [42]. However, these devices suffer from a low efficiency due to the small nonlinearities in silica fibers, or a low operation speed due to long carrier lifetimes in SOAs. Both of these drawbacks can be overcome by Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_395_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
395
using the large nonlinearities and subpicosecond absorption recovery lifetimes in strongly coupled QWs. The fundamental requirements for a semiconductor heterostructure (QW or QD) appropriate for ultrafast alloptical modulation or switching in the communication wavelength regime are as follows: 1. A large conduction band offset between the quantum well and the barrier materials, suitable for ISBT energies exceeding 0.8 eV (1.55 m) 2. Ultrafast ISB relaxation rate governed by LOphonon scattering and dependent upon the overlap of the electron wave functions of the conduction subband states 3. Favorable optical properties including transparency at the relevant wavelength, narrow ISB absorption peaks, and a large thirdorder ISB optical nonlinearity [Ȥ(3)] for lowthreshold operation There are also a few accepted limitations to the performance of devices based on ISBTs between conduction subbands. The foremost limitation is the need for the incident radiation to be linearly polarized along the growth direction of the QWs. This is related to the spherically symmetric (slike) nature of the conduction subband electronic states. Techniques such as grating coupling, textured surfaces, or end firing into a waveguide can be used to deal with this limitation for most device applications. There have also been some efforts to achieve normalincidence ISBTs, i.e., using indirectgap semiconductors, transitions between quantized valence band states, or QDs. In general, the possibility of normalincidence operation would add versatility to all ISB devices including alloptical modulators and switches. 10.3.1
Material systems
The AlGaAs/GaAs system has been one of the most extensively studied material systems for the development of midinfrared and farinfrared (terahertz) ISB devices since the first observation of ISBTs in 1985 [43]. The negligible mismatch between AlAs and GaAs (~0.1%) allows for practically unstrained epitaxial growth on GaAs substrates. However, the conduction band offset between GaAs and AlAs is insufficient to support ISBTs in the optical communication wavelength region (~0.8 eV). Presently there are four different material systems that are being extensively studied for alloptical ISB devices at communication wavelengths: InGaAs/AlAsSb QWs latticematched on InP [44], InGaAs/AlAs QWs [45], AlGaN/GaN QWs [46] and QDs [47], and IIVI systems such as CdS/ZnSe/BeTe QWs [26].
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_396_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 396
Chapter Ten
Optoelectronic devices based on InP substrates have been gaining prominence in the past several years due to the availability of latticematched ternary and quaternary alloys useful for the visible and nearinfrared wavelength regions. This is illustrated in Fig. 10.4. For InGaAs QWs (latticematched to InP substrates) and AlAs barriers, large conduction band and valence band offsets (~1.3 and ~1.1 eV, respectively) can be obtained. Also, because the lighthole (LH) mass in InGaAs is smaller than in AlAs, whereas the heavyhole (HH) masses are comparable, the energy separation between the first HH and LH subbands is relatively large. This is further enhanced by a builtin splitting caused by strain. This enhanced separation between HH and LH states is useful for avoiding LH conduction band transitions in case of interband light modulation. However, the InGaAs/AlAs/InP system is seriously limited by the large lattice mismatch between the AlAs barrier and the InP substrate. There are also segregation effects observed in the presence of high indium content, which becomes significant in the narrow wells essential for communication wavelength devices. For such narrow wells (~2 nm) there are reports of intervalley transfer of electrons from the ī valley in the well to the X valley in the barrier [49]. The other promising InPbased material system consists of latticematched InGaAs/AlAsSb QWs, which are described in detail in the next section.
Lattice match to InP
2.8 AIP
ZnSe
2.4 GaP
0.60 AlAsSb 0.70 InAlAs
1.6 GaAs
AIInGaAs InGaAsP
G In s aA
0.8
0.80 0.90 1.00
InP
1.2 Sl
AlSb
1.30 1.55
GaSb
InGaAs
2.00
Ga 0.4
3.00 5.00
InAs GaInNAs
0 5.4
5.6
InSb
5.8
Wavelength (μm)
Energy gap (eV)
0.50
ZnTe
AlAs
2.0
0.45 Direct Indirect
6.0
6.2
6.4
∞
Lattice constant (Å) Figure 10.4
InPbased material system.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_397_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
397
The other relevant IIIV material system is the nitrogenbased AlGaN/GaN system grown on sapphire or SiC substrates, which yields a type I heterostructure with a large conduction band offset [48]. However, the growth of nitride semiconductors is still not mature due to the lack of native substrates such as GaN. Thus, similar to the case of InGaAs/AlAs heterostructures, Al(Ga)N/GaN QWs are highly strained, which restricts the total number of wells that can be grown pseudomorphically, limiting the effective ISB absorption within the active medium [49, 50]. In addition, while in InGaAs/AlAs QWs nearinfrared ISBTs are restricted by In segregation and carrier leakage [51], in Al(Ga)NGaN QWs they are strongly influenced by the intrinsic electric fields due to spontaneous and piezoelectric polarizations [52]. Finally, recent reports by Akimoto et al. have suggested the possibility of using IIVI QW systems such as CdS/ZnSe QWs grown on BeTe substrates [26] for realizing nearinfrared ISBTs with subpicosecond scattering rates. 10.3.2 Properties of antimonide quantum wells
InGaAsAlAsSb QWs latticematched to InP have been found to be ideally suited for nearinfrared ISB optoelectronic devices due to their large conduction band offset [54], large [Ȥ(3)] [55], and subpicosecond optical response [56, 57]. In these QWs the well and barrier layers consist of In0.53Ga0.47As and AlAs0.56Sb0.44, respectively, both of which are latticematched to the InP substrate. Compared to AlAs, AlAsSb provides a larger conduction band offset with InGaAs, which is favorable for ISBTs at the optical communication wavelengths of 1.3 and 1.55 m. On the other hand, interband transitions in these QWs are relatively weak due to the staggered (type II) lineup with the valence band states in the InGaAs layers being unconfined. In general, interband transitions in Sbbased systems can be both direct and indirect. For the ideal case of perfectly smooth interfaces, the InGaAs/ AlAsSb system can be converted to a type I QW either by reducing the Ga fraction from 47% to 25% or by reducing the Sb fraction from 44% to 30%. The conduction band offset in the resulting strained QWs is still sufficiently large to yield ISBTs around 1.55 m, with a relatively strong and fast interband absorption around 1.3 m compared to the latticematched structure. This type I InGaAs/AlAsSb system is also less strained than InGaAs/AlAs or AlGaN/GaN QWs operating in the nearinfrared region, and its ISB absorption is not limited by carrier leakage from the conduction band states due to intervalley transitions. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_398_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 398
Chapter Ten
However, the immiscibility gap of the Sb material system makes it very difficult to form abrupt interfaces, which affects the ISB absorption characteristics. In general, interface abruptness is an important issue in devices based on ISBTs, as the transition energy is a very sensitive function of the well width. To achieve ISBTs at communication wavelengths, the well width needs to be very narrow, usually 6 to 9 monolayers (MLs), so that even a singleML fluctuation in well width causes a significant shift in the transition energy. By using dimeric group V sources and with As termination at the heterojunction planes, the interfaces become more abrupt and the band alignment of InGaAs/ AlAsSb QWs is shown to be type I with a conduction band offset of 1.6 eV. One of the unique features of the InGaAs/AlAsSb material system is the effect of doping or ntype carrier density on the interface properties and band offset. High doping in the well or barrier is necessary for devices based on ISBTs, and it can lead to shifts in the transition energies, especially in narrow QWs. In the case of InGaAsAlAsSb QWs with a uniform doping concentration of ~1 × 1019 cm–3 in the barriers, an extremely high level of outdiffusion of In and Ga atoms from the wells to the barriers, and of Al atoms from the barriers to the wells (especially from the surface side AlAsSb barrier layer), has been observed [86]. Normally, at the usual growth temperatures of MBE, bulk diffusion is not operative due to the lack of vacancies, and the atomic arrangements are determined during growth by surface or nearsurface processes. The surface mobility of atoms is necessary to obtain a highquality material, but can simultaneously lead to an exchange between substrate atoms and impinging atoms. For arsenides, the direction and extent of the segregation process follow the order In > Ga > Al. Indium and gallium show different diffusion behavior: In tends to diffuse toward the surface side, while Ga diffuses toward the substrate side. In doped InGaAsAlAsSb QWs, indium and gallium diffusion could be caused by charged vacancies produced in AlAsSb by high doping with Si. Incorporation of Sb into the InGaAs wells is also clearly observed. The diffusion rates of In, Ga, and Al atoms in undoped systems are significantly lower. The basic material parameters relevant for alloptical ISB processes are summarized in Table 10.1. It is observed that GaNbased QWs have the largest scattering rate and saturation intensity due to their comparatively higher LOphonon energy. Furthermore, the InGaAs system has the lightest effective mass, leading to more efficient electron transport compared to the GaN and ZnSe systems. In addition, the state of material synthesis of nitride or IIVI compounds is still immature.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_399_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
399
Thus, the remainder of this chapter focuses on ISB modulation and switching in InPbased antimonide QWs. TABLE 10.1
Material System for NearInfrared ISBT
Parameters me*/m0
Effective mass LOphonon energy ћωLO (meV) Dielectric const. εs ε∞ Basic scattering rate W0 (ps –1) Dephasing time T2 Saturation intensity ls
InGaAs
GaN
ZnSe
0.042 36
0.2 88
2.7 31
14.1 11.6 6.7 Slow Low
9.5 5.35 121 Fast High
8.1 5.75 40 Fast High
InGaAs QW: InGaAs/AlAs/Inp (MIT); InGaAs/AlAs/GaAs (Kyoto Univ., Stanford Univ.); InGaAs/AlAs/Inp (FESTA, NTT). Nitride QW: GaN/AlGaN (Toshiba, Lucent Tech., Sophia Univ., Univ. Tokyo). IIVI QW: CdS/ZnSe/BeTe (AIST).
10.3.3 Interband transitions in In0.53Ga0.47As/AlAs0.56Sb0.44 quantum wells
Despite the potentialities of InGaAs/AlAsSb QWs, there have been very few reports of their optical properties until recently, due to the difficulties involved in growing the AlAsSb material which includes two group V elements with a large miscibility gap [54]. The composition control of these alloys becomes problematic, because of the different incorporation rates of the two group V elements. In particular, the incorporation of Sb and As into AlAsySb1– y is reported to depend critically on the substrate temperature and on the Sb and As fluxes [58]. The valence band maximum of the AlAsSb barrier is located about 70 meV above the valence band maximum of InGaAs, whereas the lowest conduction band minimum resides in the InGaAs layers [59]. The conduction band offset varies depending on the growth condition in the range of 1.6 to 1.7 eV at the ī point and therefore provides excellent electronic confinement. This type II (staggered) band alignment leads to a spatial separation of electrons and holes, and it allows for interband optical emmision at a photon energy smaller than the bandgap energy of both materials forming the heterostructure. The structural quality of the interfaces is more important in such type II systems as compared to type I heterostructures such as GaAs/AlGaAs, because of the carrier localization at the interfaces where the spatially indirect optical transitions take place. A schematic band diagram of the InGaAs/AlAsSb heterostructure is given in Fig. 10.5. In this system electrons (holes) are confined in the Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_400_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 400
Chapter Ten
AlAsSb
AlAsSb
InGaAs
Eg = 2.47 eV
∆Ec= 1.62 eV el Indirect
Γ point
Direct
hhl ∆Ev= 0.07 eV Figure 10.5
Band diagram of a type II InGaAs/AlAsSb heterostructure.
InGaAs (AlAsSb) layers. Thus, the lowestenergy interband transition is spatially indirect (type II). Another possible optical transition in this structure is a direct (type I) transition inside the InGaAs layer between a confined electron state and a quasibound hole state. It is observed that the nature of the interband transitions in these InGaAs/ AlAsSb heterostructures also depends on the width of the InGaAs layers. Photoluminescence (PL) measurements of interband transitions in InGaAs/AlAsSb QWs show both type I and type II transitions [59]. This is clearly illustrated in Fig. 10.6a for the case of 20nm InGaAs layers in a lowexcitation regime.
77 K
mW 0.9
2.5 4.5
mW 173 79 54 28 9.2
7.4 9.2 1.2
1.6 1.4 Wavelength (μm)
(a)
1.8
77 K
Well : 20 nm Barrier : 20 nm Intensity (arb. units)
Intensity (arb. units)
Well : 20 nm Barrier : 20 nm
1.2
1.4 1.6 Wavelength (μm)
1.8
(b)
Excitation power dependence of the lowtemperature PL spectrum of a 20nm unintentionally doped InGaAs/AlAsSb QW. Results obtained (a) at low excitation powers and (b) at high excitation powers. Figure 10.6
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_401_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
401
1. The lower energy peaks in this figure correspond to type II transitions between electrons confined in the InGaAs well and holes confined in the AlAsSb barriers. 2. The higherenergy peaks correspond to direct type I transitions associated with the formation of novel excitons involving a confined electron and a quasibound hole, both in the InGaAs layer. A transition caused by the recombination of confined electrons in the first excited subband and quasibound holes, both in the InGaAs layer, is also observed in this 20nm InGaAs heterostructure in the higher excitation power regime (Fig.10.6b). CdSe/ZnTe [60] and ZnSe/BeTe [61] heterostructures also exhibit a direct type I transitions in type II QWs. A comparison of the band structures of such systems explains these optical transitions involving a quasibound state in a single barrier layer. In material systems with large band offsets such as CdSe/ZnTe and ZnSe/BeTe, continuum or abovebarrier states exist that are strongly confined in the barrier layers. They can be explained by simply considering the interference of electron waves reflected at the interfaces (planes of potential discontinuity). However, the small valence band offset of 70 meV in InGaAs/ AlAsSb QWs does not provide sufficiently strong reflections to effectively confine the abovebarrier states within the barrier layers. This is similar to the behavior of belowbarrier states in a shallow well, where significant wave function spreading into neighboring layers occurs. Another possible mechanism that can effectively confine the abovebarrier states is the Coulomb attraction between electrons and holes. The presence of spatially separated InGaAs and AlAsSb layers with high densities of electrons and holes, respectively, produces an electric field which in turn gives rise to strong bending of the conduction and valence bands [62]. The resulting local potential minima in the InGaAs layers can confine the majority of photogenerated holes and thus enhance the intensity of the direct (type I) transitions in structures with wide InGaAs layers. On the other hand, as the InGaAs layer thickness is decreased, the intensity of these direct transitions becomes weak. This explains the observed well width dependence of the PL spectra shown in Fig. 10.7. Quantum confinement in InGaAsAlAsSb QWs was first observed by measuring the PL due to interband indirect transitions as a function of well width in narrow InGaAs layers. This is shown in Fig. 10.8, where the PL spectra are normalized to their respective peak intensities. In these measurements, the excitation power was 2 mW, and all the QWs were uniformly doped to 1019 cm–3. As expected, the PL peak position undergoes a blue shift as the QW width is reduced. These PL spectra
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_402_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 402
Chapter Ten
Indirect transition
77 K
Intensity (arb. units)
Direct transition 15 nm
20 nm 50 nm 100 nm
200 nm 1.3
1.5 1.7 Wavelength (μm)
1.9
Figure 10.7 Photoluminescence spectra from 15, 20, 50, 100, and 200nm InGaAs
samples. The AlAsSb layers are 200 nm thick. Both direct (type I) and indirect (type II) transitions are observed.
are relatively broad (80 to 100 meV) compared, e.g., to typical AlGaAs/ GaAs QWs, because of the indirect nature of these transitions in type II structures, and also likely due to the interface steps characteristic of the InGaAs/AlAsSb heterojunction. As discussed earlier, the diffusion of group III atoms is significant, especially in the presence of highSi 1.0 Well Width 15 Å 20 Å 25 Å 30 Å 35 Å
Normalized intensity
0.8
0.6
0.4
0.2
0.0 0.8
1.0
1.2 Wavelength (μm)
1.4
1.6
Figure 10.8 Well width dependence of the lowtemperature PL spectrum of InGaAs/
AlAsSb QWs doped to 1019 cm–3, measured with an excitation power of 2 mW.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_403_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
403
doping concentrations, and can cause changes in the band alignment of the system. In particular, band offset calculations predict a change in band alignment from type I to type II as a result of the formation of a GaAsSb layer at the interface. As a first step toward the use of ISBTs for the modulation of interband light absorption in these QWs, the spontaneous interband carrier relaxation rate without ISB excitation was studied with timeresolved PL measurements [56]. Experimental results from a 20Å InGaAs/ AlAsSb QW sample with a Si doping density of 1019 cm–3 are shown in Fig. 10.9. The sample was pumped with optical pulses from a frequencydoubled modelocked Ti : Sapphire laser at 100 MHz, and the PL signal was measured by using a streak camera. The pump wavelength was 385 nm, well above the absorption edge of the AlAsSb barriers. Figure 10.9a shows PL spectra from this sample for an excitation power of 10 mW measured by integrating between a time delay of 0.2 and 0.8 ns. A broad PL line width of 55 meV is observed at 10 K, with a major contribution due to the intermixing at the interface leading to well width fluctuations. Figure 10.9b shows the timeresolved PL decay observed at various wavelengths for an excitation power of 5 mW. In type I QWs, the PL lifetime is usually shorter than in bulk materials, because of the stronger overlap of the electron and hole wave functions in quantum confined structures. Similarly, one should expect a faster PL decay involving confined QW states compared to the decay from unbound barrier states. The oscillator strength of a type II transitions is also expected to be only a few percent of that of type I transitions. These expectations are confirmed by transmission spectra measurements. The interband carrier lifetime in the sample of Fig. 10.9b exhibits two components: a fast component related to intraband transitions from higherk states, mainly due to scattering induced by interface roughness; and a slower component corresponding to the interband transitions. The faster carrier relaxation is observed at energies slightly higher than the resonant PL peak energy. A biexponential decay is clearly observed for the luminescence at 980 and 1000 nm. For instance, the luminescence at 980 nm exhibits a fast component with a decay time of 450 ps, followed by a slower relaxation of 2.1 ns. This relaxation rate is comparable to or slightly longer than the carrier lifetime measured in InGaAs/InAlAs or InGaAs/InP type I QWs [63, 64], and is much faster than in other type II InGaAs QWs which exhibit a transition (īX and XX) lifetime of 15 ns [65]. This indicates that the doped InGaAs/AlAsSb system used in this work has either a type I structure or a type II structure with an extremely shallow valence band offset. It can also be observed from Fig. 10.9b that the relaxation at lower energies (< 1.24 eV) is dominated by the slower component, and Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_404_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 404
Chapter Ten
5
10 K
Intensity (arb. units)
4
3
2
1
300 K
0 0.94
0.96
0.98
1.00
1.02
1.04
1.06
1.08
1.10
1.12
Wavelength (μm)
(a)
10 K
1040 nm
0.5
PL intensity (arb. units)
0.0
1020 nm
1.0 0.5 0.0 2.0
1000 nm
1.5 1.0 0.5 0.0 1.5
980 nm
1.0 0.5 0.0 1
2
3 4 Decay time (ns)
5
6
(b) (a) Photoluminescence spectra of a 20Å InGaAs/AlAsSb QW sample at 10 and 300 K. (b) PL decay at a pumping level of 5 mW for various luminescence wavelengths.
Figure 10.9
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_405_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
405
the decay process essentially reduces to a single exponential with a lifetime of ~2 to 3 ns. 10.3.4 Nearinfrared intersubband transitions in In0.53Ga0.47As/AlAs0.56Sb0.44 quantum wells Singlequantumwell systems. Intersubband transitions in InGaAs/
AlAsSb QWs depend critically on the conduction band offset, which is strongly influenced by the Si doping level. The larger the doping concentration (above 1018 cm–3), the lower the interface quality and the smaller the conduction band offset. To study ISB absorption in these heterostructures, nearinfrared polarizationresolved transmission spectra were measured at room temperature with a BRUKER IFS 66 vs FTIR, using a nearinfrared whitelight source and a cooled InSb detector. Figure 10.10 shows ISB absorption spectra measured in these experiments [53]. It is observed that at high carrier concentrations (ȡ ~ 1019 cm–3), the ISBT wavelength decreases with decreasing well width but tends to saturate around 1.9 to 2.0 m for wells narrower than 2 nm. The shortest transition wavelength achieved with normal growth conditions was 1.9 m for a 1.5nm well. At the same time, the ISB absorption was found to be considerably higher compared to strained QWs; for example, in the case of a 3.0nm well, the peak ISBT absorption coefficient was measured to be about 5000 cmí1 at 2.4 m. The observed transition wavelength is redshifted compared to theoretical estimates based on a simple envelope wave function approximation. This deviation increases for narrower wells, as the interface gradient of 2 to 3 monolayers/interface becomes comparable to the intended well thickness of 5 to 6 monolayers. The interface quality and the well width uniformity are significantly improved by reducing the doping level. For example, the ISBT energy can be reduced to 1.72 m by lowering the carrier concentration to 1017 cm–3. The AlAsSbInGaAs heterointerface is likely to form a terracelike stepped structure due to the intermixing of group V atoms [66]. This asymmetric QW structure results in an increase of the ground subband energy and a lowering of the upper conduction subband on reducing the well width, leading to a saturation of the ISBT wavelength. The reduction in ISB absorption strength with well width observed in Fig. 10.10 is also associated with the decrease in the active layer thickness (and number of carriers in the QWs), since the well number has been maintained constant. The conduction band offset at the InGaAs/AlAsSb heterojunction is insufficient to yield ISBTs at 1.5 m, especially for heavily doped QWs. By reducing the doping level to ~3 × 1017 cm3 it is
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_406_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 406
Chapter Ten
Well width 15 Å 20 Å 3 25 Å 30 Å [In(lTM / lTE )]
Intersubband absorption (arb. units)
4
2
ρ ~ 1 × 1015 cm3
35 Å 40 Å x3
1
x4
0 1.2
1.6
2.0
2.4 2.8 3.2 Wavelength (μm)
3.6
4.0
Figure 10.10 Well width dependence of the ISB absorption spectrum of uncoupled InGaAs/AlAsSb QWs, where the absorption is estimated from the logarithmic ratio of TM and TE transmission spectra. Each sample consists of a repetition of 88 QWs uniformly doped to 1019 cm–3.
possible to shorten the ISBT wavelength to the communication wavelength regime, but at the expense of a significant drop in ISB absorption strength. A more effective approach to achieve ISBTs at 1.3 and 1.55 m with appreciable absorption suitable for device applications is to use strongly coupled QW system. Coupled quantum well systems. Coupled double quantum well (CDQW)
structures provide unique opportunities for engineering novel semiconductor systems with large optical nonlinearities in the infrared [67]. This approach has inherent advantages for ultrafast optical switching and modulation due to its flexibility in tailoring quantized energy levels and carrier relaxation processes [68]. In CDQWs, the ISBT energies can be controlled through the splitting of quantized electron states that occurs when the barrier thickness is reduced and the coupling between the wells becomes sufficiently strong (Fig. 10.11a). As a result, larger ISB energy separations can be achieved with wider well widths compared to single QWs [69]. Also note that the ISB transition wavelength and absorption strength in these structures depend on the doping level and temperature due to the carrierinduced spacecharge electric field [70]. ISB absorption spectra calculated for a doped (n = 1 × 1018 cm–3) InGaAsAlAsSb CDQW system using Bastard’s threeband model are
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_407_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
407
InGaAS/AlAsSb CDQW n=4
E4 E3
λ
λ
14
n=2
Absorption coefficient (× 103 cm1)
n=3
23
E2 E1
n=1
Lw = 2.1 nm
6
Lb = 3.5 nm
3
2.6 nm 2.1 nm 1.5 nm
0
0
1.2
1.4 1.6 Wavelength (μm)
(a)
1.8
2
(b)
Δα/α
0.5
λ14
0.4
100 s
0.3
4 3 λ23 2 1
1.0 1.0
500
0.8
400 300 200
0.2
100
0.1 0 0
2
4 6 Delay time (ps)
(c)
8
0 10
Transmittance
0.6
600
Optical gain (cm1)
0.7
1.5
Wavelength (μm) 2.0 2.5
3.0
0.6 c1>c4>
c1>c3> c2>c3>
0.4
s30 p+45 p+30 p
0.2
0.0 1.0
1.5
2.0 2.5 Wavelength (μm)
3.0
(d)
(a) Schematic conduction band diagram of a coupled double QW system. (b) Calculated dependence of the ISB absorption spectra on the central barrier width in InGaAs/AlAsSb CDQWs. (c) Calculated transient response of the 1–4 absorption and the 3–2 optical gain of a CDQW designed for optical switching between 1.3 and 1.55 m, after irradiation of a control beam resonant to the 1–4 transition. (d) Measured transmission spectra of an InGaAs/AlAsSb CDQW structure with an AlAs central barrier. Figure 10.11
shown in Fig. 10.11b for different widths of the center barrier. As shown in the figure, when this barrier is sufficiently narrow, two separate absorption peaks corresponding to the 1–4 and 2–3 transitions are observed. Alloptical absorption modulation can be achieved based on the interaction between these two ISBTs. Specifically, the population difference between the second and third subbands can be reduced by irradiating a light beam (control light) resonant to the 1–4 transition, assuming that the 4–3 relaxation is sufficiently fast. The latter condition can be realized by designing the 4–3 energy difference to be larger than and close to the LOphonon energy. As a result, the absorption of the 2–3 transition decreases in the presence of the control wave, and modulation of a signal beam resonant to this transition is achieved. Although the absorption coefficient slightly decreases as the barrier
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_408_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 408
Chapter Ten
thickness is reduced, it remains larger than 103 cm–1, which is an order of magnitude larger than that of the 1–4 transition in conventional uncoupled QWs, and sufficiently large for device operation. The design of the subband structure also has considerable influence on the response speed (Fig. 10.11c). For example, rate equation calculations have indicated that the ISB absorption recovery time can be reduced to 300 fs in an optimized triplecoupled QW structure [71]. At the same time, the optical switching energy can be significantly reduced compared to single QWs due to enhanced nonlinear optical coefficients. Intersubband transitions in InGaAs/AlAsSb CDQWs are significantly influenced by the strong intermixing of In, Sb, and As in the well and barrier layers, which causes substantial interfacial roughness. To deal with this problem, the use of an AlAs (instead of AlAsSb) central barrier layer has been introduced to reduce intermixing and thus improve the quality and uniformity of the QWs [55, 56]. Shown in Fig. 10.11d are the measured polarizationresolved nearinfrared transmission spectra of such a CDQW structure designed for ISB absorption at 1.55 m, consisting of two nominally identical wells of ~2.7 nm (9 ML) width. At room temperature the interband absorption edge of these QWs occurs around 1.2 to 1.3 m. The spectra of Fig. 10.11d reveal an asymmetry in the CDQW structure induced by width fluctuations of about 0.5 to 1.0 ML in both the well and the central barrier. Due to this asymmetry an absorption dip is observed near 2.2 m corresponding to the c1>–c3> transition, which is forbidden in symmetric structure due to parity selection rules. The other two dominant transitions in the nearinfrared regime are due to the c1>–c4> transition around 1.55 m and the c2>–c3> transition around 2.7 m, which also indicates that at 300 K the Fermi level lies above the c2> state in this particular structure. The magnitude and spectral broadening are similar for the different ISBTs in this structure, but in general depend critically on the actual sheet density. The absorption coefficient Įc1>–c4> for the c1>–c4> transition is 850 cm–1. A schematic description of alloptical switching in a waveguide based on InGaAsAlAsSb QWs is shown in Fig. 10.12. An active (modulating) layer consisting of the CDQW structure just described can be employed to provide the desired large and ultrafast optical nonlinearity. In this device, a control wave resonant to the 1–4 transition can be used to modulate the transmission of an input signal resonant to the 2–3 transition, through modification of the subband carrier densities via ISB absorption. As a result, only those pulses of the input signal that are coupled in the waveguide (nearly) simultaneously with a control pulse are transmitted out. Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_409_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
Current bias
409
Optical signal output
Optical signal input
Ultrafast relaxation Control light input Giant optical nonlinearity Figure 10.12
Schematic description of alloptical modulation or switching in a waveguide
device.
10.4 AllOptical Modulation of Interband Resonant Light via Intersubband Resonant Light Absorption of interband resonant light can be modified in the presence of an ISB resonant control wave. The ultrafast modulation of a continuous wave (cw) interband signal based on this approach was first demonstrated by Noda et al. using a resonantly excited freecarrier induced nonlinearity in doped QWs [72]. The response time of this alloptical modulation scheme is on the order of 1 ps, determined by the ISB energy relaxation rate [73, 74]. Its efficiency depends on the ISB excitation intensity. To achieve high nonlinearities in the femtosecond regime, we have proposed the use of ultrashort light pulses both for the ISB control wave and for the IB signal [34]. In a threelevel undoped QW system, the manipulation of interband resonant light absorption by ISB resonant coupling light is analogous to the phenomenon of electromagnetically induced transparency in atomic systems [75]. In doped QWs the alloptical switching is due to a real carrier density modulation. To describe this alloptical modulation process, we consider a threelevel QW system as shown in Fig. 10.13. A weak probe (or signal) wave is tuned resonantly to the interband transition (from the heavyhole subband hh1> to the first conduction subband c1> at k II = 0), while a control wave consisting of a train of ultrashort pulses is tuned to the ISBT between the conduction subbands c1> and c2>. The oneelectron density matrix equation of motion under the rotatingwave approximation can be used to adequately describe the population distribution and transition probabilities among these various subbands. The polarizations of the interband signal wave and ISB control wave are assumed to be parallel (TE) and perpendicular (TM)
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_410_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 410
Chapter Ten
c2> c1>
T1
ISBcontrol light
T2
IBsignal light
IBsignal light
hh1> Without control light
With control light
Figure 10.13 Schematic description of alloptical modulation of interband resonant light
via ISBTs.
to the QW layer, respectively, so as to maximize the relevant transition dipole moments. The optical fields of the signal or probe wave and of the control wave can be written as
F p (t ) = Fp (t ) exp (íiȦ p t ) + c.c.
(10.1)
F c (t ) = Fc (t ) exp (íiȦ c t ) + c.c.
(10.2)
and
respectively. The total electronic polarization P in the QWs arising from the simultaneous presence of these interband probing field and ISB coupling field is P(t ) = İ0 Ȥ (t ) Fp (t ) + Fc (t ) =
2 ȝ ȡ (t ) + ȝba ȡab (t ) + ȝ bc ȡcb (t ) + ȝcb ȡbc (t ) V k ab ba
(10.3)
where Ȥ(t) is the complex susceptibility; the subscripts a, b, and c refer to the three subbands hh1>, c1>, and c2>, respectively; the summation extends over all values of the inplane wave vector; V is the sample volume; and the factor of 2 arises from the spin degeneracy. The probe absorption coefficient Į can be obtained from the imaginary part Im [Ȥ ba] of the linear susceptibility of the medium at the probe frequency, by assuming that the polarization due to the probe field varies slowly on the scale of the optical period. The generalized density matrix equations for the diagonal and offdiagonal elements are obtained from a timedependent perturbative analysis as follows [38, 44]:
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_411_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
ȡ j j (t ) = ( ȡ / t ) relax t
jj
411
+ i ȍ ji , f c, p (t )ȡi j (t )
í ȍ l j f c, p (t )ȡ ji (t ) + ȍ jk f c, p (t )ȡ k j (t ) í ȍk j f c, p (t )ȡ jk (t )
and
(10.4) ȡ jk (t ) = í (iǻ jk + ī jk )ȡ jk (t ) + i {ȍ jk f c, p (t ) ȡ k k (t ) t í ȡ j j (t ) + ȍ ji f c, p (t )ȡik (t ) í ȍ l k f c, p (t )ȡ ji (t )}
where ȍji is the Rabi frequency of the optical field tuned to the transition between states j> and i>; ƒc(t) and ƒp(t) are the pulse shapes of the control and signal waves, respectively; īji is the dephasing rate between levels j and i; and ലǻ jk = E j í Ek í ലȦc, p is the detuning of the relevant optical field from its resonant transition energy. The relaxation hamiltonian matrix for the QW system includes a phenomenological description of the manybody effects leading to transverse phase relaxation in the offdiagonal elements, and to energy relaxation of the carriers in the diagonal elements [76]. LOphonon scattering is considered to be the dominant dephasing process in these structures. The effective steadystate interband absorption coefficient can be expressed as Į ( Ȧ p ) = Į (1 ) ( Ȧ p ) + Į (3 ) ( Ȧ p ) = Į 1 í Ȥ ( 3) ( Ȧ p , í Ȧ p , Ȧ p ) 썉 I p
(10.5)
+ Ȥ(3)(Ȧ p , í Ȧ c , Ȧ c ) 썉 Ic
where Ip = Fp2, Ic = Fc2, and Ȥ(3) (Ȧp, íȦp, Ȧp) and Ȥ(3) (Ȧp, íȦc, Ȧc) are the nonlinear absorption coefficients due to interband and ISB resonant light, respectively. The latter is the dominant thirdorder nonlinear optical susceptibility and is several orders of magnitude larger than the interband transitions related term Ȥ(3) (Ȧp, –Ȧp, Ȧp). As the origin of the alloptical modulation or switching lies in the carrier density modulation by the control light pulses, the carrier concentration in the conduction subband c1> effectively determines the change in the absorption coefficient of the signal wave due to the ISB transitions. If we neglect coherent nonlinear effects, the modulation depth can be estimated from the difference in interband Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_412_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures 412
Chapter Ten
absorption with the c1> states partly occupied due to doping (in the absence of control light) and with the c1> states empty (in the presence of control light). Theoretical spectra of this interband absorption coefficient, computed with the model just described, are plotted in Fig. 10.14, in the presence (solid lines) and absence (dotted lines) of the control wave, for three different values of the QW doping density. As shown in the figure, the maximum change in absorption occurs near the band edge of the QW, where the resonant thirdorder nonlinear susceptibility is largest. Furthermore, the effect of the ISB control light is enhanced at higher carrier concentrations, where the lower k states are completely occupied, resulting in a very small interband absorption 4500
n = 7.5 x 1011 cm2
3000 1500 0
Absorption coefficient (cm1)
4500
n = 1 x 1012 cm2
3000
1500
0
4500
n = 2 x 1012 cm2
3000
1500
Ic = 0 Ic = 1 MW/cm2
0 0.76
0.80
0.85 0.90 Interband signal energy ħω (eV)
0.95
1.00
Figure 10.14 Steadystate absorption coefficient of interband resonant (signal) light in the threelevel system of Fig. 10.13, for different values of the QW doping concentration. Solid (dotted) lines represent the absorption in presence (absence) of the ISB control beam.
Downloaded from Digital Engineering Library @ McGrawHill (www.digitalengineeringlibrary.com) Copyright © 2006 The McGrawHill Companies. All rights reserved. Any use is subject to the Terms of Use as given at the website.
0071457925_CH10_413_03/23/2006 AllOptical Modulation and Switching in the Communication Wavelength Regime Using Intersubband Transitions in InGaAs/AlAsSb Heterostructures AllOptical Modulation and Switching
413
in the absence of control light. The ISB control wave effectively induces a red shift in the interband absorption edge, which is proportional to the ISB energy separation in case of highly doped QWs. However, manybody effects will influence the modulation process and limit the maximum achievable modulation depth. 10.4.1 Alloptical modulation or absorption recovery in InGaAs/AlAsSb single quantum wells
Figure 10.15 shows a pumpprobe measurement system used to evaluate the absorption recovery dynamics associated with ISBTs. Pump pulses with a width of 150 fs and a wavelength of 1.95 m are used to excite ISBTs in InGaAs/AlAsSb QWs, while probe pulses with a spectrum broadened by a sapphire plate (about 1m) are used to monitor the resulting interband absorption changes, as indicated in the inset of the figure. Figure 10.16 shows examplary pumpprobe data measured with an 80period InGaAs/AlAsSb MQW sample with 2nm wells doped to 1 × 1019 cm–3. From this plot, which shows the interband (probe) absorption change as a function of time delay after the ISB excitation, a relaxation time of 2.1 ps is determined [77]. Initially, in the absence of ISB pump light, the conduction subband states below the Fermi level are populated, and interband absorption involving these states does not occur. When the ISB resonant light is coupled to the sample, carriers from the bottom of the first conduction subband c1> are pumped to the second subband on a time scale of ~200 fs governed by the width of the pump pulses [78]. The resulting empty states in c1> lead to an enhancement of the interband absorption rate from hh1> to c1>, or equivalently to a red shift in the interband absorption edge [79]. The states in c1> are subsequently filled through two simultaneous processes – the excitation of carriers from the valence AlAsSb
C. B. ISBpump
E2
V. B.
Pump Delay controller Sapphire
λISB E1 InGaAs
IB probe
TiSapphire fspulse laser
Regen. amp.
λIB
Monochro. Sample
InGaAs det.
Probe Monochro. OPA
InGaAs det.
Figure 10.15 Pumpprobe measurement system used to study ISB relaxation dynamics
in In